Modelling of creep damage development in ferritic steels
Energy Technology Data Exchange (ETDEWEB)
Sandstroem, R. [Swedish Institute for Metals Research, Stockholm (Sweden)
1998-12-31
The physical creep damage, which is observed in fossil-fired power plants, is mainly due to the formation of cavities and their interaction. It has previously been demonstrated that both the nucleation and growth of creep cavities can be described by power functions in strain for low alloy and 12 % CrMoV creep resistant steels. It possible to show that the physical creep damage is proportional to the product of the number of cavities and their area. Hence, the physical creep damage can also be expressed in terms of the creep strain. In the presentation this physical creep damage is connected to the empirical creep damage classes (1-5). A creep strain-time function, which is known to be applicable to low alloy and 12 % CrMoV creep resistant steels, is used to describe tertiary creep. With this creep strain - time model the residual lifetime can be predicted from the observed damage. For a given damage class the remaining life is directly proportional to the service time. An expression for the time to the next inspection is proposed. This expression is a function of fraction of the total allowed damage, which is consumed till the next inspection. (orig.) 10 refs.
Modelling of creep damage development in ferritic steels
Energy Technology Data Exchange (ETDEWEB)
Sandstroem, R [Swedish Institute for Metals Research, Stockholm (Sweden)
1999-12-31
The physical creep damage, which is observed in fossil-fired power plants, is mainly due to the formation of cavities and their interaction. It has previously been demonstrated that both the nucleation and growth of creep cavities can be described by power functions in strain for low alloy and 12 % CrMoV creep resistant steels. It possible to show that the physical creep damage is proportional to the product of the number of cavities and their area. Hence, the physical creep damage can also be expressed in terms of the creep strain. In the presentation this physical creep damage is connected to the empirical creep damage classes (1-5). A creep strain-time function, which is known to be applicable to low alloy and 12 % CrMoV creep resistant steels, is used to describe tertiary creep. With this creep strain - time model the residual lifetime can be predicted from the observed damage. For a given damage class the remaining life is directly proportional to the service time. An expression for the time to the next inspection is proposed. This expression is a function of fraction of the total allowed damage, which is consumed till the next inspection. (orig.) 10 refs.
Creep characterization of type 316LN and HT-9 stainless steels by the K-R creep damage model
International Nuclear Information System (INIS)
Kim, Woo Gon; Kim, Sung Ho; Ryu, Woo Seog
2001-01-01
The Kachanov and Rabotnov (K-R) creep damage model was interpreted and applied to type 316LN and HT-9 stainless steels. Seven creep constants of the model, A, B, k, m, λ, γ, and q were determined for type 316LN stainless steel. In order to quantify a damage parameter, the cavity was interruptedly traced during creep for measuring cavity area to be reflected into the damage equation. For type 316LN stainless steel, λ=ε R /ε * and λ f =ε/ε R were 3.1 and increased with creep strain. The creep curve with λ=3.1 depicted well the experimental data to the full lifetime and its damage curve showed a good agreement when γ=24. However for the HT-9 stainless steel, the values of λ and λ f were different as λ=6.2 and λ f =8.5, and their K-R creep curves did not agree with the experimental data. This mismatch in the HT-9 steel was due to the ductile fracture by softening of materials rather than the brittle fracture by cavity growth. The differences of the values in the above steels were attributed to creep ductilities at the secondary and the tertiary creep stages
Creep Tests and Modeling Based on Continuum Damage Mechanics for T91 and T92 Steels
Pan, J. P.; Tu, S. H.; Zhu, X. W.; Tan, L. J.; Hu, B.; Wang, Q.
2017-12-01
9-11%Cr ferritic steels play an important role in high-temperature and high-pressure boilers of advanced power plants. In this paper, a continuum damage mechanics (CDM)-based creep model was proposed to study the creep behavior of T91 and T92 steels at high temperatures. Long-time creep tests were performed for both steels under different conditions. The creep rupture data and creep curves obtained from creep tests were captured well by theoretical calculation based on the CDM model over a long creep time. It is shown that the developed model is able to predict creep data for the two ferritic steels accurately up to tens of thousands of hours.
Unified Creep Plasticity Damage (UCPD) Model for Rigid Polyurethane Foams.
Energy Technology Data Exchange (ETDEWEB)
Neilsen, Michael K. [Sandia National Lab. (SNL-NM), Albuquerque, NM (United States); Lu, Wei-Yang [Sandia National Lab. (SNL-NM), Albuquerque, NM (United States); Scherzinger, William M. [Sandia National Lab. (SNL-NM), Albuquerque, NM (United States); Hinnerichs, Terry D. [Sandia National Lab. (SNL-NM), Albuquerque, NM (United States); Lo, Chi S. [Sandia National Lab. (SNL-NM), Albuquerque, NM (United States)
2015-06-01
Numerous experiments were performed to characterize the mechanical response of several different rigid polyurethane foams (FR3712, PMDI10, PMDI20, and TufFoam35) to large deformation. In these experiments, the effects of load path, loading rate, and temperature were investigated. Results from these experiments indicated that rigid polyurethane foams exhibit significant volumetric and deviatoric plasticity when they are compressed. Rigid polyurethane foams were also found to be very strain-rate and temperature dependent. These foams are also rather brittle and crack when loaded to small strains in tension or to larger strains in compression. Thus, a new Unified Creep Plasticity Damage (UCPD) model was developed and implemented into SIERRA with the name Foam Damage to describe the mechanical response of these foams to large deformation at a variety of temperatures and strain rates. This report includes a description of recent experiments and experimental findings. Next, development of a UCPD model for rigid, polyurethane foams is described. Selection of material parameters for a variety of rigid polyurethane foams is then discussed and finite element simulations with the new UCPD model are compared with experimental results to show behavior that can be captured with this model.
Damage in Creep Aging Process of an Al-Zn-Mg-Cu Alloy: Experiments and Modeling
Directory of Open Access Journals (Sweden)
Chao Lei
2018-04-01
Full Text Available In creep age forming (CAF, large integral panel components of high-strength aluminum alloy can be shaped and strengthened under external elastic loading at an elevated temperature through creep deformation and age hardening, simultaneously. However, the high ribbed structure on panel may induce stress concentration, inhomogeneous plastic deformation and even damage evolution on the bending rib, leading to the difficulty in controlling forming precision and material properties. Therefore, the generation and evolution of damage are necessary to be considered in the design of CAF. Taking 7050 aluminum alloy as the case material, the continuous and interrupted creep aging tests at 165 °C and three stress levels (300, 325, and 350 MPa were conducted, and the corresponding material properties, precipitate, and damage microstructures were studied by mechanical properties tests, transmission electron microscope (TEM and scanning electron microscope (SEM characterizations. With the increase of stress level, the creep deformation occurs easier, the precipitates grow up faster, the creep damage occurs earlier, the growth rate and the size of microvoids increase, the mechanical properties decrease more rapidly, and the dominant mechanism of creep fracture changes from shear to microvoid coalescence. To simulate creep aging behavior with damage, a continuum damage mechanics (CDM based model is calibrated and numerically implemented into ABAQUS solver via CREEP subroutine. The CAF of 7050 aluminum alloy panels with different height ribs were conducted by experiment and FE simulation. The forming process presents a typical stress relaxation phenomenon. The creep damage mainly occurs on the bending rib due to the severe stress concentration. With the increase of rib height, the creep strain and damage degree increase, but the springback decreases.
Modelling of microstructural creep damage in welded joints of 316L stainless steel
International Nuclear Information System (INIS)
Bouche, G.
2000-01-01
Welded joints of 316L stainless steel under service conditions at elevated temperature are known to be preferential sites of creep damage, as compared to the base material. This damage results in the formation of cavities and the development of creep cracks which can lead to a premature failure of welded components. The complex two-phase microstructure of 316L welds was simulated by manually filling a mould with longitudinal deposited weld beads. The moulded material was then aged during 2000 hours at 600 deg. C. High resolution Scanning Electron Microscopy was largely used to examine the microstructure of the simulated material before and after ageing. Smooth and notched creep specimens were cut from the mould and tested at 600 deg. C under various stress levels. A comparison of the lifetime versus nominal stress curves for the base and welded materials shows a greater dependence of the welded material to creep phenomena. Observation and EBSD analysis show that damage is preferentially located along the austenite grain boundaries. The stress and strain fields in the notched specimens were calculated by finite element method. A correlation of this field to the observed damage was made in order to propose a predictive law relating the creep damage to the mechanical conditions applied locally. Further mechanical tests and simulation on CT specimens and mode II tubular specimens allowed validating the model under various multiaxial loading conditions. (author)
le Graverend, J.-B.
2018-05-01
A lattice-misfit-dependent damage density function is developed to predict the non-linear accumulation of damage when a thermal jump from 1050 °C to 1200 °C is introduced somewhere in the creep life. Furthermore, a phenomenological model aimed at describing the evolution of the constrained lattice misfit during monotonous creep load is also formulated. The response of the lattice-misfit-dependent plasticity-coupled damage model is compared with the experimental results obtained at 140 and 160 MPa on the first generation Ni-based single crystal superalloy MC2. The comparison reveals that the damage model is well suited at 160 MPa and less at 140 MPa because the transfer of stress to the γ' phase occurs for stresses above 150 MPa which leads to larger variations and, therefore, larger effects of the constrained lattice misfit on the lifetime during thermo-mechanical loading.
A Model for Creep and Creep Damage in the γ-Titanium Aluminide Ti-45Al-2Mn-2Nb.
Harrison, William; Abdallah, Zakaria; Whittaker, Mark
2014-03-14
Gamma titanium aluminides (γ-TiAl) display significantly improved high temperature mechanical properties over conventional titanium alloys. Due to their low densities, these alloys are increasingly becoming strong candidates to replace nickel-base superalloys in future gas turbine aeroengine components. To determine the safe operating life of such components, a good understanding of their creep properties is essential. Of particular importance to gas turbine component design is the ability to accurately predict the rate of accumulation of creep strain to ensure that excessive deformation does not occur during the component's service life and to quantify the effects of creep on fatigue life. The theta (θ) projection technique is an illustrative example of a creep curve method which has, in this paper, been utilised to accurately represent the creep behaviour of the γ-TiAl alloy Ti -45Al-2Mn-2Nb. Furthermore, a continuum damage approach based on the θ-projection method has also been used to represent tertiary creep damage and accurately predict creep rupture.
Study on Creep Damage Model of 1Cr1Mo1/4V Steel for Turbine Rotor
International Nuclear Information System (INIS)
Choi, Woo Sung; Song, Gee Wook; Kim, Bum Shin; Chang, Sung Ho; Fleury, Eric
2011-01-01
It is well known that the dominant damage mechanisms in high-temperature steam turbine facilities such as rotor and casing are creep and fatigue damages. Even though coupling of creep and fatigue should be considered while predicting the life of turbine facilities, the remaining life of large steam turbine facilities is generally determined on the basis of creep damage because the turbines must generate stable base-load power and because they are operated at a high temperature and pressure for a long time. Almost every large steam turbine in Korea has been operated for more than 20 years and is made of steel containing various amounts of principal alloying elements nickel, chromium, molybdenum, and vanadium. In this study, creep damage model of 1Cr1Mo1/4V steel for turbine rotor is proposed and that can assess the high temperature creep life of large steam turbine facilities is proposed
Micromechanical Modeling of Grain Boundaries Damage in a Copper Alloy Under Creep
International Nuclear Information System (INIS)
Voese, Markus
2015-01-01
In order to include the processes on the scale of the grain structure into the description of the creep behaviour of polycrystalline materials, the damage development of a single grain boundary has been initially investigated in the present work. For this purpose, a special simulationmethod has been used, whose resolution procedure based on holomorphic functions. The mechanisms taken into account for the simulations include nucleation, growth by grain boundary diffusion, coalescence and shrinkage until complete sintering of grain boundary cavities. These studies have then been used to develop a simplified cavitation model, which describes the grain boundary damage by two state variables and the time-dependent development by a mechanism-oriented rate formulation. To include the influence of grain boundaries within continuum mechanical considerations of polycrystals, an interface model has been developed, that incorporates both damage according to the simplified cavitation model and grain boundary sliding in dependence of a phenomenological grain boundary viscosity. Furthermore a micromechanical model of a polycrystal has been developed that allows to include a material's grain structure into the simulation of the creep behaviour by means of finite element simulations. Thereby, the deformations of individual grains are expressed by a viscoplastic single crystal model and the grain boundaries are described by the proposed interface model. The grain structure is represented by a finite element model, in which the grain boundaries are modelled by cohesive elements. From the evaluation of experimental creep data, the micromechanical model of a polycrystal has been calibrated for a copper-antimony alloy at a temperature of 823 K. Thereby, the adjustment of the single crystal model has been carried out on the basis of creep rates of pure copper single crystal specimens. The experimental determination of grain boundary sliding and grain boundary porosity for coarse
Comparative analysis of coupled creep-damage model implementations and application
International Nuclear Information System (INIS)
Bhandari, S.; Feral, X.; Bergheau, J.M.; Mottet, G.; Dupas, P.; Nicolas, L.
1998-01-01
Creep rupture of a reactor pressure vessel in a severe accident occurs after complex load and temperature histories leading to interactions between creep deformations, stress relaxation, material damaging and plastic instability. The concepts of continuous damage introduced by Kachanov and Robotnov allow to formulate models coupling elasto-visco-plasticity and damage. However, the integration of such models in a finite element code creates some difficulties related to the strong non-linearity of the constitutive equations. It was feared that different methods of implementation of such a model might lead to different results which, consequently, might limit the application and usefulness of such a model. The Commissariat a l'Energie Atomique (CEA), Electricite de France (EDF) and Framasoft (FRA) have worked out numerical solutions to implement such a model in respectively CASTEM 2000, ASTER and SYSTUS codes. A ''benchmark'' was set up, chosen on the basis of a cylinder studied in the programme ''RUPTHER''. The aim of this paper is not to enter into the numerical details of the implementation of the model, but to present the results of the comparative study made using the three codes mentioned above, on a case of engineering interest. The results of the coupled model will also be compared to an uncoupled model to evaluate differences one can obtain between a simple uncoupled model and a more sophisticated coupled model. The main conclusion drawn from this study is that the different numerical implementations used for the coupled damage-visco-plasticity model give quite consistent results. The numerical difficulty inherent to the integration of the strongly non-linear constitutive equations have been resolved using Runge-Kutta or mid-point rule. The usefulness of the coupled model comes from the fact the uncoupled model leads to too conservative results, at least in the example treated and in particular for the uncoupled analysis under the hypothesis of the small
A simplified model for cumulative damage with interaction effect for creep loading
International Nuclear Information System (INIS)
Gomuc, R.; Bui-Quoc, T.; Biron, A.
1989-01-01
This paper explains that the basic creep-rupture behavior of a material at high temperature is obtained with constant stresses under isothermal conditions. Structural components operating at high temperature are, however, usually subjected to fluctuations of stresses and/or temperatures. Experimental conditions cannot cover all possible combinations of these parameters and, in addition, systematic investigations on cumulative creep damage are very limited due to long-term testing. The authors suggest that there is a need to establish a reliable procedure for evaluating the cumulative creep damage effect under non-steady stresses and temperatures
The prediction of creep damage in Type 347 weld metal: part II creep fatigue tests
International Nuclear Information System (INIS)
Spindler, M.W.
2005-01-01
Calculations of creep damage under conditions of strain control are often carried out using either a time fraction approach or a ductility exhaustion approach. In part I of this paper the rupture strength and creep ductility data for a Type 347 weld metal were fitted to provide the material properties that are used to calculate creep damage. Part II of this paper examines whether the time fraction approach or the ductility exhaustion approach gives the better predictions of creep damage in creep-fatigue tests on the same Type 347 weld metal. In addition, a new creep damage model, which was developed by removing some of the simplifying assumptions that are made in the ductility exhaustion approach, was used. This new creep damage model is a function of the strain rate, stress and temperature and was derived from creep and constant strain rate test data using a reverse modelling technique (see part I of this paper). It is shown that the new creep damage model gives better predictions of creep damage in the creep-fatigue tests than the time fraction and the ductility exhaustion approaches
Analysis of localized damage in creep rupture
International Nuclear Information System (INIS)
Wang Zhengdong; Wu Dongdi
1992-01-01
Continuum Damage Mechanics studies the effect of distributed defects, whereas the failure of engineering structures is usually caused by local damage. In this paper, an analysis of localized damage in creep rupture is carried out. The material tested is a 2 1/4Cr-1Mo pressure vessel steel and the material constants necessary for damage analysis are evaluated. Notched specimens are used to reflect localized damage in creep rupture and the amount of damage is measured using DCPD method. Through FEM computation, stress components and effective stress in the region of notch root are evaluated and it is found that the von Mises effective stress can represent the damage effective stress in the analysis of localized creep damage. It is possible to develop a method for the assessment of safety of pressure vessels under creep through localized creep damage analysis. (orig.)
Thermal ratcheting and creep damage
International Nuclear Information System (INIS)
Clement, G.; Cousseran, P.; Roche, R.L.
1983-01-01
Several proposals have been made to assist adesigners with thermal ratcheting in the creep range, the more known has been made by O'DONNELL and POROWSKY. Unfortunately these methods are not validated by experiments, and they take only inelastic distortion into consideration as creep effects. The aim of the work presented here is to correct these deficiencies - in providing an experimental basis to ratcheting analysis rules in the creep range, - in considering the effect of cyclic straining (like cyclic thermal stresses) on the time to rupture by creep. Experimental tests have been performed on austenitic stainless steel at 650 0 C for the first item. Results of these tests and results available in the open literature have been used to built a practical rule of ratcheting analysis. This rule giving a conservative value of the creep distortion, is based on the concept of effective primary stress which is an amplification of the primary stress really applied. Concerning the second point (time to rupture), it was necessary to obtain real creep rupture and not instability. According to the proposal of Pr LECKIE, tests were performed on specimens made out of copper, and of aluminium alloys at temperatures between 150 0 C and 300 0 C. With such materials creep rupture is obtained without necking. Experimental tests show that cyclic straining reduces the time to creep rupture under load controlled stress. Caution must be given to the designer: cyclic thermal stress can lead to premature creep rupture. (orig./GL)
International Nuclear Information System (INIS)
Saliba, J.
2012-01-01
In order to design reliable concrete structures, prediction of long term behaviour of concrete is important. In fact, creep deformation can cause mechanical deterioration and cracking, stress redistribution, loss in prestressed members and rarely ruin the structure. The aim of this research is to have a better understanding of the interaction between creep and crack growth in concrete. An experimental investigation on the fracture properties of concrete beams submitted to creep bending tests with high levels of sustained load is reported. The influence of creep on residual capacity and fracture energy of concrete is studied. In parallel, the acoustic emission technique (AE) was used to monitor crack development. The results give wealth information on damage evolution and show a decrease in the width of the fracture process zone (FPZ) characterizing a more brittle behaviour for beams subjected to creep. The AE shows that this may be due to the development of microcracking detected under creep. Based on those experimental results, a mesoscopic numerical study was proposed by coupling a damage model based on the micro-plan theory and a viscoelastic creep model defined by several Kelvin-voigt chains. The numerical results on concrete specimens in tension and in bending confirm the development of microcracks during creep at the mortar-aggregate interface. (author)
Thermal ratcheting and creep damage
International Nuclear Information System (INIS)
Clement, G.; Cousseran, P.; Roche, R.L.
1983-08-01
Creep is a cause of deformation; it may also result in rupture in time. Although LMFBR structures are not heavily loaded, they are subjected to large thermal transients. Can structure lifetime be shortened by such transients. Several proposals have been made to assist adesigners with thermal ratcheting in the creep range. Unfortunately these methods are not validated by experiments, and they take only inelastic distorsion into consideration as creep effects. The aim of the work presented here is to correct these deficiencies in providing an experimental basis to ratcheting analysis rules in the creep range, and in considering the effect of cyclic straining (like cyclic thermal stresses) on the time to rupture by creep. Experimental tests have been performed on austenitic stainless steel at 650 0 C for the first item. Results of these tests and results available in the open literature have been used to built a practical rule of ratcheting analysis. This rule giving a conservative value of the creep distortion, is based on the concept of effective primary stress which is an amplification of the primary stress really applied. Concerning the second point (time to rupture), it was necessary to obtain real creep rupture and not instability. According to the proposal of Pr LECKIE, tests were performed on specimen made out of copper, and of aluminium alloys at temperatures between 150 0 C and 300 0 C. With such materials creep rupture is obtained without necking. Experimental tests show that cyclic straining reduces the time to creep rupture under load controlled stress. Caution must be given to the designer: cyclic thermal stress can lead to premature creep rupture
Anisotropic creep damage in the framework of continuum damage mechanics
International Nuclear Information System (INIS)
Caboche, J.L.
1983-01-01
For some years, various works have shown the possibility of applying continuum mechanics to model the evolution of the damage variable, initially introduced by Kachanov. Of interest here are the complex problems posed by the anisotropy which affects both the elastic behaviour and the viscoplastic one, and also the rupture phenomenon. The main concepts of the Continuum Damage Mechanics are briefly reviewed together with some classical ways to introduce anisotropy of damage in the particular case of proportional loadings. Based on previous works, two generalizations are presented and discussed, which use different kinds of tensors to describe the anisotropy of creep damage: - The first one, by Murakami and Ohno introduces a second rank damage tensor and a net stress tensor through a net area definition. The effective stress-strain behaviour is then obtained by a fourth rank tensor. - The second theory, by the author, uses one effective stress tensor only, defined in terms of the macroscopic strain behaviour, through a fourth-order non-symmetrical damage tensor. The two theories are compared at several levels: difference and similarities are pointed out for the damage evolution during tensile creep as well as for anisotropy effects. The possibilities are discussed and compared on the basis of some existing experimental results, which leads to a partial validation of the two approaches. (orig.)
Advanced nondestructive evaluation for creep damage
International Nuclear Information System (INIS)
Anon.
1987-01-01
As a result of operation at elevated temperatures, power plant components experience creep. Changes in metallurgical structure and microscopic cracking occur after periods of operation and lead to component failure. In order to detect the presence of creep and avoid creep-related failures, EPRI has just initiated a five year program entitled Advanced NDE for Creep Damage (RP 1856-7). The objective of this program is to develop NDE methods for detection and characterization of microscopic creep damage. Several NDE methods will be initially evaluated to determine their potential for detecting and characterizing such damage. These NDE methods include ultrasonics, eddy current, Barkhausen, positron annihilation, and thermal-wave imaging. A prototype system will be developed and tested for commercial applications in a follow-on project, utilizing characteristics of the best NDE method for creep detection. A brief description of the project and results of a theoretical investigation, to determine feasibility of ultrasonic NDE method, for detection of creep damage are presented
International Nuclear Information System (INIS)
Gaffard, V.
2004-12-01
Chromium martensitic stainless steels are under development since the 70's with the prospect of using them as structural components in thermal and nuclear power plants. The modified 9Cr1Mo-NbV steel is already used, especially in England and Japan, as a material for structural components in thermal power plants where welding is a commonly used joining technique. New generations of chromium martensitic stainless steels with improved mechanical properties for high pressure and temperature use are currently under development. However, observations of several in-service premature failures of welded components in 9Cr1Mo-NbV steel, outline a strong need for understanding the high temperature creep flow and damage behaviour of 9Cr1Mo-NbV steels and weldments. The present study aimed at experimentally determining and then modelling the high temperature creep flow and damage behaviour of both 9Cr1Mo-NbV steels and weldments (typically in the temperature range from 450 C to 650 C). The base metal was first studied as the reference material. It was especially evidenced that tempered chromium martensitic steels exhibit a change in both creep flow and damage behaviour for long term creep exposure. As a consequence, the classically performed extrapolation of 1,000 hours creep data to 100,000 hours creep lifetime predictions might be very hazardous. Based on experimental observations, a new model, integrating and coupling multiple creep flow and damage mechanisms, was developed in the framework of the mechanics of porous media. It was then successfully used to represent creep flow and damage behaviour of the base metal from high to low stress levels even for complex multiaxial loading conditions. Although the high temperature creep properties of the base metal are quite good, the occurrence of premature failure in weldments in high temperature creep conditions largely focused the attention of the scientific community. The lower creep strength of the weld component was also
Creep fatigue damage under multiaxial conditions
International Nuclear Information System (INIS)
Lobitz, D.W.; Nickell, R.E.
1977-01-01
When structural components are subjected to severe cyclic loading conditions with intermittent periods of sustained loading at elevated temperature, the designer must guard against a failure mode caused by the interaction of time-dependent and time-independent deformation. This phenomena is referred to as creep-fatigue interaction. The most elementary form of interaction theory (called linear damage summation) is now embodied in the ASME Boiler and Pressure Vessel Code. In recent years, a competitor for the linear damage summation theory has emerged, called strainrange partitioning. This procedure is based upon the visualization of the cyclic strain in a uniaxial creep-fatigue test as a hysteresis loop, with the inelastic strains in the loop counter-balanced in one of two ways. The two theories are compared and contrasted in terms of ease of use, possible inconsistencies, and component life prediction. Future work to further test the damage theories is recommended
International Nuclear Information System (INIS)
Spindler, M.W.
2005-01-01
Calculations of creep damage under conditions of strain control are often carried out using either a time fraction approach or a ductility exhaustion approach. In the case of the time fraction approach the rupture strength is used to calculate creep damage, whereas creep ductility is used in the ductility exhaustion approach. In part I of this paper the methods that are used to determine these material properties are applied to some creep and constant strain rate tests on a Type 347 weld metal. In addition, new developments to the ductility exhaustion approach are described which give improved predictions of creep damage at failure in these tests. These developments use reverse modelling to determine the most appropriate creep damage model as a function of strain rate, stress and temperature. Hence, the new approach is no longer a ductility exhaustion approach but is a true creep damage model
Creep-fatigue damage under multiaxial conditions
International Nuclear Information System (INIS)
Lobitz, D.W.; Nickell, R.E.
1977-02-01
ASME Code rules for design against creep-fatigue damage for Class 1 nuclear components operating at elevated temperatures are currently being studied by ASME working groups and task forces with a view toward major modification. In addition, the design rules being developed for Class 2 and Class 3 components would be affected by any major modifications of Class 1 Rules. The report represents an attempt to evaluate the differences between two competing procedures--linear damage summation and strainrange partitioning--for multiaxial stress conditions. A modified version of strainrange partitioning is also developed to alleviate some limitations on nonproportional loading
Irradiation creep models - an overview
International Nuclear Information System (INIS)
Matthews, J.R.; Finnis, M.W.
1988-01-01
The modelling of irradiation creep is now highly developed but many of the basic processes underlying the models are poorly understood. A brief introduction is given to the theory of cascade interactions, point defect clustering and dislocation climb. The range of simple irradiation creep models is reviewed including: preferred nucleation of interstitial loops; preferred absorption of point defects by dislocations favourably orientated to an applied stress; various climb-enhanced glide and recovery mechanisms, and creep driven by internal stresses produced by irradiation growth. A range of special topics is discussed including: cascade effects; creep transients; structural and induced anisotropy; and the effect of impurities. The interplay between swelling and growth with thermal and irradiation creep is emphasized. A discussion is given on how irradiation creep theory should best be developed to assist the interpretation of irradiation creep observations and the requirements of reactor designers. (orig.)
Recent advances in modelling creep crack growth
International Nuclear Information System (INIS)
Riedel, H.
1988-08-01
At the time of the previous International Conference on Fracture, the C* integral had long been recognized as a promising load parameter for correlating crack growth rates in creep-ductile materials. The measured crack growth rates as a function of C* and of the temperature could be understood on the basis of micromechanical models. The distinction between C*-controlled and K I -controlled creep crack growth had been clarified and first attempts had been made to describe creep crack growth in the transient regime between elastic behavior and steady-state creep. This paper describes the progress in describing transient crack growth including the effect of primary creep. The effect of crack-tip geometry changes by blunting and by crack growth on the crack-tip fields and on the validity of C* is analyzed by idealizing the growing-crack geometry by a sharp notch and using recent solutions for the notch-tip fields. A few new three-dimensional calculations of C* are cited and important theoretical points are emphasized regarding the three-dimensional fields at crack tips. Finally, creep crack growth is described by continuum-damage models for which similarity solutions can be obtained. Crack growth under small-scale creep conditions turns out to be difficult to understand. Slightly different models yield very different crack growth rates. (orig.) With 4 figs
International Nuclear Information System (INIS)
Yamauchi, Masafumi; Chuman, Yasuharu; Otani, Tomomi; Takahashi, Yukio
2001-01-01
The effect of prior creep-fatigue damage on the creep and the fatigue characteristics was studied to investigate the creep-fatigue life evaluation procedure of 316FR stainless steel. Creep and fatigue tests were conducted at 550degC by using the specimen exposed to prior creep-fatigue cycles at the same temperature and interrupted at 1/4 Nf, 1/2 Nf and 3/4 Nf cycle. The creep and fatigue strength of the pre-damaged material showed monotonic reduction with the prior creep-fatigue damage compared with the virgin material. The creep ductility also showed monotonic reduction with the prior creep-fatigue damage. These results were evaluated by the stress-based Time Fraction Rule and the strain-based Ductility Exhaustion Method. The result showed that the application of the Ductility Exhaustion Method to the creep-fatigue damage evaluation is more promising than the Time Fraction Rule. (author)
Nondestructive evaluation of creep-fatigue damage: an interim report
International Nuclear Information System (INIS)
Nickell, R.E.
1977-02-01
In view of the uncertainties involved in designing against creep-fatigue failure and the consequences of such failures in Class 1 nuclear components that operate at elevated temperature, the possibility of intermittent or even continuous non-destructive examination of these components has been considered. In this interim report some preliminary results on magnetic force and ultrasonic evaluation of creep-fatigue damage in an LMFBR steam generator material are presented. These results indicate that the non-destructive evaluation of pure creep damage will be extremely difficult. A set of biaxial creep-fatigue tests that are designed to discriminate between various failure theories is also described
Creep damage development in welded X20 and P91
Energy Technology Data Exchange (ETDEWEB)
Brett, Steve; Holmstrom, Stefan; Hald, John; Borg, Ulrik; Aakjaer Jensen, Soeren; Vulpen, Rijk Van; Degnan, Craig; Vinter Dahl, Kristian; Vilhelmsen, Tommy
2011-03-15
The Martensitic steel X20CrMoV121 (hereinafter called X20) and the modified 9Cr1Mo steel (hereinafter called P91) have been used for a number of years in high temperature applications since they posses superior creep strength compared to low alloyed steels. Due to the simple fact that very few failures were observed, almost no knowledge as to the evolution of creep damage in welds were available despite long operation times exceeding well over 100.000 hours. It has been suggested that X20 will develop creep damage in a different manner compared to low alloyed steel, i.e damage initiation should be slow followed by accelerated growth. The research work presented in this report included systematic investigations of the first components of X20, which has developed creep during long-term operation. All of the investigated components showed creep damage evolution similar to low alloy steels
Some numerical approaches of creep, thermal shock, damage
Indian Academy of Sciences (India)
Creep can be satisfactorily described by a kinematic hardening, and exhibits different creep rates in tension and compression. Concerning the thermal shock of materials, the numerical approach depends whether or not the material is able to develop a sprayed out damage, leading to micro- or macro-cracking. Finally ...
International Nuclear Information System (INIS)
Taroco, E.; Feijoo, R.A.; Monteiro, Edson; Freire, J.L.F.; Bevilacqua, L.; Miranda, P.E.V. de; Silveira, T.L. da
1982-01-01
A pressure vessel is analized using different mechanical models for the creep phenomenon. The numerical results obtained through these models enable us to recommend on the way verifications of creep damage accumulation is structures should be made. (Author) [pt
Energy Technology Data Exchange (ETDEWEB)
Bouche, G
2000-07-01
Welded joints of 316L stainless steel under service conditions at elevated temperature are known to be preferential sites of creep damage, as compared to the base material. This damage results in the formation of cavities and the development of creep cracks which can lead to a premature failure of welded components. The complex two-phase microstructure of 316L welds was simulated by manually filling a mould with longitudinal deposited weld beads. The moulded material was then aged during 2000 hours at 600 deg. C. High resolution Scanning Electron Microscopy was largely used to examine the microstructure of the simulated material before and after ageing. Smooth and notched creep specimens were cut from the mould and tested at 600 deg. C under various stress levels. A comparison of the lifetime versus nominal stress curves for the base and welded materials shows a greater dependence of the welded material to creep phenomena. Observation and EBSD analysis show that damage is preferentially located along the austenite grain boundaries. The stress and strain fields in the notched specimens were calculated by finite element method. A correlation of this field to the observed damage was made in order to propose a predictive law relating the creep damage to the mechanical conditions applied locally. Further mechanical tests and simulation on CT specimens and mode II tubular specimens allowed validating the model under various multiaxial loading conditions. (author)
Energy Technology Data Exchange (ETDEWEB)
Fabre, G
2005-06-15
The underground radioactive waste disposal far exceeds the period of exploitation of common civil engineering works. These specific projects require to predict the irreversible deformations over a large time scale (several centuries) in order to assess the extension and to forecast the evolution of the EDZ (Excavation Damage Zone) around the cavity. In this study, the viscosity of three sedimentary argillaceous rocks has been studied under different conditions of uniaxial compression: static or cyclic creep tests, monotonic and quasistatic tests, performed across various strata orientations. Argillaceous rocks are studied as a possible host layer for radioactive waste disposals. Indeed, they present some of the physical characteristics and mechanical properties, which are essential for being a natural barrier: low permeability, high creep potential and important holding capacity of radioactive elements. The purpose of the experimental study was to shed some light over the mechanisms governing the development of delayed deformations and damage of argillaceous rocks. It relates three rocks: an argillite from East of France, a Tournemire argillite and a marl from Jurassic Mountains. On atomic scale, viscoplastic deformations are due to irreversible displacements of crystalline defects, called dislocations. The experimental study was also supplemented with observations on thin sections extracted from the argillite and marl samples using a SEM. The aim was to identify the mechanisms responsible for the time-dependent behaviour on a microstructural scale. Analytical simulations of the mechanical behaviour of the three rocks gave parameters used in different viscoplastic models. The best modeling was obtained with the viscoplastic model which takes account of the development of volumetric strains and of the damage anisotropy. (author)
Creep damage evaluation of low alloy steel weld joint by small punch creep testing
International Nuclear Information System (INIS)
Nishioka, Tomoya; Sawaragi, Yoshiatsu; Uemura, Hiromi
2013-01-01
The effect of sampling location on SPC (Small Punch Creep) tests were investigated for weld joints to establish evaluation method of Type IV creep behavior. The SPC specimen shape was 10mm diameter and 0.5mm thick round disc prepared from weld joints of 2.25Cr-1Mo low alloy steel. It was found that the center of SPC specimen should be 2mm apart from the weld interface as the recommended sampling location. Creep damage was imposed for large weld joint specimens by axial creep loading at 620degC, 52MPa with the interrupted time fraction of 0.34, 0.45, 0.64 and 0.82.SPC samples were prepared from those damaged specimens following the recommended way described in this paper. Among the various SPC tests conducted, good relationships were found for the test condition of 625degC, 200N. Namely, good relationships were obtained both between minimum deflection rate and creep life fraction, and between rupture time and creep life fraction. Consequently, creep life assessment of Type IV fracture by SPC tests could be well conducted using the sampling location and the test condition recommended in this paper. (author)
Examination of observed and predicted measures of creep cavitation damage accumulation
Energy Technology Data Exchange (ETDEWEB)
Brear, J.M.; Church, J.M. [ERA Technology Ltd., Leatherhead (United Kingdom); Eggeler, G. [University of Bochum-Ruhr (Germany)
1998-12-31
Brittle intergranular cavitation represents a primary degradation mechanism for high temperature plant operating within the creep range. Fundamental to formulating estimates of remanent life, or consumed life fraction for such components are: the observation and quantification of the level of actual creep cavitation, typically using an A-parameter type approach, and the correlation of observed creep damage accumulation with some phenomenological model which characterizes the rate of damage evolution and, thereby, rupture lifetime. The work described here treats inhomogeneous damage accumulation - in otherwise uniform material and loading situations. Extensions to the A-parameter are considered as a practical measure of damage localization and an extension of the Kachanov-Rabotnov continuum damage mechanics model is proposed to allow theoretical treatment. (orig.) 4 refs.
Examination of observed and predicted measures of creep cavitation damage accumulation
Energy Technology Data Exchange (ETDEWEB)
Brear, J M; Church, J M [ERA Technology Ltd., Leatherhead (United Kingdom); Eggeler, G [University of Bochum-Ruhr (Germany)
1999-12-31
Brittle intergranular cavitation represents a primary degradation mechanism for high temperature plant operating within the creep range. Fundamental to formulating estimates of remanent life, or consumed life fraction for such components are: the observation and quantification of the level of actual creep cavitation, typically using an A-parameter type approach, and the correlation of observed creep damage accumulation with some phenomenological model which characterizes the rate of damage evolution and, thereby, rupture lifetime. The work described here treats inhomogeneous damage accumulation - in otherwise uniform material and loading situations. Extensions to the A-parameter are considered as a practical measure of damage localization and an extension of the Kachanov-Rabotnov continuum damage mechanics model is proposed to allow theoretical treatment. (orig.) 4 refs.
A constitutive model for representing coupled creep, fracture, and healing in rock salt
International Nuclear Information System (INIS)
Chan, K.S.; Bodner, S.R.; Munson, D.E.; Fossum, A.F.
1996-01-01
The development of a constitutive model for representing inelastic flow due to coupled creep, damage, and healing in rock salt is present in this paper. This model, referred to as Multimechanism Deformation Coupled Fracture model, has been formulated by considering individual mechanisms that include dislocation creep, shear damage, tensile damage, and damage healing. Applications of the model to representing the inelastic flow and fracture behavior of WIPP salt subjected to creep, quasi-static loading, and damage healing conditions are illustrated with comparisons of model calculations against experimental creep curves, stress-strain curves, strain recovery curves, time-to-rupture data, and fracture mechanism maps
Creep damage in zircaloy-4 at LWR temperatures
International Nuclear Information System (INIS)
Keusseyan, R.L.; Hu, C.P.; Li, C.Y.
1978-08-01
The observation of creep damage in the form of grain boundary cavitation in Zircaloy-4 in the temperature range of interest to Light Water Reactor (LWR) applications is reported. The observed damage is shown to reduce the ductility of Zircaloy-4 in a tensile test at LWR temperatures
Evaluation of creep damage in power plant applications
Energy Technology Data Exchange (ETDEWEB)
Auerkari, P; Salonen, J. [VTT Manufacturing Technology, Espoo (Finland)] McNiven, U. [IVO Generation Services Ltd., Naantali (Finland)] Roennberg, J. [Imatran Voima Oy, Vantaa (Finland)] Borggreen, K. [FORCE Institute, Broendby (Germany)
1998-12-31
Metallographic inspection of creep cavitation damage provides routine support for maintenance scheduling of high temperature components in power plants. The available European inspection experience has been reviewed, particularly considering the performance of thick-section steam systems outside the boiler. Applications are highlighted with examples from plant. (orig.) 8 refs.
Evaluation of creep damage in power plant applications
Energy Technology Data Exchange (ETDEWEB)
Auerkari, P.; Salonen, J. [VTT Manufacturing Technology, Espoo (Finland)] McNiven, U. [IVO Generation Services Ltd., Naantali (Finland)] Roennberg, J. [Imatran Voima Oy, Vantaa (Finland)] Borggreen, K. [FORCE Institute, Broendby (Germany)
1997-12-31
Metallographic inspection of creep cavitation damage provides routine support for maintenance scheduling of high temperature components in power plants. The available European inspection experience has been reviewed, particularly considering the performance of thick-section steam systems outside the boiler. Applications are highlighted with examples from plant. (orig.) 8 refs.
International Nuclear Information System (INIS)
Kawasaki, Nobuchika; Asayama, Tai
2001-09-01
Both reliability and safety have to be further improved for the successful commercialization of FBRs. At the same time, construction and operation costs need to be reduced to a same level of future LWRs. To realize compatibility among reliability, safety and, cost, the Structural Mechanics Research Group in JNC started the development of System Based Code for Integrity of FBR. This code extends the present structural design standard to include the areas of fabrication, installation, plant system design, safety design, operation and maintenance, and so on. A quantitative index is necessary to connect different partial standards in this code. Failure probability is considered as a candidate index. Therefore we decided to make a model calculation using failure probability and judge its applicability. We first investigated other probabilistic standards like ASME Code Case N-578. A probabilistic approach in the structural integrity evaluation was created based on these results, and also an evaluation flow was proposed. According to this flow, a model calculation of creep-fatigue damage was performed. This trial calculation was for a vessel in a sodium-cooled FBR. As the result of this model calculation, a crack initiation probability and a crack penetration probability were found to be effective indices. Last we discussed merits of this System Based Code, which are presented in this report. Furthermore, this report presents future development tasks. (author)
Bouchard, P J; Treimer, W
2002-01-01
Grain-boundary cavitation is the dominant failure mode associated with initiation of reheat cracking, which has been widely observed in austenitic stainless steel pressure vessels operating at temperatures within the creep range (>450 C). Small angle neutron scattering (SANS) experiments at the LLB PAXE instrument (Saclay) and the V12 double-crystal diffractometer of the HMI-BENSC facility (Berlin) are used to characterise cavitation damage (in the size range R=10-2000 nm) in a variety of creep specimens extracted from ex-service plant. Factors that affect the evolution of cavities and the cavity-size distribution are discussed. The results demonstrate that SANS techniques have the potential to quantify the development of creep damage in type-316H stainless steel, and thereby link microstructural damage with ductility-exhaustion models of reheat cracking. (orig.)
Creep damage of 12% CrMoV weldments
International Nuclear Information System (INIS)
Kussmaul, K.; Maile, K.; Theofel, H.
1989-01-01
Creep tests were performed to determine the creep behaviour of similar welded joints of 12% CrMoV-steels which had been made using various heat inputs. The specimens were taken transverse to the seam. The transition from the coarse-grained to the fine-grained area of the heat affected zone (HAZ) proved to be the location of failure after longer rupture times. All tested specimens lie in the +-20% scatterband of the material standard DIN 17175. Creep rupture was initiated by the nucleation and growth of cavities. The appearance of the damage zone near the fracture face depends on testing conditions and heat input. The nucleation of cavities can be detected at an early stage of lifetime
International Nuclear Information System (INIS)
Lim, Dong-Won; Lee, Hyeong-Yeon; Eoh, Jae-Hyuk; Son, Seok-Kwon; Kim, Jong-Bum; Jeong, Ji-Young
2016-01-01
The objective of the STELLA-2 is to support the specific design approval for PGSFR by synthetic reviews of key safety issues and code validations through the integral effect tests. Due to its high temperature operation in SFRs (and in a testing facility) up to 550 °C, thermally induced creep-fatigue damage is very likely in components including a reactor vessel, reactor internals (interior structures), heat exchangers, pipelines, etc. In this study, structural integrity of the components such as reactor vessel and internals in STELLA-2 has been evaluated against creep-fatigue failures at a concept-design step. As 2D analysis yields far conservative results, a realistic 3D simulation is performed by a commercial software. A design integrity guarding against a creep-fatigue damage failure operating at high temperature was evaluated for the reactor vessel with its internal structure of the STELLA-2. Both the high temperature design codes were used for the evaluation, and results were compared. All the results showed the vessel as a whole is safely designed at the given operating conditions, while the ASME-NH gives a conservative evaluation
Energy Technology Data Exchange (ETDEWEB)
Lim, Dong-Won; Lee, Hyeong-Yeon; Eoh, Jae-Hyuk; Son, Seok-Kwon; Kim, Jong-Bum; Jeong, Ji-Young [KAERI, Daejeon (Korea, Republic of)
2016-05-15
The objective of the STELLA-2 is to support the specific design approval for PGSFR by synthetic reviews of key safety issues and code validations through the integral effect tests. Due to its high temperature operation in SFRs (and in a testing facility) up to 550 °C, thermally induced creep-fatigue damage is very likely in components including a reactor vessel, reactor internals (interior structures), heat exchangers, pipelines, etc. In this study, structural integrity of the components such as reactor vessel and internals in STELLA-2 has been evaluated against creep-fatigue failures at a concept-design step. As 2D analysis yields far conservative results, a realistic 3D simulation is performed by a commercial software. A design integrity guarding against a creep-fatigue damage failure operating at high temperature was evaluated for the reactor vessel with its internal structure of the STELLA-2. Both the high temperature design codes were used for the evaluation, and results were compared. All the results showed the vessel as a whole is safely designed at the given operating conditions, while the ASME-NH gives a conservative evaluation.
Assessment of creep-fatigue damage using the UK strain based procedure
International Nuclear Information System (INIS)
Bate, S.K.
1997-01-01
The UK strain based procedures have been developed for the evaluation of damage in structures, arising from fatigue cycles and creep processes. The fatigue damage is assessed on the basis of modelling crack growth from about one grain depth to an allowable limit which represents an engineering definition of crack formation. Creep damage is based up on the exhaustion of available ductility by creep strain accumulation. The procedures are applicable only when level A and B service conditions apply, as defined in RCC-MR or ASME Code Case N47. The procedures require the components of strain to be evaluated separately, thus they may be used with either full inelastic analysis or simplified methods. To support the development of the UK strain based creep-fatigue procedures an experimental program was undertaken by NNC to study creep-fatigue interaction of structures operating at high temperature. These tests, collectively known as the SALTBATH tests considered solid cylinder and tube-plate specimens, manufactured from Type 316 stainless steel. These specimens were subjected to thermal cycles between 250 deg. C and 600 deg. C. In all the cases the thermal cycle produces tensile residual stresses during dwells at 600 deg. C. One of the tube-plate specimens was used as a benchmark for validating the strain based creep fatigue procedures and subsequently as part of a CEC co-operative study. This benchmark work is described in this paper. A thermal and inelastic stress analysis was carried out using the finite element code ABAQUS. The inelastic behaviour of the material was described using the ORNL constitutive equations. A creep fatigue assessment using the strain based procedures has been compared with an assessment using the RCC-MR inelastic rules. The analyses indicated that both the UK strain based procedures and the RCC-MR rules were conservative, but the conservatism was greater for the RCC-MR rules. (author). 8 refs, 8 figs, 4 tabs
Creep-fatigue damage in austenitic stainless steels
International Nuclear Information System (INIS)
Rezgui, Brahim.
1980-06-01
This is a study of hold time effects on the low cycle fatigue (L.C.F.) properties of 316L austenitic stainless steel at 600 0 C in air. Results obtained for different plastic strain levels indicate that a tension hold time at peak strain lead to a reduction in fatigue life. The importance of this effect depend on the length of hold period, and also on the strain amplitude. No saturation had been observed. Metallographic and microstructural analysis of failed specimens indicates mechanisms by which failure is produced. For continuous cycling the fractures occurs by the initiation and the propagation of a trans-granular crack. Creep damage in the bulk of material is formed during periods of tensile stress relaxation; it causes a change in the failure mode which became intergranular. It is the interaction between this creep-damage and fatigue cracks which is partly responsable for the reduction in the fatigue life. Predictions based upon linear cumulative damage method indicate that virgin material properties may be irrelevant in creep-fatigue interactions [fr
Fatigue-creep of martensitic steels containing 9-12% Cr: behaviour and damage
International Nuclear Information System (INIS)
Fournier, B.
2007-09-01
It is in the framework of the research programs on nuclear reactors (generation IV) that the martensitic steels containing 9-12% Cr are studied by the CEA. Most of the structures for which they are considered will be solicited in fatigue-creep at high temperature (550 C). The aim of this work is to understand and model the cyclic behaviour and the damage of these materials. The proposed modelling are based on detailed observations studies (SEM, TEM, EBSD...). The cyclic softening is attributed to the growth of the microstructure. A micro-mechanical model based on the physical parameters is proposed and leads to encouraging results. The damage results of interactions between fatigue, creep and oxidation. Two main types of damage are revealed. A model of anticipation of service time is proposed and gives very satisfying results. The possible extrapolations are discussed. (O.M.)
The irradiation induced creep of graphite under accelerated damage produced by boron doping
International Nuclear Information System (INIS)
Brocklehurst, J.E.
1975-01-01
The presence of boron enhances fast neutron irradiation damage in graphite by providing nucleation sites for interstitial loop formation. Doping with 11 B casues an increase in the irradiation induced macroscopic dimensional changes, which have been shown to result from an acceleration in the differential crystal growth rate for a given carbon atom displacement rate. Models of irradiation induced creep in graphite have centred around those in which creep is induced by internal stresses due to the anisotopic crystal growth, and those in which creep is activated by atomic displacements. A creep test on boron doped graphite has been performed in an attempt to establish which of these mechanisms is the determining factor. An isotropic nuclear graphite was doped to a 11 B concentration of 0.27 wt.%. The irradiation induced volume shrinkage rate at 750 0 C increased by a factor of 3 over that of the virgin graphite, in agreement with predictions from the earlier work, but the total creep strains were comparable in both doped and virgin samples. This observation supports the view that irradiation induced creep is dependent only on the carbon atom displacement rate and not on the internal stress level determined by the differential crystal growth rate. The implications of this result on the irradiation behaviour of graphite containing significant concentrations of boron are briefly discussed. (author)
Energy Technology Data Exchange (ETDEWEB)
Liu, Yongming [Arizona State Univ., Tempe, AZ (United States). School for Engineering of Matter, Transport and Energy; Oskay, Caglar [Vanderbilt Univ., Nashville, TN (United States). Dept. of Civil and Environmental Engineering
2017-04-30
This report outlines the research activities that were carried out for the integrated experimental and simulation investigation of creep-fatigue damage mechanism and life prediction of Nickel-based alloy, Inconel 617 at high temperatures (950° and 850°). First, a novel experimental design using a hybrid control technique is proposed. The newly developed experimental technique can generate different combinations of creep and fatigue damage by changing the experimental design parameters. Next, detailed imaging analysis and statistical data analysis are performed to quantify the failure mechanisms of the creep fatigue of alloy 617 at high temperatures. It is observed that the creep damage is directly associated with the internal voids at the grain boundaries and the fatigue damage is directly related to the surface cracking. It is also observed that the classical time fraction approach does not has a good correlation with the experimental observed damage features. An effective time fraction parameter is seen to have an excellent correlation with the material microstructural damage. Thus, a new empirical damage interaction diagram is proposed based on the experimental observations. Following this, a macro level viscoplastic model coupled with damage is developed to simulate the stress/strain response under creep fatigue loadings. A damage rate function based on the hysteresis energy and creep energy is proposed to capture the softening behavior of the material and a good correlation with life prediction and material hysteresis behavior is observed. The simulation work is extended to include the microstructural heterogeneity. A crystal plasticity finite element model considering isothermal and large deformation conditions at the microstructural scale has been developed for fatigue, creep-fatigue as well as creep deformation and rupture at high temperature. The model considers collective dislocation glide and climb of the grains and progressive damage accumulation of
Weld repair of creep damaged steels
International Nuclear Information System (INIS)
Croker, A.B.L.; Harrison, R.P.; Moss, C.J.
1995-01-01
A cooperative research centre project 'Welding of Thermally Modified Structures' was commenced in June 1993 with support from ANSTO, CSIRO, BHP, University of Wollongong and the CRC for Materials, Welding and Joining. The main aims of the project are to quantify the effects of performing repair welds on materials which have operated for extended periods at elevated temperature. Welding is an increasingly used method for performing repairs, replacements, retrofits and modifications to elevated temperature plant, however, the effects of these repairs on the ultimate life of a component are poorly understood. This paper presents details of the three ex-service materials chosen for the project, a carbon steel and two alloy steels. Work is also presented on development of new methods of assessing materials and components both destructively, along with new methods of modelling welded components in high temperature service. 6 figs, 3 tabs
A simple model for indentation creep
Ginder, Ryan S.; Nix, William D.; Pharr, George M.
2018-03-01
A simple model for indentation creep is developed that allows one to directly convert creep parameters measured in indentation tests to those observed in uniaxial tests through simple closed-form relationships. The model is based on the expansion of a spherical cavity in a power law creeping material modified to account for indentation loading in a manner similar to that developed by Johnson for elastic-plastic indentation (Johnson, 1970). Although only approximate in nature, the simple mathematical form of the new model makes it useful for general estimation purposes or in the development of other deformation models in which a simple closed-form expression for the indentation creep rate is desirable. Comparison to a more rigorous analysis which uses finite element simulation for numerical evaluation shows that the new model predicts uniaxial creep rates within a factor of 2.5, and usually much better than this, for materials creeping with stress exponents in the range 1 ≤ n ≤ 7. The predictive capabilities of the model are evaluated by comparing it to the more rigorous analysis and several sets of experimental data in which both the indentation and uniaxial creep behavior have been measured independently.
Creep modelling of type 316LN stainless steel
International Nuclear Information System (INIS)
Kim, W. G.; Kim, D. H.; Ryu, W. S.
2000-01-01
Creep curve for type 316LN stainless steel was modelled by using the K-R damage equations. Seven coefficients used in the model, i. e., A, B, κ, m, λ, r, and q were determined from theoretical and calculated data, and their meanings were also analyzed. To quantify damage formation parameter(ω), cavity amount was measured on the crept specimen taken from an interrupted creep test with time variation, and then the amount was reflected into K-R damage equations. Coefficient λ which is regarded as a creep tolerance feature of a material increased with increase of creep strain. Theoretical curve in λ= 3.0 well coincided with an experimental one to the full level of lifetime. Master curve between damage parameter and life fraction matched with the theoretical one in exponent γ= 24 value, which decreased with increase of parameter ω which increased rapidly after 80% life fraction. It is concluded that K-R equation was reliable as the modelling equation for 316LN stainless steel. Coefficient data obtained from 316LN stainless steel can be utilized for remaining life prediction of operating material
Cumulative damage and estimation of residual life in metallic alloys under creep
International Nuclear Information System (INIS)
Silveira, T.L. da.
1980-07-01
The mechanical behavior and fracture characteristics have been determined for a group of materials tested under conditions of creep, and the ability of various models detailed in the literature to describe these observed characteristics discussed. The parametric methods employed in formulating the indices which define the allowable stresses for design codes have been analysed, and a method of Minimum Standard Deviation (MSD) for construction of reference curves has been proposed. The constitutive equations used in the methods of analysis of creep stresses have been discussed. Finally, the accumulated damage by creep in a particular structure which had been in extended service has been characterized and, based on these observations, the methods for estimation of remaining life in industrial equipment have been analysed. (Author) [pt
Modelling of creep hysteresis in ferroelectrics
He, Xuan; Wang, Dan; Wang, Linxiang; Melnik, Roderick
2018-05-01
In the current paper, a macroscopic model is proposed to simulate the hysteretic dynamics of ferroelectric ceramics with creep phenomenon incorporated. The creep phenomenon in the hysteretic dynamics is attributed to the rate-dependent characteristic of the polarisation switching processes induced in the materials. A non-convex Helmholtz free energy based on Landau theory is proposed to model the switching dynamics. The governing equation of single-crystal model is formulated by applying the Euler-Lagrange equation. The polycrystalline model is obtained by combining the single crystal dynamics with a density function which is constructed to model the weighted contributions of different grains with different principle axis orientations. In addition, numerical simulations of hysteretic dynamics with creep phenomenon are presented. Comparison of the numerical results and their experimental counterparts is also presented. It is shown that the creep phenomenon is captured precisely, validating the capability of the proposed model in a range of its potential applications.
Model for transient creep of southeastern New Mexico rock salt
International Nuclear Information System (INIS)
Herrmann, W.; Wawersik, W.R.; Lauson, H.S.
1980-11-01
In a previous analysis, existing experimental data pertaining to creep tests on rock salt from the Salado formation of S.E. New Mexico were fitted to an exponential transient creep law. While very early time portions of creep strain histories were not fitted very well for tests at low temperatures and stresses, initial creep rates in particular generally being underestimated, the exponential creep law has the property that the transient creep strain approaches a finite limit with time, and is therefore desirable from a creep modelling point of view. In this report, an analysis of transient creep is made. It is found that exponential transient creep can be related to steady-state creep through a universal creep curve. The resultant description is convenient for creep analyses where very early time behavior is not important
Factors influencing creep model equation selection
International Nuclear Information System (INIS)
Holdsworth, S.R.; Askins, M.; Baker, A.; Gariboldi, E.; Holmstroem, S.; Klenk, A.; Ringel, M.; Merckling, G.; Sandstrom, R.; Schwienheer, M.; Spigarelli, S.
2008-01-01
During the course of the EU-funded Advanced-Creep Thematic Network, ECCC-WG1 reviewed the applicability and effectiveness of a range of model equations to represent the accumulation of creep strain in various engineering alloys. In addition to considering the experience of network members, the ability of several models to describe the deformation characteristics of large single and multi-cast collations of ε(t,T,σ) creep curves have been evaluated in an intensive assessment inter-comparison activity involving three steels, 21/4 CrMo (P22), 9CrMoVNb (Steel-91) and 18Cr13NiMo (Type-316). The choice of the most appropriate creep model equation for a given application depends not only on the high-temperature deformation characteristics of the material under consideration, but also on the characteristics of the dataset, the number of casts for which creep curves are available and on the strain regime for which an analytical representation is required. The paper focuses on the factors which can influence creep model selection and model-fitting approach for multi-source, multi-cast datasets
International Nuclear Information System (INIS)
Levaillant, Christophe
1984-01-01
This research thesis reports the study of interactions between fatigue, creep and oxidation in austenitic stainless steels which are to be used in the construction of fast breeder reactors. This study is addressed by means of low cycle plastic fatigue test with imposed strain, performed at 600 C with tensile relaxation hold times which may reach 24 hours. Continuous fatigue tests (without hold time) and pure creep tests have also been performed to define 'pure' fatigue damages and 'pure' creep damages. Two grades of Z3 CND 17-13 steel have been studied. Thus fracture mechanisms, crack initiation and propagation, and crack kinetic propagation have been studied. Metallographic measurements of damage have been performed. Damage types have been identified: propagation of cracks initiated at the surface, and intergranular de-cohesion within the material. An approximate modelling is proposed, as well as a critical comparison of various published models of fatigue-creep interaction. In order to predict structure lifetime, a new test methodology is proposed, based on experimental results
Energy Technology Data Exchange (ETDEWEB)
Gaffard, V
2004-12-15
Chromium martensitic stainless steels are under development since the 70's with the prospect of using them as structural components in thermal and nuclear power plants. The modified 9Cr1Mo-NbV steel is already used, especially in England and Japan, as a material for structural components in thermal power plants where welding is a commonly used joining technique. New generations of chromium martensitic stainless steels with improved mechanical properties for high pressure and temperature use are currently under development. However, observations of several in-service premature failures of welded components in 9Cr1Mo-NbV steel, outline a strong need for understanding the high temperature creep flow and damage behaviour of 9Cr1Mo-NbV steels and weldments. The present study aimed at experimentally determining and then modelling the high temperature creep flow and damage behaviour of both 9Cr1Mo-NbV steels and weldments (typically in the temperature range from 450 C to 650 C). The base metal was first studied as the reference material. It was especially evidenced that tempered chromium martensitic steels exhibit a change in both creep flow and damage behaviour for long term creep exposure. As a consequence, the classically performed extrapolation of 1,000 hours creep data to 100,000 hours creep lifetime predictions might be very hazardous. Based on experimental observations, a new model, integrating and coupling multiple creep flow and damage mechanisms, was developed in the framework of the mechanics of porous media. It was then successfully used to represent creep flow and damage behaviour of the base metal from high to low stress levels even for complex multiaxial loading conditions. Although the high temperature creep properties of the base metal are quite good, the occurrence of premature failure in weldments in high temperature creep conditions largely focused the attention of the scientific community. The lower creep strength of the weld component was also
Development of nondestructive evaluation of creep-fatigue damage in SUS316 stainless steel
International Nuclear Information System (INIS)
Shoji, Tetsuo; Kawahara, Tetsuji; Awano, Masakazu; Sato, Yasumoto
1999-01-01
Creep-fatigue is a fatal failure mode of high temperature structural materials. It is recognized that the law of linear damage, according to which creep-fatigue damage is expressed by the sum of the creep damage and the fatigue damage, is inadequate to evaluate creep-fatigue damage. This is due to the fact that the law of linear damage does not include the effect of interaction between the creep damage and the fatigue damage. Consequently, development of direct measurement of damage accumulation on the sample of interest is required for plant life evaluation. In this study, the induced current focusing potential drop (ICFPD) technique was used to evaluate the depth of small surface cracks in SUS316FR stainless steel which was subjected to creep-fatigue damage. It is shown that the potential drop increased during the micro-crack initiation and propagation. Correspondingly, the ICFPD technique applied to estimate micro-crack depth changes was used to accurately evaluate the residual life of creep-fatigue damaged structural materials. (author)
International Nuclear Information System (INIS)
Nishino, Seiichi; Sakane, Masao; Ohnami, Masateru
1986-01-01
Experimental study was made on the damage evaluation and estimation of remaining life of SUS 304 stainless steel in creep, low-cycle fatigue and creep-fatigue at 873 K in air. Creep, fatigue and creep-fatigue damage curves were drawn by the method proposed by D.A. Woodford and the relations between these damages and non-destructive parameters, i.e., microvickers hardness and quantities obtained from X-ray diffraction, were discussed. From these tests, the following conclusions were obtained. (1) Constant damage lines in the diagram of remaining lives in creep and fatigue could be drawn by changing load levels during the tests. Constant damage lines in creep-fatigue were also made by a linear damage rule using both static creep and fatigue damage curves, which agree well with the experimental data in creep-fatigue. (2) Microvickers hardness and half-value breadth in X-ray diffraction are appropriate parameters to evaluate creep damage but are not proper to evaluate fatigue damage. Particle size and microstrain obtained by X-ray profile analysis are good parameters to evaluate both creep and fatigue damages. (author)
Unified creep-plasticity model for halite
International Nuclear Information System (INIS)
Krieg, R.D.
1980-11-01
There are two national energy programs which are considering caverns in geological salt (NaCl) as a storage repository. One is the disposal of nuclear wastes and the other is the storage of oil. Both short-time and long-time structural deformations and stresses must be predictable for these applications. At 300K, the nominal initial temperature for both applications, the salt is at 0.28 of the melting temperature and exhibits a significant time dependent behavior. A constitutive model has been developed which describes the behavior observed in an extensive set of triaxial creep tests. Analysis of these tests showed that a single deformation mechanism seems to be operative over the stress and temperature range of interest so that the secondary creep data can be represented by a power of the stress over the entire test range. This simple behavior allowed a new unified creep-plasticity model to be applied with some confidence. The resulting model recognizes no inherent difference between plastic and creep strains yet models the total inelastic strain reasonably well including primary and secondary creep and reverse loadings. A multiaxial formulation is applied with a back stress. A Bauschinger effect is exhibited as a consequence and is present regardless of the time scale over which the loading is applied. The model would be interpreted as kinematic hardening in the sense of classical plasticity. Comparisons are made between test data and model behavior
A fractal derivative constitutive model for three stages in granite creep
Directory of Open Access Journals (Sweden)
R. Wang
Full Text Available In this paper, by replacing the Newtonian dashpot with the fractal dashpot and considering damage effect, a new constitutive model is proposed in terms of time fractal derivative to describe the full creep regions of granite. The analytic solutions of the fractal derivative creep constitutive equation are derived via scaling transform. The conventional triaxial compression creep tests are performed on MTS 815 rock mechanics test system to verify the efficiency of the new model. The granite specimen is taken from Beishan site, the most potential area for the China’s high-level radioactive waste repository. It is shown that the proposed fractal model can characterize the creep behavior of granite especially in accelerating stage which the classical models cannot predict. The parametric sensitivity analysis is also conducted to investigate the effects of model parameters on the creep strain of granite. Keywords: Beishan granite, Fractal derivative, Damage evolution, Scaling transformation
Magnetic characterization of creep-fatigue damage for energy structural materials
International Nuclear Information System (INIS)
Suzuki, Takayuki; Hashidate, Ryuta; Harada, Yoshihisa
2012-01-01
Magnetic characterization of creep-fatigue damage for welded specimens of austenitic stainless steel (SUS316FR) and high-chromium steel (Mod.9Cr-1Mo) steel was performed using magnetic force microscope and Hall sensor. In SUS316FR volume fraction of δ-ferrite at weld metal region decreased by creep or creep-fatigue and the remanent magnetic flux density at weld metal region also decreased. In Mod.9Cr-1Mo steel magnetic characteristics at weld metal region were different from those at base metal initially, however, during creep or creep fatigue the difference of magnetic characteristics between welded metal and base metal became small. It was found that the degradation mechanism for these energy structural materials during creep or creep fatigue could be clarified by magnetic characterization techniques. (author)
Influenced prior loading on the creep fatigue damage accumulation of heat resistant steels
International Nuclear Information System (INIS)
Kloos, K.H.; Granacher, J.; Scholz, A.
1990-01-01
On two heat resistant power plant steels the influence of prior strain cycling on the creep rupture behaviour and the influence of prior creep loading on the strain cycling behaviour is investigated. These influences concern the number of cycles to failure and the rupture time being the reference values of the generalized damage accumulation rule and they are used for a creep fatigue analysis of the results of long term service-type strain cycling tests. (orig.) [de
Concrete creep and thermal stresses:new creep models and their effects on stress development
Westman, Gustaf
1999-01-01
This thesis deals with the problem of creep in concrete and its influence on thermal stress development. New test frames were developed for creep of high performance concrete and for measurements of thermal stress development. Tests were performed on both normal strength and high performance concretes. Two new models for concrete creep are proposed. Firstly, a viscoelastic model, the triple power law, is supplemented with two additional functions for an improved modelling of the early age cre...
Energy Technology Data Exchange (ETDEWEB)
Storesund, Jan; Eklund, Anders; Taflin, Anders; Thunvik, Thomas
2006-07-15
Recently, several cases of cracking caused by creep have occurred in components operating at temperatures below the specified limit temperature for creep. Components operating below this limit temperature have not been designed with due regard to creep cracking and have accordingly not been subjected to inspection for creep damage. This work has surveyed the extent of these cases of creep damage by reviewing earlier failures and performed metallographic studies of damaged components and made parametric calculations of creep crack growth below the limit temperature. The following critical parameters have been determined for power plants: Creep damage below the transition temperature does not usually occur until operating times above 200.000 hours. Time to rupture differs from ordinary creep crack growth because these cracks have substantially longer incubation time of 20-30 years, with relative low creep deformation, and after that a rapid creep crack growth with only some few years to the creep rupture. Operation at 470-480 deg C, i.e. up to some 10 deg C below the transition temperature for a material like EN 13CrMo4-5, can be expected to result in severe creep damages comparable with ordinary creep failures at stressed locations. Operation at a temperature of 450-460 deg C can give rise to creep damage, however, this damage shows a more sparse occurrence. Creep damaged welds occurring below the limit temperature show cracks at the melting junction of the weld bead in opposite to ordinary creep damages. System stresses can also cause a more rapid crack growth. An international survey also shows that the variation of creep strength values between individual steel batches are just as wide as for ordinary creep. Based on this work, the following complementary recommendations can be issued: Elastic stress analysis (based on expansion calculations) can also be recommended for the identification of areas with intensified stresses. One should also perform a complete
Modelling of cladding creep collapse
International Nuclear Information System (INIS)
Koundy, V.; Forgeron, T.; Hivroz, J.
1993-01-01
The effects of the initial ovality and pressure level on the collapse time of Zircaloy-4 tubing subjected to uniform external pressure were examined experimentally and analytically. Experiments were performed on end closed tubes with two metallurgical states: stress relieved and recrystallized. Numerical simulations were accomplished with a specific computer program based on an analytical approach and the calculated results were compared with the experimental ones. As a comparison, the finite element method is also partially examined in this analysis. Numerical collapse times are in good agreement with regard to experimental results in the case of stress relieved structure. They seem to be too conservative in the case of a recrystallized metallurgical state and the use of the anisotropic option ameliorates numerical results. Sensibility of numerical solutions to the formulation of primary creep laws are presented
Matsuda, Tetsuya; Okumura, Dai
2015-01-01
This volume presents a collection of contributions on materials modeling, which were written to celebrate the 65th birthday of Prof. Nobutada Ohno. The book follows Prof. Ohno’s scientific topics, starting with creep damage problems and ending with homogenization methods.
International Nuclear Information System (INIS)
Kondyr, A.; Sandstroem, R.; Samuelsson, A.
1979-02-01
A detailed analysis of creep strain results for three low alloyed steels of type 0.5 Mo, 1 Cr-0.5 Mo and 2.25 Cr-1 Mo has been undertaken. The results show that, excluding the primary stage, the true strain rate can be described by a simple analytical expression dE/dt = Aexp(B.E) where A and B are constants at constant stress and temperature. A is approximately equal to the minimum strain rate and B inversly proportional to the fracture strain. Furthermore, 1/AB equals the time t sub(r) to rupture. The residual life fraction in creep can be expressed as exp(-B.E) = 1-t/t sub(r) and a creep damage function μ is introduced as μ = 1-ABt. The expressions for strain rate and damage are shown to be a special case of the Rabotnov-Kachanov equations. The analysis has been generalized to account for multiaxial stress states, and as an example creep in a tube with internal pressure is considered. (author)
The creep analysis of shell structures using generalised models
International Nuclear Information System (INIS)
Boyle, J.T.; Spence, J.
1981-01-01
In this paper a new, more complete estimate of the accuracy of the stationary creep model is given for the general case through the evaluation of exact and approximate energy surfaces. In addition, the stationary model is extended to include more general non-stationary (combined elastic-creep) behaviour and to include the possibility of material deterioration through damage. The resulting models are then compared to existing exact solutions for several shell structures - e.g. a thin pressurised cylinder, a curved pipe in bending and an S-bellows under axial extension with large deflections. In each case very good agreement is obtained. Although requiring similar computing effort, so that the same solution techniques can be utilised, the calculation times are shown to be significantly reduced using the generalised approach. In conclusion, it has been demonstrated that a new simple mechanical model of a thin shell in creep, with or without material deterioration can be constructed; the model is assessed in detail and successfully compared to existing solutions. (orig./HP)
Effects of bone damage on creep behaviours of human vertebral trabeculae.
O'Callaghan, Paul; Szarko, Matthew; Wang, Yue; Luo, Jin
2018-01-01
A subgroup of patients suffering with vertebral fractures can develop progressive spinal deformities over time. The mechanism underlying such clinical observation, however, remains unknown. Previous studies suggested that creep deformation of the vertebral trabeculae may play a role. Using the acoustic emission (AE) technique, this study investigated effects of bone damage (modulus reduction) on creep behaviours of vertebral trabecular bone. Thirty-seven human vertebral trabeculae samples were randomly assigned into five groups (A to E). Bones underwent mechanical tests using similar experimental protocols but varied degree of bone damage was induced. Samples first underwent creep test (static compressive stress of 0.4MPa) for 30min, and then were loaded in compression to a specified strain level (0.4%, 1.0%, 1.5%, 2.5%, and 4% for group A to E, respectively) to induce different degrees of bone damage (0.4%, no damage control; 1.0%, yield strain; 1.5%, beyond yield strain, 2.5% and 4%, post-ultimate strains). Samples were creep loaded (0.4MPa) again for 30min. AE techniques were used to monitor bone damage. Bone damage increased significantly from group A to E (P30% of modulus reduction in group D and E. Before compressive loading, creep deformation was not different among the five groups and AE hits in creep test were rare. After compressive loading, creep deformation was significantly greater in group D and E than those in other groups (Pcreep test were significantly greater in group D and E than in group A, B, and C (Pcreep deformation may occur even when the vertebra was under physiological loads. The boosted creep deformation observed may be attributed to newly created trabecular microfractures. Findings provide a possible explanation as to why some vertebral fracture patients develop progressive spinal deformity over time. Copyright © 2017. Published by Elsevier Inc.
Modeling Creep Processes in Aging Polymers
Olali, N. V.; Voitovich, L. V.; Zazimko, N. N.; Malezhik, M. P.
2016-03-01
The photoelastic method is generalized to creep in hereditary aging materials. Optical-creep curves and mechanical-creep or optical-relaxation curves are used to interpret fringe patterns. For materials with constant Poisson's ratio, it is sufficient to use mechanical- or optical-creep curves for this purpose
A Creep Model for High-Density Snow
2017-04-01
proportionality, Q = activation energy (Cal/mol), R = the ideal gas constant (1.985 Cal/mol K), and T = absolute temperature in Kelvin. Applying this, I...modifies Mellor and Smith’s creep model for dense snow to conform to the more general creep power law form (Glen’s creep law for ice is a special case of...this power law ). The present study used this general form as the basis for developing two creep models: one to describe the pri- mary creep and
Energy Technology Data Exchange (ETDEWEB)
Shen, Chen [General Electric Global Research, Niskayuna, NY (United States)
2014-04-01
The goal of this project is to model creep-fatigue-environment interactions in steam turbine rotor materials for advanced ultra-supercritical (A-USC) coal power Alloy 282 plants, to develop and demonstrate computational algorithms for alloy property predictions, and to determine and model key mechanisms that contribute to the damages caused by creep-fatigue-environment interactions.
Boundary element method for modelling creep behaviour
International Nuclear Information System (INIS)
Zarina Masood; Shah Nor Basri; Abdel Majid Hamouda; Prithvi Raj Arora
2002-01-01
A two dimensional initial strain direct boundary element method is proposed to numerically model the creep behaviour. The boundary of the body is discretized into quadratic element and the domain into quadratic quadrilaterals. The variables are also assumed to have a quadratic variation over the elements. The boundary integral equation is solved for each boundary node and assembled into a matrix. This matrix is solved by Gauss elimination with partial pivoting to obtain the variables on the boundary and in the interior. Due to the time-dependent nature of creep, the solution has to be derived over increments of time. Automatic time incrementation technique and backward Euler method for updating the variables are implemented to assure stability and accuracy of results. A flowchart of the solution strategy is also presented. (Author)
Detection of creep damage in a nickel base superalloy using NDE techniques
International Nuclear Information System (INIS)
Carreon, H.; Mora, B.; Barrera, G.
2009-10-01
Due to elevated temperatures, excessive stresses and severed corrosion conditions, turbine engine components are subject to creep processes that limit the components life such as a turbine bucket. The failure mechanism of a turbine bucket is related primarily to creep and corrosion and secondarily to thermal fatigue. As a result, it is desirable to assess the current conditions of such turbine component. This study uses the eddy current nondestructive evaluation technique in an effort to monitor the creep damage in a nickel base super-alloy, turbine bucket after service. The experimental results show an important electrical conductivity variation in eddy current images on the creep damage zone of nickel base super-alloy samples cut from a turbine bucket. Thermoelectric power measurements were also conducted in order to obtain a direct correlation between the presence of material changes due to creep damage and the electrical conductivity measurements. This research work shows an alternative non-destructive method in order to detect creep damage in a nickel base super-alloy turbine bucket. (Author)
International Nuclear Information System (INIS)
Lenk, P.; Proft, D.; Kussmaul, A.; Fischer, R.
2000-01-01
The influence of multiaxial stress on creep pore formation in the steels 14MoV6-3 10CrMo9-10 and X10CrMoVNb9-1 was investigated on the basis of internal pressure experiments on smooth and notched hollow cylinders. In some cases, additional axial forces were applied in order to reproduce component-relevant multiaxial stresses. Local elongation during loading was investigated and analyzed using applied HT-DMS. When different strain levels had been reached, the samples were removed, analyzed, and characterized with regard to different damage parameters. It was found that no interdependence between the surface damage pattern and the deep damage pattern can be derived across the wall thickness if no information on the load state is available. Parallel to the experiments, inelastic FEA were carried out using the ABAQUS program system. The creep law of Graham and Walles was used for calculating flow and creep via a user-defined subroutine CREEP. The parameters of the creep law could be identified by adaptation to monoaxial creep tests [de
Cumulative fatigue and creep-fatigue damage at 3500C on recrystallized zircaloy 4
International Nuclear Information System (INIS)
Brun, G.; Pelchat, J.; Floze, J.C.; Galimberti, M.
1985-06-01
An experimental programme undertaken by C.E.A., E.D.F. and FRAGEMA with the aim of characterizing the fatigue and creep fatigue behaviour of zircaloy-4 following annealing treatments (recrystallized, stress-delived) is in progress. The results given below concern only recrystallized material. Cyclic properties, low-cycle fatigue curves and creep behaviour laws under stresses have been established. Sequential tests of pure fatigue and creep-fatigue were performed. The cumulative life fractions at fracture depend on the sequence of leading, stress history and number of cycles of prestressing. The MINER's rule appears to be conservative with regard to a low-high loading sequence whereas it is not for the reverse high-low loading sequences. Fatigue and creep damage are not interchangeable. Pre-creep improves the fatigue resistance. Pre-fatigue improves the creep strength as long as the beneficial effect of cyclic hardening overcomes the damaging effect of surface cracking. The introduction of a tension hold time into the fatigue cycle slightly increases cyclic hardening and reduces the number of cycles to failure. For hold times of less than one hour, the sum of fatigue and creep life fractions is closed to one
SANS and TEM studies of carbide precipitation and creep damage in type 304 stainless steel
International Nuclear Information System (INIS)
Yoo, M.H.; Ogle, J.C.; Schneibel, J.H.; Swindeman, R.W.
1984-01-01
Small-angle neutron scattering (SANS) and transmission electron microscopy (TEM) studies were performed to characterize the carbide (M 23 C 6 ) precipitation and creep damage induced in type 304 stainless steel in the primary creep stage. The size distribution of matrix carbides evaluated from SANS analyses was consistent with TEM data, and the expected accelerated kinetics of precipitation under applied stress was confirmed. Additional SANS measurements after the postcreep solution annealing were made in order to differentiate cavities from the carbides. Potential advantages and difficulties associated with characterization of creep-induced cavitation by the SANS techniques are discussed
International Nuclear Information System (INIS)
Smirnova, E.S.; Chuvil'deev, V.N.
1998-01-01
The model is suggested which describes the influence of large-angle grain boundary migration on a diffusion controlled creep rate in polycrystalline materials (Coble creep). The model is based on the concept about changing the value of migrating boundary free volume when introducing dislocations distributed over the grain bulk into this boundary. Expressions are obtained to calculate the grain boundary diffusion coefficient under conditions of boundary migration and the parameter, which characterized the value of Coble creep acceleration. A comparison is made between calculated and experimental data for Cd, Co and Fe
Some aspects of thermomechanical fatigue of AISI 304L stainless steel: Part I. creep- fatigue damage
Zauter, R.; Christ, H. J.; Mughrabi, H.
1994-02-01
Thermomechanical fatigue (TMF) tests on the austenitic stainless steel AISI 304L have been conducted under “true≓ plastic-strain control in vacuum. This report considers the damage oc-curring during TMF loading. It is shown how the temperature interval and the phasing (in-phase, out-of-phase) determine the mechanical response and the lifetime of the specimens. If creep-fatigue interaction takes place during in-phase cycling, the damage occurs inside the ma-terial, leading to intergranular cracks which reduce the lifetime considerably. Out-of-phase cy-cling inhibits creep-induced damage, and no lifetime reduction occurs, even if the material is exposed periodically to temperatures in the creep regime. A formula is proposed which allows prediction of the failure mode, depending on whether creep-fatigue damage occurs or not. At a given strain rate, the formula is able to estimate the temperature of transition between pure fatigue and creep-fatigue damage.
The strainrange conversion principle for treating cumulative fatigue damage in the creep range
Manson, S. S.
1983-01-01
A formula is derived for combining effects of successive hysteresis loops in the creep range of materials when one loop has excess tensile creep, while the other contains excess compressive creep. The resultant effect resembles single loops involving balanced tensile and compressive creep. The attempt to use the Interaction Damage Rule as a tool in combining loops of non-equal size and complex strainrange content has led to important new concepts useful in future studies of creep-fatigue. It turns out that the Interaction Damage Rule is basically an expression of how a set of hysteresis loops involving only single generic strains can combine to produce the same micromechanistic damage as the loop containing the combined strainranges which it analyzes. Making use of the underlying concept of Strainrange Partitioning that only the strainrange content of a hysteresis loop governs fatigue life, not order of introducing strainranges, a rational derivation of the Interaction Damage Rule is provided, showing also how it can effectively be used to synthesize independent loops and determine both damaging and healing effects.
Effect of HIP Combined with RHT Process on Creep Damage of DZ125 Superalloy
Directory of Open Access Journals (Sweden)
WANG Tian-you
2017-02-01
Full Text Available Four different processes of hot isostatic pressing (HIP combined with rejuvenation heat treatments (RHT were adopted to reveal the microstructural evolution of creep damaged DZ125 specimens, finally the mechanical properties were evaluated.The results show that both γ' precipitate degeneration and creep cavities for the creep damaged DZ125 superalloy are found after the pre-endurance damage test.However, the carbided compositions from MC type to M23C6 type or M6C type has not been observed for DZ125.In addition, it is found that the HIP temperature play a dominant role in the cavity healing process for the damaged specimens. The concentrically oriented γ' rafting structure and the incipient melting are observed at 1200℃ and 1250℃ respectively.Meanwhile, it is found that the appropriate HIP schedule adopted can effectively avoid the internal recrystallization for the directionally solidified nickel-based superalloy DZ125. The appropriate HIP schedule combined with RHT process can successfully restore the microstructure induced by creep damage and recover the degraded micro-hardness to the original one, in addition improve the creep rupture life.
Damage of multilayer polymer materials under creep loading
Czech Academy of Sciences Publication Activity Database
Zouhar, Michal; Hutař, Pavel; Náhlík, Luboš; Knésl, Zdeněk
2011-01-01
Roč. 465, - (2011), s. 153-156 ISSN 1013-9826 R&D Projects: GA ČR GA106/09/0279; GA ČR GC101/09/J027 Institutional research plan: CEZ:AV0Z20410507 Keywords : CMOD * material interface * creep * fracture mechanics Subject RIV: JL - Materials Fatigue, Friction Mechanics
International Nuclear Information System (INIS)
Maruyama, Kouichi; Kato, Syoichi; Nagae, Yuji
1999-02-01
Boiler and steam turbine components in power generating plants are used under creep and creep-fatigue conditions. It is important to measure both creep and creep-fatigue damage of the components in order to assess the residual life of the components. Modified 9Cr-1Mo steel, a candidate material for steam generator in FBR, has a tempered martensitic lath structure. It was proposed in the second report that lath width in the lath structure is closely related to creep strain, and using this relation one can assess residual creep life of a structural component made of the steel. The objectives of this study are to investigate the change of the lath structure during creep.fatigue deformation, and to estimate creep strain by measuring area of cell composing the lath structure. The area of cell can be a better measure of creep deformation than the lath width. The lath structure is covered during creep-fatigue deformation. The lath structure becomes equiaxed cell structure under creep-fatigue more quickly compared with the lath structure recovered during creep. The lath structure recovered under creep-fatigue has a stationary value of the lath width determined by maximum stress at Nf/2. (Nf: number of cycles) If the recovery process of the lath structure can be investigated under creep-fatigue, the lath width can be a measure of the life assessment under creep-fatigue. Area of cell composing the lath structure increases with creep deformation and reaches a stationary value S s determined by creep stress. The rate of increase in the area is faster at a higher stress and temperature. A normalized change in the area of cell, ΔS/ΔS s , was introduced as a measure of the recovery process of martensitic lath structure. ΔS is the change in area of cell from the initial value S 0 , ΔS s is the difference between S s and S 0 . ΔS/ΔS s is uniquely related to creep strain independent of creep conditions. However, the scatter of data in ΔS/ΔS s -strain relation is wider than
The effect of creep-fatigue damage relationships upon HTGR heat exchanger design
International Nuclear Information System (INIS)
Kozina, M.M.; King, J.H.; Basol, M.
1984-01-01
Materials for heat exchangers in the high temperature gas-cooled reactor (HTGR) are subjected to cyclic loading, extending the necessity to design against fatigue failure into the temperature region where creep processes become significant. Therefore, the fatigue life must be considered in terms of creep-fatigue interaction. In addition, since HTGR heat exchangers are subjected to holds at constant strain levels or constant stress levels in high-temperature environments, the cyclic life is substantially reduced. Of major concern in the design and analysis of HTGR heat exchangers is the accounting for the interaction of creep and fatigue. The accounting is done in conformance to the American Society of Mechanical Engineers Boiler and Pressure Vessel Code, Code Case N-47, which allows the use of the linear damage criterion for interaction of creep and fatigue. This method separates the damage incurred in the material into two parts: one due to fatigue and one due to creep. The summation of the creep-fatigue damage must be less than 1.0. Recent material test data have indicated that the assumption of creep and fatigue damage equals unity at failure may not always be valid for materials like Alloy 800H, which is used in the higher temperature sections of HTGR steam generators. Therefore, a more conservative creep-fatigue damage relationship was postulated for Alloy 800H. This more conservative bilinear damage relationship consists of a design locus drawn from D F =1.0, D C =0 to D F =0.1, D C =0.1 to D F =0, D C =1.0. D F is the fatigue damage and D C is the creep damage. A more conservative damage relationship for 2-1/4 Cr-1 Mo material consisted of including factors that degrade the fatigue curves. These revised relationships were used in a structural evaluation of the HTGR steam cycle/cogeneration (SC/C) steam generator design. The HTGR-SC/C steam generator, a once-through type, is comprised of an economizer-evaporator-superheater (ESS) helical bundle of 2-1/4 Cr-1
International Nuclear Information System (INIS)
Hiroe, Tetsuyuki; Igari, Toshihide; Nakajima, Keiichi
1986-01-01
A newly developed type of life analysis is introduced using a unified constitutive equation and a continuous damage law on 2 1/4Cr - 1Mo steel at 600 deg C. the viscoplasticity theory based on total strain and overstress used for the rate effect at room temperature is extended for application to the inelastic analysis at elevated temperature, and the extended uniaxial model is shown to reproduce the inelastic stress and strain behavior with a strain rate change observed in the experiment. The incremental life prediction law is employed and its coupling with the viscoplasticity model produces both an inelastic stress-strain response and the damage accumulation, simultaneously and continuously. The life prediction for creep, fatigue and creep-fatigue loading shows good correspondence with the experimental data. (author)
Applicability of creep damage rules to a nickel-base heat-resistant alloy Hastelloy XR
International Nuclear Information System (INIS)
Tsuji, Hirokazu; Nakajima, Najime; Tanabe, Tatsuhiko; Nakasone, Yuji
1992-01-01
A series of constant load and temperature creep rupture tests and varying load and/or temperature creep rupture tests was carried out on a nickel-base heat-resistant alloy Hastelloy XR, which was developed for applications in the High-Temperature Engineering Test Reactor, at temperatures ranging from 850 to 1000deg C in order to examine the applicability of the conventional creep damage rules, i.e., the life fraction, the strain fraction and their mixed rules. The life fraction rule showed the best applicability of these three criteria. The good applicability of the rule was considered to result from the fact that the creep strength of Hastelloy XR was not strongly affected by the change of the chemical composition and/or the microstructure during exposure to the high-temperature simulated HTGR helium environment. In conclusion the life fraction rule is applicable in engineering design of high-temperature components made of Hastelloy XR. (orig.)
Study on creep damage behaviors of Ni-based alloy C276
International Nuclear Information System (INIS)
Mao Xueping; Guo Qi; Zhang Shengyuan; Hu Suyang; Lu Daogang; Xu Hong
2013-01-01
High temperature creep tests were carried out for Ni-based alloy C276 at 650℃, 700℃ and 750℃, which is one of the candidate materials for the fuel cladding of the supercritical water reactor. Methods of damage mechanics were adopted to calculate and analyze these data. Damage factors calculated by Kachanov formula and Norton formula based on θ projection method were compared. The results show that the damage factors about the material are similar at the three temperatures according to Kachanov formula. The predicted creep curves calculated by θ projection method have a close agreement with the experimental data. The damages calculated by Norton formula start at about 0.3 - 0.4 lifetime, and the damage factors calculated by Kachanov formula are relatively conservative. (authors)
Modeling of creep-fatigue interaction of zirconium α under cyclic loading at 200 C
International Nuclear Information System (INIS)
Vogel, C.
1996-04-01
The present work deals with mechanical behaviour of zirconium alpha at 200 deg. C and crack initiation prediction methods, particularly when loading conditions lead to interaction of fatigue and creep phenomena. A classical approach used to study interaction between cyclic effects and constant loading effects does not give easy understanding of experimental results. Therefore, a new approach has been developed, which allow to determine a number of cycles for crack initiation for complex structures under large loading conditions. To study influence of fatigue and creep interaction on crack initiation, a model was chosen, using a scalar variable, giving representation of the material deterioration state. The model uses a non linear cumulating effect between the damage corresponding to cyclic loads and the damage correlated to time influence. The model belongs to uncoupled approaches between damage and behaviour, which is described here by a two inelastic deformations model. This mechanical behaviour model is chosen because it allows distinction between a plastic and a viscous part in inelastic flow. Cyclic damage is function of stress amplitude and mean stress. For the peculiar sensitivity of the material to creep, a special parameter bas been defined to be critical toward creep damage. It is the kinematic term associated to state variables describing this type of hardening in the viscous mechanism. (author)
Relaxation creep model of impending earthquake
Energy Technology Data Exchange (ETDEWEB)
Morgounov, V. A. [Russian Academy of Sciences, Institute of Physics of the Earth, Moscow (Russian Federation)
2001-04-01
The alternative view of the current status and perspective of seismic prediction studies is discussed. In the problem of the ascertainment of the uncertainty relation Cognoscibility-Unpredictability of Earthquakes, priorities of works on short-term earthquake prediction are defined due to the advantage that the final stage of nucleation of earthquake is characterized by a substantial activation of the process while its strain rate increases by the orders of magnitude and considerably increased signal-to-noise ratio. Based on the creep phenomenon under stress relaxation conditions, a model is proposed to explain different images of precursors of impending tectonic earthquakes. The onset of tertiary creep appears to correspond to the onset of instability and inevitably fails unless it unloaded. At this stage, the process acquires the self-regulating character to the greatest extent the property of irreversibility, one of the important components of prediction reliability. Data in situ suggest a principal possibility to diagnose the process of preparation by ground measurements of acoustic and electromagnetic emission in the rocks under constant strain in the condition of self-relaxed stress until the moment of fracture are discussed in context. It was obtained that electromagnetic emission precedes but does not accompany the phase of macrocrak development.
Creep Damage Evaluation of Titanium Alloy Using Nonlinear Ultrasonic Lamb Waves
International Nuclear Information System (INIS)
Xiang Yan-Xun; Xuan Fu-Zhen; Deng Ming-Xi; Chen Hu; Chen Ding-Yue
2012-01-01
The creep damage in high temperature resistant titanium alloys Ti60 is measured using the nonlinear effect of an ultrasonic Lamb wave. The results show that the normalised acoustic nonlinearity of a Lamb wave exhibits a variation of the 'increase-decrease' tendency as a function of the creep damage. The influence of microstructure evolution on the nonlinear Lamb wave propagation has been analyzed based on metallographic studies, which reveal that the normalised acoustic nonlinearity increases due to a rising of the precipitation volume fraction and the dislocation density in the early stage, and it decreases as a combined result of dislocation change and micro-void initiation in the material. The nonlinear Lamb wave exhibits the potential for the assessment of the remaining creep life in metals
Fujiyama, Kazunari; Kimachi, Hirohisa; Tsuboi, Toshiki; Hagiwara, Hiroyuki; Ogino, Shotaro; Mizutani, Yoshiki
EBSD(Electron BackScatter Diffraction) analyses were conducted for studying the quantitative microstructural metrics of creep and creep-fatigue damage for austenitic SUS304HTB boiler tube steel and ferritic Mod.9Cr piping steel. KAM(Kernel Average Misorientation) maps and GOS(Grain Orientation Spread) maps were obtained for these samples and the area averaged values KAMave and GOSave were obtained. While the increasing trends of these misorientation metrics were observed for SUS304HTB steel, the decreasing trends were observed for damaged Mod.9Cr steel with extensive recovery of subgrain structure. To establish more universal parameter representing the accumulation of damage to compensate these opposite trends, the EBSD strain parameters were introduced for converting the misorientation changes into the quantities representing accumulated permanent strains during creep and creep-fatigue damage process. As KAM values were dependent on the pixel size (inversely proportional to the observation magnification) and the permanent strain could be expressed as the shear strain which was the product of dislocation density, Burgers vector and dislocation movement distance, two KAM strain parameters MεKAMnet and MεδKAMave were introduced as the sum of product of the noise subtracted KAMnet and the absolute change from initial value δKAMave with dislocation movement distance divided by pixel size. MεδKAMave parameter showed better relationship both with creep strain in creep tests and accumulated creep strain range in creep-fatigue tests. This parameter can be used as the strain-based damage evaluation and detector of final failure.
Modeling the effect of creep deterioration on magnetic properties in heat-resistant steels
Energy Technology Data Exchange (ETDEWEB)
Zhang, S.Z.; Tu, S.T., E-mail: sttu@ecust.edu.cn
2014-11-15
Abstracts: The hysteresis parameters of the Jiles–Atherton model are modified to elucidate the variation of magnetic properties with creep deterioration based on a consideration of the effect of pinning of magnetic domain walls on the grain boundaries, dislocations as well as precipitates in short-term creep process. Experiments are carried out to evaluate the magnetic hysteresis curves of 10CrMo910 specimens with controlled levels of creep-induced damage. An intelligent optimization algorithm is used to determine the hysteresis parameters of Jiles–Atherton model. The microstructure parameters of the crept specimens are determined by a quantitative metallographic analysis. The modified model is applied to correlate the experimental data of both 10CrMo910 and 410 stainless steel creep specimens. The calculated results are in good agreement with the measured data of the hysteresis parameters. - Highlights: • The hysteresis parameters in the Jiles–Atherton model are modified to account for the effect of creep deterioration. • Magnetic properties are greatly affected by the precipitation and dislocations during creep. • Good consistency is obtained between the experimental and theoretical results of hysteresis parameters.
International Nuclear Information System (INIS)
1997-03-01
The IAEA, following the recommendations of the International Working Group on Fast Reactors, convened a Technical Committee Meeting on Creep-Fatigue Damage Rules to be used in Fast Reactor Design. The objective of the meeting was to review developments in design rules for creep-fatigue conditions and to identify any areas in which further work would be desirable. The meeting was hosted by AEA Technology, Risley, and held in Manchester, United Kingdom, 11-13 June 1996. It was attended by experts from the European Commission, France, India, Japan, the Republic of Korea, the Russian Federation and the United Kingdom. Refs, figs, tabs
Experimental and modeling results of creep fatigue life of Inconel 617 and Haynes 230 at 850 C
International Nuclear Information System (INIS)
Chen, Xiang; Sokolov, Mikhail A.; Sham, Sam; Erdman, Donald L. III; Busby, Jeremy T.; Mo, Kun; Stubbins, James
2013-01-01
Creep fatigue testing of Ni-based superalloy Inconel 617 and Haynes 230 were conducted in the air at 850 C. Tests were performed with fully reversed axial strain control at a total strain range of 0.5%, 1.0% or 1.5% and hold time at maximum tensile strain for 3, 10 or 30 min. In addition, two creep fatigue life prediction methods, i.e. linear damage summation and frequency-modified tensile hysteresis energy modeling, were evaluated and compared with experimental results. Under all creep fatigue tests, Haynes 230 performed better than Inconel 617. Compared to the low cycle fatigue life, the cycles to failure for both materials decreased under creep fatigue test conditions. Longer hold time at maximum tensile strain would cause a further reduction in both material creep fatigue life. The linear damage summation could predict the creep fatigue life of Inconel 617 for limited test conditions, but considerably underestimated the creep fatigue life of Haynes 230. In contrast, frequency-modified tensile hysteresis energy modeling showed promising creep fatigue life prediction results for both materials.
International Nuclear Information System (INIS)
Hales, R.
1983-01-01
A method of combining long term creep data with relatively short term mechanical behaviour to provide an estimate of creep-fatigue endurance is presented. It is proposed that the creep-fatigue effect in high temperature cyclic deformation is governed by a difference in strain rate around the cycle and the associated variation in ductility with strain rate. (author)
Microscopic creep models and the interpretation of stress-dip tests during creep
International Nuclear Information System (INIS)
Poirier, J.P.
1976-09-01
A critical analysis is made of the principal divergent view points concerning stress-dip tests. The raw data are examined and interpreted in the light of various creep models. The following problems are discussed: is the reverse strain anelastic or plastic; is the zero creep rate periodic due to recovery or is it spurious; can the existence or inexistence of an internal stress be deduced from stress-dip tests; can stress-dip tests allow to determine whether glide is jerky or viscous; can the internal stress be measured by stress-dip tests
Image-based creep-fatigue damage mechanism investigation of Alloy 617 at 950 °C
Energy Technology Data Exchange (ETDEWEB)
Tahir, Fraaz; Dahire, Sonam; Liu, Yongming, E-mail: yongming.liu@asu.edu
2017-01-02
Alloy 617 is a primary candidate material to be used in the next generation of nuclear power plants. Structural materials for these plants are expected to undergo creep and fatigue at temperatures as high as 950 °C. This study uses a hybrid-control creep-fatigue loading profile, as opposed to the traditional strain-controlled loading, to generate creep dominated failure. Qualitative and quantitative image analysis through SEM, EDS, and EBSD, is used to show that hybrid control testing is capable of producing creep dominated failure and that time fraction approach is not a valid indicator of creep or fatigue dominated damage. The focus of image analysis is on surface fatigue cracks and internal creep voids. A creep-fatigue damage interaction diagram based on these micro-scale features is plotted. It is shown that the classical time fraction approach suggested by the ASME code does not agree with the experimental findings and has a poor correlation with observed microscale damage features. A new definition of creep damage fraction based on an effective hold time is found to correlate well with the micro-scale image analysis.
Critical view on the creep modelling procedures
Czech Academy of Sciences Publication Activity Database
Kloc, Luboš
2015-01-01
Roč. 128, č. 4 (2015), s. 540-542 ISSN 0587-4246. [ISPMA 2014 - International Symposium on Physics of Materials /13./. Praha, 31.08.2014-04.09.2014] R&D Projects: GA MPO FR-TI4/406 Institutional support: RVO:68081723 Keywords : Creep * Creep deformation * Grain boundaries * Phase structure * Strain rate Subject RIV: JJ - Other Materials Impact factor: 0.525, year: 2015
Energy Technology Data Exchange (ETDEWEB)
Sklenicka, V.; Kucharova, K.; Svoboda, M.; Kroupa, A.; Kloc, L. [Academy of Sciences of the Czech Republic, Brno (Czech Republic). Inst. of Physics of Materials; Cmakal, J. [UJP PRAHA a.s., Praha-Zbraslav (Czech Republic)
2010-07-01
Creep behaviour and degradation of creep properties of creep resistant materials are phenomena of major practical relevance, often limiting the lives of components and structures designed to operate for long periods under stress at elevated and/or high temperatures. Since life expectancy is, in reality, based on the ability of the material to retain its high-temperature creep strength for the projected designed life, methods of creep properties assessment based on microstructural evolution in the material during creep rather than simple parametric extrapolation of short-term creep tests are necessary. In this paper we will try to further clarify the creep-strength degradation of selected advanced creep resistant steels. In order to accelerate some microstructural changes and thus to simulate degradation processes in long-term service, isothermal ageing at 650 C for 10 000 h was applied to P91 and P23 steels in their as-received states. The accelerated tensile creep tests were performed at temperature 600 C in argon atmosphere on all steels both in the as-received state and after long-term isothermal ageing, in an effort to obtain a more complete description of the role of microstructural stability in high temperature creep of these steels. Creep tests were followed by microstructural investigations by means of both transmission and scanning electron microscopy and by the thermodynamic calculations. The applicability of the accelerated creep tests was verified by the theoretical modelling of the phase equilibria at different temperatures. It is suggested that under restructed oxidation due to argon atmosphere microstructural instability is the main detrimental process in the long-term degradation of the creep rupture strength of these steels. (orig.)
International Nuclear Information System (INIS)
Nonaka, Isamu; Kitagawa, Masaki; Torihata, Shoji.
1995-01-01
In order to investigate the applicability of a ductility exhaustion rule to the creep-fatigue life assessment of FBR 316 stainless steel, a feasibility study using the published data was conducted. The assessment method was proposed based on the linear damage summation rule. In the proposed method, fatigue damage was calculated by Minor's rule and creep damage was calculated by a ductility exhaustion rule. The creep-fatigue lives in the published data were predicted by the proposed method. The results obtained are as follows: (1) All the data could be predicted within a factor of two on life by the proposed method. (2) The creep-fatigue lives under 10 minute strain hold at 550degC were overestimated, while those under 60 minute strain hold at 550degC and 600degC were estimated adequately. From the above facts, the proposed method seemed to be effective for the prediction of creep-fatigue life in which the creep damage was dominant and also the intergranular cracking was remarkable. (3) The creep damage was simultaneously calculated by the time fraction rule in order to compare with the ductility exhaustion role. All the data could be also predicted within a factor of two on life by this rule, but it tended to overestimate the life. (author)
A discrete dislocation dynamics model of creeping single crystals
Rajaguru, M.; Keralavarma, S. M.
2018-04-01
Failure by creep is a design limiting issue for metallic materials used in several high temperature applications. Current theoretical models of creep are phenomenological with little connection to the underlying microscopic mechanisms. In this paper, a bottom-up simulation framework based on the discrete dislocation dynamics method is presented for dislocation creep aided by the diffusion of vacancies, known to be the rate controlling mechanism at high temperature and stress levels. The time evolution of the creep strain and the dislocation microstructure in a periodic unit cell of a nominally infinite single crystal is simulated using the kinetic Monte Carlo method, together with approximate constitutive laws formulated for the rates of thermal activation of dislocations over local pinning obstacles. The deformation of the crystal due to dislocation glide between individual thermal activation events is simulated using a standard dislocation dynamics algorithm, extended to account for constant stress periodic boundary conditions. Steady state creep conditions are obtained in the simulations with the predicted creep rates as a function of stress and temperature in good agreement with experimentally reported values. Arrhenius scaling of the creep rates as a function of temperature and power-law scaling with the applied stress are also reproduced, with the values of the power-law exponents in the high stress regime in good agreement with experiments.
Validation of a new multiaxial criteria for creep-fatigue damage evaluation
International Nuclear Information System (INIS)
Cabrillat, M.T.; Martin, P.
1989-01-01
For many years, design codes evaluated creep damage using the Von Mises criterion to take account of multiaxiality of stresses. However, recent studies have confirmed that the Von Mises criterion is overconservative for nonuniaxial stress state. Various criteria have been put forward to take account of the real stress state. This paper describes a criterion which was introduced in 1987 and the various studies which led to its adoption
International Nuclear Information System (INIS)
Segle, P.; Samuelson, L.Aa.; Andersson, Peder; Moberg, F.
1996-01-01
Constitutive equations for creep damage mechanics are implemented into the finite element program ABAQUS using a user supplied subroutine, UMAT. A modified Kachanov-Rabotnov constitutive equation which accounts for inhomogeneity in creep damage is used. With a user defined material a number of bench mark tests are analyzed for verification. In the cases where analytical solutions exist, the numerical results agree very well. In other cases, the creep damage evolution response appear to be realistic in comparison with laboratory creep tests. The appropriateness of using the creep damage mechanics concept in design and life assessment of high temperature components is demonstrated. 18 refs
Creep modeling of textured zircaloy under biaxial stressing
International Nuclear Information System (INIS)
Adams, B.L.; Murty, K.L.
1984-01-01
Anisotropic biaxial creep behavior of textured Zircaloy tubing was modeled using a crystal-plastic uniform strain-rate upper-bound and a uniform stress lower-bound approach. Power-law steady-state creep is considered to occur on each crystallite glide system by fixing the slip rate to be proportional to the resolved shear stress raised to a power. Prismatic, basal, and pyramidal slip modes were considered. The crystallographic texture is characterized using the orientation distribution function determined from a set of three pole-figures. This method is contrasted with a Von-Mises-Hill phenomenological model in comparison with experimental data obtained at 673 deg K. The resulting creep-dissipative loci show the importance of the basal slip mode on creep in heavily cold-worked cladding, whereas prismatic slip is more important for the recrystallized materials. (author)
Development of creep damage assessment system for aged thermal power plant
Energy Technology Data Exchange (ETDEWEB)
Nonaka, Isamu [IshikawaJima-Harima Heavy Industries Co., Ltd., Tokyo (Japan); Umaki, Hideo [Ishikawajima-Harima Heavy Industries Co., Ltd., Tokyo (Japan); Nishida, Hidetalca [The Chugoku Electric Power Co., Inc., Hiroshima (Japan); Yamaguchi, Hiroshi [The Chugoku Electric Power Co., Inc., Hiroshima (Japan)
1998-12-31
IHI has developed the Creep Damage Assessment System to identify voids by processing an image observed by a small laser microscope with an advanced image processing technique jointly with Chugoku Electric Power Co., Inc. The result can be obtained immediately on the spot. Application tests of the system at the Unit No.3 boiler of the Kudamatsu Power Station showed good operability, adaptability to the environment, and accuracy. The new system can easily indicate damage conditions in parts during the periodical inspection, allowing rapid maintenance. Time reduction required for assessment and increased reliability of equipment can be also achieved. (orig.)
Development of creep damage assessment system for aged thermal power plant
Energy Technology Data Exchange (ETDEWEB)
Nonaka, Isamu [IshikawaJima-Harima Heavy Industries Co., Ltd., Tokyo (Japan); Umaki, Hideo [Ishikawajima-Harima Heavy Industries Co., Ltd., Tokyo (Japan); Nishida, Hidetalca [The Chugoku Electric Power Co., Inc., Hiroshima (Japan); Yamaguchi, Hiroshi [The Chugoku Electric Power Co., Inc., Hiroshima (Japan)
1999-12-31
IHI has developed the Creep Damage Assessment System to identify voids by processing an image observed by a small laser microscope with an advanced image processing technique jointly with Chugoku Electric Power Co., Inc. The result can be obtained immediately on the spot. Application tests of the system at the Unit No.3 boiler of the Kudamatsu Power Station showed good operability, adaptability to the environment, and accuracy. The new system can easily indicate damage conditions in parts during the periodical inspection, allowing rapid maintenance. Time reduction required for assessment and increased reliability of equipment can be also achieved. (orig.)
Energy Technology Data Exchange (ETDEWEB)
Fournier, B
2007-09-15
It is in the framework of the research programs on nuclear reactors (generation IV) that the martensitic steels containing 9-12% Cr are studied by the CEA. Most of the structures for which they are considered will be solicited in fatigue-creep at high temperature (550 C). The aim of this work is to understand and model the cyclic behaviour and the damage of these materials. The proposed modelling are based on detailed observations studies (SEM, TEM, EBSD...). The cyclic softening is attributed to the growth of the microstructure. A micro-mechanical model based on the physical parameters is proposed and leads to encouraging results. The damage results of interactions between fatigue, creep and oxidation. Two main types of damage are revealed. A model of anticipation of service time is proposed and gives very satisfying results. The possible extrapolations are discussed. (O.M.)
Triggered dynamics in a model of different fault creep regimes.
Kostić, Srđan; Franović, Igor; Perc, Matjaž; Vasović, Nebojša; Todorović, Kristina
2014-06-23
The study is focused on the effect of transient external force induced by a passing seismic wave on fault motion in different creep regimes. Displacement along the fault is represented by the movement of a spring-block model, whereby the uniform and oscillatory motion correspond to the fault dynamics in post-seismic and inter-seismic creep regime, respectively. The effect of the external force is introduced as a change of block acceleration in the form of a sine wave scaled by an exponential pulse. Model dynamics is examined for variable parameters of the induced acceleration changes in reference to periodic oscillations of the unperturbed system above the supercritical Hopf bifurcation curve. The analysis indicates the occurrence of weak irregular oscillations if external force acts in the post-seismic creep regime. When fault motion is exposed to external force in the inter-seismic creep regime, one finds the transition to quasiperiodic- or chaos-like motion, which we attribute to the precursory creep regime and seismic motion, respectively. If the triggered acceleration changes are of longer duration, a reverse transition from inter-seismic to post-seismic creep regime is detected on a larger time scale.
Time evolution of damage in thermally induced creep rupture
Yoshioka, N.
2012-01-01
We investigate the time evolution of a bundle of fibers subject to a constant external load. Breaking events are initiated by thermally induced stress fluctuations followed by load redistribution which subsequently leads to an avalanche of breakings. We compare analytic results obtained in the mean-field limit to the computer simulations of localized load redistribution to reveal the effect of the range of interaction on the time evolution. Focusing on the waiting times between consecutive bursts we show that the time evolution has two distinct forms: at high load values the breaking process continuously accelerates towards macroscopic failure, however, for low loads and high enough temperatures the acceleration is preceded by a slow-down. Analyzing the structural entropy and the location of consecutive bursts we show that in the presence of stress concentration the early acceleration is the consequence of damage localization. The distribution of waiting times has a power law form with an exponent switching between 1 and 2 as the load and temperature are varied.
Energy Technology Data Exchange (ETDEWEB)
Iltis, X., E-mail: xaviere.iltis@cea.fr [CEA, DEN, DEC, Cadarache, 13108 Saint-Paul-Lez-Durance (France); Ben Saada, M. [CEA, DEN, DEC, Cadarache, 13108 Saint-Paul-Lez-Durance (France); Laboratoire d' Etudes des Microstructures et de Mécanique des Matériaux (LEM3), CNRS UMR 7239, Université de Lorraine, Ile du Saulcy, 57045 Metz Cedex 1 (France); Mansour, H.; Gey, N.; Hazotte, A.; Maloufi, N. [Laboratoire d' Etudes des Microstructures et de Mécanique des Matériaux (LEM3), CNRS UMR 7239, Université de Lorraine, Ile du Saulcy, 57045 Metz Cedex 1 (France)
2016-06-15
Four batches of UO{sub 2} pellets were studied comparatively, before and after creep tests, to evaluate a characterization methodology aimed to determine the links between microstructure and damage mechanisms induced by compressive creep of uranium dioxide at 1500 °C. They were observed by means of scanning electron microscopy (SEM) coupled with image analysis, to quantify their fabrication porosity and the occurrence of inter-granular cavities after creep, and electron back scattered diffraction (EBSD), especially to characterize sub-structures development associated with plastic deformation. Electron channeling contrast imaging (ECCI) was also applied to evidence dislocations, at an exploratory stage, on one of the deformed pellets. This approach helped to identify and quantify microstructural differences between batches. Their as-fabricated microstructures differed in terms of grain size and fabrication porosity distribution. The pellets which had the lowest strain rates were those with the largest number of intra-granular pores, regardless of their grain size. They also exhibited less numerous sub-boundaries within the grains. These first results clearly illustrate the benefit of systematic examinations of crept UO{sub 2} pellets at a mesoscopic scale, by SEM and EBSD, to study their deformation process. In addition, ECCI appears as a powerful tool to evidence local dislocations arrangements, in bulk samples. Even if the sampling was limited, the results of this study also tend to indicate that the intra-granular pores population, resulting from the manufacturing of the samples by powder metallurgy, could have a significant influence on the UO{sub 2} viscoplastic deformation mechanisms. - Highlights: • Four different UO{sub 2} pellets batches are microstructurally compared, before and after compression creep tests. • Development of sub-boundaries within the original grains, in crept samples, is quantified by EBSD. • Links are observed between the intra
Interrelation of creep and relaxation: a modeling approach for ligaments.
Lakes, R S; Vanderby, R
1999-12-01
Experimental data (Thornton et al., 1997) show that relaxation proceeds more rapidly (a greater slope on a log-log scale) than creep in ligament, a fact not explained by linear viscoelasticity. An interrelation between creep and relaxation is therefore developed for ligaments based on a single-integral nonlinear superposition model. This interrelation differs from the convolution relation obtained by Laplace transforms for linear materials. We demonstrate via continuum concepts of nonlinear viscoelasticity that such a difference in rate between creep and relaxation phenomenologically occurs when the nonlinearity is of a strain-stiffening type, i.e., the stress-strain curve is concave up as observed in ligament. We also show that it is inconsistent to assume a Fung-type constitutive law (Fung, 1972) for both creep and relaxation. Using the published data of Thornton et al. (1997), the nonlinear interrelation developed herein predicts creep behavior from relaxation data well (R > or = 0.998). Although data are limited and the causal mechanisms associated with viscoelastic tissue behavior are complex, continuum concepts demonstrated here appear capable of interrelating creep and relaxation with fidelity.
International Nuclear Information System (INIS)
Kim, Woo Gon; Yin, Song Nan; Kim, Yong Wan
2008-01-01
Alloy 617 is a principal candidate alloy for the high temperature gas-cooled reactor (HTGR) components, because of its high creep rupture strength coupled with its good corrosion behavior in simulated HTGR-helium and its sufficient workability. To describe a creep strain-time curve well, various constitutive equations have been proposed by Kachanov-Rabotnov, Andrade, Garofalo, Evans and Maruyama, et al.. Among them, the K-R model has been used frequently, because a secondary creep resulting from a balance between a softening and a hardening of materials and a tertiary creep resulting from an appearance and acceleration of the internal or external damage processes are adequately considered. In the case of nickel-base alloys, it has been reported that a tertiary creep at a low strain range may be generated, and this tertiary stage may govern the total creep deformation. Therefore, a creep curve for nickel-based Alloy 617 will be predicted appropriately by using the K-R model that can reflect a tertiary creep. In this paper, the long-term creep curves for Alloy 617 were predicted by using the nonlinear least square fitting (NLSF) method in the K-R model. The modified K-R model was introduced to fit the full creep curves well. The values for the λ and K parameters in the modified K-R model were obtained with stresses
Numerical and experimental study of long term creep damage in austenitic stainless steels
International Nuclear Information System (INIS)
Cui, Yiting
2015-01-01
The creep fracture of 316L(N) austenitic stainless steels has been studied both experimentally and theoretically for temperatures from 525 C up to 700 C and lifetimes up to nineteen years. For short term creep, failure is due to necking. Experimental lifetimes are bounded by the lower and upper bound predictions provided by a necking model and taking into account scatter in input parameters. This model leads to fair predictions of lifetimes up to a few thousand hours at very high temperature. Based on FEG-SEM observations, the transition observed in the failure curves is due to intergranular cavitation. The Riedel modeling of cavity growth by vacancy diffusion along grain boundaries coupled with continuous nucleation is carried out. Lifetimes are predicted fairly well using this model for long term creep failure whatever the considered austenitic stainless steel (316L(N), 304H, 316H, 321H) and the applied temperature (525 C - 700 C). Taking into account low and high stress regimes of Norton-power law, the Riedel model allows us to predict the creep lifetimes up to 25 years which differ from experimental data by less than a factor 3. The effect of the heterogeneity of the microstructure on grain boundary stress concentrations and cavity nucleation is simulated by the finite element method (Cast3M software). It aims to determine the distribution of grain boundary normal stress fields around precipitates depending on time and temperature. The features of the precipitates and the creep behavior of the austenitic matrix are both taking into account. (author) [fr
Modelling of creep curves of Ni3Ge single crystals
Starenchenko, V. A.; Starenchenko, S. V.; Pantyukhova, O. D.; Solov'eva, Yu V.
2015-01-01
In this paper the creep model of alloys with L12 superstructure is presented. The creep model is based on the idea of the mechanisms superposition connected with the different elementary deformation processes. Some of them are incident to the ordered structure L12 (anomalous mechanisms), others are typical to pure metals with the fcc structure (normal mechanisms): the accumulation of thermal APBs by means of the intersection of moving dislocations; the formation of APB tubes; the multiplication of superdislocations; the movement of single dislocations; the accumulation of point defects, such as vacancies and interstitial atoms; the accumulation APBs at the climb of edge dislocations. This model takes into account the experimental facts of the wetting antiphase boundaries and emergence of the disordered phase within the ordered phase. The calculations of the creep curves are performed under different conditions. This model describes different kinds of the creep curves and demonstrates the important meaning of the deformation superlocalisation leading to the inverse creep. The experimental and theoretical results coincide rather well.
Large scale multi-zone creep finite element modelling of a main steam line branch intersection
International Nuclear Information System (INIS)
Payten, Warwick
2006-01-01
A number of papers detail the non-linear creep finite element analysis of branch pieces. Predominately these models have incorporated only a single material zone representing the parent material. Multi-zone models incorporating weld material and heat affected zones have primarily been two-dimensional analyses, in part due to the large number of elements required to adequately represent all of the zones. This paper describes a non-linear creep analysis of a main steam line branch intersection using creep properties to represent the parent metal, weld metal, and heat affected zone (HAZ), the stress redistribution over 100,000 h is examined. The results show that the redistribution leads to a complex stress state, particularly at the heat affected zone. Although, there is damage on the external surface of the branch piece as expected, the results indicate that the damage would be more widespread through extensive sections of the heat affected zone. This would appear to indicate that the time between damage indications on the surface using techniques such as replication and full thickness damage may be more limited then previously expected
Transport critical current density in flux creep model
International Nuclear Information System (INIS)
Wang, J.; Taylor, K.N.R.; Russell, G.J.; Yue, Y.
1992-01-01
The magnetic flux creep model has been used to derive the temperature dependence of the critical current density in high temperature superconductors. The generally positive curvature of the J c -T diagram is predicted in terms of two interdependent dimensionless fitting parameters. In this paper, the results are compared with both SIS and SNS junction models of these granular materials, neither of which provides a satisfactory prediction of the experimental data. A hybrid model combining the flux creep and SNS mechanisms is shown to be able to account for the linear regions of the J c -T behavior which are observed in some materials
Energy Technology Data Exchange (ETDEWEB)
Storesund, Jan [Det Norske Veritas AB, Stockholm (Sweden); Roennholm, Markku [Fortum (Sweden)
2002-04-01
Creep damage development in high temperature components can be monitored by the replica method. Damage is classified and an experience based time period for safe operation is recommended where a re-inspection should be conducted. Original recommendations are still commonly used but there are also developed ones are mostly less conservative. A data base of more than 6000 replicas, collected from welded components in Swedish and Finnish power plants, has been evaluated with respect to damage development in the present project. The results are in general in good agreement to the existing developed recommendations for re-inspections. Important factors that should be considered for use of the recommendations are highlighted: Service history, Material, welding and heat treatment, Measure of pressure and temperature, System stresses, Geometrical stress concentrations, stress distributions, Design of components and welds, Creep crack growth, Starts and stops, Extent and performance of the replica method. These factors have been analysed with respect to the evaluated data resulting in comments to the existing recommendations. In addition, recommendations and conditions for a high reliability of the replica method are described. The comments and recommendations can be read in separate sections in the end of the report.
International Nuclear Information System (INIS)
Bui-Quoc, T.
1982-01-01
A review is presented with an analysis of some recent methods proposed in the literature for predicting failure of materials under a cumulative damage effect due either to fatigue, to creep, or to fatigue-creep combinations. This review is focused on the continuous damage concepts because of their possibilities of application for a wide range of testing conditions. A discussion of the potential of each damage concept is made by examining the correlation between the resulting expressions and available experimental data. The paper also points out particularities encountered in the interpretation of some of the concepts reviewed
International Nuclear Information System (INIS)
Asayama, Tai; Hasebe, Shinichi
1997-01-01
This paper describes a newly developed analytical method of evaluation of creep-fatigue strength of stainless weld metals. Based on the observation that creep-fatigue crack initiates adjacent to the interface of sigma-phase/delta-ferrite and matrix, a mechanistic model which allows the evaluation of micro stress/strain concentration adjacent to the interface was developed. Fatigue and creep damage were evaluated using the model which describes the microstructure after exposed to high temperatures for a long time. Thus it was made possible to predict analytically the long-term creep-fatigue life of stainless steel metals whose microstructure is degraded as a result of high temperature service. (author)
Internal stress model for pre-primary stage of low-stress creep
International Nuclear Information System (INIS)
Kloc, L
2010-01-01
Initial transient stage in low-stress creep experiments was observed in all such experiments. Recently, evidences were presented that this stage cannot be considered as a normal creep primary stage, though the shape of the creep curve is similar. The strain reached during this so called pre-primary stage is fully recoverable upon unloading; the internal stresses must play important role in the effect. Model of standard linear anelastic solid was modified by introduction of creeping body instead of viscous dashpot. Both power law and hyperbolic sine creep law were used to fit observed creep curves of model and structural materials. Mainly the model using hyeprbolic sine creep law provides good fit to individual creep curves and sets of creep curves at different stresses.
Analysis of Fatigue Life of PMMA at Different Frequencies Based on a New Damage Mechanics Model
Directory of Open Access Journals (Sweden)
Aifeng Huang
2014-01-01
Full Text Available Low-cycle fatigue tests at different frequencies and creep tests under different stress levels of Plexiglas Resist 45 were conducted. Correspondingly, the creep fracture time, S-N curves, cyclic creep, and hysteresis loop were obtained. These results showed that the fatigue life increases with frequency at low frequency domain. After analysis, it was found that fatigue life is dependent on the load rate and is affected by the creep damage. In addition, a new continuum damage mechanics (CDM model was established to analyze creep-fatigue life, where the damage increment nonlinear summation rule was proposed and the frequency modification was made on the fatigue damage evolution equation. Differential evolution (DE algorithm was employed to determine the parameters within the model. The proposed model described fatigue life under different frequencies, and the calculated results agreed well with the experimental results.
Microstructural modelling of creep crack growth from a blunted crack
Onck, P.R.; Giessen, E. van der
1998-01-01
The effect of crack tip blunting on the initial stages of creep crack growth is investigated by means of a planar microstructural model in which grains are represented discretely. The actual linking-up process of discrete microcracks with the macroscopic crack is simulated, with full account of the
Creep/fatigue damage prediction of fast reactor components using shakedown methods
International Nuclear Information System (INIS)
Buckthorpe, D.E.
1997-01-01
The present status of the shakedown method is reviewed, the application of the shakedown based principles to complex hardening and creep behaviour is described and justified and the prediction of damage against design criteria outlined. Comparisons are made with full inelastic analysis solutions where these are available and against damage assessments using elastic and inelastic design code methods. Current and future developments of the method are described including a summary of the advances made in the development of the post process ADAPT, which has enabled the method to be applied to complex geometry features and loading cases. The paper includes a review of applications of the method to typical Fast Reactor structural example cases within the primary and secondary circuits. For the primary circuit this includes structures such as the large diameter internal shells which are surrounded by hot sodium and subject to slow and rapid thermal transient loadings. One specific case is the damage assessment associated with thermal stratifications within sodium and the effects of moving sodium surfaces arising from reactor trip conditions. Other structures covered are geometric features within components such as the Above Core structure and Intermediate Heat Exchanger. For the secondary circuit the method has been applied to alternative and more complex forms of geometry namely thick section tubeplates of the Steam Generator and a typical secondary circuit piping run. Both of these applications are in an early stage of development but are expected to show significant advantages with respect to creep and fatigue damage estimation compared with existing code methods. The principle application of the method to design has so far been focused on Austenitic Stainless steel components however current work shows some significant benefits may be possible from the application of the method to structures made from Ferritic steels such as Modified 9Cr 1Mo. This aspect is briefly
Energy Technology Data Exchange (ETDEWEB)
Schweda, Mario; Beck, Tilmann; Singheiser, Lorenz [Forschungszentrum Juelich GmbH (DE). Inst. fuer Energie- und Klimaforschung (IEK), Werkstoffstruktur und Eigenschaften (IEK-2)
2012-01-15
The influence of roughness profile shape, roughness depth, bond coat creep strength and pre-oxidation on the thermal cycling damage evolution and lifetime of a plasma-sprayed ZrO{sub 2} thermal barrier coating system was investigated. A simplified model system was used where FeCrAlY substrates simulated the bond coat. Substrate creep was varied by using the oxide dispersoid strengthened alloy MA956 and the conventional material Fecralloy. Stochastic 3- and periodic 2-dimensional roughness profiles were produced by sand blasting and high speed turning. Damage evolution is significantly influenced by substrate creep with a trend to higher lifetimes for the fast creeping substrate. Pre-oxidation has no influence. Lifetimes of the periodically profiled samples are up to 100 times lower than these of stochastically profiled samples. In the case of periodically profiled samples, the highest lifetime was reached for the highest roughness depth combined with local undercuttings in the roughness profile. For stochastically profiled samples the influence of roughness depth could not be determined due to the wide lifetime scatter. (orig.)
International Nuclear Information System (INIS)
Xu Qiang
2005-01-01
A generic validation methodology for a set of multi-axial creep damage constitutive equations is proposed and its use is illustrated with 0.5Cr0.5Mo0.25V ferritic steel which is featured as brittle or intergranular rupture. The objective of this research is to develop a methodology to guide systematically assess the quality of a set of multi-axial creep damage constitutive equations in order to ensure its general applicability. This work adopted a total quality assurance approach and expanded as a Four Stages procedure (Theories and Fundamentals, Parameter Identification, Proportional Load, and Non-proportional load). Its use is illustrated with 0.5Cr0.5Mo0.25V ferritic steel and this material is chosen due to its industry importance, the popular use of KRH type of constitutive equations, and the available qualitative experimental data including damage distribution from notched bar test. The validation exercise clearly revealed the deficiencies existed in the KRH formulation (in terms of mathematics and physics of damage mechanics) and its incapability to predict creep deformation accurately. Consequently, its use should be warned, which is particularly important due to its wide use as indicated in literature. This work contributes to understand the rational for formulation and the quality assurance of a set of constitutive equations in creep damage mechanics as well as in general damage mechanics. (authors)
The application of miniature disc testing for the assessment of creep damage in CrMoV rotor steel
Energy Technology Data Exchange (ETDEWEB)
Parker, J.D.; Stratford, G.C. [University of Wales, Swansea (United Kingdom); Shaw, N.; Spink, G. [National Power plc (United Kingdom); Metcalfe, H. [Siemens Power Generation (United Kingdom)
1998-12-31
A range of critical experiments has been performed studying the creep and fracture behaviour of a typical CrMoV rotor steel. Initially, uniaxial tests were carried out to provide material with a predetermined level of creep damage. Then, miniature disc tests were undertaken under accelerated conditions in a similar manner to procedures used for post-exposure uniaxial testing of service components. Data analysis demonstrates that the miniature tests accurately reflect the damage present so that this approach can be used to support run/repair/replace decisions. (orig.) 8 refs.
The application of miniature disc testing for the assessment of creep damage in CrMoV rotor steel
Energy Technology Data Exchange (ETDEWEB)
Parker, J D; Stratford, G C [University of Wales, Swansea (United Kingdom); Shaw, N; Spink, G [National Power plc (United Kingdom); Metcalfe, H [Siemens Power Generation (United Kingdom)
1999-12-31
A range of critical experiments has been performed studying the creep and fracture behaviour of a typical CrMoV rotor steel. Initially, uniaxial tests were carried out to provide material with a predetermined level of creep damage. Then, miniature disc tests were undertaken under accelerated conditions in a similar manner to procedures used for post-exposure uniaxial testing of service components. Data analysis demonstrates that the miniature tests accurately reflect the damage present so that this approach can be used to support run/repair/replace decisions. (orig.) 8 refs.
International Nuclear Information System (INIS)
Berthollet, A.
2003-10-01
Concrete structures are examined during their lifetime and often present important cracking states, which can progress with time and lead to change the structural behavior. The civil engineering works that the main function corresponds to protection's wall are very sensitive to this damage and its evolution. The growth of the time - dependent cracks represents an aging pathology linked with interaction between creep mechanism and the non-linear behavior of the material. In this thesis, a modeling for these mechanisms and their coupling are proposed. It based on creep strains analysis under different load levels, on the influence of the rate effect to the mechanical behavior. A stress limit is put on prominent manner, where beyond it, the creep - cracking interaction becomes important with the introduction of the ultimate tertiary creep kinetic. This level of strength is identified for infinitely slow loading rates and is also called intrinsic strength. It defines the limit on this side the viscous behavior of the cement paste limits the irreversibility processes as cracking. Thus, a constitutive law of viscoelastic - viscoplastic behavior with a high coupling between the cracking mechanism and the creep strains is proposed. The developments of the model are built on DUVAUT - LIONS approach integrated a generalized MAXWELL chain model. For one part, the viscoelastic behavior translates the creep mechanism under low stresses. For a second part, it associated with the viscoplastic behavior, which allows introducing both creep effect under high stresses and rate effect acting on micro-cracked zones. The cracking mechanism is described throughout a plasticity theory with multi-criteria, which induce a property of anisotropy for hardening. Qualitatively, ails of the creep kinetics are reproduced. An additional validation is based on experimental tests in compression, traction and flexion where the main parameters of the modeling are detailed. Thus, we can conclude on the
Creep simulation of adhesively bonded joints using modified generalized time hardening model
Energy Technology Data Exchange (ETDEWEB)
Sadigh, Mohammad Ali Saeimi [Azarbaijan Shahid Madani University, Tabriz (Iran, Islamic Republic of)
2016-04-15
Creep behavior of double lap adhesively bonded joints was investigated using experimental tests and numerical analysis. Firstly, uniaxial creep tests were carried out to obtain the creep characteristics and constitutive parameters of the adhesive at different stress and temperature levels. Generalized time hardening model was used to predict the creep behavior of the adhesive. This model was modified to simulate the creep behavior at different stress and temperature levels. Secondly, the developed model was used to simulate the creep behavior of bonded joints using finite element based numerical analysis. Creep deformations of the joints were measured experimentally and good agreement was observed in comparison with the results obtained using numerical simulation. Afterward, stress redistribution due to the creep along the adhesively bonded joint was obtained numerically. It was observed that temperature level had a significant effect on the stress redistribution along the adhesive thickness.
Creep-fatigue damage evaluation for SS-316LN (ORNL PLATES): - RCC-MR vs. ASME SEC III - NH
International Nuclear Information System (INIS)
Sati, Bhuwan Chandra; Jalaldeen, S.; Velusamy, K.; Selvaraj, P.
2016-01-01
Investigations of high temperature tests done on ORNL plate with deformation control loading, under creep-fatigue damage have been presented. The test results with methodology of RCC-MR and ASME-NH life prediction under creep-fatigue loading have been assessed. The stress relaxation effect in calculating the life using RCC-MR under creep-fatigue damage is found to be significant in presence of secondary stress. RCC-MR: 2007 is more realistic number of cycles (predicts 51 number of cycles) as compared to ASME-NH (predicts 312 number of cycles) which is demonstrated by the experimental work (observed 86 numbers of cycles). Between RCC-MR and experimental work, design code seems to be more conservative for life prediction due to creep-fatigue damage. For fatigue damage, the approaches are same and the difference comes from material properties and the starting stress for applying Neuber's rule. ASME approach has the limitation of stress range magnitude. ASME approach predicts lower elastic plus plastic strain for the cases having S* above the linear stress limit. For creep strain and creep damage evaluation, ASME and RCC-MR have different approaches for calculating the stress at the beginning and during the hold period. The RCC-MR takes account of cyclic hardening or softening effects (hardening in the present case of 316 LN) by means of the cyclic stress-strain curve and the benefit of symmetrization effects which are significant for this material. The ASME code neglects these effects and instead relies on an approach based on the isochronous stress-strain curves. (author)
Energy Technology Data Exchange (ETDEWEB)
Messner, M. C. [Argonne National Lab. (ANL), Argonne, IL (United States); Truster, T. J. [Univ. of Tennessee, Knoxville, TN (United States); Cochran, K. B. [DR& C Inc.; Parks, D. M. [DR& C Inc.; Sham, T. -L. [Argonne National Lab. (ANL), Argonne, IL (United States)
2017-09-01
Advanced reactors designed to operate at higher temperatures than current light water reactors require structural materials with high creep strength and creep-fatigue resistance to achieve long design lives. Grade 91 is a ferritic/martensitic steel designed for long creep life at elevated temperatures. It has been selected as a candidate material for sodium fast reactor intermediate heat exchangers and other advanced reactor structural components. This report focuses on the creep deformation and rupture life of Grade 91 steel. The time required to complete an experiment limits the availability of long-life creep data for Grade 91 and other structural materials. Design methods often extrapolate the available shorter-term experimental data to longer design lives. However, extrapolation methods tacitly assume the underlying material mechanisms causing creep for long-life/low-stress conditions are the same as the mechanisms controlling creep in the short-life/high-stress experiments. A change in mechanism for long-term creep could cause design methods based on extrapolation to be non-conservative. The goal for physically-based microstructural models is to accurately predict material response in experimentally-inaccessible regions of design space. An accurate physically-based model for creep represents all the material mechanisms that contribute to creep deformation and damage and predicts the relative influence of each mechanism, which changes with loading conditions. Ideally, the individual mechanism models adhere to the material physics and not an empirical calibration to experimental data and so the model remains predictive for a wider range of loading conditions. This report describes such a physically-based microstructural model for Grade 91 at 600° C. The model explicitly represents competing dislocation and diffusional mechanisms in both the grain bulk and grain boundaries. The model accurately recovers the available experimental creep curves at higher stresses
International Nuclear Information System (INIS)
Dubiez-Le Goff, Sophie; Couturier, Raphaeel; Guetaz, Laure; Burlet, Helene
2004-01-01
Powder metallurgy processed Udimet 720 is a high creep strength nickel-based superalloy considered for high temperature turbine disks for nuclear gas cooled reactors working under 700 deg. C. Both fine-grained and coarse-grained microstructures have been obtained by applying respectively a subsolvus or a supersolvus solution treatments, followed by ageing treatments. In both microstructures, the distribution of the strengthening γ' precipitates has been characterized by transmission electron microscopy (TEM). The creep curves of the coarse-grained microstructure show the three usual creep stages. On the contrary, the creep curves of the fine-grained microstructure show a transition directly from primary to apparent tertiary creep without any obvious steady state. According to TEM analyses, Orowan loops surround Udimet 720 CR γ' and U720 HS γ' at high stress whereas U720 HS γ' are sheared at low stress. To describe the behavior of the superalloy Udimet 720, a specific creep model is developed on the basis of McLean and Dyson models including physical damage parameters
Hindsight Bias Doesn't Always Come Easy: Causal Models, Cognitive Effort, and Creeping Determinism
Nestler, Steffen; Blank, Hartmut; von Collani, Gernot
2008-01-01
Creeping determinism, a form of hindsight bias, refers to people's hindsight perceptions of events as being determined or inevitable. This article proposes, on the basis of a causal-model theory of creeping determinism, that the underlying processes are effortful, and hence creeping determinism should disappear when individuals lack the cognitive…
International Nuclear Information System (INIS)
Hoffmann, C.L.; Urko, W.
1993-01-01
Creep damage can result from stress relaxation of residual stresses in components when exposed to high temperature thermal cycles. Pressure vessels, such as the reactor vessel of the modular high-temperature gas reactor (MHTGR), which normally operate at temperatures well below the creep range can develop relatively high residual stresses in high stress locations. During short term excursions to elevated-temperatures, creep damage can be produced by the loadings on the vessel. In addition, residual stresses will relax out, causing greater creep damage in the pressure vessel material than might otherwise be calculated. The evaluation described in this paper assesses the magnitude of the creep damage due to relaxation of residual stresses resulting from short term exposure of the pressure vessel material to temperatures in the creep range. Creep relaxation curves were generated for SA533 Grade B, Class 1 and SA508 Class 3 pressure vessel steels using finite element analysis of a simple uniaxial truss loaded under constant strain conditions to produce an initial axial stress equal to 1.25 times the material yield strength at temperature. The strain is held constant for 1000 hours at prescribed temperatures from 700 F to 1000 F. The material creep law is used to calculate the relaxed stress for each time increment. The calculated stress relaxation versus time curves are compared with stress relaxation test data. Creep damage fractions are calculated by integrating the stress relaxation versus time curves and performing a linear creep damage summation using the minimum stress to rupture curves at the respective relaxation temperatures. Cumulative creep damage due to stress relaxation as a function of time and temperature is derived from the linear damage summation
Point defects and the creep of metals
International Nuclear Information System (INIS)
Nichols, F.A.
1976-01-01
Basic concepts felt to be important in diffusion-controlled creep of metals are reviewed and it is suggested that such creep is controlled by edge-dislocation climb under a rather wide range of conditions. The effect of a damage-producing flux on such creep processes is explored. It is shown that processes such as Herring-Nabarro creep are unaffected by irradiation. Evidence is presented for a climb-plus-glide mechanism of radiation creep for stresses above unirradiated yield or flow stresses. At lower stresses a preferential dislocation loop nucleation model is suggested
Creep damage index as a sensitive indicator of damage accumulation in thermoplastic laminates
Czech Academy of Sciences Publication Activity Database
Minster, Jiří; Šperl, Martin; Šepitka, J.
2018-01-01
Roč. 37, č. 3 (2018), s. 147-154 ISSN 0731-6844 Institutional support: RVO:68378297 Keywords : damage accumulation * thermoplastic laminate * cyclic tensile loading * time-dependent properties * microindentation Subject RIV: JL - Materials Fatigue, Friction Mechanics OBOR OECD: Audio engineering, reliability analysis Impact factor: 1.086, year: 2016 http://journals.sagepub.com/doi/pdf/10.1177/0731684417735184
Directory of Open Access Journals (Sweden)
C. P. Borstad
2013-12-01
Full Text Available Around the perimeter of Antarctica, much of the ice sheet discharges to the ocean through floating ice shelves. The buttressing provided by ice shelves is critical for modulating the flux of ice into the ocean, and the presently observed thinning of ice shelves is believed to be reducing their buttressing capacity and contributing to the acceleration and thinning of the grounded ice sheet. However, relatively little attention has been paid to the role that fractures play in the ability of ice shelves to sustain and transmit buttressing stresses. Here, we present a new framework for quantifying the role that fractures play in the creep deformation and buttressing capacity of ice shelves. We apply principles of continuum damage mechanics to derive a new analytical relation for the creep of an ice shelf that accounts for the softening influence of fractures on longitudinal deformation using a state damage variable. We use this new analytical relation, combined with a temperature calculation for the ice, to partition an inverse method solution for ice shelf rigidity into independent solutions for softening damage and stabilizing backstress. Using this new approach, field and remote sensing data can be utilized to monitor the structural integrity of ice shelves, their ability to buttress the flow of ice at the grounding line, and thus their indirect contribution to ice sheet mass balance and global sea level. We apply this technique to the Larsen C ice shelf using remote sensing and Operation IceBridge data, finding damage in areas with known crevasses and rifts. Backstress is highest near the grounding line and upstream of ice rises, in agreement with patterns observed on other ice shelves. The ice in contact with the Bawden ice rise is weakened by fractures, and additional damage or thinning in this area could diminish the backstress transmitted upstream. We model the consequences for the ice shelf if it loses contact with this small ice rise
Study of creep-fatigue behavior in a 1000 MW rotor using a phenomenological lifetime model
Energy Technology Data Exchange (ETDEWEB)
Zhao, Nailong; Wang, Weizhe; Jiang, Jishen; Liu, Yingzheng [School of Mechanical Engineering, Shanghai (China)
2017-02-15
In this study, the phenomenological lifetime model was applied to part of an ultra-supercritical steam turbine rotor model to predict its lifetime as a post processing of the finite element method. To validate the accuracy and adaptation of the post processing program, stress strain hysteresis loops of a cylinderal model under service-like load cycle conditions in cycle N = 1 and 300 were constructed, and the comparison of the results with experimental data on the same cylinderal specimen showed them to be satisfactory. The temperature and von Mises stress distributions of the rotor during a startup-running-shutdown-natural cool process were numerically studied using ABAQUS and the damage caused by the interaction of creep and fatigue was subsequently computed and discussed. It was found that the maximum damage appeared at the inlet notch zone, with the blade groove areas and the front notch areas also suffering a large damage amplitude.
Implementation of creep-fatigue model into finite-element code to assess cooled turbine blade.
CSIR Research Space (South Africa)
Dedekind, MO
1994-01-01
Full Text Available Turbine blades which are designed with airfoil cooling are subject to thermo-mechanical fatigue as well as creep damage. These problems arise due to thermal cycling and high operating temperatures in service. An implementation of fatigue and creep...
A planar model study of creep in metal matrix composites with misaligned short fibres
DEFF Research Database (Denmark)
Sørensen, N.J.
1993-01-01
The effect of fibre misalignment on the creep behaviour of metal matrix composites is modelled, including hardening behaviour (stage 1), dynamic recovery and steady state creep (stage 2) of the matrix material, using an internal variable constitutive model for the creep behaviour of the metal...... matrix. Numerical plane strain results in terms of average properties and detailed local deformation behaviour up to large strains are needed to show effects of fibre misalignment on the development of inelastic strains and the resulting over-all creep resistance of the material. The creep resistance...
Energy Technology Data Exchange (ETDEWEB)
Shen, Chen
2015-01-01
We report here a constitutive model for predicting long-term creep strain evolution in’ strengthened Ni-base superalloys. Dislocation climb-bypassing’, typical in intermediate’ volume fraction (~20%) alloys, is considered as the primary deformation mechanism. Dislocation shearing’ to anti-phase boundary (APB) faults and diffusional creep are also considered for high-stress and high-temperature low-stress conditions, respectively. Additional damage mechanism is taken into account for rapid increase in tertiary creep strain. The model has been applied to Alloy 282, and calibrated in a temperature range of 1375-1450°F, and stress range of 15-45ksi. The model parameters and a MATLAB code are provided. This report is prepared by Monica Soare and Chen Shen at GE Global Research. Technical discussions with Dr. Vito Cedro are greatly appreciated. This work was supported by DOE program DE-FE0005859
International Nuclear Information System (INIS)
Maiya, P.S.
1978-07-01
The creep-fatigue life results for five different heats of Type 304 stainless steel at 593 0 C (1100 0 F), generated under push-pull conditions in the axial strain-control mode, are presented. The life predictions for the various heats based on the linear-damage rule, strain-range partitioning method, and damage-rate approach are discussed. The appropriate material properties required for computation of fatigue life are also included
International Nuclear Information System (INIS)
Boeuf, A.; Coppola, R.; Matera, R.; Rustichelli, F.; Zambonardi, F.; Puliti, P.; Melone, S.
1982-01-01
In the austenitic stainless steels, a class of materials largely used in the nuclear power plants, creep induces essentially two new microstructural effects: the nucleation and growth of grain boundary cavities and the precipitation of carbides. Carbides precipitate as a consequence of pure thermal treatment, whereas for the occurrence of voids the presence of stress is necessary. It should be noted however, that the kinetics of precipitation and even the precipitate crystal structure are changed by the introduction of dislocations due to straining during creep. The aim of the present study is a quantitative characterization of the creep damage occurring in a stainless steel of the type X 6 CrNi 8 11 (AISI 304). The experimental techniques used are optical and electron microscopy, microprobe analysis and small angle neutron scattering. This latter technique is described in more detail
Heffernan, Julieanne; Biedermann, Eric; Mayes, Alexander; Livings, Richard; Jauriqui, Leanne; Goodlet, Brent; Aldrin, John C.; Mazdiyasni, Siamack
2018-04-01
Process Compensated Resonant Testing (PCRT) is a full-body nondestructive testing (NDT) method that measures the resonance frequencies of a part and correlates them to the part's material and/or damage state. PCRT testing is used in the automotive, aerospace, and power generation industries via automated PASS/FAIL inspections to distinguish parts with nominal process variation from those with the defect(s) of interest. Traditional PCRT tests are created through the statistical analysis of populations of "good" and "bad" parts. However, gathering a statistically significant number of parts can be costly and time-consuming, and the availability of defective parts may be limited. This work uses virtual databases of good and bad parts to create two targeted PCRT inspections for single crystal (SX) nickel-based superalloy turbine blades. Using finite element (FE) models, populations were modeled to include variations in geometric dimensions, material properties, crystallographic orientation, and creep damage. Model results were verified by comparing the frequency variation in the modeled populations with the measured frequency variations of several physical blade populations. Additionally, creep modeling results were verified through the experimental evaluation of coupon geometries. A virtual database of resonance spectra was created from the model data. The virtual database was used to create PCRT inspections to detect crystallographic defects and creep strain. Quantification of creep strain values using the PCRT inspection results was also demonstrated.
Constitutive model of creep in polycrystalline halite based on workhardening and recovery
International Nuclear Information System (INIS)
Munson, D.E.
1993-01-01
A multimechanism constitutive model of creep has been developed which incorporates the workhardening and recovery transient creep behavior. This model has been applied to the creep of polycrystalline halite. The specific application of the model is in the calculation of the closure of underground rooms in layered salt deposits. Through the use of finite element calculations, this model, with appropriate laboratory material parameters and a Tresca flow potential, has predicted the measured closure of a number of large in situ experimental rooms
Enhancing uncertainty tolerance in the modelling creep of ligaments
International Nuclear Information System (INIS)
Taha, M M Reda; Lucero, J
2006-01-01
The difficulty in performing biomechanical tests and the scarcity of biomechanical experimental databases necessitate extending the current knowledge base to allow efficient modelling using limited data sets. This study suggests a framework to reduce uncertainties in biomechanical systems using limited data sets. The study also shows how sparse data and epistemic input can be exploited using fuzzy logic to represent biomechanical relations. An example application to model collagen fibre recruitment in the medial collateral ligaments during time-dependent deformation under cyclic loading (creep) is presented. The study suggests a quality metric that can be employed to observe and enhance uncertainty tolerance in the modelling process
Thermodynamic and kinetic modelling: creep resistant materials
DEFF Research Database (Denmark)
Hald, John; Korcakova, L.; Danielsen, Hilmar Kjartansson
2008-01-01
The use of thermodynamic and kinetic modelling of microstructure evolution in materials exposed to high temperatures in power plants is demonstrated with two examples. Precipitate stability in martensitic 9–12%Cr steels is modelled including equilibrium phase stability, growth of Laves phase part...
Correlation Between Intercritical Heat-Affected Zone and Type IV Creep Damage Zone in Grade 91 Steel
Wang, Yiyu; Kannan, Rangasayee; Li, Leijun
2018-04-01
A soft zone in Cr-Mo steel weldments has been reported to accompany the infamous Type IV cracking, the highly localized creep damage in the heat-affected zone of creep-resistant steels. However, the microstructural features and formation mechanism of this soft zone are not well understood. In this study, using microhardness profiling and microstructural verification, the initial soft zone in the as-welded condition was identified to be located in the intercritical heat-affected zone of P91 steel weldments. It has a mixed structure, consisting of Cr-rich re-austenitized prior austenite grains and fine Cr-depleted, tempered martensite grains retained from the base metal. The presence of these further-tempered retained grains, originating from the base metal, is directly responsible for the hardness reduction of the identified soft zone in the as-welded condition. The identified soft zone exhibits a high location consistency at three thermal stages. Local chemistry analysis and thermodynamic calculation show that the lower chromium concentrations inside these retained grains thermodynamically decrease their potentials for austenitic transformation during welding. Heterogeneous grain growth is observed in the soft zone during postweld heat treatment. The mismatch of strengths between the weak Cr-depleted grains and strong Cr-rich grains enhances the creep damage. Local deformation of the weaker Cr-depleted grains accelerates the formation of creep cavities.
International Nuclear Information System (INIS)
Pettersson, Kjell
2006-12-01
A previously developed model for the plastic deformation and creep of copper (included as an Appendix to the present report) has been used as the basis for a discussion on the possibility of brittle creep fracture of the copper canister during long term storage of nuclear waste. Reported creep tests on oxygen free (OF) copper have demonstrated that copper can have an extremely low creep ductility. However with the addition of about 50 ppm phosphorus to the copper it appears as if the creep brittleness problem is avoided and that type of copper (OFP) has consequently been chosen as the canister material. It is shown in the report that the experiments performed on OFP copper does not exclude the possibility of creep brittleness of OFP copper in the very long term. The plasticity and creep model has been used to estimate creep life under conditions of intergranular creep cracking according to a model formulated by Cocks and Ashby. The estimated life times widely exceed the design life of the canister. However the observations of creep brittleness in OF copper indicate that the Cocks-Ashby model probably does not apply to the OF copper. Thus additional calculations have been done with the plasticity and creep model in order to estimate stress as a function of time for the probably most severe loading case of the canister with regard to creep failure, an earth quake shear. Despite the fact that the stress in the canister will remain at the 100 MPa level for thousands of years after an earth quake the low temperature, about 50 deg C or less, will make the solid state diffusion process assumed to control the brittle cracking process, too slow to lead to any significant brittle creep cracking in the canister
Constitutive modelling of creep in a long fiber random glass mat thermoplastic composite
Dasappa, Prasad
, which is the reduced form of the Schapery non-linear viscoelastic model, was found to be sufficient to model the viscoelastic behaviour. The viscoplastic strains were modeled using the Zapas and Crissman viscoplastic model. A parameter estimation method which isolates the viscoelastic component from the viscoplastic part of the non-linear model has been developed. The non-linear parameters in the Findley's non-linear viscoelastic model have been found to be dependent on both stress and temperature and have been modeled as a product of functions of stress and temperature. The viscoplastic behaviour for temperatures up to 40°C was similar indicating similar damage mechanisms. Moreover, the development of viscoplastic strains at 20 and 30 MPa were similar over all the entire temperature range considered implying similar damage mechanisms. It is further recommended that the material should not be used at temperature greater than 60°C at stresses over 50 MPa. To further study the viscoplastic behaviour of continuous fibre glass mat thermoplastic composite at room temperature, multiple creep-recovery experiments of increasing durations between 1 and 24 hours have been conducted on a single specimen. The purpose of these tests was to experimentally and numerically decouple the viscoplastic strains from total creep response. This enabled the characterization of the evolution of viscoplastic strains as a function of time, stress and loading cycles and also to co-relate the development of viscoplastic strains with progression of failure mechanisms such as interfacial debonding and matrix cracking which were captured in-situ. A viscoplastic model developed from partial data analysis, as proposed by Nordin, had excellent agreement with experimental results for all stresses and times considered. Furthermore, the viscoplastic strain development is accelerated with increasing number of cycles at higher stress levels. These tests further validate the technique proposed for numerical
International Nuclear Information System (INIS)
Thai, M.Q.
2012-01-01
Concrete is a complex heterogeneous material whose deformations include a delayed part that is affected by a number of factors such as temperature, relative humidity and microstructure evolution. Taking into account differed deformations and in particular creep is essential in the computation of concrete structures such as those dedicated to radioactive waste storage. The present work aims: (1) at elaborating a simple and robust model of creep for concrete by using micro-mechanics and accounting for the effects of damage, temperature and relative humidity; (2) at numerically implementing the creep model developed in a finite element code so as to simulate the behavior of simple structural elements in concrete. To achieve this twofold objective, the present work is partitioned into three parts. In the first part the cement-based material at the microscopic scale is taken to consist of a linear viscoelastic matrix characterized by a generalized Maxwell model and of particulate phases representing elastic aggregates and pores. The Mori-Tanaka micro-mechanical scheme, the Laplace-Carson transform and its inversion are then used to obtain analytical or numerical estimates for the mechanical and hydro-mechanical parameters of the material. Next, the original micromechanical model of creep is coupled to the damage model of Mazars through the concept of pseudo-deformations introduced by Schapery. The parameters involved in the creep-damage model thus established are systematically identified using available experimental data. Finally, the effects of temperature and relative humidity are accounted for in the creep-damage model by using the equivalent time method; the efficiency of this approach is demonstrated and discussed in the case of simple creep tests. (author) [fr
Pressure sintering and creep deformation: a joint modeling approach
International Nuclear Information System (INIS)
Notis, M.R.
1979-10-01
Work related to microchemical and microstructural aspects of the joint modeling of pressure sintering and creep in ceramic oxides is reported. Quantitative techniques for the microchemical analysis of ceramic oxides and for the examination of impurity segregation effects in polycrystalline ceramic materials were developed. This has included fundamental absorption corrections for the oxygen anion species as a function of foil thickness. The evolution in microstructure during the transition from intermediate stage to final stage densification during hot pressing of cobalt oxide and preliminary studies with doped oxides were studied. This work shows promise in using time-integrated microstructural effects to elucidate the role of impurities in the sintering of ceramic materials
Validation of statistical models for creep rupture by parametric analysis
Energy Technology Data Exchange (ETDEWEB)
Bolton, J., E-mail: john.bolton@uwclub.net [65, Fisher Ave., Rugby, Warks CV22 5HW (United Kingdom)
2012-01-15
Statistical analysis is an efficient method for the optimisation of any candidate mathematical model of creep rupture data, and for the comparative ranking of competing models. However, when a series of candidate models has been examined and the best of the series has been identified, there is no statistical criterion to determine whether a yet more accurate model might be devised. Hence there remains some uncertainty that the best of any series examined is sufficiently accurate to be considered reliable as a basis for extrapolation. This paper proposes that models should be validated primarily by parametric graphical comparison to rupture data and rupture gradient data. It proposes that no mathematical model should be considered reliable for extrapolation unless the visible divergence between model and data is so small as to leave no apparent scope for further reduction. This study is based on the data for a 12% Cr alloy steel used in BS PD6605:1998 to exemplify its recommended statistical analysis procedure. The models considered in this paper include a) a relatively simple model, b) the PD6605 recommended model and c) a more accurate model of somewhat greater complexity. - Highlights: Black-Right-Pointing-Pointer The paper discusses the validation of creep rupture models derived from statistical analysis. Black-Right-Pointing-Pointer It demonstrates that models can be satisfactorily validated by a visual-graphic comparison of models to data. Black-Right-Pointing-Pointer The method proposed utilises test data both as conventional rupture stress and as rupture stress gradient. Black-Right-Pointing-Pointer The approach is shown to be more reliable than a well-established and widely used method (BS PD6605).
International Nuclear Information System (INIS)
Dufour, F.
2007-12-01
The industrial context of this research work is to study the durability of the internal barriers of nuclear power plants. This paper is divided in two parts, the first part is relative to the crack-damage state and the second part to the creep consequences on the rupture properties of concrete. In the first part, the analysis of the experimental results, (carried out on a compression cylinder on which the radial permeability has been measured), shows that the permeability decreases until a deformation of half of those at the force peak, by re-closure of the preexisting microcracks in the material; then the permeability strongly increases until after the force peak by initiation, connexion and opening of the crack, and at last it increases less rapidly until the rupture because only the opening of the macro-cracks increases. In order to simulate these phenomena, two original methods are presented, in post-treatment phase, for estimating the leaks from a mechanical computing based on finite element methods. With the first method, it is possible to measure the permeability from the damage field and from a relation between the permeability and the damage which bind the Poiseuille law to an empirical law established for weak damages. The second method is on the deformations field from which the position and opening of the crack are calculated. The Poiseuille relation is then applied along the crack to estimate the leaks rates. The relation between the concrete creep and its mechanical characteristics is analyzed in the second part. In particular, are studied the creep consequences on the long term mechanical properties. After having given the experimental results which show essentially an embrittlement of the material after creep, a qualitative analysis by the bifurcations study is proposed, and then by a discrete numerical method to find again the same influence of the visco-elasticity on the rupture embrittlement experimentally observed. At last, the first results of
Effect of welding on creep damage evolution in P91B steel
Energy Technology Data Exchange (ETDEWEB)
Baral, J., E-mail: jayshree2k4@gmail.com [Metallurgical and Materials Engineering, Indian Institute of Kharagpur, WB 721302 (India); Swaminathan, J. [CSIR–National Metallurgical Laboratory, Jamshedpur 831007 (India); Chakrabarti, D.; Ghosh, R.N. [Metallurgical and Materials Engineering, Indian Institute of Kharagpur, WB 721302 (India)
2017-07-15
Study of creep behavior of base metal (without weld) and welded specimens of P91B steel over a range of temperatures (600–650 °C) and stresses (50–180 MPa) showed similar values of minimum creep-rates for both specimens at higher stress regime (>100 MPa) whilst, significantly higher creep rates in the case of welded specimens at lower stress regime. Considering that welded specimen is comprised of two distinct structural regimes, i.e. weld affected zone and base metal, a method has been proposed for estimating the material parameters describing creep behavior of those regimes. Stress–strain distribution across welded specimen predicted from finite element analysis based on material parameters revealed preferential accumulation of stress and creep strain at the interface between weld zone and base metal. This is in-line with the experimental finding that creep rupture preferentially occurs at inter-critical heat affected zone in welded specimens owing to ferrite-martensite structure with coarse Cr{sub 23}C{sub 6} particles. - Highlights: •Comparison of creep properties of welded and virgin specimens of P91B steel. •At lower stresses (<100 MPa) welded samples show higher minimum creep-rate. •Creep rupture at inter-critical heat affected zone (IC-HAZ) in welded specimens. •FEA showing accumulation of creep strain in weld/base metal interface. •Precipitate free soft ferrite matrix accumulates strain and weakens IC-HAZ.
International Nuclear Information System (INIS)
Sawada, Kota; Maruyama, Kouichi; Komine, Ryuji; Nagae, Yuji
1998-02-01
Mod.9Cr-1Mo steel has a martensitic lath structure. Recovery of the lath structure takes place in the course of creep. Microstructural degradation due to the recovery results in the acceleration of creep rate and the subsequent failure of a specimen. Change of lath width during creep of the steel was quantitatively investigated to propose a residual life assessment methodology based on the recovery process. Since the steel was tempered at 1053K, the lath structure is thermally stable at the testing temperatures (848K-923K). However, recovery of lath structure readily takes place during creep, indicating that the recovery is induced by creep deformation. Lath width d increases with creep strain and saturates to a value d s determined by creep stress. The increase of d is faster at a higher stress and temperature. A normalized change in lath width, Δd/Δd s , was introduced to explain the variation of lath growth rate with creep stress and temperature. Δd is the change in lath width from the initial value d 0 , and Δd s is the difference between d s and d 0 . Δd/Δd s is uniquely related to creep strain ε and the relationship is independent of creep stress as well as creep temperature. This Δd/Δd s -ε relationship obtained by an accelerated creep test at a higher temperature or stress is applicable to any creep condition including service conditions of engineering plants. Creep strain can be evaluated from the measurement of Δd/Δd s based on the Δd/Δd s -ε relationship. A creep curve under any creep condition can readily be calculated by creep data of the steel. Combining these information one can assess residual life of a structural component made of the steel. (author)
Creep damage behaviour of modified 9Cr-1Mo steel weld joints
International Nuclear Information System (INIS)
Sakthivel, T.; Laha, K.; Vasudevan, M.; Panneer Selvi, S.
2016-01-01
Creep deformation and rupture behaviour of modified 9Cr-1Mo steel weld joints fabricated by single-pass activated TIG (A-TIG) and shielded metal arc welding (SMAW) processes have been investigated at 923 K over a stress range of 50 to 110 MPa after post weld heat treatment (PWHT). The weld joints exhibited significantly lower creep rupture lives than the base metal at lower applied stresses. Creep rupture location of the weld joints were found to occur in the ICHAZ. An extensive localized creep deformation, coarsening of M 23 C 6 precipitates in the ICHAZ with creep exposure led to the premature type IV failure of the joints. The coarsening of M 23 C 6 precipitates was extensive in the mid-section of the ICHAZ than the sub-surface of the joints, and was more predominant in the SMAW joint. While A-TIG weld joint exhibited reduced creep cavitation and coarsening of M 23 C 6 precipitates due to lower deformation constraints by adjacent regions in the ICHAZ. Hence, A-TIG weld joint exhibited higher creep rupture life than the SMAW joint. (author)
Multiaxial creep-fatigue rules
International Nuclear Information System (INIS)
Spindler, M.W.; Hales, R.; Ainsworth, R.A.
1997-01-01
Within the UK, a comprehensive procedure, called R5, is used to assess the high temperature response of structures. One part of R5 deals with creep-fatigue initiation, and in this paper we describe developments in this part of R5 to cover multiaxial stress states. To assess creep-fatigue, damage is written as the linear sum of fatigue and creep components. Fatigue is assessed using Miner's law with the total endurance split into initiation and growth cycles. Initiation is assessed by entering the curve of initiation cycles vs strain range using a Tresca equivalent strain range. Growth is assessed by entering the curve of growth cycles vs strain range using a Rankine equivalent strain range. The number of allowable cycles is obtained by summing the initiation and growth cycles. In this way the problem of defining an equivalent strain range applicable over a range of endurance is avoided. Creep damage is calculated using ductility exhaustion methods. In this paper we address two aspects; first, the nature of stress relaxation and, hence, accumulated creep strain in multiaxial stress fields; secondly, the effect of multiaxial stress on creep ductility. The effect of multiaxial stress state on creep ductility has been examined using experimental data and mechanistic models. Good agreement is demonstrated between an empirical description of test data and a cavity growth model, provided a simple nucleation criterion is included. A simple scaling factor is applied to uniaxial creep ductility, defined as a function of stress state. The factor is independent of the cavity growth mechanisms and yields a value of equivalent strain which can be conveniently used in determining creep damage by ductility exhaustion. (author). 14 refs, 4 figs
International Nuclear Information System (INIS)
Fossum, A.F.; Brodsky, N.S.; Chan, K.S.; Munson, D.E.
1992-01-01
Recent concern over the potential for creep induced development of a damaged rock zone adjacent to shafts and rooms at the Waste Isolation Pilot Plant (WIPP) has motivated the formulation of a coupled constitutive description of continuum salt creep and damage. This constitutive model gives time-dependent inelastic flow and pressure-sensitive damage in crystalline solids. Initially the constitutive model was successfully used to simulate multiaxial, i.e. true triaxial, experiments obtained at relatively high, 2.5 to 20 MPa, confining pressures. Predictions of the complete creep curve, including the heretofore unmodeled tertiary creep, were also demonstrated. However, comparisons of model predictions with data were hampered because the bulk of the creep data existing on WIPP salt was intentionally obtained under confining pressures typically greater than 15 MPa, in an attempt to match the underground in situ lithostatic pressure level. It was realized that the high confining pressures suppressed tertiary creep and resulted in better defined steady state creep responses. To address the tertiary creep process directly, a number of creep tests were conducted at lower confining pressures for the explicit purpose of creating dilatant behavior
Fractional order creep model for dam concrete considering degree of hydration
Huang, Yaoying; Xiao, Lei; Bao, Tengfei; Liu, Yu
2018-05-01
Concrete is a material that is an intermediate between an ideal solid and an ideal fluid. The creep of concrete is related not only to the loading age and duration, but also to its temperature and temperature history. Fractional order calculus is a powerful tool for solving physical mechanics modeling problems. Using a software element based on the generalized Kelvin model, a fractional order creep model of concrete considering the loading age and duration is established. Then, the hydration rate of cement is considered in terms of the degree of hydration, and the fractional order creep model of concrete considering the degree of hydration is established. Moreover, uniaxial tensile creep tests of dam concrete under different curing temperatures were conducted, and the results were combined with the creep test data and complex optimization method to optimize the parameters of a new creep model. The results show that the fractional tensile creep model based on hydration degree can better describe the tensile creep properties of concrete, and this model involves fewer parameters than the 8-parameter model.
Creep model of unsaturated sliding zone soils and long-term deformation analysis of landslides
Zou, Liangchao; Wang, Shimei; Zhang, Yeming
2015-04-01
Sliding zone soil is a special soil layer formed in the development of a landslide. Its creep behavior plays a significant role in long-term deformation of landslides. Due to rainfall infiltration and reservoir water level fluctuation, the soils in the slide zone are often in unsaturated state. Therefore, the investigation of creep behaviors of the unsaturated sliding zone soils is of great importance for understanding the mechanism of the long-term deformation of a landslide in reservoir areas. In this study, the full-process creep curves of the unsaturated soils in the sliding zone in different net confining pressure, matric suctions and stress levels were obtained from a large number of laboratory triaxial creep tests. A nonlinear creep model for unsaturated soils and its three-dimensional form was then deduced based on the component model theory and unsaturated soil mechanics. This creep model was validated with laboratory creep data. The results show that this creep model can effectively and accurately describe the nonlinear creep behaviors of the unsaturated sliding zone soils. In order to apply this creep model to predict the long-term deformation process of landslides, a numerical model for simulating the coupled seepage and creep deformation of unsaturated sliding zone soils was developed based on this creep model through the finite element method (FEM). By using this numerical model, we simulated the deformation process of the Shuping landslide located in the Three Gorges reservoir area, under the cycling reservoir water level fluctuation during one year. The simulation results of creep displacement were then compared with the field deformation monitoring data, showing a good agreement in trend. The results show that the creeping deformations of landslides have strong connections with the changes of reservoir water level. The creep model of unsaturated sliding zone soils and the findings obtained by numerical simulations in this study are conducive to
Microtomography and creep modeling of a short fiber reinforced aluminum piston alloy
Energy Technology Data Exchange (ETDEWEB)
Marks, Esteban; Requena, Guillermo; Degischer, Hans-Peter [Institute of Materials Science and Technology, Vienna University of Technology Karlsplatz 13/E308, A-1040 Vienna (Austria); Boller, Elodie [European Synchrotron Radiation Facility, Grenoble (France)
2011-03-15
Interconnectivity between eutectic silicon and short fibers in an AlSi12CuNiMg/Al2O3/15s composite increases with long-term creep exposure time due to diffusion. It is also observed that the stationary creep rate decreases significantly compared to the initial stationary creep rate. Interconnectivity between rigid phases is analyzed and three-dimensional statistical functions are applied to deduce the representative volume elements of the composite in different conditions. Unit cell geometrical models are generated to simulate the stationary creep behavior using the finite element method. (Copyright copyright 2011 WILEY-VCH Verlag GmbH and Co. KGaA, Weinheim)
Energy Technology Data Exchange (ETDEWEB)
Graverend, Jean-Briac le, E-mail: jblgpublications@gmail.com [Texas A& M University, Department of Aerospace Engineering and Materials Science Engineering, TAMU 3141, College Station, TX 77843 (United States); Adrien, Jérome [Université de Lyon, INSA-Lyon, MATEIS CNRS UMR5510, F-69621 Villeurbanne (France); Cormier, Jonathan [Institut Pprime, CNRS-ENSMA-Université de Poitiers, UPR CNRS 3346, Département Physique et Mécanique des Matériaux, ISAE-ENSMA, 1 avenue Clément Ader, BP 40109, F86961 Futuroscope Chasseneuil cedex (France)
2017-05-17
Creep damage by void nucleation and growth limits the lifetime of components subjected to mechanical loads at high temperatures. For the first time, the porosity of a Ni-based single crystal superalloy subjected to high temperature creep tests (T≥1000 °C) is followed by ex-situ X-ray computed tomography. A large experimental campaign consisting of nine temperature/stress conditions is carried out to determine the kinetics of the damage accumulation by voids. It is, indeed, essential to characterize their evolution to create internal variables describing properly the evolution of damage in a Continuum Damage Mechanics framework. Nonetheless, it is pointed out that the increase in the plastic strain rate during the tertiary creep stage is not necessarily related to the increase in the pore volume fraction for the alloy and temperature range explored (1000–1100 °C). Therefore, it seems that the changes in the microstructure, i.e. precipitation coarsening and γ/γ′ topological inversion, and the shearing of the γ′ particles have to be considered further to properly describe the damage evolution. Thus, the Continuum Damage Mechanics theory is undermined and should be replaced by a transformative paradigm taken into consideration microstructural evolutions in order to improve the predictability of further damage models.
Skinfold creep under load of caliper. Linear visco- and poroelastic model simulations.
Nowak, Joanna; Nowak, Bartosz; Kaczmarek, Mariusz
2015-01-01
This paper addresses the diagnostic idea proposed in [11] to measure the parameter called rate of creep of axillary fold of tissue using modified Harpenden skinfold caliper in order to distinguish normal and edematous tissue. Our simulations are intended to help understanding the creep phenomenon and creep rate parameter as a sensitive indicator of edema existence. The parametric analysis shows the tissue behavior under the external load as well as its sensitivity to changes of crucial hydro-mechanical tissue parameters, e.g., permeability or stiffness. The linear viscoelastic and poroelastic models of normal (single phase) and oedematous tissue (twophase: swelled tissue with excess of interstitial fluid) implemented in COMSOL Multiphysics environment are used. Simulations are performed within the range of small strains for a simplified fold geometry, material characterization and boundary conditions. The predicted creep is the result of viscosity (viscoelastic model) or pore fluid displacement (poroelastic model) in tissue. The tissue deformations, interstitial fluid pressure as well as interstitial fluid velocity are discussed in parametric analysis with respect to elasticity modulus, relaxation time or permeability of tissue. The creep rate determined within the models of tissue is compared and referred to the diagnostic idea in [11]. The results obtained from the two linear models of subcutaneous tissue indicate that the form of creep curve and the creep rate are sensitive to material parameters which characterize the tissue. However, the adopted modelling assumptions point to a limited applicability of the creep rate as the discriminant of oedema.
Super long-term creep tests of advanced HP and IP rotor steels
Energy Technology Data Exchange (ETDEWEB)
Tchizhik, A.A. [The Polzunov Central Boiler and Turbine Institute, Department the Fatigue Life of Materials for Power Plans Equipment, St. Petersburg (Russian Federation)
1998-12-31
A creep model has been developed for predicting the long-term creep behavior, in excess of 200,000 h for advanced materials.The new creep theory is based on a continuum microdamage model and is used to calculate the fields of stress and strain and wedge and cavities damage in critical components of steam and gas turbines. The application of this new model increases the reliability and service life of modern turbines. The accuracy of the model to predict long - term creep behavior, creep ductility was verified using the data bank of super long-term creep tests of advanced materials. (orig.) 12 refs.
Super long-term creep tests of advanced HP and IP rotor steels
Energy Technology Data Exchange (ETDEWEB)
Tchizhik, A A [The Polzunov Central Boiler and Turbine Institute, Department the Fatigue Life of Materials for Power Plans Equipment, St. Petersburg (Russian Federation)
1999-12-31
A creep model has been developed for predicting the long-term creep behavior, in excess of 200,000 h for advanced materials.The new creep theory is based on a continuum microdamage model and is used to calculate the fields of stress and strain and wedge and cavities damage in critical components of steam and gas turbines. The application of this new model increases the reliability and service life of modern turbines. The accuracy of the model to predict long - term creep behavior, creep ductility was verified using the data bank of super long-term creep tests of advanced materials. (orig.) 12 refs.
NORA-2, a model for creep deformation and rupture of zircaloy at high temperatures
International Nuclear Information System (INIS)
Raff, S.; Meyder, R.
1983-01-01
A model has been developed to describe Zircaloy cladding behaviour under LOCA and small leak conditions within specified temperature range and strain rates. The deformation model consists of a strain rate equation with two components representing strain rate controlled contributions from different deformation mechanisms. Transition from one mechanism to the other produces the strain rate dependence of the stress exponent of steady state creep. During transient creep the change of creep mechanisms produces a flow softening behaviour which induces unstable creep. Together with a strain hardening model, the strain history can be described for low and high strain values. The influence of oxidation is taken into account by modelling hardening due to solid solution of oxygen, cracking of the brittle oxide and oxygen stabilised α-phase layers, and by an oxidation-induced creep component in steam atmosphere. The rupture criterion is based on a strain fraction rule whose variables are temperature, strain rate or applied stress, and oxygen content. (author)
International Nuclear Information System (INIS)
Dobmann, G.; Kroening, M.; Theiner, W.; Willems, H.; Fiedler, U.
1995-01-01
In recent years, nondestructive testing techniques for materials characterization have been developed in Germany under the sponsorship of the Ministry of Research and Development, as part of the Reactor Safety Research Programme, in order to provide techniques for PSI and ISI that are sensitive and reliable, in particular with respect to the prediction of strength and toughness. As ferritic steels (pressure vessels and pipelines in the primary circuit) are of special interest, R and D was concentrated on micromagnetic techniques which are sensitive to the microstructure and its changes under service and/or repair conditions. In order to characterize microstructural states superimposed by residual stresses in an unambiguous way, numerical modelling was applied using advanced tools of mathematical approximation theory, i.e. multiregression algorithms and neural networks.For the detection of early creep damage in fossil power plant applications, i.e. micropores and their subsequent development to linked pores and microcracks, besides the micromagnetic techniques an ultrasonic technique was also applied and optimized for in situ applications on components such as pipe bends. Whereas the ultrasonic technique is sensitive to pore concentrations as small as about 0.2%, the parameters of the micromagnetic techniques are mainly influenced by temperature- and load-induced microstructural changes occurring in service, dependent on the steel quality. The techniques are applied at two pipe bends (steel grades 14MoV63 and X20CrMoV121) loaded under near practical conditions during seven inspection intervals between 2048h and 21000h to evaluate the progress of damage. (orig.)
A comprising steady-state creep model for the austenitic AISI 316 L(N) steel
International Nuclear Information System (INIS)
Rieth, Michael
2007-01-01
Low-stress creep data of a recently finished special long-term program now allows for much better long-term predictions of the ITER related material 316 L(N) and also enables deformation modeling for a broader stress range. The present work focuses mainly on the set-up of a steady-state creep model with help of well-known rate-equations for different deformation mechanisms. In addition, the impact of microstructure changes and precipitation formation on steady-state creep is studied. The resulting creep model consists of a summation of contributions for diffusion creep, power-law creep, and power-law breakdown. The final creep model agrees well with experimental data for temperatures between 550 and 750 deg C and for shear stresses above 30 MPa. The most important finding of this work is that for very low stresses the model predicts far higher creep rates than can be extrapolated from tests performed at the usual stress range of experimental programs
Creep-fatigue-environment interaction of 9Cr-1Mo-V-Nb steel
International Nuclear Information System (INIS)
Shibata, Hiroyuki; Ishikawa, Akiyoshi; Asada, Yasuhide
1996-01-01
An extension of the creep-fatigue damage model has been conducted in the present study. The original damage model has been developed to the predict the creep-fatigue life of 9Cr-1Mo-V-Nb steel (Modified 9Cr-1Mo steel) in a very high vacuum environment. The present study is to extend an applicability of the model to the creep-fatigue damage accumulation in the air environment. (orig.)
International Nuclear Information System (INIS)
Wareing, J.; Bretherton, I.
This paper presents preliminary results from the programme for hold period tests on a cast BQ of type 316 stainless steel at 570 deg. C. The results of tensile hold period tests on a relatively low ductility cast of type 316 stainless steel have indicated that the failure mechanism changes from a creep-fatigue interaction failure to a creep dominated failure at low strain levels. An assessment of the linear damage summation approach for failure prediction indicates that it is inappropriate for creep-fatigue interaction failures. For creep dominated fracture, failure occurs when the accumulation relaxation strain exhausts the material ductility i.e. Nsub(f epsilon R)=D. The failure criterion based on a creep summation in terms of time to fracture underestimates life
Hysteresis and creep: Comparison between a power-law model and Kuhnen's model
Energy Technology Data Exchange (ETDEWEB)
Oliveri, Alberto; Stellino, Flavio; Parodi, Mauro; Storace, Marco, E-mail: marco.storace@unige.it
2016-04-01
In this paper we analyze some properties of a recently proposed model of hysteresis and creep (related to a circuit model, whose only nonlinear element is based on a power law) and compare it with the well-known Kuhnen's model. A first qualitative comparison relies on the analysis of the behavior of the elementary cell of each model. Their responses to step inputs (which allow to better evidence the creep effect) are analyzed and compared. Then, a quantitative comparison is proposed, based on the fitting performances of the two models on experimental data measured from a commercial piezoelectric actuator.
Physical hydrodynamic propulsion model study on creeping viscous
Indian Academy of Sciences (India)
The present investigation focusses on a mathematical study of creeping viscous flow induced by metachronal wave propagation in a horizontal ciliated tube containing porous media. Creeping flow limitations are imposed, i.e. inertial forces are small compared to viscous forces and therefore a very low Reynolds number (Re ...
International Nuclear Information System (INIS)
Nakacho, Keiji; Yamazaki, Masayoshi
2001-01-01
The information of the creep behavior of the thick welded joint is very important to secure the safety of the elevated temperature vessels like the nuclear reactors. The creep behavior of the thick welded point is very complex, thence it is difficult to practice the experiment or the theoretical analysis. A simple accurate model for theoretical analysis was developed in the first study. The simple model is constructed of several one-dimensional finite elements which can analyze three-dimensional creep behavior under a assumption. The model is easy to treat, and needs only a little labor and computation time to simulate the creep curve and local strain of the thick welded joint. In this second study, the capability of the model is expanded to estimate the creep life of the thick welded joint. New model can easily estimate the time of the rupture of the thick welded joint. It is verified comparing the result with the experimental one that the model can accurately predict the creep life. The histories of the local strains to the rupture time may be observed in the simulation by using the model. The information will be useful to improve the creep characteristics of the joints. (author)
Energy Technology Data Exchange (ETDEWEB)
Zhen-Change Liu [Shandong Univ. of Technology, Jinan (China); Abe, Satoshi; Noda, Masahiro [Yushiro Chemical Industry Co. Ltd., Kanagawa (Japan)
1995-08-01
Grinding oils are widely used in precision grinding, such as tool grinding, thread grinding and gear grinding, during which processes grinding burn is the most prevalent damage affecting the integrity of ground surface. This paper discusses the influence of oil viscosity on grinding heat and burn damage in creep-feed-grinding. Experimental results indicated that, under lighter grinding conditions, the effects of oil viscosity was not observed, but under heavy grinding conditions grinding burn occurred when using low viscosity oil. When the viscosity of the oil was increased, grinding heat and burn damage tended to be reduced. As the viscosity was increased to a certain level, grinding burn reduction, by further increasing the viscosity, became less while other problems such as much higher oil pump noise and reduced oil flow occurred. It is clear that a viscosity limit exists for given grinding conditions. 5 refs., 4 figs., 3 tabs.
Energy Technology Data Exchange (ETDEWEB)
Fan, Ya-Nan, E-mail: fanyn12@mails.tsinghua.edu.cn; Shi, Hui-Ji, E-mail: shihj@mail.tsinghua.edu.cn; Qiu, Wen-Hui
2015-09-17
Rafting and creep modeling of single crystal superalloys at high temperatures are important for the safety assessment and life prediction in practice. In this research, a new model has been developed to describe the rafting evolution and incorporated into the Cailletaud single crystal plasticity model to simulate the creep behavior. The driving force of rafting is assumed to be the relaxation of the strain energy, and it is calculated with the local stress state, a superposition of the external and misfit stress tensors. In addition, the isotropic coarsening is introduced by the cube root dependence of the microstructure periodicity on creep time based on Ostwal ripening. Then the influence of rafting on creep deformation is taken into account as the Orowan stress in the single crystal plasticity model. The capability of the proposed model is validated with creep experiments of CMSX-4 at 950 °C and 1050 °C. It is able to predict the rafting direction at complex loading conditions and evaluate the channel width during rafting. For [001] tensile creep tests, good agreement has been shown between the model predictions and experimental results at different temperatures and stress levels. The creep acceleration can be captured with this model and is attributed to the microstructure degradation caused by the precipitate coarsening.
Yankovskii, A. P.
2015-05-01
An indirect verification of a structural model describing the creep of a composite medium reinforced by honeycombs and made of nonlinear hereditary phase materials obeying the Rabotnov theory of creep is presented. It is shown that the structural model proposed is trustworthy and can be used in practical calculations. For different kinds of loading, creep curves for a honeycomb core made of a D16T aluminum alloy are calculated.
Creep curve modeling of hastelloy-X alloy by using the theta projection method
International Nuclear Information System (INIS)
Woo Gon, Kim; Woo-Seog, Ryu; Jong-Hwa, Chang; Song-Nan, Yin
2007-01-01
To model the creep curves of the Hastelloy-X alloy which is being considered as a candidate material for the VHTR (Very High Temperature gas-cooled Reactor) components, full creep curves were obtained by constant-load creep tests for different stress levels at 950 C degrees. Using the experimental creep data, the creep curves were modeled by applying the Theta projection method. A number of computing processes of a nonlinear least square fitting (NLSF) analysis was carried out to establish the suitably of the four Theta parameters. The results showed that the Θ 1 and Θ 2 parameters could not be optimized well with a large error during the fitting of the full creep curves. On the other hand, the Θ 3 and Θ 4 parameters were optimized well without an error. For this result, to find a suitable cutoff strain criterion, the NLSF analysis was performed with various cutoff strains for all the creep curves. An optimum cutoff strain range for defining the four Theta parameters accurately was found to be a 3% cutoff strain. At the 3% cutoff strain, the predicted curves coincided well with the experimental ones. The variation of the four Theta parameters as the function of a stress showed a good linearity, and the creep curves were modeled well for the low stress levels. Predicted minimum creep rate showed a good agreement with the experimental data. Also, for a design usage of the Hastelloy-X alloy, the plot of the log stress versus log the time to a 1% strain was predicted, and the creep rate curves with time and a cutoff strain at 950 C degrees were constructed numerically for a wide rang of stresses by using the Theta projection method. (authors)
International Nuclear Information System (INIS)
Sawada, Kota; Maruyama, Kouichi; Komine, Ryuji; Nagae, Yuji
1997-03-01
Several microstructural changes take place in a material during the course of creep. These changes can be a measure of creep life consumption. In this paper, microstructural changes in Mod.9Cr-1Mo steel were studied in order to examine their ability as the measure of creep life consumption. Macroscopic structural changes, such as void growth, rotation of lath structure toward the tensile axis and elongation of grains, are evident only in the necked portion of ruptured specimens. These macroscopic structural changes are not useful for creep life assessment. Lath width increases and dislocation density within lath decreases with increasing creep duration. These changes in dislocation substructure start in the early stage of creep life, and cause the increase of strain rate in the tertiary creep stage. The lath width and the dislocation density reach a stationary value before rupture. The stationary values are independent of temperature, and uniquely related to creep stress normalized by shear modulus. The extent of these microstructural changes are greater at lower stresses under which the material is practically used. These facts suggest that the lath width and the dislocation density within lath can be a useful measure of creep life consumption. Hardness of crept specimens is closely related to the lath width and the dislocation density within lath. The changes of these microstructural features can be evaluated by the measurement of hardness. (author)
Recent Advances in Creep Modelling of the Nickel Base Superalloy, Alloy 720Li.
Harrison, William; Whittaker, Mark; Williams, Steve
2013-03-20
Recent work in the creep field has indicated that the traditional methodologies involving power law equations are not sufficient to describe wide ranging creep behaviour. More recent approaches such as the Wilshire equations however, have shown promise in a wide range of materials, particularly in extrapolation of short term results to long term predictions. In the aerospace industry however, long term creep behaviour is not critical and more focus is required on the prediction of times to specific creep strains. The current paper illustrates the capability of the Wilshire equations to recreate full creep curves in a modern nickel superalloy. Furthermore, a finite-element model based on this method has been shown to accurately predict stress relaxation behaviour allowing more accurate component lifing.
Modeling basic creep in concrete at early-age under compressive and tensile loading
Energy Technology Data Exchange (ETDEWEB)
Hilaire, Adrien, E-mail: adrien.hilaire@ens-cachan.fr [ENS Cachan/CNRS UMR8535/UPMC/PRES UniverSud Paris, Cachan (France); Benboudjema, Farid; Darquennes, Aveline; Berthaud, Yves [ENS Cachan/CNRS UMR8535/UPMC/PRES UniverSud Paris, Cachan (France); Nahas, Georges [ENS Cachan/CNRS UMR8535/UPMC/PRES UniverSud Paris, Cachan (France); Institut de radioprotection et de sureté nucléaire, Fontenay-aux-Roses (France)
2014-04-01
A numerical model has been developed to predict early age cracking for massive concrete structures, and especially concrete nuclear containment vessels. Major phenomena are included: hydration, heat diffusion, autogenous and thermal shrinkage, creep and cracking. Since studied structures are massive, drying is not taken into account. Such modeling requires the identification of several material parameters. Literature data is used to validate the basic creep model. A massive wall, representative of a concrete nuclear containment, is simulated; predicted cracking is consistent with observation and is found highly sensitive to the creep phenomenon.
Failure Mechanisms and Damage Model of Ductile Cast Iron Under Low-Cycle Fatigue Conditions
Wu, Xijia; Quan, Guangchun; MacNeil, Ryan; Zhang, Zhong; Sloss, Clayton
2014-10-01
Strain-controlled low-cycle fatigue (LCF) tests were conducted on ductile cast iron (DCI) at strain rates of 0.02, 0.002, and 0.0002/s in the temperature range from room temperature to 1073 K (800 °C). A constitutive-damage model was developed within the integrated creep-fatigue theory (ICFT) framework on the premise of strain decomposition into rate-independent plasticity and time-dependent creep. Four major damage mechanisms: (i) plasticity-induced fatigue, (ii) intergranular embrittlement (IE), (iii) creep, and (iv) oxidation were considered in a nonlinear creep-fatigue interaction model which represents the overall damage accumulation process consisting of oxidation-assisted fatigue crack nucleation and propagation in coalescence with internally distributed damage ( e.g., IE and creep), leading to final fracture. The model was found to agree with the experimental observations of the complex DCI-LCF phenomena, for which the linear damage summation rule would fail.
Jouiad, Mustapha
2012-01-01
An unprecedented investigation consisting of the association of X-Ray tomography and Scanning Electron Microscopy combined with Focus Ion Beam (SEM-FIB) is conducted to perform a 3D reconstruction imaging. These techniques are applied to study the non-isothermal creep behavior of close (111) oriented samples of MC2 nickel base superalloys single crystal. The issue here is to develop a strategy to come out with the 3D rafting of γ\\' particles and its interaction whether with dislocation structures or/and with the preexisting voids. This characterization is uncommonly performed away from the conventional studied orientation [001] in order to feed the viscoplastic modeling leading to its improvement by taking into account the crystal anisotropy. The creep tests were performed at two different conditions: classical isothermal tests at 1050°C under 140 MPa and a non isothermal creep test consisting of one overheating at 1200°C and 30 seconds dwell time during the isothermal creep life. The X-Ray tomography shows a great deformation heterogeneity that is pronounced for the non-isothermal tested samples. This deformation localization seems to be linked to the preexisting voids. Nevertheless, for both tested samples, the voids coalescence is the precursor of the observed damage leading to failure. SEM-FIB investigation by means of slice and view technique gives 3D views of the rafted γ\\' particles and shows that γ corridors evolution seems to be the main creep rate controlling parameter. © 2012 Trans Tech Publications, Switzerland.
International Nuclear Information System (INIS)
Nakacho, Keiji; Ueda, Yukio; Kinugawa, Junichi; Yamazaki, Masayoshi
1997-01-01
Reliable predictions of the creep behavior of thick welded joints are very important to secure the safety of elevated temperature vessels like nuclear reactors. Creep behavior is very complex, thus it is difficult to perform the experiment and conduct the theoretical analysis. A simple accurate model for theoretical analysis was developed in the first report. The simple model is constructed of seven one-dimensional finite elements which can analyze not only one-dimensional stress creep behavior but also the three-dimensional situation. The simple model is verified by comparing the analyzed results with the experimental ones in this report. The model is easy to treat, and needs only a little labor and computation time to predict the creep curve and the local strain for a thick welded joint. (author)
Elevated temperature creep and fatigue damage of a 2.25 Cr--1 Mo steel weldment
International Nuclear Information System (INIS)
Van Den Avyle, J.A.
1978-01-01
In weldments between dissimilar metals wide variations occur in metallurgical structure and mechanical properties, so that for good structural design it is necessary to understand the mechanical response of individual microstructural segments of the weld. This study investigates elevated temperature properties of a 2.25 Cr--1 Mo ferritic steel base metal welded with Chromenar 382V (Inconel 82) filler metal. Creep and low-cycle fatigue tests at 866 0 K (1100 0 F) show the filler metal and heat affected zone to be much stronger than the base metal. Optical microscopy does not show significant aging effects in the short-term fatigue tests or creep tests of 1180 hour duration
Analysis of structures based on a characteristic-strain model of creep
Energy Technology Data Exchange (ETDEWEB)
Bolton, J. [Alstom Power, Newbold Road, Rugby CV21 2NH (United Kingdom)], E-mail: janjohn.bolton@virgin.net
2008-01-15
A companion paper [Bolton J. In: A characteristic-strain model for creep, ECCC/I.Mech.E. conference on creep and fracture in high-temperature components, London, September 2005] describes a creep model based on a constant 'characteristic strain' at any temperature. The present paper discusses the application of such a model, first to simple structures and then to engineering components of general form under steady loading. A basis is proposed for identifying the stress within a structure, or within the critical part of a structure, which can be considered to govern both its overall and local deformations. The concept is similar to skeletal-point stress but is more readily applied to components of any shape. The implementation of the concept of 'structural stress' is discussed in the context of finite-element creep calculations. Consideration is given to the analysis of cracked structures, where very high strains at the crack tip must be accommodated.
Analysis of structures based on a characteristic-strain model of creep
International Nuclear Information System (INIS)
Bolton, J.
2008-01-01
A companion paper [Bolton J. In: A characteristic-strain model for creep, ECCC/I.Mech.E. conference on creep and fracture in high-temperature components, London, September 2005] describes a creep model based on a constant 'characteristic strain' at any temperature. The present paper discusses the application of such a model, first to simple structures and then to engineering components of general form under steady loading. A basis is proposed for identifying the stress within a structure, or within the critical part of a structure, which can be considered to govern both its overall and local deformations. The concept is similar to skeletal-point stress but is more readily applied to components of any shape. The implementation of the concept of 'structural stress' is discussed in the context of finite-element creep calculations. Consideration is given to the analysis of cracked structures, where very high strains at the crack tip must be accommodated
Energy Technology Data Exchange (ETDEWEB)
Hu, Dianyin [School of Energy and Power Engineering, Beihang University, Beijing 100191 (China); Collaborative Innovation Center of Advanced Aero-Engine, Beijing 100191 (China); Beijing Key Laboratory of Aero-Engine Structure and Strength, Beijing 100191 (China); Ma, Qihang [School of Energy and Power Engineering, Beihang University, Beijing 100191 (China); Shang, Lihong [Mining and Materials Engineering, McGill University, Montreal, QC H3A 0C5 (Canada); Gao, Ye [School of Energy and Power Engineering, Beihang University, Beijing 100191 (China); Wang, Rongqiao, E-mail: wangrq@buaa.edu.cn [School of Energy and Power Engineering, Beihang University, Beijing 100191 (China); Collaborative Innovation Center of Advanced Aero-Engine, Beijing 100191 (China); Beijing Key Laboratory of Aero-Engine Structure and Strength, Beijing 100191 (China)
2016-07-18
Creep-fatigue experiments have been conducted in nickel-based superalloy GH720Li at an elevated temperature of 650 °C with a stress ratio of 0.1, based on which, different dwell times at the maximum loading were applied to investigate the effect of dwell time on the creep-fatigue behaviors. The tested specimens were cut from the rim region of an actual turbine disc in the hoop direction. The grain size and precipitates of the GH720Li superalloy were examined through scanning electronic microscope (SEM) and energy-dispersive X-ray spectroscopy (EDS) analyses. Experimental data shows creep-fatigue lifetime decreases as the dwell time prolongs. Further, different scattering was observed in the creep-fatigue lifetime at different dwell times. Then a probabilistic model based on the applied mechanical work density (AMWD), with a linear heteroscedastic function that evaluates the non-constant deviation in the creep-fatigue lifetime, was formulated to describe the dependence of creep-fatigue lifetime on the dwell time. Finally, the possible microscopic mechanism of the creep-fatigue behavior has been discussed by SEM with EDS on the fracture surfaces.
A nonlinear finite element model of a piezoelectric tube actuator with hysteresis and creep
International Nuclear Information System (INIS)
Chung, S H; Fung, Eric H K
2010-01-01
Piezoelectric tube actuators are commonly used for nanopositioning in atomic force microscopes (AFMs). However, piezoelectric tube actuators exhibit hysteresis and creep which significantly limit the accuracy of nanopositioning. A finite element model of a piezoelectric tube actuator with hysteresis and creep is important for control purposes, but so far one has not been developed. The purpose of this paper is to present a nonlinear finite element (FE) model with hysteresis and creep for design purposes. Prandtl–Ishlinskii (PI) hysteresis operators and creep operators are adopted into constitutive equations. The nonlinear FE model is formulated using energy approach and Hamilton's principle. The parameters of the PI hysteresis operators and the creep operators are identified by comparing the simulation results and experimental results of other researchers. The working operation of the piezoelectric tube actuator is simulated by the reduced order FE model, and the displacement error due to hysteresis, creep and coupling effect is investigated. An output feedback controller is implemented into the reduced order FE model to show that this model is controllable
International Nuclear Information System (INIS)
Nakasone, Yuji; Tanabe, Tatsuhiko; Tsuji, Hirokazu; Nakajima, Hajime.
1992-01-01
The present paper investigates early-stage-creep damage of Hastelloy XR and XR-II alloys, modified versions of Hastelloy X alloy, which have been developed in Japan as most promising candidate structural alloys for Japanese high-temperature gas-cooled reactors (HTGRs). Creep tests were made on Hastelloy XR forging, tube and XR-II tube at 1,123 to 1,273 K in a simulated HTGR helium gas environment. The tests were interrupted at different strain levels of up to 5 % in order to evaluate creep damage via intergranular voids. The void sizes along grain boundaries and the A-parameter, the ratio of the number of damaged grain boundaries, on which one or more voids are found, to that of the total grain boundaries observed are used in order to evaluate creep damage. Statistical analysis of the A-parameter as well as the void sizes reveals that the values of the parameter show wide variations and follow the Weibull distribution, reflecting spatial randomness of the voids. The void sizes along grain boundaries, on the other hand, follow the log-normal distribution. The maximum void size d max and the mean value of the A-parameter A m are calculated and plotted against interruption creep strain ε int . The resultant d max vs. ε int and A m vs. ε int diagrams show that Hastelloy XR forging had suffered more damage than Hastelloy XR tube; nevertheless, the forging has longer interruption life, or the time to reach a given interruption creep strain. The result indicates that grains may have been deformed more easily in Hastelloy XR in the form of tube than in the form of forging. The diagrams also imply that the addition of boron has suppressed the nucleation as well as the growth of voids and thus has brought about longer interruption life of Hastelloy XR-II. (author)
Energy Technology Data Exchange (ETDEWEB)
Gariboldi, Elisabetta, E-mail: elisabetta.gariboldi@polimi.it [Politecnico di Milano, Department of Mechanical Engineering, Via La Masa 34 20156 Milano (Italy); Naumenko, Konstantin, E-mail: konstantin.naumenko@ovgu.de [Otto-von-Guericke-University Magdeburg, Institute of Mechanics, D-39106 Magdeburg (Germany); Ozhoga-Maslovskaja, Oksana, E-mail: oksana.ozhogamaslovskaja@gmail.com [Politecnico di Milano, Department of Mechanical Engineering, Via La Masa 34 20156 Milano (Italy); Zappa, Emanuele, E-mail: emanuele.zappa@polimi.it [Politecnico di Milano, Department of Mechanical Engineering, Via La Masa 34 20156 Milano (Italy)
2016-01-15
The aim of this paper is to analyze anisotropic damage mechanisms in forged Al–Cu–Mg–Si alloy based on the results of creep tests. Smooth specimens are sampled in three forging directions. Creep strain vs. time curves as well as light optical microscope and scanning electron microscope observations illustrate basic features of damage growth. Flat notch specimens are sampled in different directions to analyze stress redistributions and damage in zones of stress concentration. The digital image correlation technique has been applied in situ in order to extract the strain values on the surface of the notched specimens. All observations demonstrate that the principal origins of anisotropic creep and damage are associated with elongated grains and second phase clustered particles located at grain boundaries. Longitudinal specimens possess nucleations of decohesion sites and growth of voids around second phase particles at grain boundaries. Damage evolution for radial and transverse specimens is due to the formation and growth of cracks in second phase particles orthogonal to the principal stress axis. Residual strains are confined to the notch root as well as to the flanges of advanced macrocrack, indicating the small scale yielding during the creep fracture process.
Creep force modelling for rail traction vehicles based on the Fastsim algorithm
Spiryagin, Maksym; Polach, Oldrich; Cole, Colin
2013-11-01
The evaluation of creep forces is a complex task and their calculation is a time-consuming process for multibody simulation (MBS). A methodology of creep forces modelling at large traction creepages has been proposed by Polach [Creep forces in simulations of traction vehicles running on adhesion limit. Wear. 2005;258:992-1000; Influence of locomotive tractive effort on the forces between wheel and rail. Veh Syst Dyn. 2001(Suppl);35:7-22] adapting his previously published algorithm [Polach O. A fast wheel-rail forces calculation computer code. Veh Syst Dyn. 1999(Suppl);33:728-739]. The most common method for creep force modelling used by software packages for MBS of running dynamics is the Fastsim algorithm by Kalker [A fast algorithm for the simplified theory of rolling contact. Veh Syst Dyn. 1982;11:1-13]. However, the Fastsim code has some limitations which do not allow modelling the creep force - creep characteristic in agreement with measurements for locomotives and other high-power traction vehicles, mainly for large traction creep at low-adhesion conditions. This paper describes a newly developed methodology based on a variable contact flexibility increasing with the ratio of the slip area to the area of adhesion. This variable contact flexibility is introduced in a modification of Kalker's code Fastsim by replacing the constant Kalker's reduction factor, widely used in MBS, by a variable reduction factor together with a slip-velocity-dependent friction coefficient decreasing with increasing global creepage. The proposed methodology is presented in this work and compared with measurements for different locomotives. The modification allows use of the well recognised Fastsim code for simulation of creep forces at large creepages in agreement with measurements without modifying the proven modelling methodology at small creepages.
Energy Technology Data Exchange (ETDEWEB)
Storesund, Jan; Borggreen, Kjeld; Weilin Zang; Nilsson, Henrik; Samuelson, Aake
2004-09-01
The present project has been consisted of the following pieces of work on welds of X20 CrMoV 12 1: Analysis of, by use of replica testing, creep damage development in 368 welds in 11 Danish high pressure steam lines with operation up to 200,000 h. Metallographic investigations of four welds from a retired live steam line with approximately 182 000 h in operation. - Evaluation of the influence of the two most common etching methods on the interpretation of creep cavitation. Analysis of the time security of the material, i.e. influence of enhanced temperature or stress on creep life time. Finite element simulations of the creep behaviour of X20 welds where effects of HAZ creep properties, system stresses and degree of multiaxiality in the rupture criterion are studied. In addition a literature study on publications of creep life time in X20 steel was performed in a first, already reported part of the project. The results of the comprehensive replica testing and the metallographic investigations show clear-cut that welds of this material have an excellently long creep life that indeed will reach 200,000 h. The creep damage at that time is in general very limited. The typical creep life for welds of X20 can be evaluated to at least 250,000 h. The reason for that it is not possible to evaluate an even longer creep life is the fact that creep testing and finite element simulations show that creep elongation and creep damage will accelerate considerably later in the creep life than some low alloy steels. In the worst case this acceleration could start already just after 200,000 h. It is also demonstrated that welds of the X20 steel can stand system stresses much better than low alloy steels. Recommendations for how and when inspections and testing of welds of the current material should be performed have been issued. They have been adapted to the findings in the project. The recommendations can, as long as severe damage is absent, allow for longer inspection intervals
Numerical modeling of the creep behavior of clays with emphasis on tunnels and underground openings
International Nuclear Information System (INIS)
1990-02-01
This report presents an interpretive overview and critical assessment of the state-of-the-art for numerical modeling of the creep behavior of clays. The overview and assessment is focused upon application to underground openings. Field and laboratory observations of time-dependent behavior, constitutive modeling of creep behavior, and numerical implementation of constitutive equations are addressed. A critical assessment of the ability of existing models to predict aspects of creep behavior relevant to waste repository design and suggestions for improved analyses that can be developed with existing technology are provided. Both heuristic and mathematical constitutive models are reviewed. Heuristic models provide a basis for evaluation of the required parameters for the continuum mechanics based mathematical models. The continuum mechanics models are required for numerical analysis. It has been demonstrated that, by using iterative and incremental analysis, virtually any viscous or inviscid continuum mechanics material model can be adapted to consider time-dependent behavior. Available numerical models for numerical analysis of geotechnical problems involving creep deformations are reviewed. Models for thermo-mechanical coupling are also addressed in this review. Cases where creep-inclusive analyses have been applied to analysis of prototype behavior are cited. However, the lack of well documented case histories of time-dependent deformations over significant time spans is identified as a major obstacle to model verification. Recommendations are made for an alternative design approach capable of guaranteeing the very long term mechanical integrity of the liner. 167 refs., 22 figs., 6 tabs
Finite element modelling of the creep deformation of T91 steel weldments at 600 C
Energy Technology Data Exchange (ETDEWEB)
Bhadrui, A.K. [Indira Gandhi Centre for Atomic Research, Kalpakkam (India); Gaudig, W. [Stuttgart Univ. (Germany). Staatliche Materialpruefungsanstalt; Theofel, H. [Stuttgart Univ. (Germany). Staatliche Materialpruefungsanstalt; Maile, K. [Stuttgart Univ. (Germany). Staatliche Materialpruefungsanstalt
1996-05-01
Finite element modelling of the creep deformation of T91 steel weldments, welded using the manual metal arc (MMA) and submerged arc (SA) welding processes, was carried out to predict creep curves for both of the weldments under different stresses and compared with the experimental data. The stress and strain redistribution across the length of the transverse-weld specimens has also been predicted. Data of creep tests at 600 C at stresses between 90-130 MPa for the base metal, the MMA and SA weld metals, and the simulated heat-affected zone were used to determine Garofalo`s equation for creep strain. Finite element meshes for both of the weldments were constructed after calculating the HAZ locations using Rosenthal`s heat flow equation. (orig.)
International Nuclear Information System (INIS)
Poirier, J.-P.
1988-01-01
Creep mechanisms for metals, ceramics and rocks, effect of pressure and temperature on deformation processes are considered. The role of crystal defects is analysed, different models of creep are described. Deformation mechanisms maps for different materials are presented
Multivariate pluvial flood damage models
International Nuclear Information System (INIS)
Van Ootegem, Luc; Verhofstadt, Elsy; Van Herck, Kristine; Creten, Tom
2015-01-01
Depth–damage-functions, relating the monetary flood damage to the depth of the inundation, are commonly used in the case of fluvial floods (floods caused by a river overflowing). We construct four multivariate damage models for pluvial floods (caused by extreme rainfall) by differentiating on the one hand between ground floor floods and basement floods and on the other hand between damage to residential buildings and damage to housing contents. We do not only take into account the effect of flood-depth on damage, but also incorporate the effects of non-hazard indicators (building characteristics, behavioural indicators and socio-economic variables). By using a Tobit-estimation technique on identified victims of pluvial floods in Flanders (Belgium), we take into account the effect of cases of reported zero damage. Our results show that the flood depth is an important predictor of damage, but with a diverging impact between ground floor floods and basement floods. Also non-hazard indicators are important. For example being aware of the risk just before the water enters the building reduces content damage considerably, underlining the importance of warning systems and policy in this case of pluvial floods. - Highlights: • Prediction of damage of pluvial floods using also non-hazard information • We include ‘no damage cases’ using a Tobit model. • The damage of flood depth is stronger for ground floor than for basement floods. • Non-hazard indicators are especially important for content damage. • Potential gain of policies that increase awareness of flood risks
Multivariate pluvial flood damage models
Energy Technology Data Exchange (ETDEWEB)
Van Ootegem, Luc [HIVA — University of Louvain (Belgium); SHERPPA — Ghent University (Belgium); Verhofstadt, Elsy [SHERPPA — Ghent University (Belgium); Van Herck, Kristine; Creten, Tom [HIVA — University of Louvain (Belgium)
2015-09-15
Depth–damage-functions, relating the monetary flood damage to the depth of the inundation, are commonly used in the case of fluvial floods (floods caused by a river overflowing). We construct four multivariate damage models for pluvial floods (caused by extreme rainfall) by differentiating on the one hand between ground floor floods and basement floods and on the other hand between damage to residential buildings and damage to housing contents. We do not only take into account the effect of flood-depth on damage, but also incorporate the effects of non-hazard indicators (building characteristics, behavioural indicators and socio-economic variables). By using a Tobit-estimation technique on identified victims of pluvial floods in Flanders (Belgium), we take into account the effect of cases of reported zero damage. Our results show that the flood depth is an important predictor of damage, but with a diverging impact between ground floor floods and basement floods. Also non-hazard indicators are important. For example being aware of the risk just before the water enters the building reduces content damage considerably, underlining the importance of warning systems and policy in this case of pluvial floods. - Highlights: • Prediction of damage of pluvial floods using also non-hazard information • We include ‘no damage cases’ using a Tobit model. • The damage of flood depth is stronger for ground floor than for basement floods. • Non-hazard indicators are especially important for content damage. • Potential gain of policies that increase awareness of flood risks.
ESTIMATION MODEL OF RESIDUAL LIFE-TIME OF LOCOMOTIVE FRAME BOGIE WITH ALLOWANCE FOR CREEP
Directory of Open Access Journals (Sweden)
V. R. Skalskyi
2014-12-01
Full Text Available Purpose. The problem of determining the residual life of frame bogie elements of locomotives is a great importance for predicting their work safely and avoidance potential failures on the track. This especially concern cases when such elements have creep-fatigue cracks which grow under action of cyclic loading with excerpts T1 in the cycle and reach their critical size. Here the question of the propagation of such defects (cracks arises, their kinetics and about the period of subcritical cracks growth. The aim is to develop a calculation model for determination the period of subcritical creep-fatigue cracks growth in the bogies frames of electric locomotive. The model takes into account the basic parameters of load, geometry of the construction element and cracks. Methodology. The calculation model for determination the period of subcritical creep-fatigue cracks growth in structural elements of frame under conditions of variable load time has been formulated. It is based on the first law of thermodynamics concerning to mechanics of solids slow fracture at low temperature creep and variable loadings. It is assumed that the period of unsteady creep dominates here (the first section of the creep curve. Low-temperature creep is creep of materials at temperatures T0 < 0,5Tmp, where Tmp − the melting point of the material. Findings. The analytical formula for the determination of the stress intensity factor of truck bolster with technological hole has been obtained. It is shown that by experimentally established constants of the material using the proposed analytical relations can easily determine residual resource of the bogie frame elements. Originality. The new mathematical model for describing the kinetics of creep-fatigue cracks growth in the frames bogies of electric locomotive under variable in time loadings with various time excerpts and on this base the period determination of subcritical crack growth has been proposed. Practical value
Computational models for residual creep life prediction of power plant components
International Nuclear Information System (INIS)
Grewal, G.S.; Singh, A.K.; Ramamoortry, M.
2006-01-01
All high temperature - high pressure power plant components are prone to irreversible visco-plastic deformation by the phenomenon of creep. The steady state creep response as well as the total creep life of a material is related to the operational component temperature through, respectively, the exponential and inverse exponential relationships. Minor increases in the component temperature can thus have serious consequences as far as the creep life and dimensional stability of a plant component are concerned. In high temperature steam tubing in power plants, one mechanism by which a significant temperature rise can occur is by the growth of a thermally insulating oxide film on its steam side surface. In the present paper, an elegantly simple and computationally efficient technique is presented for predicting the residual creep life of steel components subjected to continual steam side oxide film growth. Similarly, fabrication of high temperature power plant components involves extensive use of welding as the fabrication process of choice. Naturally, issues related to the creep life of weldments have to be seriously addressed for safe and continual operation of the welded plant component. Unfortunately, a typical weldment in an engineering structure is a zone of complex microstructural gradation comprising of a number of distinct sub-zones with distinct meso-scale and micro-scale morphology of the phases and (even) chemistry and its creep life prediction presents considerable challenges. The present paper presents a stochastic algorithm, which can be' used for developing experimental creep-cavitation intensity versus residual life correlations for welded structures. Apart from estimates of the residual life in a mean field sense, the model can be used for predicting the reliability of the plant component in a rigorous probabilistic setting. (author)
Critical review of creep FRAPCON-3 model under dry storage conditions
Energy Technology Data Exchange (ETDEWEB)
Feria, F.; Herranz, L.E. [Unit of Nuclear Safety Research, CIEMAT, Avda. Complutense 22, Madrid, Madrid 28040 (Spain)
2009-06-15
There is a general agreement that cladding creep rupture is the most likely and limiting failure mechanism of spent fuel in dry storage compared to other potential mechanisms, like stress corrosion cracking and/or delayed hydride cracking. Nevertheless, occurrence of creep rupture is very improbable since both decay heat and hoop stress tend to decrease throughout dry storage. In spite of this, the current trend to higher burn up levels needs further attention that ensures safe storage of spent fuel irradiated over 45 GWd/MTU. An extensive work has been carried out during the last four decades in the area of in-reactor creep modelling. Unfortunately, the in-reactor conditions are so different from those prevailing under dry storage, that all the experience gained cannot be extrapolated in a straightforward manner. On the other side, as creep tests simulating conditions throughout a 20-40 year dry storage are impractical, post-irradiation cladding creep behaviour has been modelled by means of time-temperature dependent laws developed on the basis of currently available zirconium alloys data. Additionally, some tests have been exploring the effect of irradiation, hydrogen distribution and material composition on the materials creep behaviour. Adaptation of fuel performance codes initially developed for normal and off-normal reactor operation is not an easy task either. Creep modelling is usually dependent of host codes because a good part of its validation and update has been carried out in an integral way, and as a consequence its independent performance assessment is not an easy task. This work examines the current capability of FRAPCON-3 to model creep behaviour under dry storage conditions. To do so, a review of its major fundamentals has been done and its range of applicability discussed. Once its main approximations and drawbacks have been identified, an attempt to overcome some of them has been intended by implementing an alternative expression for creep under
Directory of Open Access Journals (Sweden)
Grondin F.
2010-06-01
Full Text Available Creep and damage in concrete govern the long-term deformability of concrete. Thus, it is important to understand the interaction between creep and damage in order to design reliable civil engineering structures subjected to high level loading during a long time. Many investigations have been performed on the influence of concrete mixture, the effect of the bond between the matrix and the aggregates, temperature, aging and the size effect on the cracking mechanism and fracture parameters of concrete. But there is a lack of results on the influence of the creep loading history. In the present paper, an experimental investigation on the fracture properties of concrete beams submitted to three point bending tests with high levels of sustained load that deals with creep is reported. The results aim first to investigate the ranges of variation of the time response due to creep damage coupled effects under constant load and secondly to evaluate the residual capacity after creep. For this purpose a series of tests were carried out on geometrically similar specimens of size 100x200x800mm with notch to depth ratio of 0.2 in all the test specimens. The exchange of moisture was prevented and beams were subjected to a constant load of 70% and 90% of the maximum capacity. Three point bending test were realized on specimen at the age of 28 days to determine the characteristics of concrete and the maximum load so we could load the specimens in creep. Threepoint bend creep tests were performed on frames placed in a climate controlled chamber [1]. Then after four months of loading, the beams subjected to creep were removed from the creep frames and then immediately subjected to three-point bending test loading up to failure with a constant loading rate as per RILEM-FMC 50 recommendations. The residual capacity on the notched beams and the evolution of the characteristics of concrete due to the basic creep was considered. The results show that sustained loading
Saliba, J.; Loukili, A.; Grondin, F.
2010-06-01
Creep and damage in concrete govern the long-term deformability of concrete. Thus, it is important to understand the interaction between creep and damage in order to design reliable civil engineering structures subjected to high level loading during a long time. Many investigations have been performed on the influence of concrete mixture, the effect of the bond between the matrix and the aggregates, temperature, aging and the size effect on the cracking mechanism and fracture parameters of concrete. But there is a lack of results on the influence of the creep loading history. In the present paper, an experimental investigation on the fracture properties of concrete beams submitted to three point bending tests with high levels of sustained load that deals with creep is reported. The results aim first to investigate the ranges of variation of the time response due to creep damage coupled effects under constant load and secondly to evaluate the residual capacity after creep. For this purpose a series of tests were carried out on geometrically similar specimens of size 100x200x800mm with notch to depth ratio of 0.2 in all the test specimens. The exchange of moisture was prevented and beams were subjected to a constant load of 70% and 90% of the maximum capacity. Three point bending test were realized on specimen at the age of 28 days to determine the characteristics of concrete and the maximum load so we could load the specimens in creep. Threepoint bend creep tests were performed on frames placed in a climate controlled chamber [1]. Then after four months of loading, the beams subjected to creep were removed from the creep frames and then immediately subjected to three-point bending test loading up to failure with a constant loading rate as per RILEM-FMC 50 recommendations. The residual capacity on the notched beams and the evolution of the characteristics of concrete due to the basic creep was considered. The results show that sustained loading had a strengthening
Energy Technology Data Exchange (ETDEWEB)
Morrow, B.M., E-mail: morrow@lanl.gov [The Ohio State University, 2041 College Rd., 477 Watts Hall, Columbus, OH 43210 (United States); Los Alamos National Laboratory, P.O. Box 1663, MS G755, Los Alamos, NM 87545 (United States); Kozar, R.W.; Anderson, K.R. [Bettis Laboratory, Bechtel Marine Propulsion Corp., West Mifflin, PA 15122 (United States); Mills, M.J., E-mail: millsmj@mse.osu.edu [The Ohio State University, 2041 College Rd., 477 Watts Hall, Columbus, OH 43210 (United States)
2016-05-17
Several specimens of Zircaloy-4 were creep tested at a single stress-temperature condition, and interrupted at different accumulated strain levels. Substructural observations were performed using bright field scanning transmission electron microscopy (BF STEM). The dislocation substructure was characterized to ascertain how creep strain evolution impacts the Modified Jogged-Screw (MJS) model, which has previously been utilized to predict steady-state strain rates in Zircaloy-4. Special attention was paid to the evolution of individual model parameters with increasing strain. Results of model parameter measurements are reported and discussed, along with possible extensions to the MJS model.
The Creep of Frozen Sands: Qualitative and Quantitative Models.
1981-03-01
values. / Accession For ?PTIS GFRA&l DTIC TAB El Unannounced 0 justificatio B y Di stribution/ Availabilit " Cr4c Dist Unclassified SCCUI CL AS SIF ICA...for his support throughout the project; and Al Tice, for carrying out the NMR unfrozen water content determinations. Also, I thank the undergraduate...Results of Creep Tests on Glass Beads ................. 296 A.4 Results of Unfrozen Water Content Determinations of MS-M Glass Beads
Development of a Zircaloy creep and failure model for LOCA conditions
International Nuclear Information System (INIS)
Raff, S.; Meyder, R.
1981-01-01
The present status of NORA model for zircaloy-4 creep and failure in the high temperature region (from 600 deg C up to 1200 deg C) is described. Temperature dependence, strain hardening and oxygen content are found to be the most important features of the strain rate creep equation. The failure criterion is based on a modified strain fraction rule. Variables of this criterion are temperature, strain rate or applied stress respectively and oxygen content. Concerning the application of the deformation model, deduced from uniaxial tests, to tube deformation calculation the axial ballooning shape has to be taken into account. Its influence on the tube stress components and therefore on strain rate is discussed. A further improvement of the deformation model concerning yield drop and irregular creep behaviour aims at the enlargement of the range of applicability and reduction of the error band of the model
International Nuclear Information System (INIS)
Ribis, J.
2007-12-01
The fuel rod cladding, strongly affected by microstructural changes due to irradiation such as high density of dislocation loops, is strained by the end-of-life fuel rod internal pressure and the potential release of fission gases and helium during dry storage. Within the temperature range that is expected during dry interim storage, cladding undergoes long term creep under over-pressure. So, in order to have a predictive approach of the behavior of zirconium alloys cladding in dry storage conditions it is essential to take into account: initial dislocation loops, thermal annealing of loops and creep straining due to over pressure. Specific experiments and modelling for irradiated samples have been developed to improve our knowledge in that field. A Zr-1%Nb-O alloy was studied using fine microstructural investigations and mechanical testing. The observations conducted by transmission electron microscopy show that the high density of loops disappears during a heat treatment. The loop size becomes higher and higher while their density falls. The microhardness tests reveal that the fall of loop density leads to the softening of the irradiated material. During a creep test, both temperature and applied stress are responsible of the disappearance of loops. The loops could be swept by the activation of the basal slip system while the prism slip system is inhibited. Once deprived of loops, the creep properties of the irradiated materials are closed to the non irradiated state, a result whose consequence is a sudden acceleration of the creep rate. Finally, a micro-mechanical modeling based on microscopic deformation mechanisms taking into account experimental dislocation loop analyses and creep test, was used for a predictive approach by constructing a deformation mechanism map of the creep behavior of the irradiated material. (author)
Influence of friction on stress and strain distributions in small punch creep test models
Czech Academy of Sciences Publication Activity Database
Dymáček, Petr; Seitl, Stanislav; Milička, Karel; Dobeš, Ferdinand
417-418, - (2010), s. 561-564 ISSN 1013-9826. [International Conference on Fracture and Damage Mechanics /8./. Malta, 08.09.2009-10.09.2009] R&D Projects: GA AV ČR(CZ) IAA200410801; GA AV ČR(CZ) 1QS200410502 Institutional research plan: CEZ:AV0Z20410507 Keywords : small punch test * creep * chromium steel * finite element method Subject RIV: JG - Metallurgy www.scientific.net/KEM.417-418.561
Revision of Drucker-Prager cap creep modelling of pebble beds in fusion blankets
International Nuclear Information System (INIS)
Hofer, D.; Kamlah, M.; Hermsmeyer, S.
2004-01-01
A continuum model commonly used in soil mechanics analysis is compiled by use of a finite element software and has been used to simulate the thermomechanical behaviour of pebble beds. The Drucker-Prager Cap theory accounts for inelastic volume change, cap hardening, nonlinear elasticity and pressure dependent shear failure. The hardening mechanism allows for defining the hydrostatic pressure yield stress as a function of the volumetric inelastic strain. Volumetric creep is considered in order to simulate the pebble bed behaviour at high temperatures. Here, the strain hardening option has been used for the consolidation creep mechanism. The model has been calibrated using the fitting curves of the oedometric test given by Reimann et al. The fitted data has been used to calculate a pebble bed with simplified boundary conditions loaded by non-uniform volumetric heating. This calculation demonstrated that the model is capable of representing creep behaviour under volumetric heating conditions. (author)
Mathematical model for creep and thermal shrinkage of concrete at high temperature
International Nuclear Information System (INIS)
Bazant, Z.P.
1983-01-01
Based on the existing limited test data, it is possible to set up an approximate constitutive model for creep and shrinkage at temperatures above 100 0 C, up to about 400 0 C. The model presented here describes the effect of various constant temperatures on the creep rate and the rate of aging, similar effects of the specific water content, the creep increase caused by simultaneous changes in moisture content, the thermal volume changes as well as the volume changes caused by changes in moisture content (drying shrinkage or thermal shrinkage), and the effect of pore pressure produced by heating. Generalizations to time-variable stresses and multiaxial stresses are also given. The model should allow more realistic analysis of reactor vessels and containments for accident situations, of concrete structures subjected to fire, of vessels for coal gasification or liquefaction, etc. (orig.)
Modelling of the fuel mechanical behavior: from creep laws to internal variable models
International Nuclear Information System (INIS)
Leclercq, S.
1998-01-01
Creep laws such as that of Bohaboy are commonly used to simulate the fuel pellet response to the demands placed upon it during its use. These laws are sufficient for describing the base operating conditions (where only creep appears), but they require improvement for describing power ramp conditions (where hardening and relaxation appear). The aim of the present paper is to develop a framework in which it will be possible to build models that are more representative of the fuel pellet in pile conditions. The approach presented here is based on the thermodynamics of irreversible processes and continuum mechanics. It is postulated that the material is made of a mixture of porous and 'sound' material. The evolution of porosity is deduced from experimental results in order to be consistent with the second law of thermodynamics. This implies the assumption of a threshold value for the existence of densification and swelling. (orig.)
Evaluation of Creep-Fatigue Damage in 304 Stainless Steel using Ultrasonic Non-Destructive Test
Energy Technology Data Exchange (ETDEWEB)
Lee, Sung Sik [Safetech Co. Ltd., Kimhae (Korea, Republic of); Oh, Yong Jun [Hanbat National Univ., Daejon (Korea, Republic of); Nam, Soo Woo [KISTI ReSEAT Program, Seoul (Korea, Republic of)
2011-12-15
It is well known that grain boundary cavitation is the main failure mechanism in austenitic stainless steel under tensile hold creep-fatigue interaction conditions. The cavities are nucleated at the grain boundary during cyclic loading and grow to become grain boundary cracks. The attenuation of ultrasound depends on scattering and absorption in polycrystalline materials. Scattering occurs when a propagation wave encounters microstructural discontinuities, such as internal voids or cavities. Since the density of the creepfatigue cavities increases with the fatigue cycles, the attenuation of ultrasound will also be increased with the fatigue cycles and this attenuation can be detected nondestructively. In this study, it is found that individual grain boundary cavities are formed and grow up to about 100 cycles and then, these cavities coalesce to become cracks. The measured ultrasonic attenuation increased with the cycles up to cycle 100, where it reached a maximum value and then decreased with further cycles. These experimental measurements strongly indicate that the open pores of cavities contribute to the attenuation of ultrasonic waves. However, when the cavities develop, at the grain boundary cracks whose crack surfaces are in contact with each other, there is no longer any open space and the ultrasonic wave may propagate across the cracks. Therefore, the attenuation of ultrasonic waves will be decreased. This phenomenon of maximum attenuation is very important to judge the stage of grain boundary crack development, which is the indication of the dangerous stage of the structures.
Gao, Siwen; Wollgramm, Philip; Eggeler, Gunther; Ma, Anxin; Schreuer, Jürgen; Hartmaier, Alexander
2018-07-01
For the purpose of good reproduction and prediction of creep deformation of nickel-base single crystal superalloys at intermediate temperatures, a phenomenological creep model is developed, which accounts for the typical γ/γ‧ microstructure and the individual thermally activated elementary deformation processes in different phases. The internal stresses from γ/γ‧ lattice mismatch and deformation heterogeneity are introduced through an efficient method. The strain hardening, the Orowan stress, the softening effect due to dislocation climb along γ/γ‧ interfaces and the formation of dislocation ribbons, and the Kear–Wilsdorf-lock effect as key factors in the main flow rules are formulated properly. By taking the cube slip in \\{100\\} slip systems and \\{111\\} twinning mechanisms into account, the creep behavior for [110] and [111] loading directions are well captured. Without specific interaction and evolution of dislocations, the simulations of this model achieve a good agreement with experimental creep results and reproduce temperature, stress and crystallographic orientation dependences. It can also be used as the constitutive relation at material points in finite element calculations with complex boundary conditions in various components of superalloys to predict creep behavior and local stress distributions.
Energy Technology Data Exchange (ETDEWEB)
Galindo-Nava, E.I., E-mail: eg375@cam.ac.uk; Rae, C.M.F.
2016-01-10
A new approach for modelling dislocation creep during primary and secondary creep in FCC metals is proposed. The Orowan equation and dislocation behaviour at the grain scale are revisited to include the effects of different microstructures such as the grain size and solute atoms. Dislocation activity is proposed to follow a jog-diffusion law. It is shown that the activation energy for cross-slip E{sub cs} controls dislocation mobility and the strain increments during secondary creep. This is confirmed by successfully comparing E{sub cs} with the experimentally determined activation energy during secondary creep in 5 FCC metals. It is shown that the inverse relationship between the grain size and dislocation creep is attributed to the higher number of strain increments at the grain level dominating their magnitude as the grain size decreases. An alternative approach describing solid solution strengthening effects in nickel alloys is presented, where the dislocation mobility is reduced by dislocation pinning around solute atoms. An analysis on the solid solution strengthening effects of typical elements employed in Ni-base superalloys is also discussed. The model results are validated against measurements of Cu, Ni, Ti and 4 Ni-base alloys for wide deformation conditions and different grain sizes.
International Nuclear Information System (INIS)
Pelah, I.
1981-03-01
Simulation of fusion-neutron induced damage by beams of light ions is discussed. It is suggested that accelerated creep measurements to determine ''end of life'' of materials may be done by the application of thermal treatment and thermal creep measurements. (author)
Description of Concrete Creep under Time-Varying Stress Using Parallel Creep Curve
Park, Yeong-Seong; Lee, Yong-Hak; Lee, Youngwhan
2016-01-01
An incremental format of creep model was presented to take account of the development of concrete creep due to loading at different ages. The formulation was attained by introducing a horizontal parallel assumption of creep curves and combining it with the vertical parallel creep curve of the rate of creep method to remedy the disadvantage of the rate of creep method that significantly underestimates the amount of creep strain, regardless of its simple format. Two creep curves were combined b...
Energy Technology Data Exchange (ETDEWEB)
Vogel, C.
1996-04-01
The present work deals with mechanical behaviour of zirconium alpha at 200 deg. C and crack initiation prediction methods, particularly when loading conditions lead to interaction of fatigue and creep phenomena. A classical approach used to study interaction between cyclic effects and constant loading effects does not give easy understanding of experimental results. Therefore, a new approach has been developed, which allow to determine a number of cycles for crack initiation for complex structures under large loading conditions. To study influence of fatigue and creep interaction on crack initiation, a model was chosen, using a scalar variable, giving representation of the material deterioration state. The model uses a non linear cumulating effect between the damage corresponding to cyclic loads and the damage correlated to time influence. The model belongs to uncoupled approaches between damage and behaviour, which is described here by a two inelastic deformations model. This mechanical behaviour model is chosen because it allows distinction between a plastic and a viscous part in inelastic flow. Cyclic damage is function of stress amplitude and mean stress. For the peculiar sensitivity of the material to creep, a special parameter bas been defined to be critical toward creep damage. It is the kinematic term associated to state variables describing this type of hardening in the viscous mechanism. (author).
International Nuclear Information System (INIS)
Wassilew, C.
1989-11-01
This report gives an overall evaluation of several in-reactor deformation and creep-rupture experiments performed in BR-2, FFTF, and Rapsodie on pressurised tubes of the stabilized austenitic stainless steels 1.4970, 1.4981, 1.4988, and the nickel base alloy Hastelloy-X. The irradiation induced deformation processes observed in the components operating in a neutron environment can be divided into two main groups: 1. volume conserving creep and 2. volumetric swelling. Since the observed deformation as well as damage accumulating phenomena are caused by the same constrained generated and free disposable point defects and helium atoms, it is obvious and advisable to analyze, and to model simultaneously the ensemble of the elementary mechanisms and processes effective at the same time. Phenomenological models based on the thermodynamics of irreversible processes have been developed, with the aim of: 1. grasping the partial relationships between the external variables and the response functions (creep, swelling, creep driven swelling, and time to rupture), 2. fathoming the rate-controlling mechanisms, 3. providing insight into the structural details and changes occurring during the deformation and the damage accumulating processes, 4. integrating the damage accumulating processes comprehensively, and 5. formulating the constitutive equations required to describe the elementary processes that generate plastic deformations as well as damage accumulation. (orig./MM)
Modeling creep deformation of a two-phase TiAI/Ti3Al alloy with a lamellar microstructure
Bartholomeusz, Michael F.; Wert, John A.
1994-10-01
A two-phase TiAl/Ti3Al alloy with a lamellar microstructure has been previously shown to exhibit a lower minimum creep rate than the minimum creep rates of the constituent TiAl and Ti3Al single-phase alloys. Fiducial-line experiments described in the present article demonstrate that the creep rates of the constituent phases within the two-phase TiAl/Ti3Al lamellar alloy tested in compression are more than an order of magnitude lower than the creep rates of single-phase TiAl and Ti3Al alloys tested in compression at the same stress and temperature. Additionally, the fiducial-line experiments show that no interfacial sliding of the phases in the TiAl/Ti3Al lamellar alloy occurs during creep. The lower creep rate of the lamellar alloy is attributed to enhanced hardening of the constituent phases within the lamellar microstructure. A composite-strength model has been formulated to predict the creep rate of the lamellar alloy, taking into account the lower creep rates of the constituent phases within the lamellar micro-structure. Application of the model yields a very good correlation between predicted and experimentally observed minimum creep rates over moderate stress and temperature ranges.
Smeared crack modelling approach for corrosion-induced concrete damage
DEFF Research Database (Denmark)
Thybo, Anna Emilie Anusha; Michel, Alexander; Stang, Henrik
2017-01-01
In this paper a smeared crack modelling approach is used to simulate corrosion-induced damage in reinforced concrete. The presented modelling approach utilizes a thermal analogy to mimic the expansive nature of solid corrosion products, while taking into account the penetration of corrosion...... products into the surrounding concrete, non-uniform precipitation of corrosion products, and creep. To demonstrate the applicability of the presented modelling approach, numerical predictions in terms of corrosion-induced deformations as well as formation and propagation of micro- and macrocracks were......-induced damage phenomena in reinforced concrete. Moreover, good agreements were also found between experimental and numerical data for corrosion-induced deformations along the circumference of the reinforcement....
Creep of trabecular bone from the human proximal tibia.
Novitskaya, Ekaterina; Zin, Carolyn; Chang, Neil; Cory, Esther; Chen, Peter; D'Lima, Darryl; Sah, Robert L; McKittrick, Joanna
2014-07-01
Creep is the deformation that occurs under a prolonged, sustained load and can lead to permanent damage in bone. Creep in bone is a complex phenomenon and varies with type of loading and local mechanical properties. Human trabecular bone samples from proximal tibia were harvested from a 71-year old female cadaver with osteoporosis. The samples were initially subjected to one cycle load up to 1% strain to determine the creep load. Samples were then loaded in compression under a constant stress for 2h and immediately unloaded. All tests were conducted with the specimens soaked in phosphate buffered saline with proteinase inhibitors at 37 °C. Steady state creep rate and final creep strain were estimated from mechanical testing and compared with published data. The steady state creep rate correlated well with values obtained from bovine tibial and human vertebral trabecular bone, and was higher for lower density samples. Tissue architecture was analyzed by micro-computed tomography (μCT) both before and after creep testing to assess creep deformation and damage accumulated. Quantitative morphometric analysis indicated that creep induced changes in trabecular separation and the structural model index. A main mode of deformation was bending of trabeculae. Copyright © 2014 Elsevier B.V. All rights reserved.
Sahoo, K. C.; Goyal, Sunil; Parameswaran, P.; Ravi, S.; Laha, K.
2018-03-01
The role of the multiaxial state of stress on creep deformation and rupture behavior of 304HCu austenitic stainless steel was assessed by performing creep rupture tests on both smooth and notched specimens of the steel. The multiaxial state of stress was introduced by incorporating circumferential U-notches of different root radii ranging from 0.25 to 5.00 mm on the smooth specimens of the steel. Creep tests were carried out at 973 K over the stress range of 140 to 220 MPa. In the presence of notch, the creep rupture strength of the steel was found to increase with the associated decrease in rupture ductility. Over the investigated stress range and notch sharpness, the strengthening was found to increase drastically with notch sharpness and tended toward saturation. The fractographic studies revealed the mixed mode of failure consisting of transgranular dimples and intergranular creep cavitation for shallow notches, whereas the failure was predominantly intergranular for relatively sharper notches. Detailed finite element analysis of stress distribution across the notch throat plane on creep exposure was carried out to assess the creep failure of the material in the presence of notch. The reduction in von-Mises stress across the notch throat plane, which was greater for sharper notches, increased the creep rupture strength of the material. The variation in fracture behavior of the material in the presence of notch was elucidated based on the von-Mises, maximum principal, and hydrostatic stresses. Electron backscatter diffraction analysis of creep strain distribution across the notch revealed localized creep straining at the notch root for sharper notches. A master curve for predicting creep rupture life under the multiaxial state of stress was generated considering the representative stress having contributions from both the von-Mises and principal stress components of the stress field in the notch throat plane. Rupture ductility was also predicted based on the
Long-term creep modeling of wood using time temperature superposition principle
Gamalath, Sandhya Samarasinghe
1991-01-01
Long-term creep and recovery models (master curves) were developed from short-term data using the time temperature superposition principle (TTSP) for kiln-dried southern pine loaded in compression parallel-to-grain and exposed to constant environmental conditions (~70Â°F, ~9%EMC). Short-term accelerated creep (17 hour) and recovery (35 hour) data were collected for each specimen at a range of temperature (70Â°F-150Â°F) and constant moisture condition of 9%. The compressive stra...
International Nuclear Information System (INIS)
Stoller, R.E.; Grossbeck, M.L.; Mansur, L.K.
1990-01-01
A theoretical model has been developed using the reaction rate theory of radiation effects to explain experimental results that showed higher than expected values of irradiation creep at low temperatures in the Oak Ridge Research Reactor. The customary assumption that the point defect concentrations are at steady state was not made; rather, the time dependence of the vacancy and interstitial concentrations and the creep rate were explicitly calculated. For temperatures below about 100 to 200 degree C, the time required for the vacancy concentration to reach steady state exceeds the duration of the experiment. For example, if materials parameters typical of austenitic stainless steel are used, the calculated vacancy transient dose at 100 degree C is about 100 dpa. At 550 degree C this transient is over by 10 -8 dpa. During the time that the vacancy population remains lower than its steady state value, dislocation climb is increased since defects of primarily one type are being absorbed. Using the time-dependent point defect concentrations, the dislocation climb velocity has been calculated as a function of time and a climb-enabled glide creep model had been invoked. The extended transient time for the vacancies leads to high creep rates at low temperatures. In agreement with the experimental observations, a minimum in the temperature dependence of creep is predicted at a temperature between 50 and 350 degree C. The temperature at which the minimum occurs decreases as the irradiation dose increases. Predicted values of creep at 8 dpa are in good agreement with the results of the ORR-MFE-6J/7J experiment
International Nuclear Information System (INIS)
Nagae, Yuji; Aoto, Kazumi
2000-09-01
In this study, the change of lath structure with the increase of distance from fractured surface was observed in detail and the localization of creep damage to decide fracture position was investigated. As the results of the relationship between lath width and distance from fractured surface, the lath width obviously increased as a distance from fractured surface decreased. Lath widths in different positions of as-received specimen were almost same. These result indicates that recovery of lath structure localizes with creep damage. It was considered that the coarsening of precipitates caused localization of recovery in lath structure. Area fraction of precipitates and cross-section of each precipitate in different positions from fractured surface were measured and compared. There were no differences in area fraction of precipitates and cross-section of each precipitate in different positions. Therefore it was found out that the reason for localization of recovery of lath structure was not coarsening of precipitates. (author)
Influence of variations in creep curve on creep behavior of a high-temperature structure
International Nuclear Information System (INIS)
Hada, Kazuhiko
1986-01-01
It is one of the key issues for a high-temperature structural design guideline to evaluate the influence of variations in creep curve on the creep behavior of a high-temperature structure. In the present paper, a comparative evaluation was made to clarify such influence. Additional consideration was given to the influence of the relationship between creep rupture life and minimum creep rate, i.e., the Monkman-Grant's relationship, on the creep damage evaluation. The consideration suggested that the Monkman-Grant's relationship be taken into account in evaluating the creep damage behavior, especially the creep damage variations. However, it was clarified that the application of the creep damage evaluation rule of ASME B and P.V. Code Case N-47 to the ''standard case'' which was predicted from the average creep property would predict the creep damage on the safe side. (orig./GL)
A fractional derivative approach to full creep regions in salt rock
DEFF Research Database (Denmark)
Zhou, H. W.; Wang, C. P.; Mishnaevsky, Leon
2013-01-01
Based on the definition of the constant-viscosity Abel dashpot, a new creep element, referred to as the variable-viscosity Abel dashpot, is proposed to characterize damage growth in salt rock samples during creep tests. Ultrasonic testing is employed to determine a formula of the variable viscosity...... coefficient, indicating that the change of the variable viscosity coefficient with the time meets a negative exponent law. In addition, by replacing the Newtonian dashpot in the classical Nishihara model with the variable-viscosity Abel dashpot, a damage-mechanism-based creep constitutive model is proposed...... on the basis of time-based fractional derivative. The analytic solution for the fractional-derivative creep constitutive model is presented. The parameters of the fractional derivative creep model are determined by the Levenberg–Marquardt method on the basis of the experimental results of creep tests on salt...
A Unified Physical Model for Creep and Hot Working of Al-Mg Solid Solution Alloys
Directory of Open Access Journals (Sweden)
Stefano Spigarelli
2017-12-01
Full Text Available The description of the dependence of steady-state creep rate on applied stress and temperature is almost invariably based on the Norton equation or on derived power-law relationships. In hot working, the Norton equation does not work, and is therefore usually replaced with the Garofalo (sinh equation. Both of these equations are phenomenological in nature and can be seldom unambiguously related to microstructural parameters, such as dislocation density, although early efforts in this sense led to the introduction of the “natural power law” with exponent 3. In an attempt to overcome this deficiency, a recent model with sound physical basis has been successfully used to describe the creep response of fcc metals, such as copper. The main advantage of this model is that it does not require any data fitting to predict the strain rate dependence on applied stress and temperature, which is a particularly attractive peculiarity when studying the hot workability of metals. Thus, the model, properly modified to take into account solid solution strengthening effects, has been here applied to the study of the creep and hot-working of simple Al-Mg single phase alloys. The model demonstrated an excellent accuracy in describing both creep and hot working regimes, still maintaining its most important feature, that is, it does not require any fitting of the experimental data.
A creep rupture model accounting for cavitation at sliding grain boundaries
Giessen, Erik van der; Tvergaard, Viggo
1991-01-01
An axisymmetric cell model analysis is used to study creep failure by grain boundary cavitation at facets normal to the maximum principal tensile stress, taking into account the influence of cavitation and sliding at adjacent inclined grain boundaries. It is found that the interaction between the
Mathematic modeling of reactor fuel radiation creep at example of uranium and its alloys
International Nuclear Information System (INIS)
Tarasov, V.A.
2001-01-01
The model of a radiation creep is explained within the framework of the mechanism of gliding and climbing dislocations based on the conception of a dislocation as not ideal sink for point radiation defects (PRD). The offered model is efficient for installed concentration PRD, considerably exceeding thermally steady state concentration. The gliding of dislocation are describing as due to moving dislocation kinks in Peierl's relief. The climbing of dislocation are describing as due to moving dislocation jogs. The mathematical model for the computer program simulating the offered model of radiation creep is developed. The complex of the computer programs simulating the radiation creep is developed. The computer simulation researches are conducted and the outcomes of a research of a kinetics of a flexible sliding and climbing dislocation interacting to obstacles of a various type (spherical centre of extension, dislocation prismatic loop and their spatially random distributions) for various installed concentration PRD, external loadings and temperatures are represented. The curves of installed rate of a radiation creep from temperature for uranium and its alloys with small additions of molybdenum (from 0,9 to 1,3 %) are obtained
Mechanism-based modeling of solute strengthening: application to thermal creep in Zr alloy
Energy Technology Data Exchange (ETDEWEB)
Tome, Carlos [Los Alamos National Lab. (LANL), Los Alamos, NM (United States); Wen, Wei [Los Alamos National Lab. (LANL), Los Alamos, NM (United States); Capolungo, Laurent [Los Alamos National Lab. (LANL), Los Alamos, NM (United States)
2017-08-01
This report focuses on the development of a physics-based thermal creep model aiming to predict the behavior of Zr alloy under reactor accident condition. The current models used for this kind of simulations are mostly empirical in nature, based generally on fits to the experimental steady-state creep rates under different temperature and stress conditions, which has the following limitations. First, reactor accident conditions, such as RIA and LOCA, usually take place in short times and involve only the primary, not the steady-state creep behavior stage. Moreover, the empirical models cannot cover the conditions from normal operation to accident environments. For example, Kombaiah and Murty [1,2] recently reported a transition between the low (n~4) and high (n~9) power law creep regimes in Zr alloys depending on the applied stress. Capturing such a behavior requires an accurate description of the mechanisms involved in the process. Therefore, a mechanism-based model that accounts for the evolution with time of microstructure is more appropriate and reliable for this kind of simulation.
Analysis of structures based on a characteristic-strain model of creep
Energy Technology Data Exchange (ETDEWEB)
Bolton, J. [Alstom Power, Newbold Road, Rugby CV21 2NH (United Kingdom)], E-mail: janjohn.bolton@virgin.net
2008-01-15
A companion paper [Bolton J. In: A characteristic-strain model for creep, ECCC/I.Mech.E. conference on creep and fracture in high-temperature components, London, September 2005] describes a creep model based on a constant 'characteristic strain' at any temperature. The present paper discusses the application of such a model, first to simple structures and then to engineering components of general form under steady loading. A basis is proposed for identifying the stress within a structure, or within the critical part of a structure, which can be considered to govern both its overall and local deformations. The concept is similar to skeletal-point stress but is more readily applied to components of any shape. The implementation of the concept of 'structural stress' is discussed in the context of finite-element creep calculations. Consideration is given to the analysis of cracked structures, where very high strains at the crack tip must be accommodated.
Continuous observation of cavity growth and coalescence by creep-fatigue tests in SEM
International Nuclear Information System (INIS)
Arai, Masayuki; Ogata, Takashi; Nitta, Akito
1995-01-01
Structural components operating at high temperatures in power plants are subjected to interaction of thermal fatigue and creep which results in creep-fatigue damage. In evaluating the life of those components, it is important to understand microscopic damage evolution under creep-fatigue conditions. In this study, static creep and creep-fatigue tests with tensile holdtime were conducted on SUS304 stainless steel by using a high-temperature fatigue machine combined with a scanning electron microscope (SEM), and cavity growth and coalescence behaviors on surface grain boundaries were observed continuously by the SEM. Quantitative analysis of creep cavity growth based on the observation was made for comparison with theoretical growth models. As a result, it was found that grain boundary cavities nucleate at random and grow preferentially on grain boundaries in a direction almost normal to the stress axis. Under the creep condition, the cavities grow monotonously on grain boundaries while they remain the elliptical shape. On the other hand, under the creep-fatigue condition the cavities grow with an effect of local strain distribution around the grain boundary due to cyclic loading and the micro cracks of one grain-boundary length were formed by coalescence of the cavities. Also, cavity nucleation and growth rates for creep-fatigue were more rapid than those for static creep and the constrained cavity growth model coincided well with the experimental data for creep. (author)
Report on fundamental modeling of irradiation-induced swelling and creep in FeCrAl alloys
Energy Technology Data Exchange (ETDEWEB)
Kohnert, Aaron A. [Oak Ridge National Lab. (ORNL), Oak Ridge, TN (United States); Dasgupta, Dwaipayan [Univ. of Tennessee, Knoxville, TN (United States); Wirth, Brian [Oak Ridge National Lab. (ORNL), Oak Ridge, TN (United States); Linton, Kory D. [Oak Ridge National Lab. (ORNL), Oak Ridge, TN (United States)
2016-09-23
In order to improve the accident tolerance of light water reactor (LWR) fuel, alternative cladding materials have been proposed to replace zirconium (Zr)-based alloys. Of these materials, there is a particular focus on iron-chromium-aluminum (FeCrAl) alloys due to much slower oxidation kinetics in high-temperature steam than Zr-alloys. This should decrease the energy release due to oxidation and allow the cladding to remain integral longer in the presence of high temperature steam, making accident mitigation more likely. As a continuation of the development for these alloys, the material response must be demonstrated to provide suitable radiation stability, in order to ensure that there will not be significant dimensional changes (e.g., swelling), as well as quantifying the radiation hardening and radiation creep behavior. In this report, we describe the use of cluster dynamics modeling to evaluate the defect physics and damage accumulation behavior of FeCrAl alloys subjected to neutron irradiation, with a particular focus on irradiation-induced swelling and defect fluxes to dislocations that are required to model irradiation creep behavior.
International Nuclear Information System (INIS)
Henes, D.; Straub, S.; Blum, W.; Moehlig, H.; Granacher, J.; Berger, C.
1999-01-01
The current state of development of the composite model of deformation of the martensitic steel X 20(22) CrMoV 12 1 under conditions of creep is briefly described. The model is able to reproduce differences in monotonic creep strength of different melts with slightly different initial microstructures and to simulate cyclic creep with alternating phases of tension and compression. (orig.)
Modelling of U-Mo/Al Dispersion fuel fission induced swelling and creep
International Nuclear Information System (INIS)
Jeong, Gwan Yoon; Sohn, Dong Seong; Kim, Yeon Soo
2014-01-01
In a Dispersion fuel which U-Mo particles are dispersed in Al metal matrix, a similar phenomenon forming a bulge region was observed but it is difficult to quantify and construct a model for explaining creep and swelling because of its complex microstructure change during irradiation including interaction layer (IL) and porosity formation. In a Dispersion fuel meat, fission product induces fuel particles swelling and it has to be accommodated by the deformation of the Al matrix and newly formed IL during irradiation. Then, it is reasonable that stress from fuel swelling in the complex structure should be relaxed by local adjustments of particles, Al matrix, and IL. For analysis of U-Mo/Al Dispersion fuel creep, the creep of U-Mo particle, Al matrix, and IL should be considered. Moreover, not only fuel particle swelling and IL growth, but also fuel and Al matrix consumptions due to IL formation are accounted in terms of their volume fraction changes during irradiation. In this work, fuel particles, Al matrix and IL are treated in a way of homogenized constituents: Fuel particles, Al matrix and IL consist of an equivalent meat during irradiation. Meat volume swelling of two representative plates was measured: One (Plate A) was a pure Al matrix with 6g/cc uranium loading, the other (Plate B) a silicon added Al matrix with 8g/cc uranium loading. The meat swelling of calculated as a function of burnup. The meat swelling of calculation and measurement was compared and the creep rate coefficients for Al and IL were estimated by repetitions. Based on assumption that only the continuous phase of Al-IL combined matrix accommodated the stress from fuel particle swelling and it was allowed to have creep deformation, the homogenization modeling was performed. The meat swelling of two U-Mo/Al Dispersion fuel plates was modeled by using homogenization model
Modelling of U-Mo/Al Dispersion fuel fission induced swelling and creep
Energy Technology Data Exchange (ETDEWEB)
Jeong, Gwan Yoon; Sohn, Dong Seong [Ulsan National Institute of Science and Technology, Ulsan (Korea, Republic of); Kim, Yeon Soo [Argonne National Laboratory, Argonne (United States)
2014-05-15
In a Dispersion fuel which U-Mo particles are dispersed in Al metal matrix, a similar phenomenon forming a bulge region was observed but it is difficult to quantify and construct a model for explaining creep and swelling because of its complex microstructure change during irradiation including interaction layer (IL) and porosity formation. In a Dispersion fuel meat, fission product induces fuel particles swelling and it has to be accommodated by the deformation of the Al matrix and newly formed IL during irradiation. Then, it is reasonable that stress from fuel swelling in the complex structure should be relaxed by local adjustments of particles, Al matrix, and IL. For analysis of U-Mo/Al Dispersion fuel creep, the creep of U-Mo particle, Al matrix, and IL should be considered. Moreover, not only fuel particle swelling and IL growth, but also fuel and Al matrix consumptions due to IL formation are accounted in terms of their volume fraction changes during irradiation. In this work, fuel particles, Al matrix and IL are treated in a way of homogenized constituents: Fuel particles, Al matrix and IL consist of an equivalent meat during irradiation. Meat volume swelling of two representative plates was measured: One (Plate A) was a pure Al matrix with 6g/cc uranium loading, the other (Plate B) a silicon added Al matrix with 8g/cc uranium loading. The meat swelling of calculated as a function of burnup. The meat swelling of calculation and measurement was compared and the creep rate coefficients for Al and IL were estimated by repetitions. Based on assumption that only the continuous phase of Al-IL combined matrix accommodated the stress from fuel particle swelling and it was allowed to have creep deformation, the homogenization modeling was performed. The meat swelling of two U-Mo/Al Dispersion fuel plates was modeled by using homogenization model.
Du, Dong-Ning; Wang, Lai-Gui; Zhang, Xiang-Dong; Zhang, Shu-Kun
2017-06-01
The sand particles in the sand - rock composite slope of the open pit mine occurs creep deformation and fatigue liquefaction under the action of vehicle load vibration and hydraulic gradient, which causes landslide geological disasters and it destroys the surface environment. To reveal the mechanism, a mechanics model based on the model considering the soil structural change with a new “plastic hinge” element is developed, to improve its constitutive and creep curve equations. Data from sand creep experiments are used to identify the parameters in the model and to validate the model. The results show that the mechanical model can describe the rotation progress between the sand particles, disclose the negative acceleration creep deformation stage during the third phase, and require fewer parameters while maintaining accuracy. It provides a new creep model considering rotation to analyze sand creep mechanism, which provides a theoretical basis for revealing the open pit mine landslide mechanism induced by creep deformation and fatigue liquefaction of sandy soil.
Modelling anelastic contribution to nuclear fuel cladding creep and stress relaxation
Energy Technology Data Exchange (ETDEWEB)
Tulkki, Ville, E-mail: ville.tulkki@vtt.fi; Ikonen, Timo
2015-10-15
In fuel behaviour modelling accurate description of the cladding mechanical response is important for both operational and safety considerations. While accuracy is desired, a certain level of simplicity is needed as both computational resources and detailed information on properties of particular cladding may be limited. Most models currently used in the integral codes divide the mechanical response into elastic and viscoplastic contributions. These have difficulties in describing both creep and stress relaxation, and often separate models for the two phenomena are used. In this paper we implement anelastic contribution to the cladding mechanical model, thus enabling consistent modelling of both creep and stress relaxation. We show that the model based on assumption of viscoelastic behaviour can be used to explain several experimental observations in transient situations and compare the model to published set of creep and stress relaxation experiments performed on similar samples. Based on the analysis presented we argue that the inclusion of anelastic contribution to the cladding mechanical models provides a way to improve the simulation of cladding behaviour during operational transients.
Modeling damage in concrete pavements and bridges.
2010-09-01
This project focused on micromechanical modeling of damage in concrete under general, multi-axial loading. A : continuum-level, three-dimensional constitutive model based on micromechanics was developed. The model : accounts for damage in concrete by...
Experimental study on creep-fatigue interaction behavior of GH4133B superalloy
International Nuclear Information System (INIS)
Hu Dianyin; Wang Rongqiao
2009-01-01
The creep-fatigue tests have been conducted with nickel-based superalloy GH4133B at 600 deg. C in three cases of type loading to study the creep-fatigue behavior of the alloy and the loading history effect on the creep-fatigue damage. Since the conventional linear cumulative damage rule failed in evaluating the creep-fatigue life based on experimental data, a continuous non-linear model proposed by Mao et al. was employed to describe the creep-fatigue interaction. The creep-fatigue damage in the cases of continuous cyclic creep loading (CF) and prior fatigue followed by creep loading (F + C) was larger than unity and smaller than unity when the type loading was prior creep followed by fatigue loading (C + F). Scanning electron microscope (SEM) analyses of the fracture surface showed that the cracks initiated from the specimen surface and the fracture modes in different loading history were different. The crack mode at CF loading depended on the cyclic period. In the case of F + C loading, the primary fracture mode was transgranular, and in the condition where the type of waveform was C + F, the fracture mode was of mixed transgranular and intergranular type. In addition, the origin of the history effect on creep-fatigue interaction was explained by the SEM observations.
Modelling of the fuel mechanical behavior. From creep laws to internal variable models
Energy Technology Data Exchange (ETDEWEB)
Leclercq, S. [Electricite de France (EDF), 77 - Moret sur Loing (France)
1997-12-31
Creep laws are nowadays commonly used to simulate the fuel rod response to the solicitations it faces during its life. These laws are sufficient for describing the base operating conditions (where only creep appears), but they have to be improved for power ramp conditions (where hardening and relaxation appear). The main objective of the present paper was to clearly exhibit the important role of the porosity on the fuel mechanical behavior. It has been shown that viscoplastic properties are activated by the evolution of the porosity. A general framework has been developed, in agreement with the principles of thermodynamics of irreversible processes. The major result of the present model concerns the fact that the viscoplastic strain is non-deviatoric, due to the porosity growth. The purely deviatoric part of the non-linear strain is taken as the Lemaitre law, but any other classical equation may be used. As concerns the hydrostatic part, it is derived from simple assumptions. The coupling between the volume fraction of porosity and the mechanical stress field is introduced into the dissipation term. (author) 6 refs.
Modelling of the fuel mechanical behavior. From creep laws to internal variable models
International Nuclear Information System (INIS)
Leclercq, S.
1997-01-01
Creep laws are nowadays commonly used to simulate the fuel rod response to the solicitations it faces during its life. These laws are sufficient for describing the base operating conditions (where only creep appears), but they have to be improved for power ramp conditions (where hardening and relaxation appear). The main objective of the present paper was to clearly exhibit the important role of the porosity on the fuel mechanical behavior. It has been shown that viscoplastic properties are activated by the evolution of the porosity. A general framework has been developed, in agreement with the principles of thermodynamics of irreversible processes. The major result of the present model concerns the fact that the viscoplastic strain is non-deviatoric, due to the porosity growth. The purely deviatoric part of the non-linear strain is taken as the Lemaitre law, but any other classical equation may be used. As concerns the hydrostatic part, it is derived from simple assumptions. The coupling between the volume fraction of porosity and the mechanical stress field is introduced into the dissipation term. (author)
An extension of a high temperature creep model to account for fuel sheath oxidation
International Nuclear Information System (INIS)
Boccolini, G.; Valli, G.
1983-01-01
Starting from the high-temperature creep model for Zircaloy fuel sheathing, the NIRVANA (developed by AECL), a multilayer model, is proposed in this paper: it includes the outer oxide plus alpha retained layers, and the inner core of beta or alpha plus beta material, all constrained to deform with the same creep rate. The model has been incorporated into the SPARA fuel computer code developed for the transient analysis of fuel rod behaviour in the CIRENE prototype reactor, but it is in principle valid for all Zircaloy fuel sheathings. Its predictions are compared with experimental results from burst tests on BWR and PWR type sheaths; the tests were carried out at CNEN under two research contracts with Ansaldo Meccanico Nucleare and Sigen-Sopren, respectively
International Nuclear Information System (INIS)
Pan, L.M.; Ghosh, R.N.; McLean, M.
1993-01-01
A physics based model has been developed that accounts for the principal features of anisotropic creep deformation of single crystal superalloys. The present paper extends this model to simulate other types of high temperature deformation under strain controlled test conditions, such as stress relaxation and tension tests at constant strain rate in single crystals subject to axial loading along an arbitrary crystal direction. The approach is applied to the SRR99 single crystal superalloy where a model parameter database is available, determined via analysis of a database of constant stress creep curves. A software package has been generated to simulate the deformation behaviour under complex stress-strain conditions taking into account anisotropic elasticity. (orig.)
Creep of plain weave polymer matrix composites
Gupta, Abhishek
composites, was experimentally evaluated for time periods ranging from 1--120 hours under both loading conditions. The composite showed increase in creep with increase in temperature and stress. Creep of composite increased with increase in angle of loading, from 1% under on-axis loading to 31% under off-axis loading, within the tested time window. The experimental creep data for plain weave composites were superposed using TTSP (Time Temperature Superposition Principle) to obtain a master curve of experimental data extending to several years and was compared with model predictions to validate the model. The experimental and model results were found in good agreement within an error range of +/-1-3% under both loading conditions. A parametric study was also conducted to understand the effect of microstructure of plain weave composites on its on-axis and off-axis creep. Generation of knowledge in this area is also "first". Additionally, this thesis generated knowledge on time-dependent damage m woven composites and its effect on creep and tensile properties and their prediction.
Creep of trabecular bone from the human proximal tibia
Energy Technology Data Exchange (ETDEWEB)
Novitskaya, Ekaterina, E-mail: eevdokim@ucsd.edu [Mechanical and Aerospace Engineering, UC, San Diego, La Jolla, CA 92093 (United States); Materials Science and Engineering Program, UC, San Diego, La Jolla, CA 92093 (United States); Zin, Carolyn [Materials Science and Engineering, Johns Hopkins University, Baltimore, MD 21218 (United States); Chang, Neil; Cory, Esther; Chen, Peter [Departments of Bioengineering and Orthopaedic Surgery, UC, San Diego, La Jolla, CA 92093 (United States); D’Lima, Darryl [Shiley Center for Orthopaedic Research and Education, Scripps Health, La Jolla, CA 92037 (United States); Sah, Robert L. [Materials Science and Engineering Program, UC, San Diego, La Jolla, CA 92093 (United States); Departments of Bioengineering and Orthopaedic Surgery, UC, San Diego, La Jolla, CA 92093 (United States); McKittrick, Joanna [Mechanical and Aerospace Engineering, UC, San Diego, La Jolla, CA 92093 (United States); Materials Science and Engineering Program, UC, San Diego, La Jolla, CA 92093 (United States)
2014-07-01
Creep is the deformation that occurs under a prolonged, sustained load and can lead to permanent damage in bone. Creep in bone is a complex phenomenon and varies with type of loading and local mechanical properties. Human trabecular bone samples from proximal tibia were harvested from a 71-year old female cadaver with osteoporosis. The samples were initially subjected to one cycle load up to 1% strain to determine the creep load. Samples were then loaded in compression under a constant stress for 2 h and immediately unloaded. All tests were conducted with the specimens soaked in phosphate buffered saline with proteinase inhibitors at 37 °C. Steady state creep rate and final creep strain were estimated from mechanical testing and compared with published data. The steady state creep rate correlated well with values obtained from bovine tibial and human vertebral trabecular bone, and was higher for lower density samples. Tissue architecture was analyzed by micro-computed tomography (μCT) both before and after creep testing to assess creep deformation and damage accumulated. Quantitative morphometric analysis indicated that creep induced changes in trabecular separation and the structural model index. A main mode of deformation was bending of trabeculae. - Highlights: • Compressive creep tests of human trabecular bone across the tibia were performed. • The creep rate was found to be inversely proportional to the density of the samples. • μ-computed tomography before and after testing identified regions of deformation. • Bending of the trabeculae was found to be the main deformation mode.
Drucker-Prager-Cap creep modelling of pebble beds in fusion blankets
International Nuclear Information System (INIS)
Hofer, D.; Kamlah, M.
2005-01-01
Modelling of thermal and mechanical behaviour of pebble beds for fusion blankets is an important issue to understand the interaction of solid breeder and beryllium pebble beds with the surrounding structural material. Especially the differing coefficients of thermal expansion of these materials cause high stresses and strains during irradiation induced volumetric heating. To describe this process, the coupled thermomechanical behaviour of both pebble bed materials has to be modelled. Additionally, creep has to be considered contributing to bed deformations and stress relaxation. Motivated by experiments, we use a continuum mechanical approach called Drucker-Prager/Cap theory to model the macroscopic pebble bed behaviour. The model accounts for pressure dependent shear failure, inelastic hardening, and volumetric creep. The elastic part is described by a nonlinear elasticity law. The model has been implemented by user-defined routines in the commercial finite-element code ABAQUS. To check the numerics, the implementation is compared to an analytical solution. Furthermore, the Drucker-Prager/Cap tool is applied to a single ceramic breeder bed subject to creep under volumetric heating
MCDIRC: A model to estimate creep produced by microcracking around a shaft in intact rock
International Nuclear Information System (INIS)
Wilkins, B.J.S.; Rigby, G.L.
1989-12-01
Atomic Energy of Canada Limited (AECL) is studying the concept of disposing of nuclear fuel waste in a vault in plutonic rock. Models are being developed to predict the mechanical behaviour of the rock in response to excavation and heat from the waste. The dominant mechanism of deformation at temperatures below 150 degrees C is microcracking, which results in rock creep and a decrease in rock strength. A model has been constructed to consider the perturbation of the stress state of intact rock by a vertical cylindrical opening. Slow crack-growth data are used to estimate time-dependent changes in rock strength, from which the movement (creep) of the opening wall and radial strain in the rock mass can be estimated
van Wees, Jan-Diederik; Osinga, Sander; Van Thienen-Visser, Karin; Fokker, Peter A.
2018-03-01
The Groningen gas field in the Netherlands experienced an immediate reduction in seismic events in the year following a massive cut in production. This reduction is inconsistent with existing models of seismicity predictions adopting compaction strains as proxy, since reservoir creep would then result in a more gradual reduction of seismic events after a production stop. We argue that the discontinuity in seismic response relates to a physical discontinuity in stress loading rate on faults upon the arrest of pressure change. The stresses originate from a combination of the direct poroelastic effect through the pressure changes and the delayed effect of ongoing compaction after cessation of reservoir production. Both mechanisms need to be taken into account. To this end, we employed finite-element models in a workflow that couples Kelvin-Chain reservoir creep with a semi-analytical approach for the solution of slip and seismic moment from the predicted stress change. For ratios of final creep and elastic compaction up to 5, the model predicts that the cumulative seismic moment evolution after a production stop is subject to a very moderate increase, 2-10 times less than the values predicted by the alternative approaches using reservoir compaction strain as proxy. This is in agreement with the low seismicity in the central area of the Groningen field immediately after reduction in production. The geomechanical model findings support scope for mitigating induced seismicity through adjusting rates of pressure change by cutting down production.
NIRVANA, a high-temperature creep model for Zircaloy fuel sheathing
International Nuclear Information System (INIS)
Sills, H.E.; Holt, R.A.
1979-05-01
We have developed a multi-component model to describe the transient plastic deformation of Zircaloy fuel sheathing during high-temperature transients. From deformation maps we identify three deformation mechanisms which, in principle, occur in all three phase fields of Zircaloy (α, α+β, β): diffusional creep, dislocation creep, and athermal strian. A strain component occurring during the α → β transformation is also identified. Microstructural changes which alter deformation rates -grain structure, recrystallization, phase transformation -are accounted for. The individual components of the model represent known metallurgical phenomena. The combined model gives excellent agreement with transient test data from 700-1800 K, a range of heating rates from 0-100 K.s -1 , and a range of strain rates from 10 -5 to 10 -1 .s -1 . To enable comparison with available data the transient creep model was combined with an axially uniform, thin-walled tube representation having anisotropic material properties. The resulting computer code, NIRVANA provides facilities for simulating uniaxial and biaxial tube tests over specified stress/temperature histories. (author)
Finite element modelling of creep process - steady state stresses and strains
Directory of Open Access Journals (Sweden)
Sedmak Aleksandar S.
2014-01-01
Full Text Available Finite element modelling of steady state creep process has been described. Using an analogy of visco-plastic problem with a described procedure, the finite element method has been used to calculate steady state stresses and strains in 2D problems. An example of application of such a procedure have been presented, using real life problem - cylindrical pipe with longitudinal crack at high temperature, under internal pressure, and estimating its residual life, based on the C*integral evaluation.
A continuum model for the anisotropic creep of single crystal nickel-based superalloys
International Nuclear Information System (INIS)
Prasad, Sharat C.; Rajagopal, K.R.; Rao, I.J.
2006-01-01
In this paper, we extend the constitutive theory developed by Prasad et al. [Prasad SC, Rao IJ, Rajagopal KR. A continuum model for the creep of single crystal nickel-base superalloys. Acta Mater 2005;53(3):669-79], to describe the creep anisotropy associated with crystallographic orientation in single crystal nickel-based superalloys. The constitutive theory is cast within a general thermodynamic framework that has been developed to describe the response of materials capable of existing in multiple stress free configurations ('natural configurations'). Central to the theory is the prescription of the forms for the stored energy and rate of dissipation functions. The stored energy reflects the fact that the elastic response exhibits cubic symmetry. The model takes into account the fact that the symmetry of single crystals does not change with inelastic deformation. The rate of dissipation function is also chosen to be anisotropic, in that it reflects invariance to transformations that belong to the cubic symmetry group. The model is used to simulate uniaxial creep of single crystal nickel-based superalloy CMSX-4 for loading along the , and orientations. The predictions of the theory agree well with the experimental data
Analytical modeling of tube-to-tubesheet joints subjected to plasticity and creep
International Nuclear Information System (INIS)
Bouzid, A.-H.; Laghzale, N-E.
2009-01-01
The mechanism of failure of heat exchanger and steam generator tube-to-tubesheet joints is related to the level of residual stresses produced in the tube expansion and transition zones during the expansion process and their variation during operation. The accurate prediction of these stresses based of the plastic and creep properties of the joint materials involved can help to design for better leak tightness and strength. Existing design calculations are based on an elastic perfectly plastic behavior of the expansion joint materials and do not account for creep. The proposed model is based on a linear strain hardening material behavior and considers the joint contact pressure relaxation with time. The interaction of the tube and the tubesheet is simulated during the process of the application of the expansion pressure and operation. The effects of the gap, material strain hardening and creep properties are to be emphasized. The developed model results are validated and confronted against the more accurate numerical FEA models. (author)
Modeling and preliminary thermal analysis of the capsule for a creep test in HANARO
International Nuclear Information System (INIS)
Choi, Myoung Hwan; Cho, Man Soon; Choo, Kee Nam; Kang, Young Hwan; Sohn, Jae Min; Shin, Yoon Taeg; Park, Sung Jae; Kim, Bong Goo; Kim, Young Jin
2005-01-01
A creep capsule is a device to investigate the creep characteristics of nuclear materials during inpile irradiation tests. To obtain the design data of the capsule through a preliminary thermal analysis, a 2-dimensional model for the cross section of the capsule including the specimens and components is generated, and an analysis using the ANSYS program is performed. The gamma-heating rates of the materials for the HANARO power of 30MW are considered, and the effect of the gap size and the control rod position on the temperature of the specimen is discussed. From the analysis it is found that the gap between the thermal media and the external tube has a significant effect on the temperature of the specimen. The temperature by increasing the position of the control rod is decreased
Damage Models for Soft Tissues: A Survey.
Li, Wenguang
Damage to soft tissues in the human body has been investigated for applications in healthcare, sports, and biomedical engineering. This paper reviews and classifies damage models for soft tissues to summarize achievements, identify new directions, and facilitate finite element analysis. The main ideas of damage modeling methods are illustrated and interpreted. A few key issues related to damage models, such as experimental data curve-fitting, computational effort, connection between damage and fractures/cracks, damage model applications, and fracture/crack extension simulation, are discussed. Several new challenges in the field are identified and outlined. This review can be useful for developing more advanced damage models and extending damage modeling methods to a variety of soft tissues.
International Nuclear Information System (INIS)
Pusch, R.; Adey, R.
1999-12-01
The study involved characterization of the microstructural arrangement and molecular forcefields in the buffer clay for getting a basis for selecting suitable creep models. It is concluded that the number of particles and wide range of the particle bond spectrum require that stochastical mechanics and thermodynamics will be considered and they are basic to the creep model proposed for predicting creep settlement of the canisters. The influence of the stress level on creep strain of MX-80 clay is not well known but for the buffer creep is approximately proportional to stress. Theoretical considerations suggest a moderate impact for temperatures up to 90 deg C and this is supported by model experiments. It is believed that the assumption of strain being proportional to temperature is conservative. The general performance of the stochastic model can be illustrated in principle by use of visco-elastic rheological models implying a time-related increase in viscosity. The shear-induced creep settlement under constant volume conditions calculated by using the proposed creep model is on the order of 1 mm in ten thousand years and up to a couple of millimeters in one million years. It is much smaller than the consolidation settlement, which is believed to be on the order of 10 mm. The general conclusion is that creep settlement of the canisters is very small and of no significance to the integrity of the buffer itself or of the canisters
Improved methods of creep-fatigue life assessment of components
Energy Technology Data Exchange (ETDEWEB)
Scholz, Alfred; Berger, Christina [Inst. fuer Werkstoffkunde (IfW), Technische Univ. Darmstadt (Germany)
2009-07-01
The improvement of life assessment methods contributes to a reduction of efforts at design and an effective long term operation of high temperature components, reduces technical risk and increases high economical advantages. Creep-fatigue at multi-stage loading, covering cold start, warm start and hot start cycles in typical loading sequences e.g. for medium loaded power plants, was investigated here. At hold times creep and stress relaxation, respectively, lead to an acceleration of crack initiation. Creep fatigue life time can be calculated by a modified damage accumulation rule, which considers the fatigue fraction rule for fatigue damage and the life fraction rule for creep damage. Mean stress effects, internal stress and interaction effects of creep and fatigue are considered. Along with the generation of advanced creep data, fatigue data and creep fatigue data as well scatter band analyses are necessary in order to generate design curves and lower bound properties inclusive. Besides, in order to improve lifing methods the enhancement of modelling activities for deformation and life time are important. For verification purposes, complex experiments at variable creep conditions as well as at creep fatigue interaction under multi-stage loading are of interest. Generally, the development of methods to transfer uniaxial material properties to multiaxial loading situations is a current challenge. For specific design purposes, a constitutive material model is introduced which is implemented as an user subroutine for Finite Element applications due to start-up and shut-down phases of components. Identification of material parameters have been performed by Neural Networks. (orig.)
Energy Technology Data Exchange (ETDEWEB)
Hernelind, Jan [5T Engineering AB, Vaesteraas (Sweden)
2006-08-15
March, 2000, a study regarding 'Earthquake induced rock shear through a deposition hole' was performed. Existing fractures crossing a deposition hole may be activated and sheared by an earthquake. The effect of such a rock shear has been investigated in a project that includes both laboratory tests and finite element calculations. The buffer material in a deposition hole acts as a cushion between the canister and the rock, which reduces the effect of a rock shear substantially. Lower density of the buffer yields softer material and reduced effect on the canister. However, at the high density that is suggested for a repository the stiffness of the buffer is rather high. The stiffness is also a function of the rate of shear, which means that there may be a substantial damage on the canister at very high shear rates. The rock shear has been modeled with finite element calculations with the code ABAQUS. A three-dimensional finite element mesh of the buffer and the canister has been created and simulation of a rock shear has been performed. The rock shear has been assumed to take place perpendicular to the canister at the quarter point. The shear calculations have been driven to a total shear of 20 cm. This report summarizes the effect of considering creep in the canister for one of the previous cases. Two different creep models have been used - the first one has been suggested by K Pettersson and the second one has been suggested by R Sandstroem. Both have been implemented in the FE-code ABAQUS as a user supplied subroutine CREEP. This report summarizes results obtained by using the first model suggested by K Pettersson. As can be seen from the obtained results using the first creep model (in the following named creep{sub k}p) the effect of creep in copper doesn't affect stresses and strains in the buffer and the steel part very much. However, especially the stresses in the canister are highly affected.
Improvements of Spiers model for compaction creep of crushed rock salt
International Nuclear Information System (INIS)
Poley, A.D.
1996-10-01
This report describes a number of improvements to the existing model for the process of compaction creep of rock salt developed by Spiers and co-workers. The process of compaction creep determines the behaviour of the seals of crushed rock salt, the last engineered barriers of a repository in rock salt for (radioactive) wastes. In Chapter 2 the derivation of the original model of Spiers and co-workers is followed except for some simplifying approximations. A comparison of the model results is made with experimental data and a number of model adjustments are suggested. In Chapter 3 one of these suggested model adjustments is explored, and an alternative model is developed. The results obtained with this model compare favourably with the experimental data without the use of adjustable shape functions as for the original model. Preliminary investigations of the impact of the new model on estimated releases to the geosphere of radionuclides form a repository in rock salt revealed striking differences: with the new model the compaction of the rock salt seals was so rapid that no releases could occur. The striking differences between the results - in terms of releases form a rock salt repository to the geosphere after groundwater intrusion - obtained using the two models clearly indicate the need for further experimental research into the end-compaction behaviour of rock salt backfill. (orig.)
Study on the creep constitutive equation of Hastelloy X, (1)
International Nuclear Information System (INIS)
Hada, Kazuhiko; Mutoh, Yasushi
1983-01-01
A creep constitutive equation of Hastelloy X was obtained from available experimental data. A sensitivity analysis of this creep constitutive equation was carried out. As the result, the following were revealed: (i) Variations in creep behavior with creep constitutive equation are not small. (ii) In a simpler stress change pattern, variations in creep behavior are similar to those in the corresponding fundamental creep characteristics (creep strain curve, stress relaxation curve, etc.). (iii) Cumulative creep damage estimated in accordance with ASME Boiler and Pressure Vessel Code Case N-47 from a stress history predicted by ''the standard creep constitutive equation'' which predicts the average behavior of creep strain curve data is not thought to be on the safe side on account of uncertainties in creep damage caused by variations in creep strain curve. (author)
Morscher, Greg; Gowayed, yasser; Miller, Robert; Ojard, Greg; Ahmad, Jalees; Santhosh, Unni; John, Reji
2008-01-01
An understanding of the elevated temperature tensile creep, fatigue, rupture, and retained properties of ceramic matrix composites (CMC) envisioned for use in gas turbine engine applications are essential for component design and life-prediction. In order to quantify the effect of stress, time, temperature, and oxidation for a state-of-the-art composite system, a wide variety of tensile creep, dwell fatigue, and cyclic fatigue experiments were performed in air at 1204 C for the SiC/SiC CMC system consisting of Sylramic-iBN SiC fibers, BN fiber interphase coating, and slurry-cast melt-infiltrated (MI) SiC-based matrix. Tests were either taken to failure or interrupted. Interrupted tests were then mechanically tested at room temperature to determine the residual properties. The retained properties of most of the composites subjected to tensile creep or fatigue were usually within 20% of the as-produced strength and 10% of the as-produced elastic modulus. It was observed that during creep, residual stresses in the composite are altered to some extent which results in an increased compressive stress in the matrix upon cooling and a subsequent increased stress required to form matrix cracks. Microscopy of polished sections and the fracture surfaces of specimens which failed during stressed-oxidation or after the room-temperature retained property test was performed on some of the specimens in order to quantify the nature and extent of damage accumulation that occurred during the test. It was discovered that the distribution of stress-dependent matrix cracking at 1204 C was similar to the as-produced composites at room temperature; however, matrix crack growth occurred over time and typically did not appear to propagate through thickness except at final failure crack. Failure of the composites was due to either oxidation-induced unbridged crack growth, which dominated the higher stress regime (> 179 MPa) or controlled by degradation of the fibers, probably caused by
Shutov, A. V.; Larichkin, A. Yu
2017-10-01
A cyclic creep damage model, previously proposed by the authors, is modified for a better description of the transient creep of D16T alloy observed in the finite strain range under rapidly changing stresses. The new model encompasses the concept of kinematic hardening, which allows us to account for the creep-induced anisotropy. The model kinematics is based on the nested multiplicative split of the deformation gradient, proposed by Lion. The damage evolution is accounted for by the classical Kachanov-Rabotnov approach. The material parameters are identified using experimental data on cyclic torsion of thick-walled samples with different holding times between load reversals. For the validation of the proposed material model, an additional experiment is analyzed. Although this additional test is not involved in the identification procedure, the proposed cyclic creep damage model describes it accurately.
International Nuclear Information System (INIS)
Lee, Jae Yong; Na, Man Gyun
2011-01-01
Diametral creep of the pressure tube (PT) is one of the principal aging mechanisms governing the heat transfer and hydraulic degradation of a heat transport system. PT diametral creep leads to diametral expansion that affects the thermal hydraulic characteristics of the coolant channels and the critical heat flux. Therefore, it is essential to predict the PT diametral creep in CANDU reactors, which is caused mainly by fast neutron irradiation, reactor coolant temperature and so forth. The currently used PT diametral creep prediction model considers the complex interactions between the effects of temperature and fast neutron flux on the deformation of PT zirconium alloys. The model assumes that long-term steady-state deformation consists of separable, additive components from thermal creep, irradiation creep and irradiation growth. This is a mechanistic model based on measured data. However, this model has high prediction uncertainty. Recently, a statistical error modeling method was developed using plant inspection data from the Bruce B CANDU reactor. The aim of this study was to develop a bundle position-wise linear model (BPLM) to predict PT diametral creep employing previously measured PT diameters and HTS operating conditions. There are twelve bundles in a fuel channel and for each bundle, a linear model was developed by using the dependent variables, such as the fast neutron fluxes and the bundle temperatures. The training data set was selected using the subtractive clustering method. The data of 39 channels that consist of 80 percent of a total of 49 measured channels from Units 2, 3 and 4 were used to develop the BPLM models. The remaining 10 channels' data were used to test the developed BPLM models. The BPLM was optimized by the maximum likelihood estimation method. The developed BPLM to predict PT diametral creep was verified using the operating data gathered from the Units 2,3 and 4 in Korea. Two error components for the BPLM, which are the epistemic
Model - including thermal creep effects - for the analysis of three-dimensional concrete structures
International Nuclear Information System (INIS)
Rodriguez, C.; Rebora, B.; Favrod, J.D.
1979-01-01
This article presents the most recent developments and results of research carried out by IPEN to establish a mathematical model for the non-linear rheological three-dimensional analysis of massive prestressed concrete structures. The main point of these latest developments is the simulation of the creep of concrete submitted to high temperatures over a long period of time. This research, financed by the Swiss National Science Foundation, has taken an increased importance with the advent of nuclear reactor vessels of the HHT type and new conceptions concerning the cooling of their concrete (replacement of the thermal insulation by a zone of hot concrete). (orig.)
Do we have an acceptable model of power-law creep?
CSIR Research Space (South Africa)
Nabarro, FRN
2004-12-15
Full Text Available 387–389 (2004) 659–664 Do we have an acceptable model of power-law creep? F.R.N. Nabarro a,b,∗ a Condensed Matter Physics Research Group, School of Physics, University of the Witwatersrand, Private Bag 3, Johannesburg WITS 2050, South Africa b... an exponential function 0921-5093/$ – see front matter © 2004 Published by Elsevier B.V. doi:10.1016/j.msea.2003.09.118 660 F.R.N. Nabarro / Materials Science and Engineering A 387–389 (2004) 659–664 of the stress. There is little evidence whether the physical...
International Nuclear Information System (INIS)
Kim, Woo-Gon; Yin, Song-Nan; Koo, Gyeong-Hoi
2009-01-01
This study dealt with the construction of long-term isochronous stress-strain curves (ISSC) by a modeling of short-term creep curves for a Grade 9Cr-1Mo steel (G91) which is a candidate material for structural applications in the next generation nuclear reactors as well as in fusion reactors. To do this, tensile material data used in the inelastic constitutive equations was obtained by tensile tests at 550degC. Creep curves were obtained by a series of creep tests with different stress levels of 300MPa to 220MPa at an identical controlled temperature of 550degC. On the basis of these experimental data, the creep curves were characterized by Garofalo's creep model. Three parameters of P 1 , P 2 and P 3 in Garofalo's model were properly optimized by a nonlinear least square fitting (NLSF) analysis. The stress dependency of the three parameters was found to be a linear relationship. But, the P 3 parameter representing the steady state creep rate exhibited a two slope behavior with different stress exponents at a transient stress of about 250 MPa. The long-term creep curves of the G91 steel was modeled by Garofalo's model with only a few short-term creep data. Using the modeled creep curves, the long-term isochronous curves up to 10 5 hours were successfully constructed. (author)
Gholamhoseini, Alireza
2016-03-01
Relatively little research has been reported on the time-dependent in-service behavior of composite concrete slabs with profiled steel decking as permanent formwork and little guidance is available for calculating long-term deflections. The drying shrinkage profile through the thickness of a composite slab is greatly affected by the impermeable steel deck at the slab soffit, and this has only recently been quantified. This paper presents the results of long-term laboratory tests on composite slabs subjected to both drying shrinkage and sustained loads. Based on laboratory measurements, a design model for the shrinkage strain profile through the thickness of a slab is proposed. The design model is based on some modifications to an existing creep and shrinkage prediction model B3. In addition, an analytical model is developed to calculate the time-dependent deflection of composite slabs taking into account the time-dependent effects of creep and shrinkage. The calculated deflections are shown to be in good agreement with the experimental measurements.
An Eulerian-Lagrangian finite-element method for modeling crack growth in creeping materials
International Nuclear Information System (INIS)
Lee Hae Sung.
1991-01-01
This study is concerned with the development of finite-element-solution methods for analysis of quasi-static, ductile crack growth in history-dependent materials. The mixed Eulerian-Langrangian description (ELD) kinematic model is shown to have several desirable properties for modeling inelastic crack growth. Accordingly, a variational statement based on the ELD for history-dependent materials is developed, and a new moving-grid finite-element method based on the variational statement is presented. The moving-grid finite-element method based on the variational statement is presented. The moving-grid finite-element method is applied to the analysis of transient, quasi-static, mode-III crack growth in creeping materials. A generalized Petrov-Galerkin method (GPG) is developed that simultaneously stabilizes the statement to admit L 2 basis functions for the nonlinear strain field. Quasi-static, model-III crack growth in creeping materials under small-scale-yielding (SSY) conditions is considered. The GPG/ELD moving-grid finite-element formulation is used to model a transient crack-growth problem. The GPG/ELD results compare favorably with previously-published numerical results and the asymptotic solutions
The importance of the strain rate and creep on the stress corrosion cracking mechanisms and models
International Nuclear Information System (INIS)
Aly, Omar F.; Mattar Neto, Miguel; Schvartzman, Monica M.A.M.
2011-01-01
Stress corrosion cracking is a nuclear, power, petrochemical, and other industries equipment and components (like pressure vessels, nozzles, tubes, accessories) life degradation mode, involving fragile fracture. The stress corrosion cracking failures can produce serious accidents, and incidents which can put on risk the safety, reliability, and efficiency of many plants. These failures are of very complex prediction. The stress corrosion cracking mechanisms are based on three kinds of factors: microstructural, mechanical and environmental. Concerning the mechanical factors, various authors prefer to consider the crack tip strain rate rather than stress, as a decisive factor which contributes to the process: this parameter is directly influenced by the creep strain rate of the material. Based on two KAPL-Knolls Atomic Power Laboratory experimental studies in SSRT (slow strain rate test) and CL (constant load) test, for prediction of primary water stress corrosion cracking in nickel based alloys, it has done a data compilation of the film rupture mechanism parameters, for modeling PWSCC of Alloy 600 and discussed the importance of the strain rate and the creep on the stress corrosion cracking mechanisms and models. As derived from this study, a simple theoretical model is proposed, and it is showed that the crack growth rate estimated with Brazilian tests results with Alloy 600 in SSRT, are according with the KAPL ones and other published literature. (author)
Kumar, Parikshith K.; Desai, Uri; Chatzigeorgiou, George; Lagoudas, Dimitris C.; Monroe, James; Karaman, Ibrahim; Noebe, Ron; Bigelow, Glen
2010-01-01
The present work is focused on studying the cycling actuation behavior of HTSMAs undergoing simultaneous creep and transformation. For the thermomechanical testing, a high temperature test setup was assembled on a MTS frame with the capability to test up to temperatures of 600 C. Constant stress thermal cycling tests were conducted to establish the actuation characteristics and the phase diagram for the chosen HTSMA. Additionally, creep tests were conducted at constant stress levels at different test temperatures to characterize the creep behavior of the alloy over the operational range. A thermodynamic constitutive model is developed and extended to take into account a) the effect of multiple thermal cycling on the generation of plastic strains due to transformation (TRIP strains) and b) both primary and secondary creep effects. The model calibration is based on the test results. The creep tests and the uniaxial tests are used to identify the viscoplastic behavior of the material. The parameters for the SMA properties, regarding the transformation and transformation induced plastic strain evolutions, are obtained from the material phase diagram and the thermomechanical tests. The model is validated by predicting the material behavior at different thermomechanical test conditions.
International Nuclear Information System (INIS)
Ogata, Takashi; Nitta, Akito
1994-01-01
Creep-fatigue damage in high temperature structural components in a FBR progress under multiaxial stress condition depending on their operating conditions and configuration. Therefore, multiaxial stress effects on creep-fatigue damage evolution must be clarified to make precise creep-fatigue damage evaluation of these components. In this study, creep-fatigue tests in FBR high temperature materials such as SUS304, 316FR stainless steels and a modified 9Cr steel were conducted under biaxial stress subjecting tension-compression and torsion loading, in order to examine biaxial stress effects on failure mechanism and life property, and to discuss creep-fatigue life evaluation methods under biaxial stress. Main results obtained in this study are summarized as follows: 1. The main cracks under cyclic torsion loading propagated by shear mode in three materials. But intergranular failure was occurred in SUS304 and 316FR, and transgranular failure was observed in Mod.9Cr steel. 2. Nonlinear damage accumulation model proposed based on uniaxial creep-fatigue test results was extended to apply for creep-fatigue damage evaluation under biaxial stress state by considering the biaxial stress effects on fatigue and creep damage evolution. 3. It was confirmed that creep-fatigue life under biaxial stress could be predicted by the extended evaluation method with higher accuracy than existing methods. (author)
Coupled Modeling of Groundwater Flow and Land Subsidence with Secular Strain (Creep)
Bakr, M.
2012-12-01
Land subsidence limits sustainable development of many areas around the world. This is especially the case in low lying regions such as deltas which accommodate a significant percentage of the human population. Among the most common human-induced factors for land subsidence, is groundwater extractions. In these cases, groundwater flow and land subsidence are coupled processes, especially in basins with extensive spatial extent of soft soils (e.g. clay, peat). Creep (or secondary consolidation) is a land subsidence component that usually contributes to total land subsidence in soft soils. It leads to a reduction in void ratio at constant effective stress, and consequently, to the development of an apparent pre-consolidation pressure. The creep component has been usually ignored in the analysis of coupled groundwater flow and land subsidence. Here, the focus is the development of a coupled model of groundwater flow and land subsidence in porous media considering secular strain (creep). The Bjerrum method for settlement calculation (Bjerrum, 1967) due to change in effective stresses is coupled with MODFLOW to tackle the problem. In particular, the SUB-WT package of MODFLOW (Leake and Galloway, 2007) is modified where the Bjerrum method is used to calculate the primary and secondary consolidation due to change in effective stresses as a result of groundwater abstraction. The Bjerrum model is based on linear strains relationship. Usage of linear strains means that the model directly supports the common parameters Cr, Cc, Cα (i.e. re-compression, compression, and secondary compression indices; respectively). The Bjerrum model assumes that creep rate will reduce with increasing over-consolidation and that over-consolidation will grow by unloading and by ageing. To verify the coupled model, a hypothetical problem is considered where a simple hydrogeological system consisting of a shallow unconfined aquifer and a deeper confined aquifer separated by a (semi
Directory of Open Access Journals (Sweden)
Milašinović Dragan D.
2015-01-01
Full Text Available A new analytical model for the prediction of concrete response under uniaxial compression and its experimental verification is presented in this paper. The proposed approach, referred to as the rheological-dynamical continuum damage model, combines rheological-dynamical analogy and damage mechanics. Within the framework of this approach the key continuum parameters such as the creep coefficient, Poisson’s ratio and damage variable are functionally related. The critical values of the creep coefficient and damage variable under peak stress are used to describe the failure mode of the concrete cylinder. The ultimate strain is determined in the post-peak regime only, using the secant stress-strain relation from damage mechanics. The post-peak branch is used for the energy analysis. Experimental data for five concrete compositions were obtained during the examination presented herein. The principal difference between compressive failure and tensile fracture is that there is a residual stress in the specimens, which is a consequence of uniformly accelerated motion of load during the examination of compressive strength. The critical interpenetration displacements and crushing energy are obtained theoretically based on the concept of global failure analysis. [Projekat Ministarstva nauke Republike Srbije, br. ON 174027: Computational Mechanics in Structural Engineering i br. TR 36017: Utilization of by-products and recycled waste materials in concrete composites for sustainable construction development in Serbia: Investigation and environmental assessment of possible applications
Buchanan, Dennis J.; John, Reji; Brockman, Robert A.; Rosenberger, Andrew H.
2010-01-01
Shot peening is a commonly used surface treatment process that imparts compressive residual stresses into the surface of metal components. Compressive residual stresses retard initiation and growth of fatigue cracks. During component loading history, shot-peened residual stresses may change due to thermal exposure, creep, and cyclic loading. In these instances, taking full credit for compressive residual stresses would result in a nonconservative life prediction. This article describes a methodical approach for characterizing and modeling residual stress relaxation under elevated temperature loading, near and above the monotonic yield strength of INI 00. The model incorporates the dominant creep deformation mechanism, coupling between the creep and plasticity models, and effects of prior plastic strain to simulate surface treatment deformation.
International Nuclear Information System (INIS)
Haste, T.J.
1982-07-01
The CANSWEL-2 code models cladding creep deformation under conditions relevant to a loss-of-coolant accident (LOCA) in a pressurised water reactor (PWR). It considers in detail the centre rod of a 3 x 3 nominally square array, taking into account azimuthal non-uniformities in cladding thickness and temperature, and the mechanical restraint imposed on contact with neighbouring rods. Any of the rods in the array may assume a non-circular shape. Models are included for primary and secondary creep, dynamic phase change and superplasticity when both alpha- and beta-phase Zircaloy are present. A simple treatment of oxidation strengthening is incorporated. Account is taken of the anisotropic creep behaviour of alpha-phase Zircaloy which leads to cladding bowing. The CANSWEL-2 model is used both as a stand-alone code and also as part of the LOCA analysis code MABEL-2. (author)
A linear model of ductile plastic damage
International Nuclear Information System (INIS)
Lemaitre, J.
1983-01-01
A three-dimensional model of isotropic ductile plastic damage based on a continuum damage variable on the effective stress concept and on thermodynamics is derived. As shown by experiments on several metals and alloys, the model, integrated in the case of proportional loading, is linear with respect to the accumulated plastic strain and shows a large influence of stress triaxiality [fr
Uniaxial and Multiaxial Creep Testing of Copper
International Nuclear Information System (INIS)
Auerkari, Pertti; Holmstroem, Stefan; Veivo, Juha; Salonen, Jorma; Nenonen, Pertti; Laukkanen, Anssi
2003-12-01
Multiaxial (compact tension, CT) creep testing has been performed for copper with 79 ppm phosphorus and 60 ppm oxygen. The test load levels were selected according to results from preceding uniaxial creep testing and FE analysis of the CT specimens. Interrupted testing was used for metallographic inspection of the specimens for creep damage. After 7,900 h and 10,300 h of testing at 150 deg C and 46 MPa (reference stress), inspected CT specimens showed cavity indications with a low maximum density ( 2 ) and a typical maximum dimension of less than about 1 μm near the notch tip. From previous experience on creep cavitation damage, the expected minimum life to crack initiation at the notch tip would be at least 40,000 hours, but could be considerably longer because the cavity indications are suspected to originate at least partly from precipitates in specimen preparation. The interrupted testing of CT specimens also showed a 'segregation zone' along some grain boundaries, mainly near the notch tip. This zone appears to contain more P and O than the surrounding matrix, but less than the narrow grain boundary films that are already present in the as-new material. The zone is readily etched and shows a relatively sharp edge towards the matrix without an obvious phase boundary. Using converted multiaxial (CT) testing results, the predicted isothermal uniaxial creep life at 150 deg C/46 MPa is about 1,900 years. The corresponding creep life directly predicted from uniaxial data is 3,100 years, when estimated from a parametric best fit expression according to PD6605. Although the two results are satisfactorily within a factor of two in time, the uncertainties in the extended extrapolations remain large. Further testing is recommended, with at least two creep enhancing factors present. Such testing could include notched creep testing at 120-180 deg C in a corrosive environment, and notched model vessel creep testing at elevated pressure. It is also recommended that longer
Strength and life under creeping
International Nuclear Information System (INIS)
Pospishil, B.
1982-01-01
Certain examples of the application of the Lepin modified creep model, which are of interest from technical viewpoint, are presented. Mathematical solution of the dependence of strength limit at elevated temperatures on creep characteristics is obtained. Tensile test at elevated temperatures is a particular case of creep or relaxation and both strength limit and conventional yield strength at elevated temperatures are completely determined by parameters of state equations during creep. The equation of fracture summing during creep is confirmed not only by the experiment data when stresses change sporadically, but also by good reflection of durability curve using the system of equations. The system presented on the basis of parameters of the equations obtained on any part of durability curve, permits to forecast the following parameters of creep: strain, strain rate, life time, strain in the process of fracture. Tensile test at elevated temperature is advisable as an addition when determining creep curves (time-strain curves) [ru
International Nuclear Information System (INIS)
Harada, Y.; Maruyama, Y.; Chino, E.; Shibazaki, H.; Kudo, T.; Hidaka, A.; Hashimoto, K.; Sugimoto, J.
2000-01-01
The analytical study on severe accident shows the possibility of the reactor coolant system (RCS) piping failure before reactor pressure vessel failure under the high primary pressure sequence at pressurized water reactors. The establishment of the high-temperature strength model of the realistic RCS piping materials is important in order to predict precisely the accident progression and to evaluate the piping behavior with small uncertainties. Based on material testing, the 0.2% proof stress and the ultimate tensile strength above 800degC were given by the equations of second degree as a function of the reciprocal absolute temperature considering the strength increase due to fine precipitates for the piping materials. The piping materials include type 316 stainless steel, type 316 stainless steel of nuclear grade, CF8M cast duplex stainless steel and STS410 carbon steel. Also the short-term creep rupture time and the minimum creep rate at high-temperature were given by the modified Norton's Law as a function of stress and temperature considering the effect of the precipitation formation and resolution on the creep strength. The present modified Norton's Law gives better results than the conventional Larson-Miller method. Correlating the creep data (the applied stress versus the minimum creep rate) with the tensile data (the 0.2% proof stress or the ultimate tensile strength versus the strain rate), it was found that the dynamic recrystallization significantly occurred at high-temperature. (author)
International Nuclear Information System (INIS)
Munson, D.E.; Fossum, A.F.
1986-01-01
The US Department of Energy is constructing and operating the Waste Isolation Pilot Plant (WIPP), a research and development facility near Carlsbad, New Mexico, to determine whether or not defense-generated high-level radioactive waste can be stored safely in bedded salt. The goal of the WIPP modeling program is to develop the capability to predict room responses from one site to another without a priori knowledge of the actual room responses. Data from one of the early WIPP excavations, called the South Drift, have already been used to form an initial evaluation of computational models for predicting room closures as a result of salt creep. In that study, a significant unresolved discrepancy existed between predicted and measured room closures. It was suggested that future studies address alternate forms of the constitutive law. In this paper, an alternate form of the creep model for salt is used that is founded upon the deformation-mechanism map for the micromechanical deformation processes. This model embodies both steady-state and transient creep. Also, quasi-static plasticity is incorporated into the complete constitutive model for salt. The conclusion is drawn that the combination of the mechanistic creep model, plasticity, and flow potential can approximate the late time South Drift deformation. Further improvement of the model fit of plasticity in the future is expected to further improve the simulation
Intelligent-based Structural Damage Detection Model
International Nuclear Information System (INIS)
Lee, Eric Wai Ming; Yu, K.F.
2010-01-01
This paper presents the application of a novel Artificial Neural Network (ANN) model for the diagnosis of structural damage. The ANN model, denoted as the GRNNFA, is a hybrid model combining the General Regression Neural Network Model (GRNN) and the Fuzzy ART (FA) model. It not only retains the important features of the GRNN and FA models (i.e. fast and stable network training and incremental growth of network structure) but also facilitates the removal of the noise embedded in the training samples. Structural damage alters the stiffness distribution of the structure and so as to change the natural frequencies and mode shapes of the system. The measured modal parameter changes due to a particular damage are treated as patterns for that damage. The proposed GRNNFA model was trained to learn those patterns in order to detect the possible damage location of the structure. Simulated data is employed to verify and illustrate the procedures of the proposed ANN-based damage diagnosis methodology. The results of this study have demonstrated the feasibility of applying the GRNNFA model to structural damage diagnosis even when the training samples were noise contaminated.
Intelligent-based Structural Damage Detection Model
Lee, Eric Wai Ming; Yu, Kin Fung
2010-05-01
This paper presents the application of a novel Artificial Neural Network (ANN) model for the diagnosis of structural damage. The ANN model, denoted as the GRNNFA, is a hybrid model combining the General Regression Neural Network Model (GRNN) and the Fuzzy ART (FA) model. It not only retains the important features of the GRNN and FA models (i.e. fast and stable network training and incremental growth of network structure) but also facilitates the removal of the noise embedded in the training samples. Structural damage alters the stiffness distribution of the structure and so as to change the natural frequencies and mode shapes of the system. The measured modal parameter changes due to a particular damage are treated as patterns for that damage. The proposed GRNNFA model was trained to learn those patterns in order to detect the possible damage location of the structure. Simulated data is employed to verify and illustrate the procedures of the proposed ANN-based damage diagnosis methodology. The results of this study have demonstrated the feasibility of applying the GRNNFA model to structural damage diagnosis even when the training samples were noise contaminated.
Irradiation creep of candidate materials for advanced nuclear plants
Energy Technology Data Exchange (ETDEWEB)
Chen, J., E-mail: jiachao.chen@psi.ch; Jung, P.; Hoffelner, W.
2013-10-15
In the present paper, irradiation creep results of an intermetallic TiAl alloy and two ferritic oxide dispersion strengthened (ODS) steels are summarized. In situ irradiation creep measurements were performed using homogeneous implantation with α- and p-particles to maximum doses of 0.8 dpa at displacement damage rates of 2–8 × 10{sup −6} dpa/s. The strains of miniaturized flat dog-bone specimens were monitored under uniaxial tensile stresses ranging from 20 to 400 MPa at temperatures of 573, 673 and 773 K, respectively. The effects of material composition, ODS particle size, and bombarding particle on the irradiation creep compliance was studied and results are compared to literature data. Evolution of microstructure during helium implantation was investigated in detail by TEM and is discussed with respect to irradiation creep models.
Creep and creep-rupture behavior of Alloy 718
International Nuclear Information System (INIS)
Brinkman, C.R.; Booker, M.K.; Ding, J.L.
1991-01-01
Data obtained from creep and creep-rupture tests conducted on 18 heats of Alloy 718 were used to formulate models for predicting high temperature time dependent behavior of this alloy. Creep tests were conducted on specimens taken from a number of commercial product forms including plate, bar, and forgoing material that had been procured and heat treated in accordance with ASTM specifications B-670 or B-637. Data were obtained over the temperature range of 427 to 760 degree C ad at test times to about 87,000 h. Comparisons are given between experimental data and the analytical models. The analytical models for creep-rupture included one based on lot-centering regression analysis and two based on the Minimum Commitment Method. A ''master'' curve approach was used to develop and equation for estimating creep deformation up to the onset of tertiary creep. 11 refs., 13 figs
Creep of fibrous composite materials
DEFF Research Database (Denmark)
Lilholt, Hans
1985-01-01
Models are presented for the creep behaviour of fibrous composite materials with aligned fibres. The models comprise both cases where the fibres remain rigid in a creeping matrix and cases where the fibres are creeping in a creeping matrix. The treatment allows for several contributions...... to the creep strength of composites. The advantage of combined analyses of several data sets is emphasized and illustrated for some experimental data. The analyses show that it is possible to derive creep equations for the (in situ) properties of the fibres. The experiments treated include model systems...... such as Ni + W-fibres, high temperature materials such as Ni + Ni3Al + Cr3C2-fibres, and medium temperature materials such as Al + SiC-fibres. For the first two systems reasonable consistency is found for the models and the experiments, while for the third system too many unquantified parameters exist...
Statistical analysis and modelling of in-reactor diametral creep of Zr-2.5Nb pressure tubes
Energy Technology Data Exchange (ETDEWEB)
Jyrkama, Mikko I., E-mail: mjyrkama@uwaterloo.ca [Department of Civil and Environmental Engineering, University of Waterloo, 200 University Avenue West, Waterloo, ON, Canada N2L 3G1 (Canada); Bickel, Grant A., E-mail: grant.bickel@cnl.ca [Canadian Nuclear Laboratories, Chalk River Laboratories, Chalk River, ON, Canada K0J 1J0 (Canada); Pandey, Mahesh D., E-mail: mdpandey@uwaterloo.ca [Department of Civil and Environmental Engineering, University of Waterloo, 200 University Avenue West, Waterloo, ON, Canada N2L 3G1 (Canada)
2016-04-15
Highlights: • New and simple statistical model of pressure tube diametral creep. • Based on surveillance data of 328 pressure tubes from eight different CANDU reactors. • Uses weighted least squares (WLS) to regress out operating conditions. • The shape of the diametral creep profiles are predicted very well. • Provides insight and relative ranking of strain behaviour of in-service tubes. - Abstract: This paper presents the development of a simplified regression approach for modelling the diametral creep over time in Zr-2.5 wt% Nb pressure tubes used in CANDU reactors. The model is based on a large dataset of in-service inspection data of 328 different pressure tubes from eight different CANDU reactor units. The proposed weighted least squares (WLS) regression model is linear in time as a function of flux and temperature, with a temperature-dependent variance function. The model predicts the shape of the observed diametral creep profiles very well, and is useful not merely for prediction, but also for assessing tube-to-tube variability and manufacturing properties among the inspected tubes.
Creep behaviour and creep mechanisms of normal and healing ligaments
Thornton, Gail Marilyn
Patients with knee ligament injuries often undergo ligament reconstructions to restore joint stability and, potentially, abate osteoarthritis. Careful literature review suggests that in 10% to 40% of these patients the graft tissue "stretches out". Some graft elongation is likely due to creep (increased elongation of tissue under repeated or sustained load). Quantifying creep behaviour and identifying creep mechanisms in both normal and healing ligaments is important for finding clinically relevant means to prevent creep. Ligament creep was accurately predicted using a novel yet simple structural model that incorporated both collagen fibre recruitment and fibre creep. Using the inverse stress relaxation function to model fibre creep in conjunction with fibre recruitment produced a superior prediction of ligament creep than that obtained from the inverse stress relaxation function alone. This implied mechanistic role of fibre recruitment during creep was supported using a new approach to quantify crimp patterns at stresses in the toe region (increasing stiffness) and linear region (constant stiffness) of the stress-strain curve. Ligament creep was relatively insensitive to increases in stress in the toe region; however, creep strain increased significantly when tested at the linear region stress. Concomitantly, fibre recruitment was evident at the toe region stresses; however, recruitment was limited at the linear region stress. Elevating the water content of normal ligament using phosphate buffered saline increased the creep response. Therefore, both water content and fibre recruitment are important mechanistic factors involved in creep of normal ligaments. Ligament scars had inferior creep behaviour compared to normal ligaments even after 14 weeks. In addition to inferior collagen properties affecting fibre recruitment and increased water content, increased glycosaminoglycan content and flaws in scar tissue were implicated as potential mechanisms of scar creep
Model of designating the critical damages
Directory of Open Access Journals (Sweden)
Zwolińska Bożena
2017-06-01
Full Text Available The article consists of two parts which make for an integral body. This article depicts the method of designating the critical damages in accordance with lean maintenance method. Author considered exemplary production system (serial-parallel in which in time Δt appeared a damage on three different objects. Article depicts the mathematical model which enables determination of an indicator called “prioritized digit of the device”. In the developed model there were considered some parameters: production abilities of devices, existence of potential vicarious devices, position of damage in the production stream based on the capacity of operational buffers, time needed to remove the damages and influence of damages to the finalization of customers’ orders – CEF indicator.
The creep low application for numerical modeling of elastic-plastic flows
Tyapin, Anatoly; Rudenko, Vladimir; Chekhunov, Evgeny; Shaburov, Michail
1999-06-01
The present paper demonstrates the applicability of Lomnitz logarithm creep law [1] in some approximated version for calculating the elastic-plastic flows. The model has been developed resulting from the intention to have appropriate calculation approximation for particle-velocity -vs-time histories observed in plate 6061-T6 Al samples of various thickness under shock loading and subsequent release and additional compression. The approximation is unique in the whole loading range, from very low to such that elastic precursor is swallowed up by plastic wave . The model is based on Lipkin and Asay [2] remark on scale similarity of the above mentioned particle velocity -vs-time histories for equal shock loading and on approximate equality of velocities that initial portions of release and recompression waves travel at. A Lomnitz creep law presents an ideal phenomenological tool providing both of the requirements be fulfilled at the same time. Its application to high rate processes of loading and release has required some law modification and a nontrivial review of the dislocation mechanism for stress relaxation. The agreement achieved with the experiment is illustrated in figures. The model is worked out and realized in the 1D user software MAG. 1. Lomnitz C. Joun. of Geology, 1956, vol. 64, p. 473-479. 2. Lipkin J., Asay J.R. J. Appl. Phys. ,1977, vol. 48, 1, p.182-189. 3. Johnson J., Barker L. J. Appl. Phys., 1969, vol. 40, 11, p. 4321-4334. 4. Asay J.R., Chhabildas L. M.: Metallurgia., 1984, p. 110-120.
Energy Technology Data Exchange (ETDEWEB)
Ubic, Rick; Butt, Darryl; Windes, William
2014-03-13
An understanding of the underlying mechanisms of irradiation creep in graphite material is required to correctly interpret experimental data, explain micromechanical modeling results, and predict whole-core behavior. This project will focus on experimental microscopic data to demonstrate the mechanism of irradiation creep. High-resolution transmission electron microscopy should be able to image both the dislocations in graphite and the irradiation-induced interstitial clusters that pin those dislocations. The team will first prepare and characterize nanoscale samples of virgin nuclear graphite in a transmission electron microscope. Additional samples will be irradiated to varying degrees at the Advanced Test Reactor (ATR) facility and similarly characterized. Researchers will record microstructures and crystal defects and suggest a mechanism for irradiation creep based on the results. In addition, the purchase of a tensile holder for a transmission electron microscope will allow, for the first time, in situ observation of creep behavior on the microstructure and crystallographic defects.
International Nuclear Information System (INIS)
Matsuda, Akihiro; Yabana, Shuichi
2000-01-01
In this report, to evaluate creep properties and effects of creep deformation on mechanical properties of thick rubber bearings for three-dimensional isolation system, we show results of compression creep test for rubber bearings of various rubber materials and shapes and development of numerical simulation method. Creep properties of thick rubber bearings were obtained from compression creep tests. The creep strain shows steady creep that have logarithmic relationships between strain and time and accelerated creep that have linear relationships. We make numerical model of a rubber material with nonlinear viscoelastic constitutional equations. Mechanical properties after creep loading test are simulated with enough accuracy. (author)
Intermediate Co/Ni-base model superalloys — Thermophysical properties, creep and oxidation
International Nuclear Information System (INIS)
Zenk, Christopher H.; Neumeier, Steffen; Engl, Nicole M.; Fries, Suzana G.; Dolotko, Oleksandr; Weiser, Martin; Virtanen, Sannakaisa; Göken, Mathias
2016-01-01
The mechanical properties of γ′-strengthened Co–Ni–Al–W–Cr model superalloys extending from pure Ni-base to pure Co-base superalloys have been assessed. Differential scanning calorimetry measurements and thermodynamic calculations match well and show that the γ′ solvus temperature decreases with increasing Co-content. The γ/γ′ lattice misfit is negative on the Ni- and positive on the Co-rich side. High Ni-contents decelerate the oxidation kinetics up to a factor of 15. The creep strength of the Ni-base alloy increases by an order of magnitude with additions of Co before it deteriorates strongly upon higher additions despite an increasing γ′ volume fraction.
Modeling laser damage to the retina
Clark, Clifton D.
This dissertation presents recent progress in several areas related to modeling laser damage to the retina. In Chapter 3, we consider the consequences of using the Arrhenius damage model to predict the damage thresholds of multiple pulse, or repetitive pulse, exposures. We have identified a few fundamental trends associated with the multiple pulse damage predictions made by the Arrhenius model. These trends differ from what would be expected by non-thermal mechanisms, and could prove useful in differentiating thermal and non-thermal damage. Chapter 4 presents a new rate equation damage model hypothesized to describe photochemical damage. The model adds a temperature dependent term to the simple rate equation implied by the principle of reciprocity that is characteristic of photochemical damage thresholds. A recent damage threshold study, conducted in-vitro, has revealed a very sharp transition between thermal and photochemical damage threshold trends. For the wavelength used in the experiment (413 nm), thermal damage thresholds were observed at exposure levels that were twice the expected photochemical damage threshold, based on the traditional understanding of photochemical damage. Our model accounts for this observed trend by introducing a temperature dependent quenching, or repair, rate to the photochemical damage rate. For long exposures that give a very small temperature rise, the model reduces to the principle of reciprocity. Near the transition region between thermal and photochemical damage, the model allows the damage threshold to be set by thermal mechanisms, even at exposure above the reciprocity exposure. In Chapter 5, we describe a retina damage model that includes thermal lensing in the eye by coupling beam propagation and heat transfer models together. Thermal lensing has recently been suggested as a contributing factor to the large increase in measured retinal damage thresholds in the near infrared. The transmission of the vitreous decreases
Modelling the impact of creep on the probability of failure of a solid oxidefuel cell stack
DEFF Research Database (Denmark)
Greco, Fabio; Frandsen, Henrik Lund; Nakajo, Arata
2014-01-01
In solid oxide fuel cell (SOFC) technology a major challenge lies in balancing thermal stresses from an inevitable thermal field. The cells are known to creep, changing over time the stress field. The main objective of this study was to assess the influence of creep on the failure probability of ...
Creep of ex-service AISI-316H steel at very low strain rates
Energy Technology Data Exchange (ETDEWEB)
Kloc, Lubos; Sklenicka, Vaclav [Academy of Sciences of the Czech Republic, Brno (Czech Republic). Inst. of Physics of Materials; Spindler, Michael [British Energy Generation, Barbwood, Gloucester (United Kingdom)
2010-07-01
The creep response of ex-service Type 316H austenitic steel was investigated at temperatures from 470 to 550 C and stresses from 80 to 120 MPa. These conditions lead to very low strain rates. Both helicoid spring specimen tests and conventional uniaxial creep tests were used to measure these very low creep strains. An internal stress model was used to analyse the creep curves and the results were compared to creep curves obtained on a Type 316H in the as-received condition, which for austenitic steels is after solution heat treatment. The creep behavior of the ex-service steel was very similar to that of the as-received steel. Thus, no creep damage or significant change of microstructure was detected during the service period of 65,000 hours at {proportional_to} 520 C. It was found that the helicoid spring specimen technique provides results compatible with that of conventional creep tests, but with superior accuracy with very low creep strains. (orig.)
International Nuclear Information System (INIS)
Potirniche, Gabriel; Barlow, Fred D.; Charit, Indrajit; Rink, Karl
2013-01-01
A recent workshop on next-generation nuclear plant (NGNP) topics underscored the need for research studies on the creep fracture behavior of two materials under consideration for reactor pressure vessel (RPV) applications: 9Cr-1Mo and SA-5XX steels. This research project will provide a fundamental understanding of creep fracture behavior of modified 9Cr-1Mo steel welds for through modeling and experimentation and will recommend a design for an RPV structural health monitoring system. Following are the specific objectives of this research project: Characterize metallurgical degradation in welded modified 9Cr-1Mo steel resulting from aging processes and creep service conditions; Perform creep tests and characterize the mechanisms of creep fracture process; Quantify how the microstructure degradation controls the creep strength of welded steel specimens; Perform finite element (FE) simulations using polycrystal plasticity to understand how grain texture affects the creep fracture properties of welds; Develop a microstructure-based creep fracture model to estimate RPVs service life; Manufacture small, prototypic, cylindrical pressure vessels, subject them to degradation by aging, and measure their leak rates; Simulate damage evolution in creep specimens by FE analyses; Develop a model that correlates gas leak rates from welded pressure vessels with the amount of microstructural damage; Perform large-scale FE simulations with a realistic microstructure to evaluate RPV performance at elevated temperatures and creep strength; Develop a fracture model for the structural integrity of RPVs subjected to creep loads; and Develop a plan for a non-destructive structural health monitoring technique and damage detection device for RPVs.
Energy Technology Data Exchange (ETDEWEB)
Potirniche, Gabriel [Univ. of Idaho, Moscow, ID (United States); Barlow, Fred D. [Univ. of Idaho, Moscow, ID (United States); Charit, Indrajit [Univ. of Idaho, Moscow, ID (United States); Rink, Karl [Univ. of Idaho, Moscow, ID (United States)
2013-11-26
A recent workshop on next-generation nuclear plant (NGNP) topics underscored the need for research studies on the creep fracture behavior of two materials under consideration for reactor pressure vessel (RPV) applications: 9Cr-1Mo and SA-5XX steels. This research project will provide a fundamental understanding of creep fracture behavior of modified 9Cr-1Mo steel welds for through modeling and experimentation and will recommend a design for an RPV structural health monitoring system. Following are the specific objectives of this research project: Characterize metallurgical degradation in welded modified 9Cr-1Mo steel resulting from aging processes and creep service conditions; Perform creep tests and characterize the mechanisms of creep fracture process; Quantify how the microstructure degradation controls the creep strength of welded steel specimens; Perform finite element (FE) simulations using polycrystal plasticity to understand how grain texture affects the creep fracture properties of welds; Develop a microstructure-based creep fracture model to estimate RPVs service life; Manufacture small, prototypic, cylindrical pressure vessels, subject them to degradation by aging, and measure their leak rates; Simulate damage evolution in creep specimens by FE analyses; Develop a model that correlates gas leak rates from welded pressure vessels with the amount of microstructural damage; Perform large-scale FE simulations with a realistic microstructure to evaluate RPV performance at elevated temperatures and creep strength; Develop a fracture model for the structural integrity of RPVs subjected to creep loads; and Develop a plan for a non-destructive structural health monitoring technique and damage detection device for RPVs.
Rusinko, Andrew; Varga, Peter
2018-04-01
The paper deals with modelling of the plastic and creep deformation of metals coupled with current. The passage of DC manifests itself in the increase in creep deformation and leads to primary creep time shortening. With plastic deformation, a short electric impulse results in the step-wise decrease of stress (stress-drop) on the stress-strain diagram. To catch these phenomena, we utilize the synthetic theory of recoverable deformation. The constitutive equation of this theory is supplemented by a term taking into account the intensity of DC. Further, we introduce DC intensity into the function governing transient creep. As a result, we predict the parameters of transient creep and calculate the stress-drop as a function of current intensity. The model results show good agreement with experimental data.
Improving Flood Damage Assessment Models in Italy
Amadio, M.; Mysiak, J.; Carrera, L.; Koks, E.
2015-12-01
The use of Stage-Damage Curve (SDC) models is prevalent in ex-ante assessments of flood risk. To assess the potential damage of a flood event, SDCs describe a relation between water depth and the associated potential economic damage over land use. This relation is normally developed and calibrated through site-specific analysis based on ex-post damage observations. In some cases (e.g. Italy) SDCs are transferred from other countries, undermining the accuracy and reliability of simulation results. Against this background, we developed a refined SDC model for Northern Italy, underpinned by damage compensation records from a recent flood event. Our analysis considers both damage to physical assets and production losses from business interruptions. While the first is calculated based on land use information, production losses are measured through the spatial distribution of Gross Value Added (GVA). An additional component of the model assesses crop-specific agricultural losses as a function of flood seasonality. Our results show an overestimation of asset damage from non-calibrated SDC values up to a factor of 4.5 for tested land use categories. Furthermore, we estimate that production losses amount to around 6 per cent of the annual GVA. Also, maximum yield losses are less than a half of the amount predicted by the standard SDC methods.
Modeling the viscoplastic and damage behavior in deep argillaceous rocks
International Nuclear Information System (INIS)
Souley, M.; Armand, G.; Su, K.; Ghoreychi, M.
2011-01-01
In order to demonstrate the feasibility of a radioactive waste repository in the Callovo-Oxfordian clay-stone formation, the French national radioactive waste management agency (ANDRA) started in 2000 to build an underground research laboratory at Bure (East of France). One of the key issues is to understand long term behavior of the drifts. More than 400 m horizontal galleries at the main level of -490 m have been instrumented since April 2005. The continuous measurements of convergence of the galleries are available, allowing a better understanding of the time-dependent response of the clay-stone at natural scale. Results indicate that the viscoplastic strain rates observed in the undamaged area far from the gallery walls are of the same order of magnitude as those obtained on rock samples, whereas those recorded in the damaged or fractured zone near the gallery walls are one to two orders of magnitude higher, indicating the significant influence of damage or/and macro-fractures on the viscoplastic strains. Based on these observations, a macroscopic viscoplastic model which aims to improve the viscoplastic strain prediction in the EDZ is proposed and implemented in FLAC 3Dc . Both the instantaneous and the time-dependent behavior are considered in the model. The short term response is assumed to be elastoplastic with strain hardening/softening whereas the time-dependent behavior is based on the concepts of visco-plasticity (Lemaitre's model). Finally, the damage-induced viscoplastic strains changes is examined through the plastic deformation (assumed to approach the damage rate).In order to verify both constitutive equations and their implementations, several simulations are performed: (a) triaxial tests at different confining pressures; (b) single- and multi-stage creep tests; (c) relaxation tests with different total axial strain levels, etc. Finally, an example of a blind prediction of the excavation of a drift parallel to the horizontal minor stress,
Koharchik, Michael; Murphy, Lindsay; Parker, Paul
2012-01-01
An impact model was developed to predict how three specific foam types would damage the Space Shuttle Orbiter insulating tiles. The inputs needed for the model are the foam type, the foam mass, the foam impact velocity, the foam impact incident angle, the type being impacted, and whether the tile is new or aged (has flown at least one mission). The model will determine if the foam impact will cause damage to the tile. If it can cause damage, the model will output the damage cavity dimensions (length, depth, entry angle, exit angle, and sidewall angles). It makes the calculations as soon as the inputs are entered (less than 1 second). The model allows for the rapid calculation of numerous scenarios in a short time. The model was developed from engineering principles coupled with significant impact testing (over 800 foam impact tests). This model is applicable to masses ranging from 0.0002 up to 0.4 pound (0.09 up to 181 g). A prior tool performed a similar function, but was limited to the assessment of a small range of masses and did not have the large test database for verification. In addition, the prior model did not provide outputs of the cavity damage length, entry angle, exit angle, or sidewall angles.
Bast, Callie Corinne Scheidt
1994-01-01
This thesis presents the on-going development of methodology for a probabilistic material strength degradation model. The probabilistic model, in the form of a postulated randomized multifactor equation, provides for quantification of uncertainty in the lifetime material strength of aerospace propulsion system components subjected to a number of diverse random effects. This model is embodied in the computer program entitled PROMISS, which can include up to eighteen different effects. Presently, the model includes four effects that typically reduce lifetime strength: high temperature, mechanical fatigue, creep, and thermal fatigue. Statistical analysis was conducted on experimental Inconel 718 data obtained from the open literature. This analysis provided regression parameters for use as the model's empirical material constants, thus calibrating the model specifically for Inconel 718. Model calibration was carried out for four variables, namely, high temperature, mechanical fatigue, creep, and thermal fatigue. Methodology to estimate standard deviations of these material constants for input into the probabilistic material strength model was developed. Using the current version of PROMISS, entitled PROMISS93, a sensitivity study for the combined effects of mechanical fatigue, creep, and thermal fatigue was performed. Results, in the form of cumulative distribution functions, illustrated the sensitivity of lifetime strength to any current value of an effect. In addition, verification studies comparing a combination of mechanical fatigue and high temperature effects by model to the combination by experiment were conducted. Thus, for Inconel 718, the basic model assumption of independence between effects was evaluated. Results from this limited verification study strongly supported this assumption.
International Nuclear Information System (INIS)
Bocek, M.
A phenomenological cavitation model is presented by means of which the life time as well as the creep curve equations can be calculated for cavitating materials subjected to time variable tensile loads. The model precludes the proportionality between the damage A and the damage rate (dA/dt) resp. Both are connected by the life time function tau. The latter is derived from static stress rupture tests and contains the loading conditions. From this model the life fraction rule (LFR) is derived. The model is used to calculate the creep curves of cavitating materials subjected at high temperatures to non-stationary tensile loading conditions. In the present paper the following loading procedures are considered: creep at constant load F and true stress s; creep at linear load increase ((dF/dt)=const) and creep at constant load amplitude cycling (CLAC). For these loading procedures the creep equations for cavitating and non-cavitating specimens are derived. Under comparable conditions the creep rate of cavitating materials are higher than for non-cavitating ones. (author)
Modelling of Damage During Hot Forging of Ingots
DEFF Research Database (Denmark)
Christiansen, Peter; Hattel, Jesper Henri; Bay, Niels
2013-01-01
Ductile damage modelling in the ingot forging process is discussed. Advantages and disadvantages of both coupled and uncoupled ductile damage models are presented. Some uncoupled damage models are examined in greater detail regarding their applicability to different processes, where hydrostatic...
Energy Technology Data Exchange (ETDEWEB)
Neu, Richard W.
2017-09-30
The aim of this project is to develop a microstructure-sensitive crystal viscoplasticity (CVP) model for single-crystal Ni-base superalloys to model the behavior of the material and components in the hot gas path sections of industrial gas turbines (IGT). Microstructure degradation associated with aging critical to predicting long-term creep-fatigue interactions will be embedded into the model through the γ' precipitate morphology evolution by coupling the coarsening drivers and kinetics into the constitutive equations of the CVP model. Model parameters will be determined using new experimental protocols that involve systematically artificially aging the alloy under different stress conditions to determine the relationship between the size and morphology g' precipitates on the creep and thermomechanical fatigue response.
Energy Technology Data Exchange (ETDEWEB)
Neu, Richard W
2016-09-30
The aim of this project is to develop a microstructure-sensitive crystal viscoplasticity (CVP) model for single-crystal Ni-base superalloys to model the behavior of the material and components in the hot gas path sections of industrial gas turbines (IGT). Microstructure degradation associated with aging critical to predicting long-term creep-fatigue interactions will be embedded into the model through the γ' precipitate morphology evolution by coupling the coarsening drivers and kinetics into the constitutive equations of the CVP model. Model parameters will be determined using new experimental protocols that involve systematically artificially aging the alloy under different stress conditions to determine the relationship between the size and morphology g' precipitates on the creep and thermomechanical fatigue response.
Creep crack growth in phosphorus alloyed oxygen free copper
Energy Technology Data Exchange (ETDEWEB)
Wu, Rui; Seitisleam, Facredin (Swerea KIMAB (Sweden)); Sandstroem, Rolf; Jin, Lai-Zhe (Materials Science and Engineering, Royal Inst. of Technology (Sweden))
2011-01-15
Using standard compact tension (CT) specimens taken from a pierce and draw cylinder, creep crack growth (CCG) has been studied in phosphorus-alloyed oxygen-free copper (Cu-OFP) parent metal at 22, 75, 175, and 215 deg C. Pre- and post-test metallography are performed. At higher temperatures the rupture time of CCG is shorter by a factor up of 65 than that of uniaxial at same stress/reference stress. At 175 and 215 deg C, crack does grow by creep about 10 mm before final instantaneous failure. In contrast, there is hardly any visible crack growth at 22 and 75 deg C. The tests were interrupted after 5000 to 13000 hours. For ruptured tests at 175 and 215 deg C, strongly elongated and deformed grains are observed adjacent to crack. Extensive and intergranular creep cavities and microcracks are found several mm around crack. For interrupted tests at 22 and 75 deg C, strongly elongated and deformed grains, creep cavities, as well as microcracks are observed close to crack tip. Surface cracks from both sides have initiated and grown about 45 deg to the load direction towards inside. For the interrupted tests, hardness adjacent to crack tip has more than doubled because of work hardening, or heavy deformation. This is consistent with large crack tip opening. The true strain at the crack tip is estimated to 10 and 4 for the tests at 22 and 75 deg C, respectively. The stress state behind the crack tip has been modelled with FEM. Stress relaxation after loading has also been taken into account. A model for the creep damage based on the creep strain rate has been formulated that can describe the uniaxial creep rupture data without fitting parameters. Based on the formulation for the creep damage, a model for the crack propagation has been set up. When the creep damage has reached the value unity in front of the crack tip, the crack is assumed to propagate. Taking multiaxial effects into account the observed life times of the CT specimens can be well described. The multiaxial
Creep crack growth in phosphorus alloyed oxygen free copper
International Nuclear Information System (INIS)
Wu, Rui; Seitisleam, Facredin; Sandstroem, Rolf; Jin, Lai-Zhe
2011-01-01
Using standard compact tension (CT) specimens taken from a pierce and draw cylinder, creep crack growth (CCG) has been studied in phosphorus-alloyed oxygen-free copper (Cu-OFP) parent metal at 22, 75, 175, and 215 deg C. Pre- and post-test metallography are performed. At higher temperatures the rupture time of CCG is shorter by a factor up of 65 than that of uniaxial at same stress/reference stress. At 175 and 215 deg C, crack does grow by creep about 10 mm before final instantaneous failure. In contrast, there is hardly any visible crack growth at 22 and 75 deg C. The tests were interrupted after 5000 to 13000 hours. For ruptured tests at 175 and 215 deg C, strongly elongated and deformed grains are observed adjacent to crack. Extensive and intergranular creep cavities and microcracks are found several mm around crack. For interrupted tests at 22 and 75 deg C, strongly elongated and deformed grains, creep cavities, as well as microcracks are observed close to crack tip. Surface cracks from both sides have initiated and grown about 45 deg to the load direction towards inside. For the interrupted tests, hardness adjacent to crack tip has more than doubled because of work hardening, or heavy deformation. This is consistent with large crack tip opening. The true strain at the crack tip is estimated to 10 and 4 for the tests at 22 and 75 deg C, respectively. The stress state behind the crack tip has been modelled with FEM. Stress relaxation after loading has also been taken into account. A model for the creep damage based on the creep strain rate has been formulated that can describe the uniaxial creep rupture data without fitting parameters. Based on the formulation for the creep damage, a model for the crack propagation has been set up. When the creep damage has reached the value unity in front of the crack tip, the crack is assumed to propagate. Taking multiaxial effects into account the observed life times of the CT specimens can be well described. The multiaxial
Finite Element Modeling of Thermo Creep Processes Using Runge-Kutta Method
Directory of Open Access Journals (Sweden)
Yu. I. Dimitrienko
2015-01-01
Full Text Available Thermo creep deformations for most heat-resistant alloys, as a rule, nonlinearly depend on stresses and are practically non- reversible. Therefore, to calculate the properties of these materials the theory of plastic flow is most widely used. Finite-element computations of a stress-strain state of structures with account of thermo creep deformations up to now are performed using main commercial software, including ANSYS package. However, in most cases to solve nonlinear creep equations, one should apply explicit or implicit methods based on the Euler method of approximation of time-derivatives. The Euler method is sufficiently efficient in terms of random access memory in computations, however this method is cumbersome in computation time and does not always provide a required accuracy for creep deformation computations.The paper offers a finite-element algorithm to solve a three-dimensional problem of thermo creep based on the Runge-Kutta finite-difference schemes of different orders with respect to time. It shows a numerical test example to solve the problem on the thermo creep of a beam under tensile loading. The computed results demonstrate that using the Runge-Kutta method with increasing accuracy order allows us to obtain a more accurate solution (with increasing accuracy order by 1 a relative error decreases, approximately, by an order too. The developed algorithm proves to be efficient enough and can be recommended for solving the more complicated problems of thermo creep of structures.
International Nuclear Information System (INIS)
Sham, Sam; Walker, Kevin P.
2008-01-01
The expected service life of the Next Generation Nuclear Plant is 60 years. Structural analyses of the Intermediate Heat Exchanger (IHX) will require the development of unified viscoplastic constitutive models that address the material behavior of Alloy 617, a construction material of choice, over a wide range of strain rates. Many unified constitutive models employ a yield stress state variable which is used to account for cyclic hardening and softening of the material. For low stress values below the yield stress state variable these constitutive models predict that no inelastic deformation takes place which is contrary to experimental results. The ability to model creep deformation at low stresses for the IHX application is very important as the IHX operational stresses are restricted to very small values due to the low creep strengths at elevated temperatures and long design lifetime. This paper presents some preliminary work in modeling the unified viscoplastic constitutive behavior of Alloy 617 which accounts for the long term, low stress, creep behavior and the hysteretic behavior of the material at elevated temperatures. The preliminary model is presented in one-dimensional form for ease of understanding, but the intent of the present work is to produce a three-dimensional model suitable for inclusion in the user subroutines UMAT and USERPL of the ABAQUS and ANSYS nonlinear finite element codes. Further experiments and constitutive modeling efforts are planned to model the material behavior of Alloy 617 in more detail
Energy Technology Data Exchange (ETDEWEB)
Shen, Chen [GE Global Research, NIskayuna, NY (United States); Gupta, Vipul [GE Global Research, NIskayuna, NY (United States); Huang, Shenyan [GE Global Research, NIskayuna, NY (United States); Soare, Monica [GE Global Research, NIskayuna, NY (United States); Zhao, Pengyang [GE Global Research, NIskayuna, NY (United States); Wang, Yunzhi [GE Global Research, NIskayuna, NY (United States)
2017-02-28
The goal of this project is to model long-term creep performance for nickel-base superalloy weldments in high temperature power generation systems. The project uses physics-based modeling methodologies and algorithms for predicting alloy properties in heterogeneous material structures. The modeling methodology will be demonstrated on a gas turbine combustor liner weldment of Haynes 282 precipitate-strengthened nickel-base superalloy. The major developments are: (1) microstructure-property relationships under creep conditions and microstructure characterization (2) modeling inhomogeneous microstructure in superalloy weld (3) modeling mesoscale plastic deformation in superalloy weld and (4) a constitutive creep model that accounts for weld and base metal microstructure and their long term evolution. The developed modeling technology is aimed to provide a more efficient and accurate assessment of a material’s long-term performance compared with current testing and extrapolation methods. This modeling technology will also accelerate development and qualification of new materials in advanced power generation systems. This document is a final technical report for the project, covering efforts conducted from October 2014 to December 2016.
Eccentric pressurized tube for measuring creep rupture
International Nuclear Information System (INIS)
Schwab, P.R.
1981-01-01
Creep rupture is a long term failure mode in structural materials that occurs at high temperatures and moderate stress levels. The deterioration of the material preceding rupture, termed creep damage, manifests itself in the formation of small cavities on grain boundaries. To measure creep damage, sometimes uniaxial tests are performed, sometimes density measurements are made, and sometimes the grain boundary cavities are measured by microscopy techniques. The purpose of the present research is to explore a new method of measuring creep rupture, which involves measuring the curvature of eccentric pressurized tubes. Theoretical investigations as well as the design, construction, and operation of an experimental apparatus are included in this research
Directory of Open Access Journals (Sweden)
Partov Doncho
2017-01-01
Full Text Available The paper presents analysis of the stress-strain behaviour and deflection changes due to creep in statically determinate composite steel-concrete beam according to EUROCODE 2, ACI209R-92 and Gardner&Lockman models. The mathematical model involves the equation of equilibrium, compatibility and constitutive relationship, i.e. an elastic law for the steel part and an integral-type creep law of Boltzmann - Volterra for the concrete part considering the above mentioned models. On the basis of the theory of viscoelastic body of Maslov-Arutyunian-Trost-Zerna-Bažant for determining the redistribution of stresses in beam section between concrete plate and steel beam with respect to time 't', two independent Volterra integral equations of the second kind have been derived. Numerical method based on linear approximation of the singular kernel function in the integral equation is presented. Example with the model proposed is investigated.
Directory of Open Access Journals (Sweden)
Andrea Sorzia
2016-01-01
Full Text Available A tensile test until breakage and a creep and relaxation test on a polypropylene fibre are carried out and the resulting creep and stress relaxation curves are fit by a model adopting a fraction-exponential kernel in the viscoelastic operator. The models using fraction-exponential functions are simpler than the complex ones obtained from combination of dashpots and springs and, furthermore, are suitable for fitting experimental data with good approximation allowing, at the same time, obtaining inverse Laplace transform in closed form. Therefore, the viscoelastic response of polypropylene fibres can be modelled straightforwardly through analytical methods. Addition of polypropylene fibres greatly improves the tensile strength of composite materials with concrete matrix. The proposed analytical model can be employed for simulating the mechanical behaviour of composite materials with embedded viscoelastic fibres.
Creep of high temperature composites
International Nuclear Information System (INIS)
Sadananda, K.; Feng, C.R.
1993-01-01
High temperature creep deformation of composites is examined. Creep of composites depends on the interplay of many factors. One of the basic issues in the design of the creep resistant composites is the ability to predict their creep behavior from the knowledge of the creep behavior of the individual components. In this report, the existing theoretical models based on continuum mechanics principles are reviewed. These models are evaluated using extensive experimental data on molydisilicide-silicon carbide composites obtained by the authors. The analysis shows that the rule of mixture based on isostrain and isostress provides two limiting bounds wherein all other theoretical predictions fall. For molydisilicide composites, the creep is predominantly governed by the creep of the majority phase, i.e. the matrix with fibers deforming elastically. The role of back stresses both on creep rates and activation energies are shown to be minimum. Kinetics of creep in MoSi 2 is shown to be controlled by the process of dislocation glide with climb involving the diffusion of Mo atoms
Implementation of an anisotropic damage material model using general second order damage tensor
Niazi, Muhammad Sohail; Mori, K.; Wisselink, H.H.; Pietrzyk, M.; Kusiak, J.; Meinders, Vincent T.; ten Horn, Carel; Majta, J.; Hartley, P.; Lin, J.
2010-01-01
Damage in metals is mainly the process of the initiation and growth of voids. With the growing complexity in materials and forming proc-esses, it becomes inevitable to include anisotropy in damage (tensorial damage variable). Most of the anisotropic damage models define the damage tensor in the
International Nuclear Information System (INIS)
Inoue, T.; Ohno, N.; Suzuki, A.; Igari, T.
1987-01-01
The authorization of constitutive models under plasticity-creep condition and life estimation methods in fatigue-creep regime is expected to be achieved from the viewpoint of design purposes of high temperature components of reactor structures. The present Subcommittee has performed the cooperative project consisting of the following two parts: (A) To review and evaluate inelastic constitutive models relevant to the material response under plasticity-creep interaction and (B) to recommend some adequate methods to estimate material life under fatigue-creep interaction by taking account of the effect of plasticity-creep interaction on the stress-strain hysteresis loops. The material treated is normalized and tempered 2 1/4 Cr-1Mo steel at 600 0 C. The part (A) plays a preliminary role for the part (B), since the constitutive models examined in the part (A) were used to describe the stress-strain hysteresis loops necessary to predict analytically the lives under fatigue-creep interaction. In the part (A), thererfore, it is important to check how accurately the constitutive models simulate the stress-strain hysteresis loops especially by taking account of the effect of plasticity-creep interaction. (orig./GL)
International Nuclear Information System (INIS)
Yang, F.Q.; Xue, H.; Zhao, L.Y.; Fang, X.R.
2014-01-01
Highlights: • Creep is considered to be the primary mechanical factor of crack tip film degradation. • The prediction model of SCC rate is based on crack tip creep strain rate. • The SCC rate calculated at the secondary stage of creep is recommended. • The effect of stress intensity factor on SCC growth rate is discussed. - Abstract: The quantitative prediction of stress corrosion cracking (SCC) of structure materials is essential in safety assessment of nuclear power plants. A new quantitative prediction model is proposed by combining the Ford–Andresen model, a crack tip creep model and an elastic–plastic finite element method. The creep at the crack tip is considered to be the primary mechanical factor of protective film degradation, and the creep strain rate at the crack tip is suggested as primary mechanical factor in predicting the SCC rate. The SCC rates at secondary stage of creep are recommended when using the approach introduced in this study to predict the SCC rates of materials in high temperature water. The proposed approach can be used to understand the SCC crack growth in structural materials of light water reactors
A stochastic model for the interaction of plasticity and creep in metals
International Nuclear Information System (INIS)
Steck, E.
1987-01-01
Describing the basic mechanisms for plastic deformations in crystalline materials by transition probabilities of a stochastic matrix over the state space of the internal barriers, results in a stochastic model which has the properties of a Markov-chain. It is possible to include in this model properties of the internal structure of the material and their changes during macroscopic deformation processes, such as hardening and recovery, or the influence of temperature on thermal activation. This description can be based on findings from metal physics and metallurgy, so that the stochastic model can be used as an intermediate model between the microscopic and the macroscopic description of the processes during plastic deformations. Inelastic deformations of crystalline materials (plasticity, creep, relaxation) are caused by slip processes in the crystal-lattice which are supported by movements of dislocations. The dislocation movements are opposed by internal barriers which have to be overcome by activation of the dislocations. This activation can be performed by stresses, which are in equilibrium with external forces, or by thermal energy. With the movements of dislocations and the connected slip processes, production of new dislocations occurs. The dislocations interact. This can result either in a reduction of their mobility or in annihilation. These processes are partially responsible for hardening or recovery. (orig./GL)
A Semi-analytical model for creep life prediction of butt-welded joints in cylindrical vessels
International Nuclear Information System (INIS)
Zarrabi, K.
2001-01-01
There have been many investigations on the life assessment of high temperature weldments used in cylindrical pressure vessels, pipes and tubes over the last two decades or so. But to the author's knowledge, currently, there exists no practical, economical and relatively accurate model for creep life assessment of butt-welded joints in cylindrical pressure vessels. This paper describes a semi-analytical and economical model for creep life assessment of butt-welded joints. The first stage of the development of the model is described where the model takes into account the material discontinuities at the welded joint only. The development of the model to include other factors such as geometrical stress concentrations, residual stresses, etc will be reported separately. It has been shown that the proposed model can estimate the redistributions of stresses in the weld and Haz with an error of less than 4%. It has also been shown that the proposed model can conservatively predict the creep life of a butt-welded joint with an error of less than 16%
Early models of DNA damage formation
International Nuclear Information System (INIS)
Śmiałek, Małgorzata A
2012-01-01
Quantification of DNA damage, induced by various types of incident radiation as well as chemical agents, has been the subject of many theoretical and experimental studies, supporting the development of modern cancer therapy. The primary observations showed that many factors can lead to damage of DNA molecules. It became clear that the development of experimental techniques for exploring this phenomenon is required. Another problem was simultaneously dealt with, anticipating on how the damage is distributed within the double helix of the DNA molecule and how the single strand break formation and accumulation can influence the lethal double strand break formation. In this work the most important probabilistic models for DNA strand breakage and damage propagation are summarized and compared.
Molecular models for DNA damaged by photoreaction
International Nuclear Information System (INIS)
Pearlman, D.A.; Holbrook, S.R.; Pirkle, D.H.; Kim, S.H.
1985-01-01
Structural models of a DNA molecule containing a radiation-induced psoralen cross-link and of a DNA containing a thymine photodimer were constructed by applying energy-minimization techniques and model-building procedures to data from x-ray crystallographic studies. The helical axes of the models show substantial kinking and unwinding at the sites of the damage, which may have long-range as well as local effects arising from the concomitant changes in the supercoiling and overall structure of the DNA. The damaged areas may also serve as recognition sites for repair enzymes. These results should help in understanding the biologic effects of radiation-induced damage on cells
Zhao, Dong; Sakoda, Hideyuki; Sawyer, W Gregory; Banks, Scott A; Fregly, Benjamin J
2008-02-01
Wear of ultrahigh molecular weight polyethylene remains a primary factor limiting the longevity of total knee replacements (TKRs). However, wear testing on a simulator machine is time consuming and expensive, making it impractical for iterative design purposes. The objectives of this paper were first, to evaluate whether a computational model using a wear factor consistent with the TKR material pair can predict accurate TKR damage measured in a simulator machine, and second, to investigate how choice of surface evolution method (fixed or variable step) and material model (linear or nonlinear) affect the prediction. An iterative computational damage model was constructed for a commercial knee implant in an AMTI simulator machine. The damage model combined a dynamic contact model with a surface evolution model to predict how wear plus creep progressively alter tibial insert geometry over multiple simulations. The computational framework was validated by predicting wear in a cylinder-on-plate system for which an analytical solution was derived. The implant damage model was evaluated for 5 million cycles of simulated gait using damage measurements made on the same implant in an AMTI machine. Using a pin-on-plate wear factor for the same material pair as the implant, the model predicted tibial insert wear volume to within 2% error and damage depths and areas to within 18% and 10% error, respectively. Choice of material model had little influence, while inclusion of surface evolution affected damage depth and area but not wear volume predictions. Surface evolution method was important only during the initial cycles, where variable step was needed to capture rapid geometry changes due to the creep. Overall, our results indicate that accurate TKR damage predictions can be made with a computational model using a constant wear factor obtained from pin-on-plate tests for the same material pair, and furthermore, that surface evolution method matters only during the initial
Energy Technology Data Exchange (ETDEWEB)
Wen, Wei [Los Alamos National Lab. (LANL), Los Alamos, NM (United States); Capolungo, Laurent [Los Alamos National Lab. (LANL), Los Alamos, NM (United States); Patra, Anirban [Los Alamos National Lab. (LANL), Los Alamos, NM (United States); Tome, Carlos [Los Alamos National Lab. (LANL), Los Alamos, NM (United States)
2017-02-02
This Report addresses the Milestone M2MS-16LA0501032 of NEAMS Program (“Develop hardening model for FeCrAl cladding), with a deadline of 09/30/2016. Here we report a constitutive law for thermal creep of FeCrAl. This Report adds to and complements the one for Milestone M3MS-16LA0501034 (“Interface hardening models with MOOSE-BISON”), where we presented a hardening law for irradiated FeCrAl. The last component of our polycrystal-based constitutive behavior, namely, an irradiation creep model for FeCrAl, will be developed as part of the FY17 Milestones, and the three regimes will be coupled and interfaced with MOOSE-BISON.
Constitutive modelling of creep-ageing behaviour of peak-aged aluminium alloy 7050
Directory of Open Access Journals (Sweden)
Yang Yo-Lun
2015-01-01
Full Text Available The creep-ageing behaviour of a peak-aged aluminium alloy 7050 was investigated under different stress levels at 174 ∘C for up to 8 h. Interrupted creep tests and tensile tests were performed to investigate the influences of creep-ageing time and applied stress on yield strength. The mechanical testing results indicate that the material exhibits an over-ageing behaviour which increases with the applied stress level during creep-ageing. As creep-ageing time approaches 8 h, the material's yield strength under different stress levels gradually converge, which suggests that the difference in mechanical properties under different stress conditions can be minimised. This feature can be advantageous in creep-age forming to the formed components such that uniformed mechanical properties across part area can be achieved. A set of constitutive equations was calibrated using the mechanical test results and the alloy-specific material constants were obtained. A good agreement is observed between the experimental and calibrated results.
International Nuclear Information System (INIS)
Nakasone, Yuji; Kizuki, Yuta; Suzuki, Hayao; Minowa, Takuya
2013-01-01
The present study has investigated microstructural changes due to laser peening in modified 9Cr-1Mo steel subjected to creep. The EBSD or Electron Backscatter Diffraction studies have been made on round-bar type specimens creeping at applied stresses of 230 and 240 MPa at 823 K and 105 MPa at 923K in air. Prior to the creep tests, laser peening was applied to specimens at laser power of 8.4-22GW/cm 2 per pulse in water. Microstructural change in each specimen after its creep test was investigated by EBSD/SEM. The EBSD/SEM analyses revealed that the laser peening treatment makes creep rupture time longer and it reveals local misorientation value for rupture. (author)
Impact damages modeling in laminated composite structures
Directory of Open Access Journals (Sweden)
Kreculj Dragan D.
2014-01-01
Full Text Available Laminated composites have an important application in modern engineering structures. They are characterized by extraordinary properties, such as: high strength and stiffness and lightweight. Nevertheless, a serious obstacle to more widespread use of those materials is their sensitivity to the impact loads. Impacts cause initiation and development of certain types of damages. Failures that occur in laminated composite structures can be intralaminar and interlaminar. To date it was developed a lot of simulation models for impact damages analysis in laminates. Those models can replace real and expensive testing in laminated structures with a certain accuracy. By using specialized software the damage parameters and distributions can be determined (at certain conditions on laminate structures. With performing numerical simulation of impact on composite laminates there are corresponding results valid for the analysis of these structures.
Luo, Junhui; Mi, Decai; Ye, Qiongyao; Deng, Shengqiang; Zeng, Fuquan; Zeng, Yongjun
2018-01-01
Carbonaceous rock has the characteristics of easy disintegration, softening, swelling and environmental sensitivity, which belongs to soft surrounding rock, and the deformation during excavation and long-term stability of the surrounding rock of carbonaceous rock tunnel are common problems in the construction of carbonaceous rock tunnel. According to the above, the Monitor and measure the displacement, temperature and osmotic pressure of the surrounding carbonaceous rock of the tunnel of Guangxi Hebai highway. Then it based on the obtaining data to study the creep mechanism of surrounding rock using Singh-Mitchell model and predict the deformation of surrounding rock before the tunnel is operation. The results show that the Singh-Mitchell creep model can effectively analyse and predict the deformation development law of surrounding rock of tunnel without considering temperature and osmotic pressure, it can provide reference for the construction of carbonaceous rock tunnel and the measures to prevent and reinforce it..
The assessment of creep-fatigue initiation and crack growth
International Nuclear Information System (INIS)
Priest, R.H.; Miller, D.A.
1991-01-01
An outline of Nuclear Electric's Assessment Procedure for the High Temperature Response of Structures ('R5') for creep-fatigue initiation and crack growth is given. A unified approach is adopted for both regimes. For initiation, total damage is described in terms of separate creep and fatigue components. Ductility exhaustion is used for estimating creep damage whilst continuous cycling endurance data are used to evaluate the fatigue damage term. Evidence supporting this approach is given through the successful prediction of creep-fatigue endurances for a range of materials, cycle types, dwell period times, etc. Creep-fatigue crack growth is similarly described in terms of separated creep and fatigue components. Crack growth rates for each component are characterised in terms of fracture mechanics parameters. It is shown that creep crack growth rates can be rationalised on a ductility basis. Creep-fatigue interactions are accommodated in the cyclic growth component through the use of materials coefficients which depend on dwell time. (orig.)
Creep rupture behavior of welded Grade 91 steel
Energy Technology Data Exchange (ETDEWEB)
Shrestha, Triratna [Department of Chemical and Materials Engineering, University of Idaho, Moscow, ID 83844 (United States); Basirat, Mehdi [Department of Mechanical Engineering, University of Idaho, Moscow, ID 83844 (United States); Alsagabi, Sultan; Sittiho, Anumat [Department of Chemical and Materials Engineering, University of Idaho, Moscow, ID 83844 (United States); Charit, Indrajit, E-mail: icharit@uidaho.edu [Department of Chemical and Materials Engineering, University of Idaho, Moscow, ID 83844 (United States); Potirniche, Gabriel P. [Department of Mechanical Engineering, University of Idaho, Moscow, ID 83844 (United States)
2016-07-04
Creep rupture behavior of fusion welded Grade 91 steel was studied in the temperature range of 600 – 700 °C and at stresses of 50–200 MPa. The creep data were analyzed in terms of the Monkman-Grant relation and Larson-Miller parameter. The creep damage tolerance factor was used to identify the origin of creep damage. The creep damage was identified as the void growth in combination with microstructural degradation. The fracture surface morphology of the ruptured specimens was studied by scanning electron microscopy and deformed microstructure examined by transmission electron microscopy, to further elucidate the rupture mechanisms.
Modelling of settlement induced building damage
Giardina, G.
2013-01-01
This thesis focuses on the modelling of settlement induced damage to masonry buildings. In densely populated areas, the need for new space is nowadays producing a rapid increment of underground excavations. Due to the construction of new metro lines, tunnelling activity in urban areas is growing.
Incorporating damage mechanics into explosion simulation models
International Nuclear Information System (INIS)
Sammis, C.G.
1993-01-01
The source region of an underground explosion is commonly modeled as a nested series of shells. In the innermost open-quotes hydrodynamic regimeclose quotes pressures and temperatures are sufficiently high that the rock deforms as a fluid and may be described using a PVT equation of state. Just beyond the hydrodynamic regime, is the open-quotes non-linear regimeclose quotes in which the rock has shear strength but the deformation is nonlinear. This regime extends out to the open-quotes elastic radiusclose quotes beyond which the deformation is linear. In this paper, we develop a model for the non-linear regime in crystalline source rock where the nonlinearity is mostly due to fractures. We divide the non-linear regime into a open-quotes damage regimeclose quotes in which the stresses are sufficiently high to nucleate new fractures from preexisting ones and a open-quotes crack-slidingclose quotes regime where motion on preexisting cracks produces amplitude dependent attenuation and other non-linear effects, but no new cracks are nucleated. The boundary between these two regimes is called the open-quotes damage radius.close quotes The micromechanical damage mechanics recently developed by Ashby and Sammis (1990) is used to write an analytic expression for the damage radius in terms of the initial fracture spectrum of the source rock, and to develop an algorithm which may be used to incorporate damage mechanics into computer source models for the damage regime. Effects of water saturation and loading rate are also discussed
Evaluation of long term creep-fatigue life for type 304 stainless steel
International Nuclear Information System (INIS)
Kawasaki, Hirotsugu; Ueno, Fumiyoshi; Aoto, Kazumi; Ichimiya, Masakazu; Wada, Yusaku
1992-01-01
The long term creep-fatigue life of type 304 stainless steel was evaluated by the creep-fatigue life prediction method based on a linear damage fraction rule. The displacement controlled creep-fatigue tests were carried out, and the time to failure of longer than 10000 hours was obtained. The creep damage of long term creep-fatigue was evaluated by taking into account the stress relaxation behavior with elastic follow-up during the hold period. The relationship between life reduction of creep-fatigue and fracture mode was provided by the creep cavity growth. The results of this study are summarized as follows; (1) The long term creep-fatigue data can be reasonably evaluated by the present method. The predicted lives were within a factor of 3 of the observed ones. (2) The present method provides the capability to predict the long term creep-fatigue life at lower temperatures as well as that at the creep dominant temperature. (3) The value of creep damage for the long term creep-fatigue data increased by elastic follow-up. The creep-fatigue damage diagram intercepted between 0.3 and 1 can represent the observed creep-fatigue damages. (4) The cavity growth depends on the hold time. The fracture of long term creep-fatigue is caused by the intergranular cavity growth. The intergranular fracture of creep-fatigue is initiated by the cavity growth and followed by the microcrack propagation along grain boundaries starting from creep cavities. (author)
Creep-fatigue life assessment of cruciform weldments using the linear matching method
International Nuclear Information System (INIS)
Gorash, Yevgen; Chen, Haofeng
2013-01-01
This paper presents a creep-fatigue life assessment of a cruciform weldment made of the steel AISI type 316N(L) and subjected to reversed bending and cyclic dwells at 550 °C using the Linear Matching Method (LMM) and considering different weld zones. The design limits are estimated by the shakedown analysis using the LMM and elastic-perfectly-plastic material model. The creep-fatigue analysis is implemented using the following material models: 1) Ramberg–Osgood model for plastic strains under saturated cyclic conditions; 2) power-law model in “time hardening” form for creep strains during primary creep stage. The number of cycles to failure N ⋆ under creep-fatigue interaction is defined by: a) relation for cycles to fatigue failure N ∗ dependent on numerical total strain range Δε tot for the fatigue damage ω f ; b) long-term strength relation for the time to creep rupture t ∗ dependent on numerical average stress σ ¯ during dwell Δt for the creep damage ω cr ; c) non-linear creep-fatigue interaction diagram for the total damage. Numerically estimated N ⋆ for different Δt and Δε tot shows good quantitative agreement with experiments. A parametric study of different dwell times Δt is used to formulate the functions for N ⋆ and residual life L ⋆ dependent on Δt and normalised bending moment M -tilde , and the corresponding contour plot intended for design applications is created. -- Highlights: ► Ramberg–Osgood model is used for plastic strains under saturated cyclic conditions. ► Power-law model in time-hardening form is used for creep strains during dwells. ► Life assessment procedure is based on time fraction rule to evaluate creep damage. ► Function for cycles to failure is dependent on dwell period and normalised moment. ► Function for FSRF dependent on dwell period takes into account the effect of creep
MCCREEP - a model to estimate creep produced by microcracking around a cavity in an intact rock mass
International Nuclear Information System (INIS)
Wilkins, B.J.S.; Rigby, G.L.
1991-11-01
AECL Research is examining the disposal of nuclear fuel waste in a vault in plutonic rock. Models (MCDIRC and MCROC) have been developed to predict the mechanical behaviour of the rock in response to excavation and heat from the waste. The dominant mechanism of deformation at temperatures below 150 degrees C is microcracking, which results in rock creep and a decrease in rock strength. MCDIRC has been constructed to consider the perturbation of the stress state of intact rock by long cylindrical cavities. Slow crack-growth data are used to estimate time-dependent changes in rock strength, from which possible movements (creep strain) in the rock mass are estimated. MCDIRC depends on analytical solutions for stress-state perturbations. MCCREEP has been developed from MCDIRC and relies on the use of finite-element methods to solve for stress states. It is more flexible than MCDIRC and can deal with non-homogeneous rock properties and non-symmetrical cavities
Tensile cracks in creeping solids
International Nuclear Information System (INIS)
Riedel, H.; Rice, J.R.
1979-02-01
The loading parameter determining the stress and strain fields near a crack tip, and thereby the growth of the crack, under creep conditions is discussed. Relevant loading parameters considered are the stress intensity factor K/sub I/, the path-independent integral C*, and the net section stress sigma/sub net/. The material behavior is modelled as elastic-nonlinear viscous where the nonlinear term describes power law creep. At the time t = 0 load is applied to the cracked specimen, and in the first instant the stress distribution is elastic. Subsequently, creep deformation relaxes the initial stress concentration at the crack tip, and creep strains develop rapidly near the crack tip. These processes may be analytically described by self-similar solutions for short times t. Small scale yielding may be defined. In creep problems, this means that elastic strains dominate almost everywhere except in a small creep zone which grows around the crack tip. If crack growth ensues while the creep zone is still small compared with the crack length and the specimen size, the stress intensity factor governs crack growth behavior. If the calculated creep zone becomes larger than the specimen size, the stresses become finally time-independent and the elastic strain rates can be neglected. In this case, the stress field is the same as in the fully-plastic limit of power law hardening plasticity. The loading parameter which determines the near tip fields uniquely is then the path-independent integral C*.K/sub I/ and C* characterize opposite limiting cases. The case applied in a given situation is decided by comparing the creep zone size with the specimen size and the crack length. Besides several methods of estimating the creep zone size, a convenient expression for a characteristic time is derived, which characterizes the transition from small scale yielding to extensive creep of the whole specimen
Creep in crystalline rock with application to high level nuclear waste repository
International Nuclear Information System (INIS)
Eloranta, P.; Simonen, A.
1992-06-01
The time-dependent strength and deformation properties of hard crystalline rock are studied. Theoretical models defining the phenomena which can effect these properties are reviewed. The time- dependent deformation of the openings in the proposed nuclear waste repository is analysed. The most important factors affecting the subcritical crack growth in crystalline rock are the stress state, the chemical environment, temperature and microstructure of the rock. There are several theoretical models for the analysis of creep and cyclic fatigue: deformation diagrams, rheological models thermodynamic models, reaction rate models, stochastic models, damage models and time-dependent safety factor model. They are defective in describing the three-axial stress condition and strength criteria. In addition, the required parameters are often too difficult to determine with adequate accuracy. Therefore these models are seldom applied in practice. The effect of microcrack- driven creep on the stability of the work shaft, the emplacement tunnel and the capsulation hole of a proposed nuclear waste repository was studied using a numerical model developed by Atomic Energy of Canada Ltd. According to the model, the microcrack driven creep progresses very slowly in good quality rock. Poor rock quality may accelerate the creep rate. The model is very sensitive to the properties of the rock and secondary stress state. The results show that creep causes no stability problems on excavations in good rock. The results overestimate the effect of the creep, because the analysis omitted the effect of support structures and backfilling
Microstructural modeling of Vienne granite damage
International Nuclear Information System (INIS)
Homand, F.; Hoxha, D.
2002-01-01
The microstructural approach in damage modeling, which is presented in this paper describes the evolution of micro-crack geometry as a function of history loading. If the crack geometry is known, the effective properties could then be calculated foe any cracked rock by the mean of a micro-mechanical model. The P L evolution law which is necessary in the describing of crack geometry evolution is hardly based on the crack microscope observation as well as on the theory of fabric tensors. This approach is applied in the modeling of mechanical behaviour of Vienne granite. The result of model simulations are compared with laboratory tests. (author)
Li, Xiaozhao; Shao, Zhushan
2016-07-01
The growth of subcritical cracks plays an important role in the creep of brittle rock. The stress path has a great influence on creep properties. A micromechanics-based model is presented to study the effect of the stress path on creep properties. The microcrack model of Ashby and Sammis, Charles' Law, and a new micro-macro relation are employed in our model. This new micro-macro relation is proposed by using the correlation between the micromechanical and macroscopic definition of damage. A stress path function is also introduced by the relationship between stress and time. Theoretical expressions of the stress-strain relationship and creep behavior are derived. The effects of confining pressure on the stress-strain relationship are studied. Crack initiation stress and peak stress are achieved under different confining pressures. The applied constant stress that could cause creep behavior is predicted. Creep properties are studied under the step loading of axial stress or the unloading of confining pressure. Rationality of the micromechanics-based model is verified by the experimental results of Jinping marble. Furthermore, the effects of model parameters and the unloading rate of confining pressure on creep behavior are analyzed. The coupling effect of step axial stress and confining pressure on creep failure is also discussed. The results provide implications on the deformation behavior and time-delayed rockburst mechanism caused by microcrack growth on surrounding rocks during deep underground excavations.
Damage-induced nonassociated inelastic flow in rock salt
International Nuclear Information System (INIS)
Chan, K.S.; Bodner, S.R.; Brodsky, N.S.; Fossum, A.F.; Munson, D.E.
1993-01-01
The multi-mechanism deformation coupled fracture model recently developed by CHAN, et al. (1992), for describing time-dependent, pressure-sensitive inelastic flow and damage evolution in crystalline solids was evaluated against triaxial creep experiments on rock salt. Guided by experimental observations, the kinetic equation and the flow law for damage-induced inelastic flow in the model were modified to account for the development of damage and inelastic dilatation in the transient creep regime. The revised model was then utilized to obtain the creep response and damage evolution in rock salt as a function of confining pressure and stress difference. Comparison between model calculation and experiment revealed that damage-induced inelastic flow is nonassociated, dilatational, and contributes significantly to the macroscopic strain rate observed in rock salt deformed at low confining pressures. The inelastic strain rate and volumetric strain due to damage decrease with increasing confining pressures, and all are suppressed at sufficiently high confining pressures
Analysis of irradiation creep and the structural integrity of fusion in-vessel components
International Nuclear Information System (INIS)
Karditsas, Panayiotis J.
2000-01-01
This paper presents a brief review of the irradiation creep mechanism, analyses of the effect on the performance and behaviour of fusion in-vessel components, and discusses procedures for the estimation of in-service time (or lifetime) of components under combined creep-fatigue. The irradiation creep models and proposed theories are examined and analysed to produce a creep law relevant to fusion conditions. The necessary material data, constitutive equations and other parameters needed for estimation of in-service time from the combination of creep and fatigue damage are identified. Wherever possible, design curves are proposed for stress and strain. Time dependent non-linear elastoplastic example calculations are performed, for a typical first wall structure under power plant loading conditions, assuming austenitic and martensitic steel as structural materials, including material irradiation creep. The results of calculations for the stress and strain history of the first wall are used together with the proposed cumulative damage expressions derived in this study to estimate the in-service time, including the effects of stress relaxation due to creep, reduction of ductility (or fracture strain) and helium-to-displacement-damage ratio. The calculations give a displacement damage of ∼70 dpa for the 316 austenitic steel and ∼110-130 dpa for the martensitic steel. Provided there are no power transients, for a design strain of 0.5%, the in-service time is estimated to be ∼3 years for the 316 steel case (at 2.2 MW/m 2 wall load) and the high wall loading martensitic steel (5.0 MW/m 2 case), and ∼5.3 years for the martensitic steel at lower wall load (2.2 MW/m 2 case). The difficulty in defending these results lies in the uncertainty arising from the limited database and experience of the material properties, especially the creep constitutive law, when exposed to fusion environments
Boyina, Gangadhara Rao T.; Rayavarapu, Vijaya Kumar; V. V., Subba Rao
2017-02-01
The prediction of ultimate strength remains the main challenge in the simulation of the mechanical response of composite structures. This paper examines continuum damage model to predict the strength and size effects for deformation and failure response of polymer composite laminates when subjected to complex state of stress. The paper also considers how the overall results of the exercise can be applied in design applications. The continuum damage model is described and the resulting prediction of size effects are compared against the standard benchmark solutions. The stress analysis for strength prediction of rotary wing aircraft cabin door is carried out. The goal of this study is to extend the proposed continuum damage model such that it can be accurately predict the failure around stress concentration regions. The finite element-based continuum damage mechanics model can be applied to the structures and components of arbitrary configurations where analytical solutions could not be developed.
Tensile creep behavior in an advanced silicon nitride
International Nuclear Information System (INIS)
Lofaj, F.
2000-01-01
Tensile creep behavior and changes in the microstructure of the advanced silicon nitride, SN 88M, were studied at temperatures from 1250 to 1400 C to reveal the creep resistance and lifetime-controlling processes. Assuming power law dependence of the minimum strain rate on stress, stress exponents from 6 to 8 and an apparent activation energy of 780 kJ/mol were obtained. Extensive electron microscopy observations revealed significant changes in the crystalline secondary phases and creep damage development. Creep damage was classified in two groups: 'inter-granular' defects in the amorphous boundary phases, and 'intra-granular' defects in silicon nitride grains. The inter-granular defects involved multigrain junction cavities, two-grain junction cavities, microcracks and cracks. The intra-granular defects included broken large grains, small symmetrical and asymmetrical cavities, and crack-like intragranular cavities. Cavities are generated continuously during the whole deformation starting from the threshold strain of ∝0.1%, and they contribute linearly to the tensile strain. Cavities produce more than 90% of the total tensile strain, and it is concluded that cavitation is the main creep mechanism in silicon nitride ceramics. The multigrain junction cavities are considered to be the most important for generating new volume and producing tensile strain. The Luecke and Wiederhorn (L and W) creep model, based on cavitation at multigrain junctions according to an exponential law, was proven to correspond to the stress dependence of the minimum strain rate. A qualitative model based on the L and W model was suggested and expanded to include intragranular cavitation. The basic mechanisms involve a repeating of the sequence grain boundary sliding (GBS) => cavitation at multigrain junctions => viscous flow and dissolution-precipitation. (orig.)
Simulation of irradiation creep
International Nuclear Information System (INIS)
Reiley, T.C.; Jung, P.
1977-01-01
The results to date in the area of radiation enhanced deformation using beams of light ions to simulate fast neutron displacement damage are reviewed. A comparison is made between these results and those of in-reactor experiments. Particular attention is given to the displacement rate calculations for light ions and the electronic energy losses and their effect on the displacement cross section. Differences in the displacement processes for light ions and neutrons which may effect the irradiation creep process are discussed. The experimental constraints and potential problem areas associated with these experiments are compared to the advantages of simulation. Support experiments on the effect of thickness on thermal creep are presented. A brief description of the experiments in progress is presented for the following laboratories: HEDL, NRL, ORNL, PNL, U. of Lowell/MIT in the United States, AERE Harwell in the United Kingdom, CEN Saclay in France, GRK Karlsruhe and KFA Julich in West Germany
Fatigue and damage tolerance scatter models
Raikher, Veniamin L.
1994-09-01
Effective Total Fatigue Life and Crack Growth Scatter Models are proposed. The first of them is based on the power form of the Wohler curve, fatigue scatter dependence on mean life value, cycle stress ratio influence on fatigue scatter, and validated description of the mean stress influence on the mean fatigue life. The second uses in addition are fracture mechanics approach, assumption of initial damage existence, and Paris equation. Simple formulas are derived for configurations of models. A preliminary identification of the parameters of the models is fulfilled on the basis of experimental data. Some new and important results for fatigue and crack growth scatter characteristics are obtained.
Don S. Stone; Joseph E. Jakes; Jonathan Puthoff; Abdelmageed A. Elmustafa
2010-01-01
Finite element analysis is used to simulate cone indentation creep in materials across a wide range of hardness, strain rate sensitivity, and work-hardening exponent. Modeling reveals that the commonly held assumption of the hardness strain rate sensitivity (mΗ) equaling the flow stress strain rate sensitivity (mσ...
Simulation of creep test on 316FR stainless steel in sodium environment at 550degC
International Nuclear Information System (INIS)
Satmoko, A.; Asayama, Tai
1999-04-01
In sodium environment, material 316FR stainless steel risks to suffer from carburization. In this study, an analysis using a Fortran program is conducted to evaluate the carbon influence on the creep behavior of 316FR based on experimental results from uni-axial creep test that had been performed at temperature 550degC in sodium environment simulating Fast Breeder Reactor condition. As performed in experiments, two parts are distinguished. At first, elastic-plastic behavior is used to simulate the fact that just before the beginning of creep test, specimen suffers from load or stress much higher than initial yield stress. In second part, creep condition occurs in which the applied load is kept constant. The plastic component should be included, since stresses increase due to section area reduction. For this reason, elastic-plastic-creep behavior is considered. Through time carbon penetration occurs and its concentration is evaluated empirically. This carburization phenomena are assumed to affect in increasing yield stress, decreasing creep strain rate, and increasing creep rupture strength of material. The model is capable of simulating creep test in sodium environment. Material near from surface risks to be carburized. Its material properties change leading to non-uniform distribution of stresses. Those layers of material suffer from stress concentration, and are subject to damage. By introducing a damage criteria, crack initialization can thus be predicted. And even, crack growth can be evaluated. For high stress levels, tensile strength criterion is more important than creep damage criterion. But in low stress levels, the latter gives more influence in fracture. Under high stress, time to rupture of a specimen in sodium environment is shorter than in air. But for stresses lower than 26 kgf/mm 2 , the time to rupture of creep in sodium environment is the same or little longer than in air. Quantitatively, the carburization effect at 550degC is not important. This
A Coupled Plastic Damage Model for Concrete considering the Effect of Damage on Plastic Flow
Zhou, Feng; Cheng, Guangxu
2015-01-01
A coupled plastic damage model with two damage scalars is proposed to describe the nonlinear features of concrete. The constitutive formulations are developed by assuming that damage can be represented effectively in the material compliance tensor. Damage evolution law and plastic damage coupling are described using the framework of irreversible thermodynamics. The plasticity part is developed without using the effective stress concept. A plastic yield function based on the true stress is ado...
Tree-based flood damage modeling of companies: Damage processes and model performance
Sieg, Tobias; Vogel, Kristin; Merz, Bruno; Kreibich, Heidi
2017-07-01
Reliable flood risk analyses, including the estimation of damage, are an important prerequisite for efficient risk management. However, not much is known about flood damage processes affecting companies. Thus, we conduct a flood damage assessment of companies in Germany with regard to two aspects. First, we identify relevant damage-influencing variables. Second, we assess the prediction performance of the developed damage models with respect to the gain by using an increasing amount of training data and a sector-specific evaluation of the data. Random forests are trained with data from two postevent surveys after flood events occurring in the years 2002 and 2013. For a sector-specific consideration, the data set is split into four subsets corresponding to the manufacturing, commercial, financial, and service sectors. Further, separate models are derived for three different company assets: buildings, equipment, and goods and stock. Calculated variable importance values reveal different variable sets relevant for the damage estimation, indicating significant differences in the damage process for various company sectors and assets. With an increasing number of data used to build the models, prediction errors decrease. Yet the effect is rather small and seems to saturate for a data set size of several hundred observations. In contrast, the prediction improvement achieved by a sector-specific consideration is more distinct, especially for damage to equipment and goods and stock. Consequently, sector-specific data acquisition and a consideration of sector-specific company characteristics in future flood damage assessments is expected to improve the model performance more than a mere increase in data.
Czech Academy of Sciences Publication Activity Database
Kuhnen, K.; Krejčí, Pavel
2009-01-01
Roč. 54, č. 3 (2009), s. 537-550 ISSN 0018-9286 Institutional research plan: CEZ:AV0Z10190503 Keywords : compensation * creep * hysteresis Subject RIV: BA - General Mathematics Impact factor: 2.556, year: 2009 http://ieeexplore.ieee.org/xpl/freeabs_all.jsp?arnumber=4797784
Creep Modeling in a Composite Rotating Disc with Thickness Variation in Presence of Residual Stress
Directory of Open Access Journals (Sweden)
Vandana Gupta
2012-01-01
Full Text Available Steady-state creep response in a rotating disc made of Al-SiC (particle composite having linearly varying thickness has been carried out using isotropic/anisotropic Hoffman yield criterion and results are compared with those using von Mises yield criterion/Hill's criterion ignoring difference in yield stresses. The steady-state creep behavior has been described by Sherby's creep law. The material parameters characterizing difference in yield stresses have been used from the available experimental results in literature. Stress and strain rate distributions developed due to rotation have been calculated. It is concluded that the stress and strain distributions got affected from the thermal residual stress in an isotropic/anisotropic rotating disc, although the effect of residual stress on creep behavior in an anisotropic rotating disc is observed to be lower than those observed in an isotropic disc. Thus, the presence of residual stress in composite rotating disc with varying thickness needs attention for designing a disc.
Creep cavitation effects in polycrystalline alumina
International Nuclear Information System (INIS)
Porter, J.R.; Blumenthal, W.; Evans, A.G.
1981-01-01
Fine grained polycrystalline alumina has been deformed in creep at high temperatures, to examine the evolution of cavities at grain boundaries. Cavities with equilibrium and crack-like morphologies have been observed, distributed nonuniformly throughout the material. The role of these cavities during creep has been described. A transition from equilibrium to crack-like morphology has been observed and correlated with a model based on the influence of the surface to boundary diffusivity ratio and the local tensile stress. The contribution of cavitation to the creep rate and total creep strain has been analyzed and excluded as the principal cause of the observed non-linear creep rate
Finite Element Creep-Fatigue Analysis of a Welded Furnace Roll for Identifying Failure Root Cause
Yang, Y. P.; Mohr, W. C.
2015-11-01
Creep-fatigue induced failures are often observed in engineering components operating under high temperature and cyclic loading. Understanding the creep-fatigue damage process and identifying failure root cause are very important for preventing such failures and improving the lifetime of engineering components. Finite element analyses including a heat transfer analysis and a creep-fatigue analysis were conducted to model the cyclic thermal and mechanical process of a furnace roll in a continuous hot-dip coating line. Typically, the roll has a short life, modeling heat convection from hot air inside the furnace. The creep-fatigue analysis was performed by inputting the predicted temperature history and applying mechanical loads. The analysis results showed that the failure was resulted from a creep-fatigue mechanism rather than a creep mechanism. The difference of material properties between the filler metal and the base metal is the root cause for the roll failure, which induces higher creep strain and stress in the interface between the weld and the HAZ.
Understanding Creep Mechanisms in Graphite with Experiments, Multiscale Simulations, and Modeling
International Nuclear Information System (INIS)
2014-01-01
Disordering mechanisms in graphite have a long history with conflicting viewpoints. Using Raman and x-ray photon spectroscopy, electron microscopy, x-ray diffraction experiments and atomistic modeling and simulations, the current project has developed a fundamental understanding of early-to-late state radiation damage mechanisms in nuclear reactor grade graphite (NBG-18 and PCEA). We show that the topological defects in graphite play an important role under neutron and ion irradiation.
Understanding Creep Mechanisms in Graphite with Experiments, Multiscale Simulations, and Modeling
Energy Technology Data Exchange (ETDEWEB)
Eapen, Jacob [North Carolina State Univ., Raleigh, NC (United States); Murty, Korukonda [North Carolina State Univ., Raleigh, NC (United States); Burchell, Timothy [Oak Ridge National Lab. (ORNL), Oak Ridge, TN (United States)
2014-06-02
Disordering mechanisms in graphite have a long history with conflicting viewpoints. Using Raman and x-ray photon spectroscopy, electron microscopy, x-ray diffraction experiments and atomistic modeling and simulations, the current project has developed a fundamental understanding of early-to-late state radiation damage mechanisms in nuclear reactor grade graphite (NBG-18 and PCEA). We show that the topological defects in graphite play an important role under neutron and ion irradiation.
Model of designating the critical damages
Directory of Open Access Journals (Sweden)
Zwolińska Bożena
2017-06-01
Full Text Available Managing company in the lean way presumes no breakdowns nor reserves in the whole delivery chain. However, achieving such low indicators is impossible. That is why in some production plants it is extremely important to focus on preventive actions which can limit damages. This article depicts the method of designating the critical damages in accordance with lean maintenance method. The article consists of two parts which make for an integral body. Part one depicts the characteristic of a realistic object, it also contains productions capabilities analysis of certain areas within the production structure. Part two depicts the probabilistic model of shaping maximal time loss basing on emptying and filling interoperational buffers.
International Nuclear Information System (INIS)
Pfeifle, T.W.; Mellegard, K.D.; Munson, D.E.
1992-10-01
The modified Munson-Dawson (M-D) constitutive model that describes the creep behavior of salt will be used in performance assessment calculations to assess compliance of the Waste Isolation Pilot Plant (WIPP) facility with requirements governing the disposal of nuclear waste. One of these standards requires that the uncertainty of future states of the system, material model parameters, and data be addressed in the performance assessment models. This paper presents a method in which measurement uncertainty and the inherent variability of the material are characterized by treating the M-D model parameters as random variables. The random variables can be described by appropriate probability distribution functions which then can be used in Monte Carlo or structural reliability analyses. Estimates of three random variables in the M-D model were obtained by fitting a scalar form of the model to triaxial compression creep data generated from tests of WIPP salt. Candidate probability distribution functions for each of the variables were then fitted to the estimates and their relative goodness-of-fit tested using the Kolmogorov-Smirnov statistic. A sophisticated statistical software package obtained from BMDP Statistical Software, Inc. was used in the M-D model fitting. A separate software package, STATGRAPHICS, was used in fitting the candidate probability distribution functions to estimates of the variables. Skewed distributions, i.e., lognormal and Weibull, were found to be appropriate for the random variables analyzed
Modeling of Corrosion-induced Concrete Damage
DEFF Research Database (Denmark)
Thybo, Anna Emilie A.; Michel, Alexander; Stang, Henrik
2013-01-01
In the present paper a finite element model is introduced to simulate corrosion-induced damage in concrete. The model takes into account the penetration of corrosion products into the concrete as well as non-uniform formation of corrosion products around the reinforcement. To ac-count for the non...... of corrosion products affects both the time-to cover cracking and the crack width at the concrete surface.......In the present paper a finite element model is introduced to simulate corrosion-induced damage in concrete. The model takes into account the penetration of corrosion products into the concrete as well as non-uniform formation of corrosion products around the reinforcement. To ac-count for the non......-uniform formation of corrosion products at the concrete/reinforcement interface, a deterministic approach is used. The model gives good estimates of both deformations in the con-crete/reinforcement interface and crack width when compared to experimental data. Further, it is shown that non-uniform deposition...
Damage Model of Reinforced Concrete Members under Cyclic Loading
Wei, Bo Chen; Zhang, Jing Shu; Zhang, Yin Hua; Zhou, Jia Lai
2018-06-01
Based on the Kumar damage model, a new damage model for reinforced concrete members is established in this paper. According to the damage characteristics of reinforced concrete members subjected to cyclic loading, four judgment conditions for determining the rationality of damage models are put forward. An ideal damage index (D) is supposed to vary within a scale of zero (no damage) to one (collapse). D should be a monotone increasing function which tends to increase in the case of the same displacement amplitude. As for members under large displacement amplitude loading, the growth rate of D should be greater than that of D under small amplitude displacement loading. Subsequently, the Park-Ang damage model, the Niu-Ren damage model, the Lu-Wang damage model and the proposed damage model are analyzed for 30 experimental reinforced concrete members, including slabs, walls, beams and columns. The results show that current damage models do not fully matches the reasonable judgment conditions, but the proposed damage model does. Therefore, a conclusion can be drawn that the proposed damage model can be used for evaluating and predicting damage performance of RC members under cyclic loading.
The role of particle ripening on the creep acceleration of Nimonic 263 superalloy
Directory of Open Access Journals (Sweden)
Angella Giuliano
2014-01-01
Full Text Available Physically based constitutive equations need to incorporate the most relevant microstructural features of materials to adequately describe their mechanical behaviour. To accurately model the creep behaviour of precipitation hardened alloys, the value and the evolution of strengthening particle size are important parameters to be taken into account. In the present work, creep tests have been run on virgin and overaged (up to 3500 h at 800 ∘C Nimonic 263, a polycrystalline nickel base superalloy used for combustion chambers of gas turbines. The experimental results suggest that the reinforcing particle evolution is not the main reason for the creep acceleration that seems to be better described by a strain correlated damage, such as the accumulation of mobile dislocations or the grain boundary cavitation. The coarsened microstructure, obtained by overageing the alloy at high temperature before creep testing, mainly influences the initial stage of the creep, resulting in a higher minimum creep rate and a corresponding reduction of the creep resistance.
Dip-Test Internal Stress and the Composite Model of Creep Deformation
Czech Academy of Sciences Publication Activity Database
Dobeš, Ferdinand; Orlová, Alena
2005-01-01
Roč. 482, - (2005), s. 291-294 ISSN 0255-5476. [Materials Structure & Micromechanics of Fracture /4./. Brno, 23.06.2004-25.06.2004] R&D Pro jects: GA AV ČR(CZ) IAA2041202 Institutional research plan: CEZ:AV0Z20410507 Keywords : creep * internal stress * subgrain Subject RIV: BM - Solid Matter Physics ; Magnetism Impact factor: 0.399, year: 2005
Multi-scale modeling of the mechanical behavior of polycrystalline ice under transient creep.
Suquet , Pierre; Moulinec , Hervé; Castelnau , O.; Montagnat , Maurine; Lahellec , Noël; Grennerat , Fanny; Duval , Paul; Brenner , Renald
2012-01-01
International audience; Ice is a challenging material for understanding the overall behavior of polycrystalline materials and more specifically the coupling between elastic and viscous effects during transient creep. At the single crystal level, ice is an hexagonal material with a rather weak elastic anisotropy but with a strong viscoplastic anisotropy. The strain-stress curve of ice single crystals shows a softening behavior depending on the strain-rate. The strong viscous anisotropy of ice ...
Lattice continuum and diffusional creep.
Mesarovic, Sinisa Dj
2016-04-01
Diffusional creep is characterized by growth/disappearance of lattice planes at the crystal boundaries that serve as sources/sinks of vacancies, and by diffusion of vacancies. The lattice continuum theory developed here represents a natural and intuitive framework for the analysis of diffusion in crystals and lattice growth/loss at the boundaries. The formulation includes the definition of the Lagrangian reference configuration for the newly created lattice, the transport theorem and the definition of the creep rate tensor for a polycrystal as a piecewise uniform, discontinuous field. The values associated with each crystalline grain are related to the normal diffusional flux at grain boundaries. The governing equations for Nabarro-Herring creep are derived with coupled diffusion and elasticity with compositional eigenstrain. Both, bulk diffusional dissipation and boundary dissipation accompanying vacancy nucleation and absorption, are considered, but the latter is found to be negligible. For periodic arrangements of grains, diffusion formally decouples from elasticity but at the cost of a complicated boundary condition. The equilibrium of deviatorically stressed polycrystals is impossible without inclusion of interface energies. The secondary creep rate estimates correspond to the standard Nabarro-Herring model, and the volumetric creep is small. The initial (primary) creep rate is estimated to be much larger than the secondary creep rate.
Okada, Kyle S; Kuo, Wan-Yuan; Lee, Youngsoo
2018-02-01
The effects of varying formulation and processing parameters on rheological properties in a model lipid/protein-based emulsion gel were studied. Heat-set model lipoproteic emulsion gels were prepared with varying levels of protein, lipid, and NaCl contents and high pressure homogenization treatments. Small deformation oscillatory rheometry, creep compliance, and pore size analysis experiments were used to characterize intrinsic structural properties, matrix interactions, and microstructure. Creep compliance behavior of the gel system was successfully modeled by a four-component Burgers model. Shear storage and loss moduli and Newtonian viscosity increased while instantaneous compliance, retarded compliance, and pore size decreased with increasing protein or fat content or homogenization pressure. The data obtained in this study provide information on factors affecting protein network structure and strength, properties may be useful for creating desirable attributes in lipid/protein-based foods with a further optimization process. This research evaluates the effects of formulation and processing factors on the properties of a protein/fat-based food system. These properties may be related to sodium mobility and salty taste perception. This research provides information on strategies that can be used to control factors influencing the physical properties of protein/fat-based food systems targeting sodium reduction. © 2017 Wiley Periodicals, Inc.
International Nuclear Information System (INIS)
Tanaka, Eiichi; Yamada, Hiroshi
1993-01-01
The purpose of the present paper is to elucidate inelastic behavior of modified 9Cr-1Mo steel as a candidate material for the next-generation fast breeder reactor and to provide the information for the formulation of a unified constitutive model. For this purpose, cyclic creep, mechanical ratchetting and amplitude history dependence of cyclic hardening were first examined at 550degC. As a result, systematic cyclic creep and mechanical ratchetting behavior were observed under various loading conditions, and little amplitude history dependence was found. Then these results were simulated by three unified constitutive models, i.e. the Chaboche, Bodner-Partom and modified Chaboche models. The simulated results show that these models cannot describe the cyclic creep and mechanical ratchetting behavior with high accuracy, but succeed in describing the inelastic behavior of amplitude variation experiments. (author)
Influence of creep ductility on creep-fatigue behaviour of 20%Cr/25%Ni/Nb stainless steel
International Nuclear Information System (INIS)
Gladwin, D.; Miller, D.A.
1985-01-01
The influence of creep ductility on creep-fatigue endurance of 20%Cr/25%Ni/Nb stainless steel has been examined. In order to induce different creep ductilities in the 20/25/Nb stainless steel, three different thermo-mechanical routes were employed. These resulted in a range of ductilities (3-36%) being obtained at the strain rates of interest. Strain controlled slow-fast creep-fatigue cycles were used with strain rates of 10 -6 s -1 , 10 -7 s -1 in tension and 10 -3 s -1 in compression. It was found that creep ductility strongly influenced the creep-fatigue endurance of the 20/25/Nb stainless steel. When failure was creep dominated endurance was found to be directly proportional to the creep ductility. A ductility exhaustion model has been used to successfully predict creep-fatigue endurance when failure was creep dominated. (author)
Modeling the damage of welded steel, using the GTN model
Directory of Open Access Journals (Sweden)
El-Ahmar Kadi
2014-11-01
Full Text Available The aim of our work is the modeling of the damage in the weld metal according to the finite element method and the concepts of fracture mechanics based on local approaches using the code ABAQUS calculates. The use of the Gurson-Tvergaard-Needleman model axisymmetric specimens AE type to three different zones (Base metal, molten metal and heat affected Zone with four levels of triaxiality (AE2, AE4, AE10 and AE80, we have used to model the behavior of damage to welded steel, which is described as being due to the growth and coalescence of cavities with high rates of triaxiality
Prediction of stress-strain state of municipal solid waste with application of soft soil creep model
Directory of Open Access Journals (Sweden)
Ofrikhter Vadim Grigor'evich
Full Text Available The deformation of municipal solid waste is a complex process caused by the nature of MSW, the properties of which differ from the properties of common soils. The mass of municipal solid waste shows the mixed behaviour partially similar to granular soils, and partially - to cohesive. So, one of mechanical characteristics of MSW is the cohesion typical to cohesive soils, but at the same time the filtration coefficient of MSW has an order of 1 m/day that is characteristic for granular soils. It has been established that MSW massif can be simulated like the soil reinforced by randomly oriented fibers. Today a significant amount of the verified and well proved software products are available for numerical modelling of soils. The majority of them use finite element method (FEM. The soft soil creep model (SSC-model seems to be the most suitable for modelling of municipal solid waste, as it allows estimating the development of settlements in time with separation of primary and secondary consolidation. Unlike the soft soil, one of the factors of secondary consolidation of MSW is biological degradation, the influence of which is possible to consider at the definition of the modified parameters essential for soft soil model. Application of soft soil creep model allows carrying out the calculation of stress-strain state of waste from the beginning of landfill filling up to any moment of time both during the period of operation and in postclosure period. The comparative calculation presented in the paper is executed in Plaxis software using the soft-soil creep model in contrast to the calculation using the composite model of MSW. All the characteristics for SSC-model were derived from the composite model. The comparative results demonstrate the advantage of SSC-model for prediction of the development of MSW stress-strain state. As far as after the completion of the biodegradation processes MSW behaviour is similar to cohesion-like soils, the demonstrated
Low stress creep of stainless steel
International Nuclear Information System (INIS)
Crossland, I.G.; Clay, B.D.; Baker, C.
1976-06-01
The creep of 20%Cr, 25%Ni, Nb stainless steel has been examined at temperatures from 675 to 775 0 C at sheer stressed below 13 MPa and grain sizes from 6 to 20μm. The results have indicated that the initial creep rates were linearly dependent upon stress but with a threshold stress below which no creep occurred, i.e. Bingham behaviour; in addition, the creep activation energy at small strains was substantially lower than the lattice self-diffusion value and the initial creep rates were approximately related to the grain size through an inverse cube relation. It has been concluded that at low strains (approaching the initial elastic deflection) the creep mechanism was probably that of grain boundary diffusion creep (Coble, 1963) and this is further supported by the close agreement between the observed and theoretically predicted creep rate values. Steady-state creep rates were not observed; initially the creep rates fell rapidly with strain after which a more gradual decrease occurred. Whilst the creep rate - stress relationship continued to be of a Bingham form, the progressive reduction in creep rate with strain was found to be mainly attributable to an increase in the effective viscosity, threshold stress effects being generally of secondary importance. A model has been proposed which explains the initial creep rates as being due to Cable creep with elastic accommodation at grain boundary particles. At higher strains grain boundary collapse caused by vacancy sinking is accommodated at precipitate particles by plastic deformation of the adjacent matrix material. (author)
Viscoelastic creep of high-temperature concrete
International Nuclear Information System (INIS)
Pfeiffer, P.A.; Marchertas, A.H.; Bazant, Z.P.
1985-01-01
Presented in this report is the analytical model for analysis of high temperature creep response of concrete. The creep law used is linear (viscoelastic), the temperature and moisture effects on the creep rate and also aging are included. Both constant and transient temperature as well as constant and transient moisture conditions are considered. Examples are presented to correlate experimental data with parameters of the analytical model by the use of a finite element scheme
Lin, Jeffrey Chun-Hui
2011-06-01
The glass transition temperature of as-deposited parylene-C is first measured to be 50°C with a ramping-temperature-dependent modulus experiment. The creep behavior of parylene-C film in the primary and secondary creep region is then investigated below and above this glass transition temperature using a dynamic mechanical analysis (DMA) machine Q800 from TA instruments at 8 different temperatures: 10, 25, 40, 60, 80, 100, 120 and 150°C. The Burger\\'s model, which is the combined Maxwell model and Kelvin-Voigt model, fits well with our primary and secondary creep data. Accordingly, the results show that there\\'s little or no creep below the glass transition temperature. Above the glass transition temperature, the primary creep and creep rate increases with the temperature, with a retardation time constant around 6 minutes. © 2011 IEEE.
Constitutive representation of damage development and healing in WIPP salt
International Nuclear Information System (INIS)
Chan, K.S.; Bodner, S.R.; Fossum, A.F.; Munson, D.E.
1994-01-01
There has been considerable interest in characterizing and modeling the constitutive behavior of rock salt with particular reference to long-term creep and creep failure. The interest is motivated by the projected use of excavated rooms in salt rock formations as repositories for nuclear waste. It is presumed that closure of those rooms by creep ultimately would encapsulate the waste material, resulting in its effective isolation. A continuum mechanics approach for treating damage healing is formulated as part of a constitutive model for describing coupled creep, fracture, and healing in rock salt. Formulation of the healing term is, described and the constitutive model is evaluated against experimental data of rock salt from the Waste Isolation Pilot Plant (WIPP) site. The results indicate that healing anistropy in WIPP salt can be modeled with an appropriate power-conjugate equivalent stress, kinetic equation, and evolution equation for damage healing
New considerations on variability of creep rupture data and life prediction
International Nuclear Information System (INIS)
Kim, Seon Jin; Jeong, Won Taek; Kong, Yu Sik
2009-01-01
This paper deals with the variability analysis of short term creep rupture test data based on the previous creep rupture tests and the possibility of the creep life prediction. From creep tests performed by constant uniaxial stresses at 600, 650 and 700 .deg. C elevated temperature, in order to investigate the variability of short-term creep rupture data, the creep curves were analyzed for normalized creep strain divided by initial strain. There are some variability in thee creep rupture data. And, the difference between general creep curves and normalized creep curves were obtained. The effects of the creep rupture time and state steady creep rate on the Weibull distribution parameters were investigated. There were good relation between normal Weibull parameters and normalized Weibull parameters. Finally, the predicted creep life were compared with the Monkman-Grant model.
New Considerations on Variability of Creep Rupture Data and Life Prediction
International Nuclear Information System (INIS)
Jung, Won Taek; Kong, Yu Sik; Kim, Seon Jin
2009-01-01
This paper deals with the variability analysis of short term creep rupture test data based on the previous creep rupture tests and the possibility of the creep life prediction. From creep tests performed by constant uniaxial stresses at 600, 650 and 700 .deg. C elevated temperature, in order to investigate the variability of short-term creep rupture data, the creep curves were analyzed for normalized creep strain divided by initial strain. There are some variability in the creep rupture data. And, the difference between general creep curves and normalized creep curves were obtained. The effects of the creep rupture time (RT) and steady state creep rate (SSCR) on the Weibull distribution parameters were investigated. There were good relation between normal Weibull parameters and normalized Weibull parameters. Finally, the predicted creep life were compared with the Monkman-Grant model
International Nuclear Information System (INIS)
Andersson, Peder; Segle, Peter; Samuelson, Lars Aa.
1999-04-01
A 3D finite element study of creep crack growth in cross-weld CT specimens with material properties of 2.25Cr1Mo at 550 deg C is carried out, where large strain and displacement theory is used. The creep crack growth rate is calculated using a creep ductility based damage model, in which the creep strain rate perpendicular to the crack plane ahead of the crack tip is integrated, considering the multiaxial stress state. The influence of specimen size on creep crack growth rate under constant load is given special attention, but the possibility to transfer results from cross-weld CT specimens to welded high temperature components is also investigated. The creep crack growth rate of a crack in a circumferentially welded pipe is compared with the creep crack growth rate of cross-weld CT specimens of three different sizes, cut out from the pipe. Although the constraint ahead of the crack tip is higher for a larger CT specimen, the creep crack growth rate is higher for a smaller specimen than for a larger one if they are loaded to attain the same stress intensity factor. If the specimens are loaded to the same C* value, however, a more complicated pattern occurs; depending on the material properties of the weldment constituents, the CT specimen with the intermediate size will either yield the highest or the lowest creep crack growth rate
Vertebral deformity arising from an accelerated "creep" mechanism.
Luo, Jin; Pollintine, Phillip; Gomm, Edward; Dolan, Patricia; Adams, Michael A
2012-09-01
Vertebral deformities often occur in patients who recall no trauma, and display no evident fracture on radiographs. We hypothesise that vertebral deformity can occur by a gradual creep mechanism which is accelerated following minor damage. "Creep" is continuous deformation under constant load. Forty-five thoracolumbar spine motion segments were tested from cadavers aged 42-92 years. Vertebral body areal BMD was measured using DXA. Specimens were compressed at 1 kN for 30 min, while creep in each vertebral body was measured using an optical MacReflex system. After 30 min recovery, each specimen was subjected to a controlled overload event which caused minor damage to one of its vertebrae. The creep test was then repeated. Vertebral body creep was measurable in specimens with BMD Creep was greater anteriorly than posteriorly (p creep by 800 % (anteriorly), 1,000 % (centrally) and 600 % (posteriorly). In 34 vertebrae with complete before-and-after data, anterior wedging occurring during the 1st creep test averaged 0.07° (STD 0.17°), and in the 2nd test (after minor damage) it averaged 0.79° (STD 1.03°). The increase was highly significant (P creep test was proportional to the severity of damage, as quantified by specimen height loss during the overload event (r (2) = 0.51, p creep to such an extent that it makes a substantial contribution to vertebral deformity.
Directory of Open Access Journals (Sweden)
Andrew V. Khokhlov
2017-04-01
Full Text Available The nonlinear Maxwell-type constitutive relation with two arbitrary material functions for viscoelastoplastic multi-modulus materials is studied analytically in uniaxial isothermic case to reveal the model abilities and applicability scope and to develop techniques of its identification, tuning and fitting. The constitutive equation is aimed at adequate modeling of the rheological phenomena set which is typical for reonomic materials exhibiting non-linear hereditary properties, strong strain rate sensitivity, secondary creep, yielding at constant stress, tension compression asymmetry and such temperature effects as increase of material compliance, strain rate sensitivity and rates of dissipation, relaxation, creep and plastic strain accumulation with temperature growth. The model is applicable for simulation of mechanical behaviour of various polymers, their solutions and melts, solid propellants, sand-asphalt concretes, composite materials, titanium and aluminum alloys, ceramics at high temperature and so on. To describe the influence of temperature on material mechanical behavior (under isothermic conditions, two scalar material parameters of the model (viscosity coefficient and “modulus of elasticity” are considered as a functions of temperature level. The general restrictions on their properties which are necessary and sufficient for adequate qualitative description of the basic thermomechanical phenomena related to typical temperature influence on creep and relaxation curves, creep recovery curves, creep curves under step-wise loading and quasi-static stress-strain curves of viscoelastoplastic materials are obtained. The restrictions are derived using systematic analytical study of general qualitative features of the theoretic creep and relaxation curves, creep curves under step-wise loading, long-term strength curves and stress-strain curves at constant strain or stress rates generated by the constitutive equation (under minimal
Flexural creep behaviour of jute polypropylene composites
Chandekar, Harichandra; Chaudhari, Vikas
2016-09-01
Present study is about the flexural creep behaviour of jute fabric reinforced polypropylene (Jute-PP) composites. The PP sheet and alkali treated jute fabric is stacked alternately and hot pressed in compression molding machine to get Jute-PP composite laminate. The flexural creep study is carried out on dynamic mechanical analyzer. The creep behaviour of the composite is modeled using four-parameter Burgers model. Short-term accelerated creep testing is conducted which is later used to predict long term creep behaviour. The feasibility of the construction of a master curve using the time-temperature superposition (TTS) principle to predict long term creep behavior of unreinforced PP and Jute-PP composite is investigated.
Magnetothermoelastic creep analysis of functionally graded cylinders
International Nuclear Information System (INIS)
Loghman, A.; Ghorbanpour Arani, A.; Amir, S.; Vajedi, A.
2010-01-01
This paper describes time-dependent creep stress redistribution analysis of a thick-walled FGM cylinder placed in uniform magnetic and temperature fields and subjected to an internal pressure. The material creep, magnetic and mechanical properties through the radial graded direction are assumed to obey the simple power law variation. Total strains are assumed to be the sum of elastic, thermal and creep strains. Creep strains are time, temperature and stress dependent. Using equations of equilibrium, stress-strain and strain-displacement a differential equation, containing creep strains, for displacement is obtained. Ignoring creep strains in this differential equation a closed form solution for the displacement and initial magnetothermoelastic stresses at zero time is presented. Initial magnetothermoelastic stresses are illustrated for different material properties. Using Prandtl-Reuss relation in conjunction with the above differential equation and the Norton's law for the material uniaxial creep constitutive model, the radial displacement rate is obtained and then the radial and circumferential creep stress rates are calculated. Creep stress rates are plotted against dimensionless radius for different material properties. Using creep stress rates, stress redistributions are calculated iteratively using magnetothermoelastic stresses as initial values for stress redistributions. It has been found that radial stress redistributions are not significant for different material properties, however major redistributions occur for circumferential and effective stresses.
International Nuclear Information System (INIS)
Ohnuma, Hiroshi; Abe, Hirotoshi
1979-01-01
In order to design rationally the vessels made of prestressed concrete for nuclear power stations and to improve the accuracy of high temperature creep analysis, the Central Research Institute of Electric Power Industry had carried out the proving experiments with scale models. In order to improve the accuracy of analysis, it is important to grasp the creep behavior of the concrete subjected to triaxial compressive stresses at high temperature as the basic property of concrete, because actual prestressed concrete vessels are in such conditions. In this paper, the triaxial compression creep test at 60 deg. C using the concrete specimens with same mixing ratio as the scale models is reported. The compressive strength of the concrete at the age of 28 days was 406 kg/cm 2 , and the age of the concrete at the time of loading was 63 days. Creep and creep recovery were measured for 5 months and 2 months, respectively. The creep of concrete due to uniaxial compression increased with temperature rise, and the creep strain at 60 deg. C was 2.54 times as much as that at 20 deg. C. The effective Poisson's ratio in triaxial compression creep was 0.15 on the average, based on the creep strain due to uniaxial compression at 60 deg. C. The creep recovery rate in high temperature, triaxial compression creep was 33% on the average. (Kako, I.)
Exploring the potential of multivariate depth-damage and rainfall-damage models
DEFF Research Database (Denmark)
van Ootegem, Luc; van Herck, K.; Creten, T.
2018-01-01
In Europe, floods are among the natural catastrophes that cause the largest economic damage. This article explores the potential of two distinct types of multivariate flood damage models: ‘depth-damage’ models and ‘rainfall-damage’ models. We use survey data of 346 Flemish households that were...... victim of pluvial floods complemented with rainfall data from both rain gauges and weather radars. In the econometrical analysis, a Tobit estimation technique is used to deal with the issue of zero damage observations. The results show that in the ‘depth-damage’ models flood depth has a significant...... impact on the damage. In the ‘rainfall-damage’ models there is a significant impact of rainfall accumulation on the damage when using the gauge rainfall data as predictor, but not when using the radar rainfall data. Finally, non-hazard indicators are found to be important for explaining pluvial flood...
High temperature creep-fatigue design
International Nuclear Information System (INIS)
Tavassoli, A. A. F.; Fournier, B.; Sauzay, M.
2010-01-01
Generation IV fission and future fusion reactors envisage development of more efficient high temperature concepts where materials performances are key to their success. This paper examines different types of high temperature creep-fatigue interactions and their implications on design rules for the structural materials retained in both programmes. More precisely, the paper examines current status of design rules for the stainless steel type 316L(N), the conventional Modified 9Cr-1Mo martensitic steel and the low activation Eurofer steel. Results obtained from extensive high temperature creep, fatigue and creep-fatigue tests performed on these materials and their welded joints are presented. These include sequential creep-fatigue and relaxation creep-fatigue tests with hold times in tension, in compression or in both. Effects of larger plastic deformations on fatigue properties are studied through cyclic creep tests or fatigue tests with extended hold time in creep. In most cases, mechanical test results are accompanied with microstructural and fractographic observations. In the case of martensitic steels, the effect of oxidation is examined by performing creep-fatigue tests on identical specimens in vacuum. Results obtained are analyzed and their implications on design allowable and creep-fatigue interaction diagrams are presented. While reasonable confidence is found in predicting creep-fatigue damage through existing code procedures for austenitic stainless steels, effects of cyclic softening and coarsening of microstructure of martensitic steels throughout the fatigue life on materials properties need to be taken into account for more precise damage calculations. In the long-term, development of ferritic/martensitic steels with stable microstructure, such as ODS steels, is proposed. (authors)
High temperature creep-fatigue design
Energy Technology Data Exchange (ETDEWEB)
Tavassoli, A. A. F.; Fournier, B.; Sauzay, M. [CEA Saclay, DEN DMN, F-91191 Gif Sur Yvette (France)
2010-07-01
Generation IV fission and future fusion reactors envisage development of more efficient high temperature concepts where materials performances are key to their success. This paper examines different types of high temperature creep-fatigue interactions and their implications on design rules for the structural materials retained in both programmes. More precisely, the paper examines current status of design rules for the stainless steel type 316L(N), the conventional Modified 9Cr-1Mo martensitic steel and the low activation Eurofer steel. Results obtained from extensive high temperature creep, fatigue and creep-fatigue tests performed on these materials and their welded joints are presented. These include sequential creep-fatigue and relaxation creep-fatigue tests with hold times in tension, in compression or in both. Effects of larger plastic deformations on fatigue properties are studied through cyclic creep tests or fatigue tests with extended hold time in creep. In most cases, mechanical test results are accompanied with microstructural and fractographic observations. In the case of martensitic steels, the effect of oxidation is examined by performing creep-fatigue tests on identical specimens in vacuum. Results obtained are analyzed and their implications on design allowable and creep-fatigue interaction diagrams are presented. While reasonable confidence is found in predicting creep-fatigue damage through existing code procedures for austenitic stainless steels, effects of cyclic softening and coarsening of microstructure of martensitic steels throughout the fatigue life on materials properties need to be taken into account for more precise damage calculations. In the long-term, development of ferritic/martensitic steels with stable microstructure, such as ODS steels, is proposed. (authors)
Computational model for the assessment of oil spill damages
Energy Technology Data Exchange (ETDEWEB)
Seip, K L; Heiberg, A B; Brekke, K A
1985-06-01
A description is given of the method and the required data of a model for calculating oil spill damages. Eleven damage attributes are defined: shorelength contaminated, shore restitution time, birds dead, restitution time for three groups of birds, open sea damages-two types, damages to recreation, economy and fisheries. The model has been applied in several cases of oil pollution assessments: in an examination of alternative models for the organization of oil spill combat in Norway, in the assessment of the damages coused by a blowout at Tromsoeflaket and in assessing a possible increase in oil spill preparedness for Svalbard. 56 references.
Directory of Open Access Journals (Sweden)
Huang-bin Lin
2015-01-01
Full Text Available A new method of characterizing the damage of high strength concrete structures is presented, which is based on the deformation energy double parameters damage model and incorporates both of the main forms of damage by earthquakes: first time damage beyond destruction and energy consumption. Firstly, test data of high strength reinforced concrete (RC columns were evaluated. Then, the relationship between stiffness degradation, strength degradation, and ductility performance was obtained. And an expression for damage in terms of model parameters was determined, as well as the critical input data for the restoring force model to be used in analytical damage evaluation. Experimentally, the unloading stiffness was found to be related to the cycle number. Then, a correction for this changing was applied to better describe the unloading phenomenon and compensate for the shortcomings of structure elastic-plastic time history analysis. The above algorithm was embedded into an IDARC program. Finally, a case study of high strength RC multistory frames was presented. Under various seismic wave inputs, the structural damages were predicted. The damage model and correction algorithm of stiffness unloading were proved to be suitable and applicable in engineering design and damage evaluation of a high strength concrete structure.
Computational simulation for creep fracture properties taking microscopic mechanism into account
International Nuclear Information System (INIS)
Tabuchi, Masaaki
2003-01-01
Relationship between creep crack growth rate and microscopic fracture mechanism i.e., wedge-type intergranular, transgranular and cavity-type intergranular crack growth, has been investigated. The growth rate of wedge-type and transgranular creep crack could be characterized by creep ductility. Creep damages formed ahead of the cavity-type crack tip accelerated the crack growth rate. Based on the experimental results, FEM code that simulates creep crack growth has been developed by taking the fracture mechanism into account. The effect of creep ductility and void formation ahead of the crack tip on creep crack growth behavior could be simulated. (author)
Creep Properties of Walikukun (Schouthenia ovata Timber Beams
Directory of Open Access Journals (Sweden)
Ali Awaludin
2016-09-01
Full Text Available This study presents an evaluation of creep constants of Walikukun (Schoutheniaovata timber beams when rheological model of four solid elements, which is obtained byassembling Kelvin and Maxwell bodies in parallel configuration, was adopted. Creep behaviorobtained by this method was further discussed and compared with creep behavior developedusing phenomenological model of the previous study. Creep data of previous study was deformationmeasurement of Walikukun beams having cross-section of 15 mm by 20 mm with a clearspan of 550 mm loaded for three weeks period under two different room conditions: with andwithout Air Conditioner. Creep behavior given by both four solid elements model and phenomenological(in this case are power functions had good agreement during the period of creepmeasurement, but they give different prediction of creep factor beyond this period. The powerfunction of phenomenological model could give a reasonable creep prediction, while for the foursolid elements model a necessary modification is required to adjust its long-term creep behavior.
Assessment of concrete creep and shrinkage
International Nuclear Information System (INIS)
Trivedi, Neha; Singh, R.K.
2012-01-01
B-3 model prediction of concrete creep and shrinkage strains on cylindrical specimen and BARC Containment test model (BARCOM) are presented. Experimental shrinkage strain is shown to be in agreement with B-3 model predictions for cylindrical specimen and BARCOM. Creep strain in cylindrical specimen is found to be in agreement with B-3 model. In BARCOM for wall cast in different pores, creep strain is in agreement with B-3 model in hoop direction however in longitudinal direction, observed creep strain in higher than B-3 model. For dome structure cast in a single pour, experimental creep strain shows confirmity with B-3 model both in hoop and longitudinal directions. The study on concrete aging and average longitudinal shrinkage strain is carried out. (author)
Room temperature creep in metals and alloys
Energy Technology Data Exchange (ETDEWEB)
Deibler, Lisa Anne [Sandia National Lab. (SNL-NM), Albuquerque, NM (United States). Materials Characterization and Performance
2014-09-01
Time dependent deformation in the form of creep and stress relaxation is not often considered a factor when designing structural alloy parts for use at room temperature. However, creep and stress relaxation do occur at room temperature (0.09-0.21 T_{m} for alloys in this report) in structural alloys. This report will summarize the available literature on room temperature creep, present creep data collected on various structural alloys, and finally compare the acquired data to equations used in the literature to model creep behavior. Based on evidence from the literature and fitting of various equations, the mechanism which causes room temperature creep is found to include dislocation generation as well as exhaustion.
Creep rupture behavior of unidirectional advanced composites
Yeow, Y. T.
1980-01-01
A 'material modeling' methodology for predicting the creep rupture behavior of unidirectional advanced composites is proposed. In this approach the parameters (obtained from short-term tests) required to make the predictions are the three principal creep compliance master curves and their corresponding quasi-static strengths tested at room temperature (22 C). Using these parameters in conjunction with a failure criterion, creep rupture envelopes can be generated for any combination of in-plane loading conditions and ambient temperature. The analysis was validated experimentally for one composite system, the T300/934 graphite-epoxy system. This was done by performing short-term creep tests (to generate the principal creep compliance master curves with the time-temperature superposition principle) and relatively long-term creep rupture tensile tests of off-axis specimens at 180 C. Good to reasonable agreement between experimental and analytical results is observed.
Creep-fatigue interactions in an austenitic stainless steel
International Nuclear Information System (INIS)
Majumdar, S.; Maiya, P.S.
1978-01-01
A phenomenological model of the interaction between creep and fatigue in Type 304 stainless steel at elevated temperatures is presented. The model is based on a crack-growth equation and an equation governing cavity growth, expressed in terms of current plastic strain and plastic strain rate. Failure is assumed to occur when a proposed interaction equation is satisfied. Various parameters of the equations can be obtained by correlation with continuously cycling fatigue and monotonic creep-rupture test data, without the use of any hold-time fatigue tests. Effects of various wave shapes such as tensile, compressive, and symmetrical hold on the low-cycle fatigue life can be computed by integrating the damage-rate equations along the appropriate loading path. Microstructural evidence in support of the proposed model is also discussed
Blackburn, E. D.; Hadizadeh, J.; Babaie, H. A.
2009-12-01
The prevailing models of shear localization in fault gouges are mainly based on experimental aggregates that necessarily neglect the effects of chemical and mechanical maturation with time. The SAFOD cores have provided a chance to test whether cataclasis as a deformation mechanism and factors such as porosity and particle size, critical in some existing shear localization models continue to be critical in mature gouges. We studied a core sample from 3194m MD in the SAFOD phase 3, which consists of intensely foliated shale-siltstone cataclasites in contact with less deformed shale. Microstructures were studied in 3 perpendicular planes with reference to foliation using high resolution scanning electron microscopy, cathodoluminescence imaging, X-ray fluorescence mapping, and energy dispersive X-ray spectroscopy. The cataclastic foliation, recognizable at length scales >100 μm, is primarily defined by bands of clay gouge with distinct microstructure, clay content, and porosity. Variations in elemental composition and porosity of the clay gouge were measured continuously across the foliation. Prominent features within the foliation bands include lens-shaped clusters of highly brecciated and veined siltstone fragments, pyrite smears, and pyrite-cemented cataclasites. The microstructural relations and chemical data provide clear evidence of multiple episodes of veining and deformation with some possibility of relative age determination for the episodes. There is evidence of syn-deformation hydrothermal changes including growth and brittle shear of pyrite, alteration of host shale clays to illite-smectite clays and Fe-rich smectite. Evidence of grain-boundary corrosion of non-clay mineral fragments suggests pressure solution creep. The gouge porosity estimates varied from 0-18% (about 3% in less deformed shale) with the highest value in the bands with abundant siltstone fragments. The banding is mechanically significant since it pervasively segregates the gouge into
Micromechanical modeling of strength and damage of fiber reinforced composites
Energy Technology Data Exchange (ETDEWEB)
Mishnaevsky, L. Jr.; Broendsted, P.
2007-03-15
The report for the first year of the EU UpWind project includes three parts: overview of concepts and methods of modelling of mechanical behavior, deformation and damage of unidirectional fiber reinforced composites, development of computational tools for the automatic generation of 3D micromechanical models of fiber reinforced composites, and micromechanical modelling of damage in FRC, and phenomenological analysis of the effect of frequency of cyclic loading on the lifetime and damage evolution in materials. (au)
Experimental Damage Identification of a Model Reticulated Shell
Directory of Open Access Journals (Sweden)
Jing Xu
2017-04-01
Full Text Available The damage identification of a reticulated shell is a challenging task, facing various difficulties, such as the large number of degrees of freedom (DOFs, the phenomenon of modal localization and transition, and low modeling accuracy. Based on structural vibration responses, the damage identification of a reticulated shell was studied. At first, the auto-regressive (AR time series model was established based on the acceleration responses of the reticulated shell. According to the changes in the coefficients of the AR model between the damaged conditions and the undamaged condition, the damage of the reticulated shell can be detected. In addition, the damage sensitive factors were determined based on the coefficients of the AR model. With the damage sensitive factors as the inputs and the damage positions as the outputs, back-propagation neural networks (BPNNs were then established and were trained using the Levenberg–Marquardt algorithm (L–M algorithm. The locations of the damages can be predicted by the back-propagation neural networks. At last, according to the experimental scheme of single-point excitation and multi-point responses, the impact experiments on a K6 shell model with a scale of 1/10 were conducted. The experimental results verified the efficiency of the proposed damage identification method based on the AR time series model and back-propagation neural networks. The proposed damage identification method can ensure the safety of the practical engineering to some extent.
Influence of creep and cyclic oxidation in thermal barrier coatings
Energy Technology Data Exchange (ETDEWEB)
Seiler, Philipp; Baeker, Martin; Roesler, Joachim [Technische Univ. Braunschweig (Germany). Inst. fuer Werkstoffe
2012-01-15
The lifetime of thermal barrier coating systems is limited by cracks close to the interfaces, causing delamination. To study the failure mechanisms, a simplified model system is analysed which consists of a bond-coat bulk material, a thermally grown oxide, and an yttria-stabilised zirconia topcoat. The stresses in the model system are calculated using a finite element model which covers the simulation of full thermal cycles, creep in all layers, and the anisotropic oxidation during dwelling. Creep in the oxide and the thermal barrier coating is varied with the use of different creep parameter sets. The influence of creep in the bondcoat is analysed by using two different bond-coat materials: fast creeping Fecralloy and slow creeping oxide dispersion strengthened MA956. It is shown that creep in the bondcoat influences the lifetime of the coatings. Furthermore, a fast creeping thermally grown oxide benefits the lifetime of the coating system. (orig.)
Creep fatigue assessment for EUROFER components
Energy Technology Data Exchange (ETDEWEB)
Özkan, Furkan, E-mail: oezkan.furkan@partner.kit.edu; Aktaa, Jarir
2015-11-15
Highlights: • Design rules for creep fatigue assessment are developed to EUROFER components. • Creep fatigue assessment tool is developed in FORTRAN code with coupling MAPDL. • Durability of the HCPB-TBM design is discussed under typical fusion reactor loads. - Abstract: Creep-fatigue of test blanket module (TBM) components built from EUROFER is evaluated based on the elastic analysis approach in ASME Boiler Pressure Vessel Code (BPVC). The required allowable number of cycles design fatigue curve and stress-to-rupture curve to estimate the creep-fatigue damage are used from the literature. Local stress, strain and temperature inputs for the analysis of creep-fatigue damage are delivered by the finite element code ANSYS utilizing the Mechanical ANSYS Parametric Design Language (MAPDL). A developed external FORTRAN code used as a post processor is coupled with MAPDL. Influences of different pulse durations (hold-times) and irradiation on creep-fatigue damage for the preliminary design of the Helium Cooled Pebble Bed Test Blanket Module (HCPB-TBM) are discussed for the First Wall component of the TBM box.
Vinogradov, Aleksandra M.; Ihlefeld, Curtis M.; Henslee, Issac
2009-01-01
The paper concerns the time-dependent behavior of electroactive polymers (EAP) and their use in advanced intelligent structures for space exploration. Innovative actuator design for low weight and low power valves required in small plants planned for use on the moon for chemical analysis is discussed. It is shown that in-depth understanding of cyclic loading effects observed through accelerated creep rates due to creep-fatigue interaction in polymers is critical in terms of proper functioning of EAP based actuator devices. In the paper, an overview of experimental results concerning the creep properties and cyclic creep response of a thin film piezoelectric polymer polyvinylidene fluoride (PVDF) is presented. The development of a constitutive creep-fatigue interaction model to predict the durability and service life of electroactive polymers is discussed. A novel method is proposed to predict damage accumulation and fatigue life of polymers under oyclic loading conditions in the presence of creep. The study provides a basis for ongoing research initiatives at the NASA Kennedy Space Center in the pursuit of new technologies using EAP as active elements for lunar exploration systems.
Energy Technology Data Exchange (ETDEWEB)
Freeze, G.A.; Larson, K.W. [INTERA, Inc., Albuquerque, NM (United States); Davies, P.B. [Sandia National Labs., Albuquerque, NM (United States)
1995-10-01
Eight alternative methods for approximating salt creep and disposal room closure in a multiphase flow model of the Waste Isolation Pilot Plant (WIPP) were implemented and evaluated: Three fixed-room geometries three porosity functions and two fluid-phase-salt methods. The pressure-time-porosity line interpolation method is the method used in current WIPP Performance Assessment calculations. The room closure approximation methods were calibrated against a series of room closure simulations performed using a creep closure code, SANCHO. The fixed-room geometries did not incorporate a direct coupling between room void volume and room pressure. The two porosity function methods that utilized moles of gas as an independent parameter for closure coupling. The capillary backstress method was unable to accurately simulate conditions of re-closure of the room. Two methods were found to be accurate enough to approximate the effects of room closure; the boundary backstress method and pressure-time-porosity line interpolation. The boundary backstress method is a more reliable indicator of system behavior due to a theoretical basis for modeling salt deformation as a viscous process. It is a complex method and a detailed calibration process is required. The pressure lines method is thought to be less reliable because the results were skewed towards SANCHO results in simulations where the sequence of gas generation was significantly different from the SANCHO gas-generation rate histories used for closure calibration. This limitation in the pressure lines method is most pronounced at higher gas-generation rates and is relatively insignificant at lower gas-generation rates. Due to its relative simplicity, the pressure lines method is easier to implement in multiphase flow codes and simulations have a shorter execution time.
International Nuclear Information System (INIS)
Freeze, G.A.; Larson, K.W.; Davies, P.B.
1995-10-01
Eight alternative methods for approximating salt creep and disposal room closure in a multiphase flow model of the Waste Isolation Pilot Plant (WIPP) were implemented and evaluated: Three fixed-room geometries three porosity functions and two fluid-phase-salt methods. The pressure-time-porosity line interpolation method is the method used in current WIPP Performance Assessment calculations. The room closure approximation methods were calibrated against a series of room closure simulations performed using a creep closure code, SANCHO. The fixed-room geometries did not incorporate a direct coupling between room void volume and room pressure. The two porosity function methods that utilized moles of gas as an independent parameter for closure coupling. The capillary backstress method was unable to accurately simulate conditions of re-closure of the room. Two methods were found to be accurate enough to approximate the effects of room closure; the boundary backstress method and pressure-time-porosity line interpolation. The boundary backstress method is a more reliable indicator of system behavior due to a theoretical basis for modeling salt deformation as a viscous process. It is a complex method and a detailed calibration process is required. The pressure lines method is thought to be less reliable because the results were skewed towards SANCHO results in simulations where the sequence of gas generation was significantly different from the SANCHO gas-generation rate histories used for closure calibration. This limitation in the pressure lines method is most pronounced at higher gas-generation rates and is relatively insignificant at lower gas-generation rates. Due to its relative simplicity, the pressure lines method is easier to implement in multiphase flow codes and simulations have a shorter execution time
A continuous damage approach for the analysis of creep-fatigue behavior of 2 1/4 Cr - 1 Mo steel
International Nuclear Information System (INIS)
Gomuc, R.; Biron, A.; Bui-Quoc, T.
1985-01-01
Components made from 2 1/4 Cr-1 Mo in thermal and nuclear power plants have usually been designed for lifetimes as long as forty years at service temperatures approaching 593 o C. While several experimental investigations on the creep-fatigue behaviour of such materials have been reported, a detailed analysis of material behavior under these loading conditions is not available, to the authors knowledge. The aim of the present paper is to report the results of an analysis on these experimental data using a recently developed procedure. (author)
Effect of microstructure on light ion irradiation creep in nickel
International Nuclear Information System (INIS)
Henager, C.H. Jr.; Simonen, E.P.; Bradley, E.R.; Stang, R.G.
1983-01-01
The concept of inhomogeneous slip or localized deformation is introduced to account for a weak dependence of irradiation creep on initial microstructure. Specimens of pure nickel (Ni) with three different microstructures were irradiated at 473 K with 15-17 MeV deuterons in the Pacific Northwest Laboratory (PNL) light ion irradiation creep apparatus. A dispersed barrier model for Climb-Glide (CG) creep was unable to account for the observed creep rates and creep strains. The weak dependence on microstructure was consistent with the Stress Induced Preferential Absorption (SIPA) creep mechanism but a high stress enhanced bias had to be assumed to account for the creep rates. Also, SIPA was unable to account for the observed creep strains. The CG and SIPA modeling utilized rate theory calculations of point defect fluxes and transmission electron microscopy for sink sizes and densities. (orig.)
Effects of microstructure on light ion irradiation creep in nickel
International Nuclear Information System (INIS)
Henager, C.H. Jr.; Simonen, E.P.; Bradley, E.R.; Stang, R.G.
1982-10-01
The concept of inhomogeneous slip or localized deformation is introduced to account for a weak dependence of irradiation creep on initial microstructure. Specimens of pure Ni with three different microstructures were irradiated at 473 0 K with 15 to 17 MeV deuterons in the PNL light ion irradiation creep apparatus. A dispersed barrier model for climb-glide creep was unable to account for the observed creep rates and creep strains. The weak dependence on microstructure was consistent with the SIPA creep mechanism but a high stress enhanced bias had to be assumed to account for the creep rates. Also, SIPA was unable to account for the observed creep strains. The modeling utilized rate theory calculations of point defect fluxes and transmission electron microscopy for sink sizes and densities
Steady-state creep of discontinuous fibre composites
International Nuclear Information System (INIS)
Boecker Pedersen, O.
1975-07-01
A review is given of the relevant literature on creep of composites, including a presentation of existing models for the steady-state creep of composites containing aligned discontinuous fibres where creep of the matrix and fibres is assumed to follow a power law. A model is suggested for predicting the composite creep law from a matrix creep law given in a general form, in the case where the fibres do not creep. The composite creep law predicted by this model is compared with those predicted by previous models, when these are extended to comprise a general matrix creep law. Experimentally, pure copper and composites consisting of aligned discontinuous tungsten fibres in a copper matrix were creep tested at a temperature of 500 deg C. The results indicate a relatively low stress sensitivity of the steady-state creep-rate for pure copper and relatively high stress sensitivity for the composites. This may be explained by the creep models based upon a general matrix creep law. A quantitative prediction shows promising agreement with the present experimental results. (author)
Simultaneous consolidation and creep
DEFF Research Database (Denmark)
Krogsbøll, Anette
1997-01-01
Materials that exhibit creep under constant effective stress typically also show rate dependent behavior. The creep deformations and the rate sensitive behavior is very important when engineering and geological problems with large time scales are considered. When stress induced compaction...
Significance of primary irradiation creep in graphite
CSIR Research Space (South Africa)
Erasmus, C
2013-05-01
Full Text Available Traditionally primary irradiation creep is introduced into graphite analysis by applying the appropriate amount of creep strain to the model at the initial time-step. This is valid for graphite components that are subjected to high fast neutron flux...
Towards self-healing creep resistant steels
Van der Zwaag, S.; Zhang, S.; Fang, H.; Bruck, E.; Van Dijk, N.H.
2016-01-01
We report the main findings of our work on the behaviour of binary Fe-Cu and Fe-Au model alloys designed to explore routes to create new creep resistant steels having an in-built ability to autonomously fill creep induced porosity at grain boundaries. The alloying elements were selected on the basis
Creep behaviour of thin walled composite tubes
International Nuclear Information System (INIS)
Thiebaud, F.; Muzic, B.; Perreux, D.; Varchon, D.; Oytana, C.; Lebras, J.
1993-01-01
Fiber reinforced composites are more and more employed in high performance structure for nuclear power plant, mainly as water piping tubes. The increase of the use of composites is due to the advantages that they give : high stiffness, large ultimate strength, corrosion resistance. This last advantage is sought for the pieces in contact with water, and it's one of the reason why the composite can be preferred to metal. However the mechanical behaviour of composite is actually poorly known. The high anisotropy is the main difficulty to obtain a realistic model of behaviour. This problem implies that the safety factor used in the design of structure is often too large. In this article a general overview of the mechanical behaviour of tube made in glass epoxy material is proposed. We discuss especially the creep behaviour under biaxial loadings. The form of the proposed model presently allows predicting a nonlinearity of the behaviour and provides a good correlation with the experimental data of several tests not described in this paper. It accounts for the change of the Poisson ratio during creep and cyclic tests. However the complete identification requires long time testings and consequently the model must be corrected to take into account the damage which occurs in these cases
International Nuclear Information System (INIS)
Blass, J.J.
1982-01-01
An improved multiaxial fatigue failure criterion was developed based on the results of combined axial-torsional strain cycling tests of AISI 304 and 2-1/4 Cr-1 Mo steel conducted at 538 0 C (1000 0 F). The formulation of this criterion involves the shear and normal components of inelastic strain range on the planes of maximum inelastic shear strain range. Optimum values of certain parameters contained in the formulation were obtained for each material by the method of least squares. The ability of this criterion to correlate the test results was compared with that of the usual (Mises) equivalent inelastic strain range criterion. An improved definition of equivalent inelastic strain range resulting from these considerations was used to generalize the theory of Strain Range Partitioning to multiaxial stress-strain conditions and was also applied to the linear summation of creep and fatigue damage
A new method for measuring creep-strain
International Nuclear Information System (INIS)
Joas, H.D.
2001-01-01
To realise a safe and economic operation of components undergoing creep damage, sometimes a theoretical and an experimental evaluation is necessary. The discussed Creep-Replica-Method is a new possibility to estimate the creep-strain due to the real loading conditions of a component during a certain time of operation which gives a chance to assess the integrity, the consumed life and the possible repairing of a component. (Author)
International Nuclear Information System (INIS)
Villani, Aurelien
2015-01-01
Radiation damage is known to lead to material failure and thus is of critical importance to lifetime and safety within nuclear reactors. While mechanical behaviour of materials under irradiation has been the subject of numerous studies, the current predictive capabilities of such phenomena appear limited. The clustering of point defects such as vacancies and self interstitial atoms gives rise to creep, void swelling and material embrittlement. Nano-scale metallic multilayer systems have be shown to have the ability to evacuate such point defects, hence delaying the occurrence of critical damage. In addition, they exhibit outstanding mechanical properties. The objective of this work is to develop a thermodynamically consistent continuum framework at the meso and nano-scales, which accounts for the major physical processes encountered in such metallic multilayer systems and is able to predict their microstructural evolution and behavior under irradiation. Mainly three physical phenomena are addressed in the present work: stress-diffusion coupling and diffusion induced creep, the void nucleation and growth in multilayer systems under irradiation, and the interaction of dislocations with the multilayer interfaces. In this framework, the microstructure is explicitly modeled, in order to account accurately for their effects on the system behavior. The diffusion creep strain rate is related to the gradient of the vacancy flux. A Cahn-Hilliard approach is used to model void nucleation and growth, and the diffusion equations for vacancies and self interstitial atoms are complemented to take into account the production of point defects due to irradiation cascades, the mutual recombination of defects and their evacuation through grain boundaries. In metallic multilayers, an interface affected zone is defined, with an additional slip plane to model the interface shearable character, and where dislocations cores are able to spread. The model is then implemented numerically
Integrated geomechanical modelling for deep subsurface damage
Wees, J.D. van; Orlic, B.; Zijl, W.; Jongerius, P.; Schreppers, G.J.; Hendriks, M.
2001-01-01
Government, E&P and mining industry increasingly demand fundamental insight and accurate predictions on subsurface and surface deformation and damage due to exploitation of subsurface natural resources, and subsurface storage of energy residues (e.g. CO2). At this moment deformation is difficult to
High-Temperature Creep-Fatigue Behavior of Alloy 617
Directory of Open Access Journals (Sweden)
Rando Tungga Dewa
2018-02-01
Full Text Available This paper presents the high-temperature creep-fatigue testing of a Ni-based superalloy of Alloy 617 base metal and weldments at 900 °C. Creep-fatigue tests were conducted with fully reversed axial strain control at a total strain range of 0.6%, 1.2%, and 1.5%, and peak tensile hold time of 60, 180, and 300 s. The effects of different constituents on the combined creep-fatigue endurance such as hold time, strain range, and stress relaxation behavior are discussed. Under all creep-fatigue tests, weldments’ creep-fatigue life was less than base metal. In comparison with the low-cycle fatigue condition, the introduction of hold time decreased the cycle number of both base metal and weldments. Creep-fatigue lifetime in the base metal was continually decreased by increasing the tension hold time, except for weldments under longer hold time (>180 s. In all creep-fatigue tests, intergranular brittle cracks near the crack tip and thick oxide scales at the surface were formed, which were linked to the mixed-mode creep and fatigue cracks. Creep-fatigue interaction in the damage-diagram (D-Diagram (i.e., linear damage summation was evaluated from the experimental results. The linear damage summation was found to be suitable for the current limited test conditions, and one can enclose all the data points within the proposed scatter band.
IFMIF - Design Study for in Situ Creep Fatigue Tests
International Nuclear Information System (INIS)
Gordeev, S.; Heinzel, V.; Simakov, St.; Stratmanns, E.; Vladimirov, P.; Moeslang, A.
2006-01-01
While the high flux volume (20-50 dpa/fpy) of the International Fusion Materials Irradiation Facility (IFMIF) is dedicated to the irradiation of ∼ 1100 qualified specimens that will be post irradiation examined after disassembling in dedicated Hot Cells, various in situ experiments are foreseen in the medium flux volume (1-20 dpa/fpy). Of specific importance for structural lifetime assessments of fusion power reactors are instrumented in situ creep-fatigue experiments, as they can simulate realistically a superposition of thermal fatigue or creep fatigue and irradiation with fusion relevant neutrons. Based on former experience with in situ fatigue tests under high energy light ion irradiation, a design study has been performed to evaluate the feasibility of in situ creep fatigue tests in the IFMIF medium flux position. The vertically arranged test module for such experiments consists basically of a frame similar to a universal testing machine, but equipped with three pulling rods, driven by independent step motors, instrumentation systems and specimen cooling systems. Therefore, three creep fatigue specimens may be tested at one time in this apparatus. Each specimen is a hollow tube with coolant flow in the specimen interior to maintain individual specimen temperatures. The recently established IFMIF global 3D geometry model was used together the latest McDeLicious code for the neutral and charged particle transport calculations. These comprehensive neutronics calculations have been performed with a fine special resolution of 0.25 cm 3 , showing among others that the specimens will be irradiated with a homogeneous damage rate of up to 13(∼ 9%) dpa/fpy and a fusion relevant damage to helium ratio of 10-12 appm He/dpa. In addition, damage and gas production rates as well as the heat deposition in structural parts of the test module have been calculated. Despite of the vertical gradients in the nuclear heating, CFD code calculations with STAR-CD revealed very
Effect of loading rate on creep of phosphorous doped copper
Energy Technology Data Exchange (ETDEWEB)
Andersson-Oestling, Henrik C.M.; Sandstroem, Rolf (Swerea KIMAB (Sweden))
2011-12-15
Creep testing of copper intended for nuclear waste disposal has been performed on continuous creep tests machines at a temperature of 75 deg C. The loading time has been varied from 1 hour to 6 months. The rupture strain including both loading and creep strains does not differ from traditional dead weight lever creep test rigs. The loading strain increases with increasing loading time, at the expense of the creep strain. The time dependence of the creep strain has been modelled taking athermal plastic deformation and creep into account. During loading the contribution to the strain from the athermal plastic deformation dominates until the stress is close to the constant load level. When the constant load has been reached there is no more athermal strain and all of the strain comes from creep
Studies of Grain Boundaries in Materials Subjected to Diffusional Creep
DEFF Research Database (Denmark)
Nørbygaard, Thomas
Grain boundaries in crystalline Cu(2%Ni) creep specimens have been studied by use of scanning and transmission electron microscopy in order to establish the mechanism of deformation. Creep rate measurements and dependencies were found to fit reasonably well with the model for diffusional creep......) with the activity displayed during diffusional creep testing. It was found that boundaries with low deviation from perfect Σ did not contribute macroscopically to the creep strain. A resist deposition procedure was examined to improve the reference surface grid so as to allow determination of the grain boundary...... plane by use of simple stereomicroscopy directly on the surface. The etched pattern deteriorated heav-ily during creep testing, supposedly because of dislocation creep, due to exces-sive creep stress. Grain boundaries have been studied and characterised by TEM providing an insight into the diversity...
Diffusion creep and its inhibition in a stainless steel
International Nuclear Information System (INIS)
Crossland, I.G.; Clay, B.D.
1977-01-01
The creep of 20% Cr, 25% Ni, Nb stainless steel was examined at low stresses and temperatures around 0.55 T/sub m/. The initial creep behaviour was consistent with the Coble theory of grain boundary diffusion creep; however, steady state creep was not observed and the creep rates quickly fell below the Coble theoretical values although they still remained greater than the Herring--Nabarro predictions. This reduction in creep rate was attributable to an increase in the effective viscosity of the steel rather than to any change in threshold stress. A model is proposed which explains the initial creep rates as being due to Coble creep with elastic accommodation at grain boundary particles. At higher strains grain boundary collapse caused by vacancy sinking is accommodated at precipitate particles by plastic deformation of the adjacent matrix material. 11 figures
Documentation for the viscoplastic and creep program
DEFF Research Database (Denmark)
Bellini, Anna
2004-01-01
of this workpackage is to simulate creep behavior of aluminum cast samples subjected to high temperature. In this document a two-state variables unified model is applied in order to simulate creep behavior and time-dependent metallurgical changes. The fundamental assumption of the unified theory is that creep...... is run using the material data obtained through the mentioned experimental study. The results obtained for the simulation of tensile tests and of creep tests are compared with experimental curves, showing a good agreement. Moreover, the document describes the results obtained during the first...... is quite stable and convergence can be reached also with big time steps. Keywords: Viscoplasticity, creep, unified constitutive model, aluminum, high temperature....
Modelling low velocity impact induced damage in composite laminates
Shi, Yu; Soutis, Constantinos
2017-12-01
The paper presents recent progress on modelling low velocity impact induced damage in fibre reinforced composite laminates. It is important to understand the mechanisms of barely visible impact damage (BVID) and how it affects structural performance. To reduce labour intensive testing, the development of finite element (FE) techniques for simulating impact damage becomes essential and recent effort by the composites research community is reviewed in this work. The FE predicted damage initiation and propagation can be validated by Non Destructive Techniques (NDT) that gives confidence to the developed numerical damage models. A reliable damage simulation can assist the design process to optimise laminate configurations, reduce weight and improve performance of components and structures used in aircraft construction.
International Nuclear Information System (INIS)
Luyt, P.C.B.; Theron, N.J.; Pietra, F.
2017-01-01
It is well known that gasket creep-relaxation results in a reduction of contact pressure between the surface of a gasket and the face of a flange over an extended period of time. This reduction may result in the subsequent failure of the circular bolted flange connection due to leakage. In this paper a pair of flat and raised face integral flanges, PN 10 DN 50 (in accordance with the European EN 1092-1 standard), with non-asbestos compressed fibre ring gaskets with aramid and a nitrile rubber binder were considered. Finite element modelling and analyses were done, for both the circular bolted flange configurations, during the seating condition. The results of the finite element analyses were experimentally validated. It was found that the number of bolt tightening increments as well as the time between the bolt tightening increments had a significant impact on the effect which gasket creep-relaxation had after the seating condition. An increase in either the number of bolting increments or the time between the bolting increments will reduce the effect which gasket creep-relaxation has once the bolts had been fastened. Based on these results it is possible to develop an optimisation scheme to minimize the effect which gasket creep-relaxation has on the contact pressure between the face of the flange and the gasket, after seating, by either increasing or decreasing the number of bolt tightening increments or the time between the bolt tightening increments. - Highlights: • Number of bolt tightening increments and time between bolt tightening increments had significant impact on effect of gasket creep-relaxation after the seating condition. • Impact of gasket creep-relaxation during seating and operating phases investigated by means of finite element analysis and experimentally verified. • Possible to develop optimisation scheme to minimize effect ofh gasket creep-relaxation on contact pressure between flange face and gasket. • Knowing the contact pressure is
Riva, Federico; Agliardi, Federico; Amitrano, David; Crosta, Giovanni B.
2018-01-01
Large alpine rock slopes undergo long-term evolution in paraglacial to postglacial environments. Rock mass weakening and increased permeability associated with the progressive failure of deglaciated slopes promote the development of potentially catastrophic rockslides. We captured the entire life cycle of alpine slopes in one damage-based, time-dependent 2-D model of brittle creep, including deglaciation, damage-dependent fluid occurrence, and rock mass property upscaling. We applied the model to the Spriana rock slope (Central Alps), affected by long-term instability after Last Glacial Maximum and representing an active threat. We simulated the evolution of the slope from glaciated conditions to present day and calibrated the model using site investigation data and available temporal constraints. The model tracks the entire progressive failure path of the slope from deglaciation to rockslide development, without a priori assumptions on shear zone geometry and hydraulic conditions. Complete rockslide differentiation occurs through the transition from dilatant damage to a compacting basal shear zone, accounting for observed hydraulic barrier effects and perched aquifer formation. Our model investigates the mechanical role of deglaciation and damage-controlled fluid distribution in the development of alpine rockslides. The absolute simulated timing of rock slope instability development supports a very long "paraglacial" period of subcritical rock mass damage. After initial damage localization during the Lateglacial, rockslide nucleation initiates soon after the onset of Holocene, whereas full mechanical and hydraulic rockslide differentiation occurs during Mid-Holocene, supporting a key role of long-term damage in the reported occurrence of widespread rockslide clusters of these ages.
Pelleg, Joshua
2017-01-01
This textbook is one of its kind, since there are no other books on Creep in Ceramics. The book consist of two parts: A and B. In part A general knowledge of creep in ceramics is considered, while part B specifies creep in technologically important ceramics. Part B covers creep in oxide ceramics, carnides and nitrides. While covering all relevant information regarding raw materials and characterization of creep in ceramics, the book also summarizes most recent innovations and developments in this field as a result of extensive literature search.
A creep life assessment method for boiler pipes using small punch creep test
International Nuclear Information System (INIS)
Izaki, Toru; Kobayashi, Toshimi; Kusumoto, Junichi; Kanaya, Akihiro
2009-01-01
The small punch creep (SPC) test is considered as a highly useful method for creep life assessment for high temperature plant components. SPC uses miniature-sized specimens and does not cause any serious sampling damages, and its assessment accuracy is at a high level. However, in applying the SPC test to the residual creep life assessment of the boiler in service, there are some issues to be studied. In order to apply SPC test to the residual creep life assessment of the 2.25Cr-1Mo steel boiler pipe, the relationship between uniaxial creep stress and the SPC test load has been studied. The virgin material, pre-crept, weldment and service aged samples of 2.25Cr-1Mo steel were tested. It was confirmed that the relationship between uniaxial creep stress and the SPC test load at the same rupture time can be described as a single straight line independent of test conditions and materials. Therefore a life assessment is possible by using SPC test in place of uniaxial creep tests. The creep life assessment using SPC was applied to actual thermal power plant components which are in service.
Creep theories compared by means of high sensitivity tensile creep data
International Nuclear Information System (INIS)
Salim, A.
1987-01-01
Commonly used creep theories include time-hardening, strain-hardening and Rabotnov's modified strain-hardening. In the paper they are examined by using high sensitivity tensile creep data produced on 1% CrMoV steel at a temperatue of 565 0 C. A special creep machine designed and developed by the author is briefly described and is compared with other existing machines. Tensile creep data reported cover a stress range of 100-260 MN m -2 ; four variable-creep tests each in duplicate are also reported. Test durations are limited to 3000 h, or failure, whichever occurs earlier. The strain-hardening theory and Rabotnov's modified strain-hardening theory are found to give good prediction of creep strain under variable stress conditions. The time-hardening theory shows a relatively poor agreement and considerably underestimates the accumulated inelastic strain under increasing stress condition. This discrepancy increases with the increased stress rate. The theories failed to predict the variable stress results towards the later part of the test where tertiary effects were significant. The use of creep equations which could account for creep strain at higher stress levels seems to improve the situation considerably. Under conditions of variable stress, it is suggested that a theory based on continuous damage mechanics concepts might give a better prediction. (author)
Probabilistic flood damage modelling at the meso-scale
Kreibich, Heidi; Botto, Anna; Schröter, Kai; Merz, Bruno
2014-05-01
Decisions on flood risk management and adaptation are usually based on risk analyses. Such analyses are associated with significant uncertainty, even more if changes in risk due to global change are expected. Although uncertainty analysis and probabilistic approaches have received increased attention during the last years, they are still not standard practice for flood risk assessments. Most damage models have in common that complex damaging processes are described by simple, deterministic approaches like stage-damage functions. Novel probabilistic, multi-variate flood damage models have been developed and validated on the micro-scale using a data-mining approach, namely bagging decision trees (Merz et al. 2013). In this presentation we show how the model BT-FLEMO (Bagging decision Tree based Flood Loss Estimation MOdel) can be applied on the meso-scale, namely on the basis of ATKIS land-use units. The model is applied in 19 municipalities which were affected during the 2002 flood by the River Mulde in Saxony, Germany. The application of BT-FLEMO provides a probability distribution of estimated damage to residential buildings per municipality. Validation is undertaken on the one hand via a comparison with eight other damage models including stage-damage functions as well as multi-variate models. On the other hand the results are compared with official damage data provided by the Saxon Relief Bank (SAB). The results show, that uncertainties of damage estimation remain high. Thus, the significant advantage of this probabilistic flood loss estimation model BT-FLEMO is that it inherently provides quantitative information about the uncertainty of the prediction. Reference: Merz, B.; Kreibich, H.; Lall, U. (2013): Multi-variate flood damage assessment: a tree-based data-mining approach. NHESS, 13(1), 53-64.
International Nuclear Information System (INIS)
Vivier, F.
2009-03-01
With the increase in worldwide energy demand, the nuclear industry is a way of producing electricity on a large scale and to answer to this need. For the design of a new generation of fission nuclear reactors and among six chosen fission reactor systems, France develops in particularly the Very High Temperature Reactor (VHTR) concept. This implies the use of materials that are more and more resistant to high temperature for long-term exposure. AREVA focuses on materials already used in fossil-fuel power plant, so that the mechanical behaviour of Grade 91 (Fe 9 Cr 1 MoNbV) has to be investigated. This ferritic-martensitic steel is considered to be a potential candidate for welded components. Such structures are combined with welded joints, which have to be studied. Three industrial partners (AREVA, CEA, EDF) have launched a study with the Centre des Materiaux in order to investigate the creep of welded joint of Grade 91. The aim of this work is to complete the available database about the mechanical behaviour of Grade 91, base metal and welded joint, during creep tests performed at 500 C up to 4500 h exposure. Thermal aging tests, tensile tests, and creep tests were performed at 450 C and 500 C using both base metal and cross-weld samples. Several geometries of cross-weld creep specimens were tested. The microstructure has not remarkably changed after tests concerning both nature and size of precipitates, and the characteristic size of the matrix sub-structure. The creep damage is not developed in the ruptured specimens after creep tests. Only little damage by cavity nucleation and growth was found in the creep specimens. Creep fracture at 500 C takes places by viscoplastic flow, contrary to tests performed at 625 C where the creep-induced damage governs the creep rupture at least for long-term lifetime. From creep curves of base metal and cross-weld specimens, a phenomenological model is proposed. The flow rule is a Norton power law with a stress exponent of 19 in
Measuring damage in physical model tests of rubble mounds
Hofland, B.; Rosa-Santos, Paulo; Taveira-Pinto, Francisco; Lemos, Rute; Mendonça, A.; Juana Fortes, C
2017-01-01
This paper studies novel ways to evaluate armour damage in physical models of coastal structures. High-resolution damage data for reference rubble mound breakwaters obtained under the HYDRALAB+ joint-research project are analysed and discussed. These tests are used to analyse the way to describe
Use of heavy ions to model radiation damage of metals
International Nuclear Information System (INIS)
Shirokov, S.V.; Vyshemirskij, M.P.
2011-01-01
The methods for modeling radiation damage of metals using heavy ions are reviewed and the results obtained are analyzed. It is shown that irradiation of metals with heavy ion can simulate neutron exposure with the equivalent dose with adequate accuracy and permits a detailed analysis of radiation damage of metals
Deformation mechanisms in cyclic creep and fatigue
International Nuclear Information System (INIS)
Laird, C.
1979-01-01
Service conditions in which static and cyclic loading occur in conjunction are numerous. It is argued that an understanding of cyclic creep and cyclic deformation are necessary both for design and for understanding creep-fatigue fracture. Accordingly a brief, and selective, review of cyclic creep and cyclic deformation at both low and high strain amplitudes is provided. Cyclic loading in conjunction with static loading can lead to creep retardation if cyclic hardening occurs, or creep acceleration if softening occurs. Low strain amplitude cyclic deformation is understood in terms of dislocation loop patch and persistent slip band behavior, high strain deformation in terms of dislocation cell-shuttling models. While interesting advances in these fields have been made in the last few years, the deformation mechanisms are generally poorly understood
Cleavage and creep fracture of rock salt
International Nuclear Information System (INIS)
Chan, K.S.; Munson, D.E.; Bodner, S.R.
1996-01-01
The dominant failure mechanism in rock salt at ambient temperature is either cleavage or creep fracture. Since the transition of creep fracture to cleavage in a compressive stress field is not well understood, failure of rock salt by cleavage and creep fracture is analyzed in this paper to elucidate the effect of stress state on the competition between these two fracture mechanisms. For cleavage fracture, a shear crack is assumed to cause the formation and growth of a symmetric pair of wing cracks in a predominantly compressive stress field. The conditions for wing-crack instability are derived and presented as the cleavage fracture boundary in the fracture mechanism map. Using an existing creep fracture model, stress conditions for the onset of creep fracture and isochronous failure curves of specified times-to-rupture are calculated and incorporated into the fracture mechanism map. The regimes of dominance by cleavage and creep fracture are established and compared with experimental data. The result indicates that unstable propagation of cleavage cracks occurs only in the presence of tensile stress. The onset of creep fracture is promoted by a tensile stress, but can be totally suppressed by a high confining pressure. Transition of creep fracture to cleavage occurs when critical conditions of stress difference and tensile stress for crack instability are exceeded
Track structure model of cell damage in space flight
Katz, Robert; Cucinotta, Francis A.; Wilson, John W.; Shinn, Judy L.; Ngo, Duc M.
1992-01-01
The phenomenological track-structure model of cell damage is discussed. A description of the application of the track-structure model with the NASA Langley transport code for laboratory and space radiation is given. Comparisons to experimental results for cell survival during exposure to monoenergetic, heavy-ion beams are made. The model is also applied to predict cell damage rates and relative biological effectiveness for deep-space exposures.
Creep-Fatigue Failure Diagnosis
Holdsworth, Stuart
2015-01-01
Failure diagnosis invariably involves consideration of both associated material condition and the results of a mechanical analysis of prior operating history. This Review focuses on these aspects with particular reference to creep-fatigue failure diagnosis. Creep-fatigue cracking can be due to a spectrum of loading conditions ranging from pure cyclic to mainly steady loading with infrequent off-load transients. These require a range of mechanical analysis approaches, a number of which are reviewed. The microstructural information revealing material condition can vary with alloy class. In practice, the detail of the consequent cracking mechanism(s) can be camouflaged by oxidation at high temperatures, although the presence of oxide on fracture surfaces can be used to date events leading to failure. Routine laboratory specimen post-test examination is strongly recommended to characterise the detail of deformation and damage accumulation under known and well-controlled loading conditions to improve the effectiveness and efficiency of failure diagnosis. PMID:28793676
Ji, Zhaojie; Guan, Zhidong; Li, Zengshan
2017-10-01
In this paper, a progressive damage model was established on the basis of ABAQUS software for predicting permanent indentation and impact damage in composite laminates. Intralaminar and interlaminar damage was modelled based on the continuum damage mechanics (CDM) in the finite element model. For the verification of the model, low-velocity impact tests of quasi-isotropic laminates with material system of T300/5228A were conducted. Permanent indentation and impact damage of the laminates were simulated and the numerical results agree well with the experiments. It can be concluded that an obvious knee point can be identified on the curve of the indentation depth versus impact energy. Matrix cracking and delamination develops rapidly with the increasing impact energy, while considerable amount of fiber breakage only occurs when the impact energy exceeds the energy corresponding to the knee point. Predicted indentation depth after the knee point is very sensitive to the parameter μ which is proposed in this paper, and the acceptable value of this parameter is in range from 0.9 to 1.0.
The interpretation of stress reductions in creep-fatigue cycles of 316 stainless steel
International Nuclear Information System (INIS)
Hales, R.
1986-11-01
A statistical analysis of stress-drop results obtained on a number of different casts of 316 stainless steel in the temperature range 550 0 C to 700 0 C is presented. In all cases the results were obtained from strain controlled fatigue tests. The equations used to describe stress relaxation here are derived from forward creep equations which describe the dependence of creep rate on time, stress and temperature. Although there is no clear correspondence between creep and stress relaxation, creep equations offer an attractive starting point. Not all the models considered exhibited the expected response to changes in temperature. A revised analysis was carried out on the assumption that stress relaxation is thermally activated according to the Arrhenius equation. Two models were found to fit the data equally well and it was not possible to choose which of these relationships is the more appropriate to describe stress relaxation of cyclically conditioned material. On the basis of the evidence both are acceptable and may be used to calculate the creep damage according to the various high temperature design codes. Whichever gives the more conservative assessment should be used until a more mechanistically based judgement can be reached. (author)
Creep behaviour of modified 9Cr-1Mo ferritic steel
International Nuclear Information System (INIS)
Choudhary, B.K.; Isaac Samuel, E.
2011-01-01
Creep deformation and fracture behaviour of indigenously developed modified 9Cr-1Mo steel for steam generator (SG) tube application has been examined at 823, 848 and 873 K. Creep tests were performed on flat creep specimens machined from normalised and tempered SG tubes at stresses ranging from 125 to 275 MPa. The stress dependence of minimum creep rate obeyed Norton's power law. Similarly, the rupture life dependence on stress obeyed a power law. The fracture mode remained transgranular at all test conditions examined. The analysis of creep data indicated that the steel obey Monkman-Grant and modified Monkman-Grant relationships and display high creep damage tolerance factor. The tertiary creep was examined in terms of the variations of time to onset of tertiary creep with rupture life, and a recently proposed concept of time to reach Monkman-Grant ductility, and its relationship with rupture life that depends only on damage tolerance factor. SG tube steel exhibited creep-rupture strength comparable to those reported in literature and specified in the nuclear design code RCC-MR.
International Nuclear Information System (INIS)
Rezgui, B.
1982-12-01
The resistance of steel to continuous fatigue is directly related to its behaviour towards the surroundings (oxidation). This interaction considerably lowers resistance to crack initiation but has no effect on propagation, and rupture is transgranular. Conversely the influence of the environment is negligible under fatigue conditions with a hold time and rupture becomes intergranular whatever the surroudings. Cavities are created inside the material during the hold time and their interaction with each other and with cracks from the surface are the factors responsible for the degradation of fatigue properties. Transgranular rupture initiated in slip bands, which characterises damage by pure fatigue, is gradually replaced by intergranular rupture under fatigue with hold time. Meanwhile a new deformation mode appears: intergranular slip. The longer the hold time the stronger its effect, a tendency offset at high temperature. Hold time, temperature and deformation promote dynamic structural aging and restoration in the material. Since the mechanisms and kinetics of creep fatigue damage are different according to the deformation level and the hold time duration it would not be safe to extrapolate the results [fr
A plastic damage model with stress triaxiality-dependent hardening
International Nuclear Information System (INIS)
Shen Xinpu; Shen Guoxiao; Zhou Lin
2005-01-01
Emphases of this study were placed on the modelling of plastic damage behaviour of prestressed structural concrete, with special attention being paid to the stress-triaxiality dependent plastic hardening law and the corresponding damage evolution law. A definition of stress triaxiality was proposed and introduced in the model presented here. Drucker-Prager -type plasticity was adopted in the formulation of the plastic damage constitutive equations. Numerical validations were performed for the proposed plasticity-based damage model with a driver subroutine developed in this study. The predicted stress-strain behaviour seems reasonably accurate for the uniaxial tension and uniaxial compression compared with the experimental data reported in references. Numerical calculations of compressions under various hydrostatic stress confinements were carried out in order to validate the stress triaxiality dependent properties of the model. (authors)
A Plastic Damage Mechanics Model for Engineered Cementitious Composites
DEFF Research Database (Denmark)
Dick-Nielsen, Lars; Stang, Henrik; Poulsen, Peter Noe
2007-01-01
This paper discusses the establishment of a plasticity-based damage mechanics model for Engineered Cementitious Composites (ECC). The present model differs from existing models by combining a matrix and fiber description in order to describe the behavior of the ECC material. The model provides...
Numerical modelling of damage evolution in ingot forging
DEFF Research Database (Denmark)
Christiansen, Peter; Martins, Paulo A.F.; Bay, Niels Oluf
2015-01-01
The ingot forging process is numerically simulated applying both the Shima-Oyane porous plasticity model as a coupled damage model and the uncoupled normalized Cockcroft & Latham criterion. Four different cases including two different lower die angles (120º and 180º) and two different sizes of feed...... (400mm and 800mm) are analysed. Comparison of the simulation results with recommendations in literature on ingot forging, indicates the normalized Cockcroft & Latham damage criterion to be the most realistic of the two....
Creep and Creep-Fatigue Crack Growth at Structural Discontinuities and Welds
Energy Technology Data Exchange (ETDEWEB)
Dr. F. W. Brust; Dr. G. M. Wilkowski; Dr. P. Krishnaswamy; Mr. Keith Wichman
2010-01-27
The subsection ASME NH high temperature design procedure does not admit crack-like defects into the structural components. The US NRC identified the lack of treatment of crack growth within NH as a limitation of the code and thus this effort was undertaken. This effort is broken into two parts. Part 1, summarized here, involved examining all high temperature creep-fatigue crack growth codes being used today and from these, the task objective was to choose a methodology that is appropriate for possible implementation within NH. The second part of this task, which has just started, is to develop design rules for possible implementation within NH. This second part is a challenge since all codes require step-by-step analysis procedures to be undertaken in order to assess the crack growth and life of the component. Simple rules for design do not exist in any code at present. The codes examined in this effort included R5, RCC-MR (A16), BS 7910, API 579, and ATK (and some lesser known codes). There are several reasons that the capability for assessing cracks in high temperature nuclear components is desirable. These include: (1) Some components that are part of GEN IV reactors may have geometries that have sharp corners - which are essentially cracks. Design of these components within the traditional ASME NH procedure is quite challenging. It is natural to ensure adequate life design by modeling these features as cracks within a creep-fatigue crack growth procedure. (2) Workmanship flaws in welds sometimes occur and are accepted in some ASME code sections. It can be convenient to consider these as flaws when making a design life assessment. (3) Non-destructive Evaluation (NDE) and inspection methods after fabrication are limited in the size of the crack or flaw that can be detected. It is often convenient to perform a life assessment using a flaw of a size that represents the maximum size that can elude detection. (4) Flaws that are observed using in-service detection
Creep and Creep-Fatigue Crack Growth at Structural Discontinuities and Welds
International Nuclear Information System (INIS)
Brust, F.W.; Wilkowski, G.M.; Krishnaswamy, P.; Wichman, Keith
2010-01-01
The subsection ASME NH high temperature design procedure does not admit crack-like defects into the structural components. The US NRC identified the lack of treatment of crack growth within NH as a limitation of the code and thus this effort was undertaken. This effort is broken into two parts. Part 1, summarized here, involved examining all high temperature creep-fatigue crack growth codes being used today and from these, the task objective was to choose a methodology that is appropriate for possible implementation within NH. The second part of this task, which has just started, is to develop design rules for possible implementation within NH. This second part is a challenge since all codes require step-by-step analysis procedures to be undertaken in order to assess the crack growth and life of the component. Simple rules for design do not exist in any code at present. The codes examined in this effort included R5, RCC-MR (A16), BS 7910, API 579, and ATK (and some lesser known codes). There are several reasons that the capability for assessing cracks in high temperature nuclear components is desirable. These include: (1) Some components that are part of GEN IV reactors may have geometries that have sharp corners - which are essentially cracks. Design of these components within the traditional ASME NH procedure is quite challenging. It is natural to ensure adequate life design by modeling these features as cracks within a creep-fatigue crack growth procedure. (2) Workmanship flaws in welds sometimes occur and are accepted in some ASME code sections. It can be convenient to consider these as flaws when making a design life assessment. (3) Non-destructive Evaluation (NDE) and inspection methods after fabrication are limited in the size of the crack or flaw that can be detected. It is often convenient to perform a life assessment using a flaw of a size that represents the maximum size that can elude detection. (4) Flaws that are observed using in-service detection
Reassembling Surveillance Creep
DEFF Research Database (Denmark)
Bøge, Ask Risom; Lauritsen, Peter
2017-01-01
We live in societies in which surveillance technologies are constantly introduced, are transformed, and spread to new practices for new purposes. How and why does this happen? In other words, why does surveillance “creep”? This question has received little attention either in theoretical developm......We live in societies in which surveillance technologies are constantly introduced, are transformed, and spread to new practices for new purposes. How and why does this happen? In other words, why does surveillance “creep”? This question has received little attention either in theoretical...... development or in empirical analyses. Accordingly, this article contributes to this special issue on the usefulness of Actor-Network Theory (ANT) by suggesting that ANT can advance our understanding of ‘surveillance creep’. Based on ANT’s model of translation and a historical study of the Danish DNA database......, we argue that surveillance creep involves reassembling the relations in surveillance networks between heterogeneous actors such as the watchers, the watched, laws, and technologies. Second, surveillance creeps only when these heterogeneous actors are adequately interested and aligned. However...
Advances in the assessment of creep data
Energy Technology Data Exchange (ETDEWEB)
Holdsworth, S.R.
2010-07-01
Many of the classical models representing the creep and rupture behaviour of metals were developed prior to and during the 1950s and 1960s, and their subsequent exploitation, in particular for the assessment of large creep property datasets, was initially limited by the capability of the analytical tools available at the time. The formation of ECCC (the European Creep Collaborative Committee) in 1991, with a main objective of providing reliable peer reviewed long-time creep property values for European Design and Product Standards, led to the development of rigorous assessment procedures such as PD6605 and DESA incorporating post assessment tests to verify: physical realism, effectiveness of model-fit within the range of the source experimental data, and extrapolation credibility. The first ECCC assessment recommendations published in 1996 undoubtedly provided a catalyst for others to exploit the availability of low cost, powerful desktop computers to develop rigorous methodologies for the physically realistic analysis of uniaxial and multi-axial data for the reliable and accurate characterisation of creep strain, and rupture strength and ductility properties. More recent improvements in data assessment methodologies have been driven by the need to effectively model the creep deformation and rupture characteristics of the complex new generation alloys and fabrications being designed to cater for the continually evolving requirements of modern advanced power plant. These advances in the assessment of creep data are reviewed. (orig.)
Higgins, N.; Lapusta, N.
2016-12-01
What physical mechanism drives the occurrence of foreshocks? Many studies have suggested that slow slip from the mainshock nucleation is a necessary ingredient for explaining foreshock observations. We explore this view, investigating asperity-type foreshock sources driven by nucleation-induced creep using rate-and-state fault models, and numerically simulatie their behavior over many rupture cycles. Inspired by the unique laboratory experiments of earthquake nucleation and rupture conducted on a meter-scale slab of granite by McLaskey and colleagues, we model potential foreshock sources as "bumps" on the fault interface by assigning a significantly higher normal compression and, in some cases, increased smoothness (lower characteristic slip) over small patches within a seismogenic fault. In order to study the mechanics of isolated patch-induced seismic events preceding the mainshock, we separate these patches sufficiently in space. The simulation results show that our rate-and-state fault model with patches of locally different properties driven by the slow nucleation of the mainshock is indeed able to produce isolated microseismicity before the mainshock. Remarkably, the stress drops of these precursory events are compatible with observations and approximately independent of the patch compression, despite the wide range of the elevated patch compression used in different simulations. We find that this unexpected property of stress drops for this type of model is due to two factors. Firstly, failure of stronger patches results in rupture further into the surrounding fault, keeping the average stress drop down. Secondly, patches close to their local nucleation size relieve a significant amount of stress via aseismic pre-slip, which also helps to keep the stress drop down. Our current work is directed towards investigating the seismic signature of such events and the potential differences with other types of microseismicity.
Flood damage: a model for consistent, complete and multipurpose scenarios
Menoni, Scira; Molinari, Daniela; Ballio, Francesco; Minucci, Guido; Mejri, Ouejdane; Atun, Funda; Berni, Nicola; Pandolfo, Claudia
2016-12-01
Effective flood risk mitigation requires the impacts of flood events to be much better and more reliably known than is currently the case. Available post-flood damage assessments usually supply only a partial vision of the consequences of the floods as they typically respond to the specific needs of a particular stakeholder. Consequently, they generally focus (i) on particular items at risk, (ii) on a certain time window after the occurrence of the flood, (iii) on a specific scale of analysis or (iv) on the analysis of damage only, without an investigation of damage mechanisms and root causes. This paper responds to the necessity of a more integrated interpretation of flood events as the base to address the variety of needs arising after a disaster. In particular, a model is supplied to develop multipurpose complete event scenarios. The model organizes available information after the event according to five logical axes. This way post-flood damage assessments can be developed that (i) are multisectoral, (ii) consider physical as well as functional and systemic damage, (iii) address the spatial scales that are relevant for the event at stake depending on the type of damage that has to be analyzed, i.e., direct, functional and systemic, (iv) consider the temporal evolution of damage and finally (v) allow damage mechanisms and root causes to be understood. All the above features are key for the multi-usability of resulting flood scenarios. The model allows, on the one hand, the rationalization of efforts currently implemented in ex post damage assessments, also with the objective of better programming financial resources that will be needed for these types of events in the future. On the other hand, integrated interpretations of flood events are fundamental to adapting and optimizing flood mitigation strategies on the basis of thorough forensic investigation of each event, as corroborated by the implementation of the model in a case study.
International Nuclear Information System (INIS)
Kim, J. B.; Lee, H. Y.; Lee, J. H.
2002-01-01
It is necessary to develop a reliable numerical analysis method to simulate the plasticity and creep behavior of LMR high temperature structures. Since general purpose finite element analysis codes such as ABAQUS and ANSYS provide various models for plastic hardening and creep equation of Norton's power law, it is possible to perform the separate iscoplasticity analysis. In this study, the high temperature structural analysis program(NONSTA-VP) implementing Chaboche's unified visco plasticity equation into ABAQUS has been developed and the viscoplastic response of the 316 SS plate having a circular hole subjected to a cyclic creep loading has been analyzed. The results among the separate visco plasticity analyses and the unified visco plasticity analysis using NONSTA-VP have been compared and the results from NONSTA-VP shows remarkable responses of stress relaxation and creep behavior during hold time compared to those from separate visco plasticity analyses. Also, it is anticipated to reduce the conservatism arising from using elastic approach for creep-fatigue damage analysis since the stress range and the strain range from the unified visco plasticity analysis has been greatly reduced compared to those from separate visco plasticity analyses and elastic analysis
Transitional Thermal Creep of Early Age Concrete
DEFF Research Database (Denmark)
Hauggaard-Nielsen, Anders Boe; Damkilde, Lars; Freiesleben Hansen, Per
1999-01-01
Couplings between creep of hardened concrete and temperature/water effects are well-known. Both the level and the gradients in time of temperature or water content influence the creep properties. In early age concrete the internal drying and the heat development due to hydration increase the effect...... of these couplings. The purpose of this work is to set up a mathematical model for creep of concrete which includes the transitional thermal effect. The model govern both early age concrete and hardened concrete. The development of the material properties in the model are assumed to depend on the hydration process...... termed the microprestresses, which reduces the stiffness of the concrete and increase the creep rate. The aging material is modelled in an incremental way reflecting the hydration process in which new layers of cement gel solidifies in a stress free state and add stiffness to the material. Analysis...
A Study of the Creep Effect in Loudspeaker Suspension
DEFF Research Database (Denmark)
Agerkvist, Finn T.; Thorborg, Knud; Tinggaard, Carsten
2008-01-01
This paper investigates the creep effect, the visco elastic behaviour of loudspeaker suspension parts, which can be observed as an increase in displacement far below the resonance frequency. The creep effect means that the suspension cannot be modelled as a simple spring. The need for an accurate...... creep model is even larger as the validity of loudspeaker models are now sought extended far into the nonlinear domain of the loudspeaker. Different creep models are investigated and implemented both in simple lumped parameter models as well as time domain non-linear models, the simulation results...
Microstructural causes of negative creep in cast superalloys
International Nuclear Information System (INIS)
Frank, G.
1990-01-01
The dissertation examines by means of microstructural investigations and modelling calculations two types of superalloys: the nickel-base cast alloy IN 738 LC (γ'-hardened, containing MC and M 23 C 6 carbides), and the cobalt-base cast alloy FSX 414 (containing M 23 C 6 carbides, solid solution-hardened). The task was to determine the causes of microstructural volume contraction, in order to improve and facilitate explanation and extrapolation of the materials' long-term behaviour at high temperatures, and to derive if possible information on appropriate measures preventing negative creep, which may lead to critical damage of bolted joints, for instance. (orig./MM) [de
Irradiation-induced creep in graphite: a review
International Nuclear Information System (INIS)
Price, R.J.
1981-08-01
Data on irradiation-induced creep in graphite published since 1972 are reviewed. Sources include restrained shrinkage tests conducted at Petten, the Netherlands, tensile creep experiments with continuous strain registration at Petten and Grenoble, France, and controlled load tests with out-of-reactor strain measurement performed at Oak Ridge National Laboratory, Petten, and in the United Kingdom. The data provide reasonable confirmation of the linear viscoelastic creep model with a recoverable transient strain component followed by a steady-state strain component, except that the steady-state creep coefficient must be treated as a function of neutron fluence and is higher for tensile loading than for compressive loading. The total transient creep strain is approximately equal to the preceding elastic strain. No temperature dependence of the transient creep parameters has been demonstrated. The initial steady-state creep coefficient is inversely proportional to the unirradiated Young modulus
Creep behaviour of heat resistant steels. Pt. 2
International Nuclear Information System (INIS)
Kloos, K.H.; Granacher, J.; Oehl, M.
1993-01-01
Creep data scatter bands of steels 2.25 Cr-1 Mo and 12 Cr-1 Mo-0.3 V were evaluated with the aid of model functions based on time temperature parameters. From the times to reach given strain values, mean isostrain curves in the stress time diagramme were calculated and therefrom, mean creep curves were derived. On this basis, creep equations were established, which include primary-, secondary- and tertiary-creep and are valid in the main range of application of each steel. Further, mean stress strain curves from hot tensile tests were used to describe the initial plastic strain in the creep equations. The values calculated with the established creep equations agreed relatively well with the correspondent original scatter band values from the creep tests. (orig.) [de
A 3D Orthotropic Elastic Continuum Damage Material Model
Energy Technology Data Exchange (ETDEWEB)
English, Shawn Allen [Sandia National Lab. (SNL-CA), Livermore, CA (United States); Brown, Arthur A. [Sandia National Lab. (SNL-CA), Livermore, CA (United States)
2013-08-01
A three dimensional orthotropic elastic constitutive model with continuum damage is implemented for polymer matrix composite lamina. Damage evolves based on a quadratic homogeneous function of thermodynamic forces in the orthotropic planes. A small strain formulation is used to assess damage. In order to account for large deformations, a Kirchhoff material formulation is implemented and coded for numerical simulation in Sandia’s Sierra Finite Element code suite. The theoretical formulation is described in detail. An example of material parameter determination is given and an example is presented.
Modeling of laser damage initiated by surface contamination
International Nuclear Information System (INIS)
Feit, M.D.; Rubenchik, A.M.; Faux, D.R.; Riddle, R.A.; Shapiro, A.; Eder, D.C.; Penetrante, B.M.; Milam, D.; Genin, F.Y.; Kozlowski, M.R.
1996-11-01
The authors are engaged in a comprehensive effort to understand and model the initiation and growth of laser damage initiated by surface contaminants. This includes, for example, the initial absorption by the contaminant, heating and plasma generation, pressure and thermal loading of the transparent substrate, and subsequent shockwave propagation, 'splashing' of molten material and possible spallation, optical propagation and scattering, and treatment of material fracture. The integration use of large radiation hydrodynamics codes, optical propagation codes and material strength codes enables a comprehensive view of the damage process The following picture of surface contaminant initiated laser damage is emerging from our simulations
Research on damage evolution and damage model of 316LN steel during forging
Energy Technology Data Exchange (ETDEWEB)
Duan, X.W., E-mail: dxwmike1998@sina.com; Liu, J.S.
2013-12-20
The tensile tests and unloading tensile experiments of 316LN steel were conducted. The damage evolution processes were investigated by optical microscope. The fracture was studied using a Scanning Electron Microscope (SEM) and optical microscope, of which, the chemical compositions were analyzed by Energy Dispersive Spectrometer (EDS). The results show that voids nucleate by decohesion of Al{sub 2}O{sub 3} inclusions–matrix interface and mainly along the grain boundary, especially, at triangular grain boundary junctions. The tensile processes were simulated by Deform2D under different deformation conditions. The critical damage values were obtained. The model between the critical damage value, temperature and strain rate was established by regression analysis. A combination of numerical simulation and upsetting experiments was applied for verifying the accuracy and reliability of critical damage value. These damage values can be used to predict the initiation of voids during 316LN steel hot forging. So, they have important instructional effects on designing forging technology of 316LN steel.
Correlation of Creep Behavior of Domal Salts
International Nuclear Information System (INIS)
Munson, D.E.
1999-01-01
The experimentally determined creep responses of a number of domal salts have been reported in, the literature. Some of these creep results were obtained using standard (conventional) creep tests. However, more typically, the creep data have come from multistage creep tests, where the number of specimens available for testing was small. An incremental test uses abrupt changes in stress and temperature to produce several time increments (stages) of different creep conditions. Clearly, the ability to analyze these limited data and to correlate them with each other could be of considerable potential value in establishing the mechanical characteristics of salt domes, both generally and specifically. In any analysis, it is necessary to have a framework of rules to provide consistency. The basis for the framework is the Multimechanism-Deformation (M-D) constitutive model. This model utilizes considerable general knowledge of material creep deformation to supplement specific knowledge of the material response of salt. Because the creep of salt is controlled by just a few micromechanical mechanisms, regardless of the origin of the salt, certain of the material parameters are values that can be considered universal to salt. Actual data analysis utilizes the methodology developed for the Waste Isolation Pilot Plant (WIPP) program, and the response of a bedded pure WIPP salt as the baseline for comparison of the domal salts. Creep data from Weeks Island, Bryan Mound, West Hackberry, Bayou Choctaw, and Big Hill salt domes, which are all sites of Strategic Petroleum Reserve (SPR) storage caverns, were analyzed, as were data from the Avery Island, Moss Bluff, and Jennings salt domes. The analysis permits the parameter value sets for the domal salts to be determined in terms of the M-D model with various degrees of completeness. In turn this permits detailed numerical calculations simulating cavern response. Where the set is incomplete because of the sparse database, reasonable
Sequential creep-fatigue interaction in austenitic stainless steel type 316L-SPH
International Nuclear Information System (INIS)
Tavassoli, A.A.; Mottot, M.; Petrequin, P.
1986-01-01
Influence of a prior creep or fatigue exposure on subsequent fatigue or creep properties of stainless steel type 316 L SPH has been investigated. The results obtained are used to verify the validity of time and cycle fraction rule and to obtain information on the effect of very long intermittent hold times on low cycle fatigue properties, as well as on transitory loads occurring during normal service of some structural components of LMFBR reactors. Creep and fatigue tests have been carried out at 600 0 C and under conditions yielding equal or different fatigue saturation and creep stresses. Prior creep damage levels introduced range from primary to tertiary creep, whilst those of fatigue span from 20 to 70 percent of fatigue life. In both creep-fatigue and fatigue-creep sequences in the absence of a permanent prior damage (cavitation or cracking) the subsequent resistance of 316 L-SPH to fatigue or creep is unchanged, if not improved. Thin foils prepared from the specimens confirmed these observations and showed that the dislocation substructure developed during the first mode of testing is quickly replaced by that of the second mode. Grain boundary cavitation does not occur in 316 L-SPH during creep exposures to well beyond the apparent end of secondary stage and as a result prior creep exposures up to approximately 80% of rupture life do not affect fatigue properties. Conversely, significant surface cracks were found in the prior fatigue tested specimens after above about 50% life. In the presence of such cracks the subsequent creep damage was localized at the tip of the main crack and the remaining creep life was found to be usually proportional to the effective specimen cross section. Creep and fatigue sequential damage are not necessarily additive and this type of loadings are in general less severe than the repeated creep-fatigue cycling. 17 refs.
Damage modeling in Small Punch Test specimens
DEFF Research Database (Denmark)
Martínez Pañeda, Emilio; Cuesta, I.I.; Peñuelas, I.
2016-01-01
. Furthermore,Gurson-Tvergaard-Needleman model predictions from a top-down approach are employed to gain insightinto the mechanisms governing crack initiation and subsequent propagation in small punch experiments.An accurate assessment of micromechanical toughness parameters from the SPT...
Creep fracture and creep-fatigue fracture in ceramics and ceramic composites
International Nuclear Information System (INIS)
Suresh, S.
1993-01-01
This paper summarizes recent advances in the areas of subcritical crack growth in ceramics subjected to static and cyclic loads at elevated temperatures. Attention is devoted to the specific role of pre-existing and in-situ-formed glass films in influencing creep fracture and creep-fatigue fracture. Experimental results on the effects of cyclic frequency and load ratio, along with detailed transmission electron microscopy of crack-tip and crack-wake damage are highlighted. Some general conclusions are drawn about the dependence of high-temperature damage tolerance on interfacial glass films and about the susceptibility of ceramic materials to cyclic fatigue fracture
DeLong, S.; Donnellan, A.; Pickering, A.
2017-12-01
Aseismic fault creep, coseismic fault displacement, distributed deformation, and the relative contribution of each have important bearing on infrastructure resilience, risk reduction, and the study of earthquake physics. Furthermore, the impact of interseismic fault creep in rupture propagation scenarios, and its impact and consequently on fault segmentation and maximum earthquake magnitudes, is poorly resolved in current rupture forecast models. The creeping section of the San Andreas Fault (SAF) in Central California is an outstanding area for establishing methodology for future scientific response to damaging earthquakes and for characterizing the fine details of crustal deformation. Here, we describe how data from airborne and terrestrial laser scanning, airborne interferometric radar (UAVSAR), and optical data from satellites and UAVs can be used to characterize rates and map patterns of deformation within fault zones of varying complexity and geomorphic expression. We are evaluating laser point cloud processing, photogrammetric structure from motion, radar interferometry, sub-pixel correlation, and other techniques to characterize the relative ability of each to measure crustal deformation in two and three dimensions through time. We are collecting new and synthesizing existing data from the zone of highest interseismic creep rates along the SAF where a transition from a single main fault trace to a 1-km wide extensional stepover occurs. In the stepover region, creep measurements from alignment arrays 100 meters long across the main fault trace reveal lower rates than those in adjacent, geomorphically simpler parts of the fault. This indicates that deformation is distributed across the en echelon subsidiary faults, by creep and/or stick-slip behavior. Our objectives are to better understand how deformation is partitioned across a fault damage zone, how it is accommodated in the shallow subsurface, and to better characterize the relative amounts of fault creep
Irreversible entropy model for damage diagnosis in resistors
Energy Technology Data Exchange (ETDEWEB)
Cuadras, Angel, E-mail: angel.cuadras@upc.edu; Crisóstomo, Javier; Ovejas, Victoria J.; Quilez, Marcos [Instrumentation, Sensor and Interfaces Group, Electronic Engineering Department, Escola d' Enginyeria de Telecomunicació i Aeronàutica de Castelldefels EETAC, Universitat Politècnica de Catalunya, Barcelona Tech (UPC), Castelldefels-Barcelona (Spain)
2015-10-28
We propose a method to characterize electrical resistor damage based on entropy measurements. Irreversible entropy and the rate at which it is generated are more convenient parameters than resistance for describing damage because they are essentially positive in virtue of the second law of thermodynamics, whereas resistance may increase or decrease depending on the degradation mechanism. Commercial resistors were tested in order to characterize the damage induced by power surges. Resistors were biased with constant and pulsed voltage signals, leading to power dissipation in the range of 4–8 W, which is well above the 0.25 W nominal power to initiate failure. Entropy was inferred from the added power and temperature evolution. A model is proposed to understand the relationship among resistance, entropy, and damage. The power surge dissipates into heat (Joule effect) and damages the resistor. The results show a correlation between entropy generation rate and resistor failure. We conclude that damage can be conveniently assessed from irreversible entropy generation. Our results for resistors can be easily extrapolated to other systems or machines that can be modeled based on their resistance.
Irreversible entropy model for damage diagnosis in resistors
International Nuclear Information System (INIS)
Cuadras, Angel; Crisóstomo, Javier; Ovejas, Victoria J.; Quilez, Marcos
2015-01-01
We propose a method to characterize electrical resistor damage based on entropy measurements. Irreversible entropy and the rate at which it is generated are more convenient parameters than resistance for describing damage because they are essentially positive in virtue of the second law of thermodynamics, whereas resistance may increase or decrease depending on the degradation mechanism. Commercial resistors were tested in order to characterize the damage induced by power surges. Resistors were biased with constant and pulsed voltage signals, leading to power dissipation in the range of 4–8 W, which is well above the 0.25 W nominal power to initiate failure. Entropy was inferred from the added power and temperature evolution. A model is proposed to understand the relationship among resistance, entropy, and damage. The power surge dissipates into heat (Joule effect) and damages the resistor. The results show a correlation between entropy generation rate and resistor failure. We conclude that damage can be conveniently assessed from irreversible entropy generation. Our results for resistors can be easily extrapolated to other systems or machines that can be modeled based on their resistance
Irradiation creep, stress relaxation and a mechanical equation of state
International Nuclear Information System (INIS)
Foster, J.P.
1976-01-01
Irradiation creep and stress relaxation data are available from the United Kingdom for 20 percent CW M316, 20 percent CW FV 548 and FHT PE16 using pure torsion in the absence of swelling at 300 0 C. Irradiation creep models were used to calculate the relaxation and permanent deflection of the stress relaxation tests. Two relationships between irradiation creep and stress relaxation were assessed by comparing the measured and calculated stress relaxation and permanent deflection. The results show that for M316 and FV548, the stress relaxation and deflection may be calculated using irradiation creep models when the stress rate term arising from the irradiation creep model is set equal to zero. In the case of PE16, the inability to calculate the stress relaxation and permanent deflection from the irradiation creep data was attributed to differences in creep behavior arising from lot-to-lot variations in alloying elements and impurity content. A modification of the FV548 and PE16 irradiation creep coefficients was necessary in order to calculate the stress relaxation and deflection. The modifications in FV548 and PE16 irradiation creep properties reduces the large variation in the transient or incubation parameter predicted by irradiation creep tests for M316, FV548 and PE16
Two-dimensional strain gradient damage modeling: a variational approach
Placidi, Luca; Misra, Anil; Barchiesi, Emilio
2018-06-01
In this paper, we formulate a linear elastic second gradient isotropic two-dimensional continuum model accounting for irreversible damage. The failure is defined as the condition in which the damage parameter reaches 1, at least in one point of the domain. The quasi-static approximation is done, i.e., the kinetic energy is assumed to be negligible. In order to deal with dissipation, a damage dissipation term is considered in the deformation energy functional. The key goal of this paper is to apply a non-standard variational procedure to exploit the damage irreversibility argument. As a result, we derive not only the equilibrium equations but, notably, also the Karush-Kuhn-Tucker conditions. Finally, numerical simulations for exemplary problems are discussed as some constitutive parameters are varying, with the inclusion of a mesh-independence evidence. Element-free Galerkin method and moving least square shape functions have been employed.
Formability prediction for AHSS materials using damage models
Amaral, R.; Santos, Abel D.; José, César de Sá; Miranda, Sara
2017-05-01
Advanced high strength steels (AHSS) are seeing an increased use, mostly due to lightweight design in automobile industry and strict regulations on safety and greenhouse gases emissions. However, the use of these materials, characterized by a high strength to weight ratio, stiffness and high work hardening at early stages of plastic deformation, have imposed many challenges in sheet metal industry, mainly their low formability and different behaviour, when compared to traditional steels, which may represent a defying task, both to obtain a successful component and also when using numerical simulation to predict material behaviour and its fracture limits. Although numerical prediction of critical strains in sheet metal forming processes is still very often based on the classic forming limit diagrams, alternative approaches can use damage models, which are based on stress states to predict failure during the forming process and they can be classified as empirical, physics based and phenomenological models. In the present paper a comparative analysis of different ductile damage models is carried out, in order numerically evaluate two isotropic coupled damage models proposed by Johnson-Cook and Gurson-Tvergaard-Needleman (GTN), each of them corresponding to the first two previous group classification. Finite element analysis is used considering these damage mechanics approaches and the obtained results are compared with experimental Nakajima tests, thus being possible to evaluate and validate the ability to predict damage and formability limits for previous defined approaches.
Formability prediction for AHSS materials using damage models
International Nuclear Information System (INIS)
Amaral, R.; Miranda, Sara; Santos, Abel D.; José, César de Sá
2017-01-01
Advanced high strength steels (AHSS) are seeing an increased use, mostly due to lightweight design in automobile industry and strict regulations on safety and greenhouse gases emissions. However, the use of these materials, characterized by a high strength to weight ratio, stiffness and high work hardening at early stages of plastic deformation, have imposed many challenges in sheet metal industry, mainly their low formability and different behaviour, when compared to traditional steels, which may represent a defying task, both to obtain a successful component and also when using numerical simulation to predict material behaviour and its fracture limits. Although numerical prediction of critical strains in sheet metal forming processes is still very often based on the classic forming limit diagrams, alternative approaches can use damage models, which are based on stress states to predict failure during the forming process and they can be classified as empirical, physics based and phenomenological models. In the present paper a comparative analysis of different ductile damage models is carried out, in order numerically evaluate two isotropic coupled damage models proposed by Johnson-Cook and Gurson-Tvergaard-Needleman (GTN), each of them corresponding to the first two previous group classification. Finite element analysis is used considering these damage mechanics approaches and the obtained results are compared with experimental Nakajima tests, thus being possible to evaluate and validate the ability to predict damage and formability limits for previous defined approaches. (paper)
International Nuclear Information System (INIS)
Stone, C.M.; Nickell, R.E.
1977-01-01
Because of the characteristics of LMFBR primary piping components (thin-walled, low pressure, high temperature), the designer must guard against creep buckling as a potential failure mode for certain critical regions, such as elbows, where structural flexibility and inelastic response may combine to concentrate deformation and cause instability. The ASME Boiler and Pressure Vessel Code, through its elevated temperature Code Case 1592 (Section III, Division 1) provides design rules for Class 1 components aimed at preventing creep buckling during the design life. A similar set of rules is being developed for Class 2 and 3 components at this time. One of the original concepts behind the creep buckling rules was that the variability in creep properties (especially due to the effects of prior heat treatment), the uncertainty about initial imperfections, and the lack of confirmed accuracy of design analysis meant that conservatism would be difficult to assure. As a result, a factor of ten on service life was required (i.e. analysis must show that, under service conditions that extrapolate the life of the component by ten times, creep buckling does not occur). Two obvious problems with this approach are that: first, the creep behavior must also be extrapolated (since most creep experiments are terminated at a small fraction of the design life, extrapolation of creep data is already an issue, irrespective of the creep buckling question); second the nonlinear creep analysis, which is very nearly prohibitively expensive for design life histograms, becomes even more costly. Analytical results for an aluminum cylindrical shell subjected to axial loads at elevated temperatures are used to examine the supposed equivalence of two types of time-dependent buckling safety factors - a factor of ten on service life and a factor of 1.5 on loading
Bayesian inference method for stochastic damage accumulation modeling
International Nuclear Information System (INIS)
Jiang, Xiaomo; Yuan, Yong; Liu, Xian
2013-01-01
Damage accumulation based reliability model plays an increasingly important role in successful realization of condition based maintenance for complicated engineering systems. This paper developed a Bayesian framework to establish stochastic damage accumulation model from historical inspection data, considering data uncertainty. Proportional hazards modeling technique is developed to model the nonlinear effect of multiple influencing factors on system reliability. Different from other hazard modeling techniques such as normal linear regression model, the approach does not require any distribution assumption for the hazard model, and can be applied for a wide variety of distribution models. A Bayesian network is created to represent the nonlinear proportional hazards models and to estimate model parameters by Bayesian inference with Markov Chain Monte Carlo simulation. Both qualitative and quantitative approaches are developed to assess the validity of the established damage accumulation model. Anderson–Darling goodness-of-fit test is employed to perform the normality test, and Box–Cox transformation approach is utilized to convert the non-normality data into normal distribution for hypothesis testing in quantitative model validation. The methodology is illustrated with the seepage data collected from real-world subway tunnels.
Effect of PVA fiber content on creep property of fiber reinforced high-strength concrete columns
Xu, Zongnan; Wang, Tao; Wang, Weilun
2018-04-01
The effect of PVA (polyvinyl alcohol) fiber content on the creep property of fiber reinforced high-strength concrete columns was investigated. The correction factor of PVA fiber content was proposed and the creep prediction model of ACI209 was modified. Controlling the concrete strength as C80, changing the content of PVA fiber (volume fraction 0%, 0.25%, 0.5%, 1% respectively), the creep experiment of PVA fiber reinforced concrete columns was carried out, the creep coefficient of each specimen was calculated to characterize the creep property. The influence of PVA fiber content on the creep property was analyzed based on the creep coefficient and the calculation results of several frequently used creep prediction models. The correction factor of PVA fiber content was proposed to modify the ACI209 creep prediction model.
Predicting creep rupture from early strain data
International Nuclear Information System (INIS)
Holmstroem, Stefan; Auerkari, Pertti
2009-01-01
To extend creep life modelling from classical rupture modelling, a robust and effective parametric strain model has been developed. The model can reproduce with good accuracy all parts of the creep curve, economically utilising the available rupture models. The resulting combined model can also be used to predict rupture from the available strain data, and to further improve the rupture models. The methodology can utilise unfailed specimen data for life assessment at lower stress levels than what is possible from rupture data alone. Master curves for creep strain and rupture have been produced for oxygen-free phosphorus-doped (OFP) copper with a maximum testing time of 51,000 h. Values of time to specific strain at given stress (40-165 MPa) and temperature (125-350 deg. C) were fitted to the models in the strain range of 0.1-38%. With typical inhomogeneous multi-batch creep data, the combined strain and rupture modelling involves the steps of investigation of the data quality, extraction of elastic and creep strain response, rupture modelling, data set balancing and creep strain modelling. Finally, the master curves for strain and rupture are tested and validated for overall fitting efficiency. With the Wilshire equation as the basis for the rupture model, the strain model applies classical parametric principles with an Arrhenius type of thermal activation and a power law type of stress dependence for the strain rate. The strain model also assumes that the processes of primary and secondary creep can be reasonably correlated. The rupture model represents a clear improvement over previous models in the range of the test data. The creep strain information from interrupted and running tests were assessed together with the rupture data investigating the possibility of rupture model improvement towards lower stress levels by inverse utilisation of the combined rupture based strain model. The developed creep strain model together with the improved rupture model is
Spherical Indentation Techniques for Creep Property Evaluation Considering Transient Creep
Energy Technology Data Exchange (ETDEWEB)
Lim, Dongkyu; Kim, Minsoo; Lee, Hyungyil [Sogang Univ., Seoul, (Korea, Republic of); Lee, Jin Haeng [Korea Atomic Energy Research Institute, Daejeon (Korea, Republic of)
2013-11-15
Creep through nanoindentations has attracted increasing research attention in recent years. Many studies related to indentation creep tests, however, have simply focused on the characteristics of steady-state creep, and there exist wide discrepancies between the uniaxial test and the indentation test. In this study, we performed a computational simulation of spherical indentations, and we proposed a method for evaluating the creep properties onsidering transient creep. We investigated the material behavior with variation of creep properties and expressed it using regression equations for normalized variables. We finally developed a program to evaluate the creep properties considering transient creep. By using the proposed method, we successfully obtained creep exponents with an average error less than 1.1 and creep coefficients with an average error less than 2.3 from the load-depth curve.
Spherical Indentation Techniques for Creep Property Evaluation Considering Transient Creep
International Nuclear Information System (INIS)
Lim, Dongkyu; Kim, Minsoo; Lee, Hyungyil; Lee, Jin Haeng
2013-01-01
Creep through nanoindentations has attracted increasing research attention in recent years. Many studies related to indentation creep tests, however, have simply focused on the characteristics of steady-state creep, and there exist wide discrepancies between the uniaxial test and the indentation test. In this study, we performed a computational simulation of spherical indentations, and we proposed a method for evaluating the creep properties onsidering transient creep. We investigated the material behavior with variation of creep properties and expressed it using regression equations for normalized variables. We finally developed a program to evaluate the creep properties considering transient creep. By using the proposed method, we successfully obtained creep exponents with an average error less than 1.1 and creep coefficients with an average error less than 2.3 from the load-depth curve
Creep properties of discontinuous fibre composites with partly creeping fibres
International Nuclear Information System (INIS)
Bilde-Soerensen, J.B.; Lilholt, H.
1977-05-01
In a previous report (RISO-M-1810) the creep properties of discontinuous fibre composites with non-creeping fibres were analyzed. In the present report this analysis is extended to include the case of discontinuous composites with partly creeping fibres. It is shown that the creep properties of the composite at a given strain rate, epsilonsub(c), depend on the creep properties of the matrix at a strain rate higher than epsilonsub(c), and on the creep properties of the fibres at epsilonsub(c). The composite creep law is presented in a form which permits a graphical determination of the composite creep curve. This can be constructed on the basis of the matrix and the fibre creep curves by vector operations in a log epsilon vs. log sigma diagram. The matrix contribution to the creep strength can be evaluated by a simple method. (author)
International Nuclear Information System (INIS)
Asayama, Tai; Tachibana, Yukio
2007-01-01
This report describes the results of investigation on Task 5 of DOE/ASME Materials Project based on a contract between ASME Standards Technology, LLC (ASME ST-LLC) and Japan Atomic Energy Agency (JAEA). Task 5 is to collect available creep-fatigue data and study existing creep-fatigue evaluation procedures for Grade 91 steel and Hastelloy XR. Part I of this report is devoted to Grade 91 steel. Existing creep-fatigue data were collected (Appendix A) and analyzed from the viewpoints of establishing a creep-fatigue procedure for VHTR design. A fair amount of creep-fatigue data has been obtained and creep-fatigue phenomena have been clarified to develop design standards mainly for fast breeder reactors. Following this, existing creep-fatigue procedures were studied and it was clarified that the creep-fatigue evaluation procedure of the ASME-NH has a lot of conservatisms and they were analyzed in detail from the viewpoints of the evaluation of creep damage of material. Based on the above studies, suggestions to improve the ASME-NH procedure along with necessary research and development items were presented. Part II of this report is devoted to Hastelloy XR. Existing creep-fatigue data used for development of the high temperature structural design guideline for High Temperature Gas-cooled Reactor (HTGR) were collected. Creep-fatigue evaluation procedure in the design guideline and its application to design of the intermediate heat exchanger (IHX) for High Temperature Engineering Test Reactor (HTTR) was described. Finally, some necessary research and development items in relation to creep-fatigue evaluation for Gen IV and VHTR reactors were presented.
Progressive Damage Modeling of Durable Bonded Joint Technology
Leone, Frank A.; Davila, Carlos G.; Lin, Shih-Yung; Smeltzer, Stan; Girolamo, Donato; Ghose, Sayata; Guzman, Juan C.; McCarville, Duglas A.
2013-01-01
The development of durable bonded joint technology for assembling composite structures for launch vehicles is being pursued for the U.S. Space Launch System. The present work is related to the development and application of progressive damage modeling techniques to bonded joint technology applicable to a wide range of sandwich structures for a Heavy Lift Launch Vehicle. The joint designs studied in this work include a conventional composite splice joint and a NASA-patented Durable Redundant Joint. Both designs involve a honeycomb sandwich with carbon/epoxy facesheets joined with adhesively bonded doublers. Progressive damage modeling allows for the prediction of the initiation and evolution of damage. For structures that include multiple materials, the number of potential failure mechanisms that must be considered increases the complexity of the analyses. Potential failure mechanisms include fiber fracture, matrix cracking, delamination, core crushing, adhesive failure, and their interactions. The joints were modeled using Abaqus parametric finite element models, in which damage was modeled with user-written subroutines. Each ply was meshed discretely, and layers of cohesive elements were used to account for delaminations and to model the adhesive layers. Good correlation with experimental results was achieved both in terms of load-displacement history and predicted failure mechanisms.
Influence of phosphorus on the creep ductility of copper
International Nuclear Information System (INIS)
Sandström, Rolf; Wu, Rui
2013-01-01
Around 1990 it was discovered that pure copper could have extra low creep ductility in the temperature interval 180–250 °C. The material was intended for use in canisters for nuclear waste disposal. Although extra low creep ductility was not observed much below 180 °C and the temperature in the canister will never exceed 100 °C, it was feared that the creep ductility could reach low values at lower temperatures after long term exposure. If 50 ppm phosphorus was added to the copper the low creep ductility disappeared. A creep cavitation model is presented that can quantitatively describe the cavitation behaviour in uniaxial and multiaxial creep tests as well as the observed creep ductility for copper with and without phosphorus. A so-called double ledge model has been introduced that demonstrates why the nucleation rate of creep cavities is often proportional to the creep rate. The phosphorus agglomerates at the grain boundaries and limits their local deformation and thereby reduces the formation and growth of cavities. This explains why extra low creep ductility does not occur in phosphorus alloyed copper
Creep analysis of silicone for podiatry applications.
Janeiro-Arocas, Julia; Tarrío-Saavedra, Javier; López-Beceiro, Jorge; Naya, Salvador; López-Canosa, Adrián; Heredia-García, Nicolás; Artiaga, Ramón
2016-10-01
This work shows an effective methodology to characterize the creep-recovery behavior of silicones before their application in podiatry. The aim is to characterize, model and compare the creep-recovery properties of different types of silicone used in podiatry orthotics. Creep-recovery phenomena of silicones used in podiatry orthotics is characterized by dynamic mechanical analysis (DMA). Silicones provided by Herbitas are compared by observing their viscoelastic properties by Functional Data Analysis (FDA) and nonlinear regression. The relationship between strain and time is modeled by fixed and mixed effects nonlinear regression to compare easily and intuitively podiatry silicones. Functional ANOVA and Kohlrausch-Willians-Watts (KWW) model with fixed and mixed effects allows us to compare different silicones observing the values of fitting parameters and their physical meaning. The differences between silicones are related to the variations of breadth of creep-recovery time distribution and instantaneous deformation-permanent strain. Nevertheless, the mean creep-relaxation time is the same for all the studied silicones. Silicones used in palliative orthoses have higher instantaneous deformation-permanent strain and narrower creep-recovery distribution. The proposed methodology based on DMA, FDA and nonlinear regression is an useful tool to characterize and choose the proper silicone for each podiatry application according to their viscoelastic properties. Copyright © 2016 Elsevier Ltd. All rights reserved.
Relaxation of Shot-Peened Residual Stresses Under Creep Loading (Preprint)
National Research Council Canada - National Science Library
Buchanan, Dennis J; John, Reji; Brockman, Robert A
2008-01-01